/

**Author**:
Lemaitre J.
Desmorat R.

**Tags:**
physics
engineering
mechanics
damage mechanics

**ISBN**: 3-540-21503-4

**Year**: 2005

Text

Engineering Damage Mechanics

Jean Lemaitre Rodrigue Desmorat Engineering Damage Mechanics Ductile, Creep, Fatigue and Brittle Failures With 135 Figures 13

Professor Jean Lemaitre Professor Rodrigue Desmorat Universit´ e Paris 6 ´ 61, Av. du Président Wilson ISBN 3-540-21503-4 Springer Berlin Heidelberg New York Library of Congress Control Number: 2004111141 This work is subject to copyright. All rights are reserved, whether the whole or part of the material is concerned, specifically the rights of translation, reprinting, reuse of illustrations, recitation, broad- casting, reproduction on microfilm or in any other way, and storage in data banks. Duplication of this publication or parts thereof is permitted only under the provisions of the German Copyright Law of September 9, 1965, in its current version, and permission for use must always be obtained from Springer. Violations are liable to prosecution under the German Copyright Law. Springer is a part of Springer Science+Business Media springeronline.com © Springer-Verlag Berlin Heidelberg 2005 Printed in The Netherlands The use of general descriptive names, registered names, trademarks, etc. in this publication does not imply, even in the absence of a specific statement, that such names are exempt from the relevant pro- tective laws and regulations and therefore free for general use. Typesetting and Production: LE-TeX Jelonek, Schmidt und Vöckler GbR, Leipzig Cover design: design & production GmbH, Heidelberg Printed on acid-free paper 55/3141/YL 543210 94230 Cachan, France L.M.T. Cachan Ecole Normale Supérieure de Cachan

Foreword The analysis of stress and deformation of structures and components is not an end in itself. The aim is to predict the serviceability, reliability, and manu- facturability of both existing structures and components and of proposed designs. In order to make such assessments, the mode (or modes) of failure need to be known and accounted for. The damage can take many forms, e.g., cracks, voids, chemical attack. In any case, the result is deterioration of the structure or component. Predicting the implications of that deterioration for mechanical integrity is the goal of damage mechanics. The concept of damage and the realization of its importance for engineer- ing are not new. What is relatively new (within the last 35 years or so) is the development of the framework of Continuum Damage Mechanics. There have been many contributors to this development, but the contributions of the French school and particularly those of Jean Lemaitre stand out. The field of damage mechanics has advanced to the point where it is an engineer- ing tool, with wide applications in industry. In practice, needs arise at several levels. In a preliminary design stage, the need is often for rapid methods of analysis that exhibit trends. In a final design stage or in carrying out a safety assessment the need can be for accurate quantitative predictions. This book provides formulations that span such a range for a variety of technologically important modes of failure, providing a perspective on the advantages and disadvantages of various approaches -- from uncoupled, post-processing anal- yses to fully coupled damage analyses. After introductory chapters on Continuum Damage Mechanics and nu- merical analysis of damage, the remaining chapters focus on a mode of dam- age -- ductile failures; low-cycle fatigue; creep, creep-fatigue and dynamic failures; high-cycle fatigue; and failure of brittle and quasi-brittle materials. Each of these chapters appropriately begins with a section on engineering considerations to set the stage and provides a guide to analysis methods and tools. It is quite remarkable that such a wide range of behaviors are incor- porated within a unified presentation. The damage mechanics "apple" has blossomed into a tree with many branches!

VI Foreword Since failure is a complex nonlinear process, the predicted behavior can be sensitive to parameter values. Their appropriate identification is key for reliable engineering predictions, as is understanding the sensitivity of predic- tions to the particular choice of parameter values. The presentation here pays attention to parameter sensitivity as well as to parameter identification. This book provides a comprehensive guide to Engineering Damage Me- chanics. It should appeal to all engineers and students of engineering con- cerned with lifetime prediction and with the failure resistant design of struc- tures, components, and processes. Brown University, USA Alan Needleman

Introduction The single apple has become a tree, an apple tree painted by Annie Lemaitre from which two apples fell on the cover page! A decade after "A Course on Damage Mechanics" the topic has grown up to reach the field of applications. Aircraft engines and, more generally, aeronautics, nuclear power plants, metal forming, civil engineering, and the automotive industry have already devel- oped and benifited from damage-based methods to increase performance and security. The time has come to propose simplified or more advanced methods, structured in a unified framework to designers of any mechanical components such as early design with fast calculation of structural failures by closed-form solutions and final validation of solutions by numerical failures analysis. This was the ambition for this book! This is the reason for having many basic examples and insisting on prac- tical methods such as the difficult problem of the material parameters identi- fication for which a systematic sensitivity analysis is performed for each type of application. Very accurate calculations are too often made with a very poor accuracy of the material parameters! To help, probability concepts are introduced either for random loadings or scatter due to microdefects in the materials. This is done mainly for fatigue failure phenomena and brittle ma- terials but may apply to other cases. Damage mechanics applies to all materials, including metals and alloys, polymers, elastomers, composites, and concrete, because even if the mecha- nisms are different on a microscale, they have more or less the same qualita- tive behaviors on meso- or macroscales. Nevertheless, due to data availability most quantitative examples are related to metals. • The first chapter reassembles the main concepts of Continuum Damage Mechanics, that is the theoretical tools to apply to specific cases: dam- age variable, isotropic and anisotropic description, thermodynamics which yields methods of damage measurements, damage laws, coupling with strain behavior, localization, and mesocrack initiation. • The second chapter is a set of numerical tools for solving the nonlinear problems related to damage evaluation in structures. Post-processing clas-

VIII Introduction sical structure analysis, either by the time integration of a damage law, solving a micromechanical two-scale damage model, or when damage is not localized, by solving fully coupled strain-damage structural problems. • The five following chapters are organized in the same way: four sections from the simplest methods with closed-form solutions to more advanced numerical analyses. The first sections "Engineering Considerations" give the domain of application of the chapter. The second sections "Fast Cal- culations of Structural Failures" describe some simplified methods to be used in early design. They are applied in the third sections "Basic En- gineering Examples" to damage failures of members having stress con- centration zones, pressurized cylinders and beams in bending. The fourth sections "Numerical Failure Analysis" describe, using examples, more ac- curate methods for numerical calculations with computers. -- The third chapter is devoted to ductile failures involving large defor- mations for applications in metal forming processes or effects of large overloadings on structures in service. -- The fourth chapter deals with low-cycle fatigue involving important coupling between damage and plasticity for applications on structures heavily burdened by cyclic loadings. -- The fifth chapter introduces the effects of temperature-inducing creep and its nonlinear interaction with damage for applications on struc- tures loaded statically or cyclically at elevated temperature, or dy- namically. -- The sixth chapter concerns high-cycle fatigue which uses a two-scale damage model of an elasto-plastic damaged inclusion in an elastic matrix with "elastic fatigue" applications from complex histories of loading to three-dimensional and random loadings. -- The seventh chapter is devoted to brittle and quasi-brittle materials: quasi-brittle when an irreversible process induces damage, brittle when the fracture occurs without any measurable precursor. Statistical and probabilistic methods are used to represent the large scatter generally observed in the failure of these materials. Their applications concern structures made of concrete, ceramics or composite materials. How should you use the book? As you like it of course but be aware that each chapter is more or less self-contained, with many referrals to the two first chapters of basic concepts of damage mechanics and its numerical pro- cessing. Furthermore, at the end of each chapter on applications, the section "Hierachic Approach" is more or less a summary of the chapter with indica- tions on the domain of validity of each model or method. To help engineers, researchers, students, beginners or not, each section is categorized by the number of apples: means easy to read, easy to apply. means a read with attention and an application with care. means a more advanced theory needing a numerical analysis.

Introduction IX Of course this classification is subjective but it has been checked by some friends working mostly in industry: J. Besson from ENSMP Centre des ma- t´ eriaux (Chap. 1), E. Lorentz from Electricit´ e de France (Chap. 2), F. Moussy from Renault (Chap. 3), J.P. Sermage from E.D.F. SEPTEN (Chap. 4), B. Dambrine from SNECMA (Chap. 5), A. Galtier from ARCELOR for (Chap. 6), B. Bary from C.E.A. (Chap. 7), A. Benallal from C.N.R.S.-LMT Cachan and M. Elgueta from Chili University (overall book), and A. Needle- man from Brown University who wrote the foreword. Our thanks to all of them for their expertise and advice. "Merci" also to our friends from "Lab- oratoire de M´ ecanique et Technologie" at Cachan who participated in the birth of many parts of this book and particularly to Catherine G´ enin. Bon courage pour une lecture fructueuse LMT Cachan, France Jean Lemaitre Rodrigue Desmorat

Contents 1 Background on Continuum Damage Mechanics .. .. .. .. .. . 1 1.1 Physics and Damage Variables ........................... 1 1.1.1 DefinitionofaScalarDamageVariable. . . . . . . . . . . . . . 3 1.1.2 Definition of Several Scalar Damage Variables . . . . . . . . 3 1.1.3 DefinitionofaTensorialDamageVariable. . . . . . . . . . . 4 1.1.4 Effective Stress Concept........................... 5 1.1.5 Effects of Damage ................................ 7 1.2 Thermodynamics of Damage............................. 7 1.2.1 General Framework............................... 7 1.2.2 State Potential for Isotropic Damage... .. .. .. .. .. .. . 10 1.2.3 StatePotentialforAnisotropicDamage . . . . . . . . . . . . . 11 1.2.4 Quasi-Unilateral Conditions of Microdefects Closure . . 12 1.3 Measurement of Damage ................................ 16 1.3.1 Isotropic Elasticity Change ........................ 17 1.3.2 Isotropic Elasticity Change by Ultrasonic Waves . . . . . . 17 1.3.3 Anisotropic Elasticity Change...................... 18 1.3.4 Hardness Change................................. 22 1.3.5 Elasticity Field Change ........................... 23 1.4 Kinetic Laws of Damage Evolution ....................... 26 1.4.1 Damage Threshold and Mesocrack Initiation . . . . . . . . . 27 1.4.2 Formulation of the Isotropic Unified Damage Law . . . . 32 1.4.3 Formulation of the Anisotropic Damage Law . . . . . . . . . 34 1.4.4 Fast Identification of Damage Material Parameters . . . 35 1.4.5 GeneralizationoftheUnifiedDamageLaw . . . . . . . . . . 41 1.5 Elasto-(Visco-)PlasticityCoupled with Damage ............ 45 1.5.1 Basic Equations without Damage Coupling . . . . . . . . . . 45 1.5.2 Coupling with Isotropic Damage .. .. .. .. .. .. .. .. .. . 52 1.5.3 Coupling with Anisotropic Damage .. .. .. .. .. .... .. . 56 1.5.4 Non-Isothermal Behavior .......................... 60 1.5.5 Two-Scale Model for Damage at Microscale . . . . . . . . . . 60

XII Contents 1.6 Localization and MesocrackInitiation..................... 65 1.6.1 Critical Damage Criterion ......................... 65 1.6.2 StrainDamageLocalizationCriterion. . . . . . . . . . . . . . . 65 1.6.3 SizeandOrientationoftheCrackInitiated. . . . . . . . . . 73 2 Numerical Analysis of Damage ........................... 77 2.1 Uncoupled Analysis..................................... 78 2.1.1 Uniaxial Loading................................. 79 2.1.2 ProportionalLoading ............................. 82 2.1.3 Post-processing a (Visco-)Plastic Computation . . . . . . . 85 2.1.4 Post-processing an Elastic Computation . . . . . . . . . . . . . 86 2.1.5 Jump-in-Cycles Procedure in Fatigue .. .. .. .. .. .. .. . 88 2.2 Fully-Coupled Analysis.................................. 90 2.2.1 Nonlinear Material Behavior FEA .................. 91 2.2.2 FEResolutionoftheGlobalEquilibrium. . . . . . . . . . . . 94 2.2.3LocalIntegrationSubroutines......................96 2.2.4 Single Implicit Algorithm for Damage Models . . . . . . . . 97 2.2.5 Damage Models with Microdefects Closure Effect ................... 105 2.2.6 Performing FE Damage Computations .............. 111 2.2.7 Localization Limiters ............................. 112 2.3 Locally-Coupled Analysis................................ 114 2.3.1 Post-Processing a Reference Structure Calculation . . . . 115 2.3.2 Implicit Scheme for the Two-Scale Model............ 117 2.3.3DAMAGE2000Post-Processor.....................119 2.4 Precise Identification of Material Parameters............... 120 2.4.1 Formulation of an Identification Problem . . . . . . . . . . . . 121 2.4.2 Minimization Algorithm for Least Squares Problems . . 123 2.4.3 Procedure for Numerical Identification .............. 127 2.4.4 Cross Identification of Damage Evolution Laws . . . . . . . 132 2.4.5 Validation Procedure ............................. 133 2.4.6 Sensitivity Analysis............................... 135 2.5 Hierarchic Approach and Model Updating ................. 137 2.6 Table of Material Damage Parameters.. .. .. .. .. .. .. .. .. .. . 138 3 Ductile Failures ........................................... 141 3.1 Engineering Considerations .............................. 142 3.2 Fast Calculation of Structural Failures . .. .. .. .. .. .. .. .. .. . 142 3.2.1 Uniaxial Behavior and Validation of the Damage Law............................... 143 3.2.2 Case of Proportional Loading ...................... 144 3.2.3 Sensitivity Analysis............................... 146 3.2.4 Stress Concentration and the Neuber Method . . . . . . . . 147 3.2.5 Safety Margin and Crack Arrest.................... 152

Contents XIII 3.3 Basic Engineering Examples ............................. 154 3.3.1 Plates or Members with Holes or Notches .. .. .. .. .. . 154 3.3.2 Pressurized Shallow Cylinders...................... 156 3.3.3 Post-Buckling in Bending.......................... 158 3.3.4 Damage Criteria in Proportional Loading . . . . . . . . . . . . 160 3.4 Numerical Failure Analysis .............................. 166 3.4.1 Finite Strains .................................... 167 3.4.2 Deep Drawing Limits ............................. 170 3.4.3 Damage in Cold Extrusion Process ................. 172 3.4.4 Crack Initiation Direction ......................... 174 3.4.5 PorousMaterials--theGursonModel. . . . . . . . . . . . . . .176 3.4.6 Frames Analysis by Lumped Damage Mechanics . . . . . . 181 3.4.7 Predeformed and Predamaged Initial Conditions . . . . . 184 3.4.8 Hierarchic Approach up to Full Anisotropy . . . . . . . . . . 188 4L o w C y c l e F a t i g u e ........................................ 191 4.1 Engineering Considerations .............................. 192 4.2 Fast Calculation of Structural Failures . .. .. .. .. .. .. .. .. .. . 192 4.2.1 Uniaxial Behavior and Validation of the Damage Law............................... 192 4.2.2 Case of Proportional Loading ...................... 198 4.2.3 Sensitivity Analysis............................... 199 4.2.4 Cyclic Elasto-Plastic Stress Concentration . . . . . . . . . . . 201 4.2.5 Safety Margin and Crack Growth................... 208 4.3 Basic Engineering Examples ............................. 208 4.3.1 PlateorMemberswithHolesorNotches . . . . . . . . . . . .208 4.3.2 Pressurized Shallow Cylinders...................... 210 4.3.3 Cyclic Bending of Beams .......................... 212 4.4 Numerical Failure Analysis .............................. 213 4.4.1 Effects of Loading History ......................... 214 4.4.2 Multiaxial and Multilevel Fatigue Loadings . . . . . . . . . . 216 4.4.3DamageandFatigueofElastomers.................221 4.4.4 Predeformed and Predamaged Initial Conditions . . . . . 227 4.4.5 Hierarchic Approach up to Non-ProportionalEffects..................... 228 5 Creep, Creep-Fatigue, and Dynamic Failures ... .. .. .. .. .. . 233 5.1 Engineering Considerations .............................. 234 5.2 Fast Calculation of Structural Failures . .. .. .. .. .. .. .. .. .. . 234 5.2.1 Uniaxial Behavior and Validation of the Damage Law............................... 235 5.2.2 Case of Proportional Loading ...................... 237 5.2.3 Sensitivity Analysis............................... 241 5.2.4 Elasto-Visco-Plastic Stress Concentration . . . . . . . . . . . . 244 5.2.5 Safety Margin and Crack Growth................... 247

XIV Contents 5.3 Basic Engineering Examples ............................. 248 5.3.1 Strain Rate and Temperature-Dependent Yield Stress... .. .. .. .. . 248 5.3.2 Plates or Members with Holes or Notches .. .. .. .. .. . 250 5.3.3 Pressurized Shallow Cylinder ...................... 253 5.3.4 Adiabatic Dynamics Post-Buckling in Bending . . . . . . . 255 5.4 Numerical Failure Analysis .............................. 257 5.4.1 HollowSphereunderExternalPressure . . . . . . . . . . . . .258 5.4.2 Effect of Loading History: Creep-Fatigue . . . . . . . . . . . . 262 5.4.3 Creep-Fatigue and Thermomechanical Loadings .. .. .. .. .. .. .. .. .. . 263 5.4.4 DynamicAnalysisofCrashProblems. . . . . . . . . . . . . . .267 5.4.5 Ballistic Impact and Penetration of Projectiles . . . . . . . 269 5.4.6 Predeformed and Predamaged Initial Conditions . . . . . 272 5.4.7 Hierarchic Approach up to Viscous Elastomers.......................... 274 6 High Cycle Fatigue ....................................... 277 6.1 Engineering Considerations .............................. 278 6.2 Fast Calculation of Structural Failures . .. .. .. .. .. .. .. .. .. . 279 6.2.1 Characteristic Effects in High-Cycle Fatigue .. .. .. .. . 279 6.2.2 Fatigue Limit Criteria ............................ 281 6.2.3 Two-Scale Damage Model in ProportionalLoading........................... 283 6.2.4 Sensitivity Analysis............................... 289 6.2.5 Safety Margin and Crack Growth................... 292 6.3 Basic Engineering Examples ............................. 294 6.3.1 Plates or Members with Holes or Notches .. .. .. .. .. . 294 6.3.2 Pressurized Shallow Cylinders...................... 295 6.3.3 Bending of Beams ................................ 297 6.3.4 Random Loadings ................................ 297 6.4 Numerical Failure Analysis .............................. 300 6.4.1 Effects of Loading History ......................... 300 6.4.2 Non-Proportional Loading of a Thinned Shell . . . . . . . . 303 6.4.3 Random Distribution of Initial Defects . .. .. .. .. .. .. . 307 6.4.4 Stochastic Resolution by Monte Carlo Method . . . . . . . 309 6.4.5 Predeformed and Predamaged Initial Conditions . . . . . 312 6.4.6 Hierarchic Approaches up to Surface and Gradient Effects ................. 314 7 Failure of Brittle and Quasi-Brittle Materials .. .. .. .. .. .. . 321 7.1 Engineering Considerations .............................. 321 7.2 Fast Calculations of Structural Failures... .. .. .. .. .. .. .. .. . 324 7.2.1 Damage Equivalent Stress Criterion . .. .. .. .. .. .. .. . 324 7.2.2 Interface Debonding Criterion...................... 327

Contents XV 7.2.3 The Weibull Model ............................... 328 7.2.4 Two-Scale Damage Model forQuasi-Brittle Failures .......................... 332 7.2.5 Sensitivity Analysis............................... 333 7.2.6 SafetyMarginandCrackPropagation. . . . . . . . . . . . . . .334 7.3 Basic Engineering Examples ............................. 336 7.3.1 Plates or Members with Holes and Notches . .. .. .. .. . 336 7.3.2 Pressurized Shallow Cylinders...................... 337 7.3.3 Fracture of Beams in Bending...................... 338 7.4 Numerical Failure Analysis .............................. 339 7.4.1 Quasi-Brittle Damage Models...................... 339 7.4.2 Failure of Pre-stressed Concrete 3D Structures . . . . . . . 346 7.4.3 Seismic Response of Reinforced Concrete Structures .................. 350 7.4.4 Damage and Delamination in Laminate Structures............................ 356 7.4.5 Failure of CMC Structures......................... 361 7.4.6 Single and Multifragmentation of Brittle Materials ............................... 364 7.4.7 Hierarchic Approach up to Homogenized Behavior....................... 368 Bibliography..................................................373 Index ......................................................... 375

Notations It was impossible to avoid using the same letter for different meanings! Operators x scalar xi component of a vector x xij component of a second order tensor x xijkl component of a fourth order tensor x [M]m a t r i x ˙ x time derivative of x (˙ x =dx/dt) xi,j gradient of x also x xij,j divergence of x xkk trace of x xH 1 3traceofx xD ij component of the deviatoric tensor xD, xD ij = xij-xHδij δij Kronecker delta, δij =1ifi = j and δij =0ifi = j |x| absolute value of the scalar x |x|ij absolute value in terms of principal components of the tensor x [[ x]] discontinuity of x x Macauley bracket, x = x if x ≥ 0and x =0ifx<0 x + or x + ij positive part in terms of principal components of ten- sor x x - or x - ij negative part in terms of principal components of ten- sor x x mean value of x x standard deviation of the random variable x Δx range of x (peak to peak amplitude) or time increment xn+1 - xn d,∂,δ differential operators

XVIII Notations H Heaviside function ln neperian logarithm σij,j derivative ∂ ∂xj σij det determinant operator gradient operator 2 laplacian operator Symbols a rate elasticity tensor A damage threshold parameter A crack area Ak material parameter AD Kachanov law damage parameter A Almansi strain tensor b, by isotropic hardening exponents bS Sines criterion parameter C, Cy kinematic hardening parameters C heat capacity Ch specific heat CMC Manson--Coffin law parameter CP Paris law parameter C dilatation tensor D scalar damage variable Dij component of the second order damage tensor D DT, DS transverse and shear damage variables Dijkl component of the fourth order damage tensor Dc critical damage parameter ep ij component of the effective plastic strain tensor ep E Young modulus of elasticity Eijkl component of the elasticity tensor E E Green--Lagrange strain tensor f yield function of plastic criterion fv porosity F force F dissipative potential function FX plastic potential of dissipation FD damage potential of dissipation F gradient of deformation transformation

Notations XIX g plastic strain-stress function G shear elasticity modulus G strain energy release rate Gc material toughness parameter h, ha microdefect closure parameters H hardness material parameter H activation energy parameter HN creep temperature exponent Hij =(1 - D)-1/2 ij component of the damage effective operator H =(1 - D)-1/2 Iijkl component of the unit fourth order tensor I [Jac] Jacobian matrix k heat conductivity parameter K elastic compressibility modulus K stress intensity factor Kc cyclic hardening law coefficient KT elastic stress concentration coefficient kNeuber Neuber stress concentration correction Kp, K0 p, Ky p , K fp hardening material parameters KN, K0 N Norton law parameters K∞ viscous material parameter L strain rate tensor L fourth order tangent tensorial operator m damage threshold exponent mooni Mooney parameters M , M0, My, Mf isotropic hardening exponents Mc cyclic hardening law exponent Mijkl component of the effective operator M n viscous material parameter exponent n unit normal vector N,n number of cycles NR number of cycles to rupture N, N0 Norton law viscous exponents Nij shape functions

XX Notations p accumulated plastic strain pD damage threshold accumulated plastic strain pR rupture accumulated plastic strain P pressure P ponderation matrix q1, q2 Gurson law parameters q state variable of the reversible domain Q stress increase of the reversibility domain q thermal flux vector r isotropic hardening state variable rh heat source rD Kachanov law damage exponent R isotropic hardening stress variable R∞, Ry ∞ saturated isotropic hardening parameters Rν,Rνh triaxiality function s specific entropy s unified damage law exponent S energetic damage law parameter S surface SD damage surface Saf safety factor S.Ak sensitivity coefficient S second Piola--Kirchhoff stress tensor t time tR rupture time T temperature TX stress triaxiality, TX = σH/σeq u displacement U displacement vector {U} nodal displacement vector {U e} elementary nodal displacement vector v wave speed V volume V0 reference volume of Weibull law Veff effective volume of Weibull law

Notations XXI w energy density wD damage threshold stored energy density we elastic strain energy density ws stored energy density We elastic strain energy W1, W2 hyperelatic energy densities X uniaxial kinematic back stress Xij component of the back stress deviatoric tensor X X∞, Xy ∞ saturated kinematic hardening material parameter Y energy density release rate Yij component of the energy density release rate tensor Y Y effective elastic energy density Z necking parameter in pure tension α dilatation parameter coefficient α kinematic hardening state variable β Eshelby coefficient γ, γy kinematic hardening material parameter γMC Manson--Coffin law exponent Γ(a) gamma function: Γ(a)= ∞ 0 ta-1 exp (-t)dt γ(a, x) incomplete gamma function: γ(a, x)= x 0 ta-1 exp (-t)dt δ0 size of the mesocrack initiated δGTN Gurson law coalescence parameter Δ hypoelastic strain rate tensor , ij, uniaxial and tensorial total strains e, eij, e uniaxial and tensorial elastic strains p, p ij, p uniaxial and tensorial plastic strains pD damage threshold plastic strain in pure tension pR, pR rupture plastic strains in pure tension pu plastic strain for ultimate stress in pure tension R rupture strain in pure tension pΣ signed equivalent plastic strain π irreversible strain η hydrostatic sensitivity damage parameter ηP Paris law exponent

XXII Notations φD damage dissipated energy density φp plastic dissipated energy density φDp, φF fracture dissipated energy density λ Lam´ e elastic parameter λ elongation ˙λ plastic multiplier μ Lam´ e elastic parameter in shear ˙μ internal sliding multiplier ν Poisson ratio of elastic contraction ν unit reference vector νij anisotropic contraction ratio π cumulative internal sliding πD damage threshold θ numerical parameter of the θ-method ρ mass density ρ radius of curvature σ, σij, σ uniaxial and tensorial Cauchy stresses ˜ σ,˜ σij, ˜ σ uniaxial and tensorial effective stresses σμ, σμ ij, σμ stresses at microscale σH hydrostatic stress, σH = 1 3 σkk σeq von Mises equivalent stress σΣ signed von Mises stress σ damage equivalent stress, σ = σeqR1/2 ν σn nominal stress σv viscous stress σR rupture stress σu ultimate stress σy yield stress σy02 engineering yield stress for p =0.2 · 10-2 σf engineering fatigue limit at 106 or 107 cycles σ∞ f asymptotic fatigue limit σs reversibility threshold Σij component of normalized stress tensor Σ ψ Helmholtz specific free energy

Notations XXIII ψe elastic state potential ψp plastic state potential ψT thermal state potential ψ Gibbs specific free enthalpy ψ e elastic specific free enthalpy

1 Background on Continuum Damage Mechanics This chapter gives the reader the necessary and sufficient information to deal with practical applications of Continuum Damage Mechanics (the term was first introduced by J. Hult in 1972) to predict the crack initiation in struc- tures subjected to heavy loadings. This ranges from the early definition of a scalar damage variable by L.M. Kachanov in 1958 to the anisotropic tenso- rial damage variable, from classical thermodynamics aspects to the effective stress that take into account the closure of microdefects in compression- like loadings, from simple measurement of local damage to fields of dam- age, from a simple damage law to induced anisotropy and a generalization to quasi-brittle materials, from elasto-(visco-)plasticity coupled with dam- age to the phenomenon of localization, the ultimate stage before crack initiation. The basic concepts are written in a concise and sufficiently general way in order to be applied to any material: metals and alloys, polymers, elastomers, composites, concretes, ceramics . . . For more basic details please refer to the book A Course on Damage Mechanics written by Jean Lemaitre and published by Springer-Verlag in 1992 and 1996. Other (good!) references are given at the end of the book. 1.1 Physics and Damage Variables Damage, in its mechanical sense in solid materials is the creation and growth of microvoids or microcracks which are discontinuities in a medium consid- ered as continuous at a larger scale. In engineering, the mechanics of con- tinuous media introduces a Representative Volume Element (RVE) on which all properties are represented by homogenized variables. To give an order of magnitude, its size can vary from about (0.1 mm)3 for metals and ceramics to about (100 mm)3 for concrete. The damage discontinuities are "small" with respect to the size of the RVE but of course large compared to the atomic spacing (Fig. 1.1).

2 1 Background on Continuum Damage Mechanics From a physical point of view, damage is always related to plastic or irreversible strains and more generally to a strain dissipation either on the mesoscale, the scale of the RVE, or on the microscale, the scale of the dis- continuities: Fig. 1.1. Examples of damage in a metal (left, micro-cavities in copper from L. En- gel and H. Klingele), in a composite (middle, microcracks in carbon-fiber/epoxy resin laminate from O. Allix), and in a concrete (right, crack pattern in a ASTM I cement, 4.8 and 9.5 mm aggregates, petrography from S.P. Shah) • In the first case (mesolevel), the damage is called ductile damage if it is nucleation and growth of cavities in a mesofield of plastic strains under static loadings; it is called creep damage when it occurs at elevated tem- perature and is represented by intergranular decohesions in metals; it is called low cycle fatigue damage when it occurs under repeated high level loadings, inducing mesoplasticity. • In the second case (microlevel), it is called brittle failure, or quasi-brittle damage, when the loading is monotonic; it is called high cycle fatigue damage when the loading is a large number of repeated cycles. Ceramics, concrete, and metals under repeated loads at low level below the yield stress are subjected to quasi-brittle damage. In all cases, these are volume defects such as microcavities, or surface defects such as microcracks. This is the reason to have several definitions of a damage variable: • If only ductile damage is considered, it may be defined as the volume density of microvoids, Dv = δVvoids δVRVE =fv . (1.1) This is the starting point of the Gurson model described in Sect. 3.4.5.

1.1 Physics and Damage Variables 3 • For a larger generality where microcavities and microcracks may exist, the damage variable is physically defined by the surface density of microcracks and intersections of microvoids lying on a plane cutting the RVE of cross section δS (Fig. 1.2). For the plane with normal n where this density is maximum, we have D( n)=δSD δS. (1.2) Fig. 1.2. Physical damage and mathematical continuous damage 1.1.1 Definition of a Scalar Damage Variable If the damage is isotropic, the scalar variable D( n) does not depend on the normal. The intrinsic variable is a scalar (L.M. Kachanov 1958): D=δSD δS (1.3) It can be used as such for one-dimensional problems. It can also be used as an easy evaluation of the approximate damage in three-dimensional problems (particularly in proportional loading). 1.1.2 Definition of Several Scalar Damage Variables If several mechanisms of damage occur, simultaneously or not, each of them may be represented by a scalar variable (Dk) with the same physical meaning as above. This is the case in classical composites where delamination of fibers and matrix cracking may occur. Two or three independent variables are used (P. Ladev` eze 1983), for instance: • DF for quasi-brittle fibers breakage, • DT for transverse matrix cracking, and • DS acting on shear for splitting.

4 1 Background on Continuum Damage Mechanics 1.1.3 Definition of a Tensorial Damage Variable Damage is often non-isotropic due to microcracking more or less perpen- dicular to the largest positive principal stress. Then, the surface density of microdefects in a plane with normal n acts through an operator which trans- forms the surface δS and n of Fig. 1.2 into a smaller but continuous area, δ˜ S = δS - δSD, and into another normal ˜ n (S. Murakami 1981). To keep the same physical meaning as above the damage acts through the operator (1 - D)and (δij - Dij)njδS =˜ niδ ˜ S, (1.4) where δij is the Kronecker delta and D is a second order tensor. As there is no distorsion of the surface δS, it induces the property of orthotropy consistent with the fact that the damage is governed by the plastic strain represented by the second order tensor p. Remark -- In fact, the largest generality for a damage variable is a representation by a fourth order tensor, as it can be shown in several ways (J.L. Chaboche 1978, D. Krajcinovic 1981, F.A. Leckie and E.T. Onat 1981, C.L. Chow 1987). Such a tensor is difficult to use and is not necessary for damage-induced by meso- or microplasticity. • As in the previous section, consider a damage plane area, δS,withn o r m al n and a reference vector ν such that the tensor νi nj δS defines the geometri- cal reference configuration. Continuum Damage Mechanics defines the effective continuous configuration by a modified area δ ˜ S and a modified normal ˜ n,a s shown in Fig. 1.3. The damage D is the operator which transforms the second order tensor νi nj δS of the reference configuration into the tensor of the effective configuration νi˜ njδ˜ S. This is a fourth order tensor, where (Iijkl - Dijkl)νknlδS = νi ˜ njδ˜ S, (1.5) with the following symmetries: Dijkl = Dijlk = Djikl = Dklij . Fig. 1.3. Reference and effective configurations

1.1 Physics and Damage Variables 5 • Another way to define a fourth order tensor D is to consider the operator which changes the initial elasticity tensor Eijkl into the actual elasticity tensor ˜ Eijkl softened by damage: (Iijrs - Dijrs) Erskl = ˜ Eijkl . (1.6) From a purely theoretical point of view, this definition does not yield a real state variable because it requires the knowledge of a particular behavior (elasticity here). 1.1.4 Effective Stress Concept The constitutive equations for strain and damage characterize the plain ma- terial itself without the volume or the surface discontinuities. An interest- ing concept to introduce next is the stress acting on the resisting area, δ˜ S = δS - δSD, as shown in Fig. 1.2 -- the effective stress. • In the uniaxial case of isotropic damage without the closure effect of microcracks in compression, this mean value of the microstresses is simply given by the force equilibrium (Y.N. Rabotnov 1968): ˜ σδ˜ S=σδS with D=δSD δS =δS-δ˜ S δS (1.7) or ˜ σ=σ 1-D. (1.8) • In the multiaxial case of isotropic damage, all the stress components act on the same effective area. The effective stress tensor is simply ˜ σij = σij 1-D. (1.9) • The case of anisotropic damage is much more complicated to en- sure a good representation of the physics as well as compatibility with thermodynamics. In fact, the effective stress with a second order damage tensor representation is an approximation of the exact effective stress de- duced from the general representation of the damage by the fourth order tensor D, as defined in the remark in the previous section. This effective stress is defined as previously, but, here, by the projection of the stress vector on the reference vector ν in Fig. 1.3: νi˜ σij ˜ njδ˜ S = νiσijnjδS (1.10) or ˜ σij(Iijkl - Dijkl)νk nlδS = σklνk nlδS (1.11) using the preceeding equation (1.5).

6 1 Background on Continuum Damage Mechanics With the symmetry properties of the damage tensor Dijkl given in Sect. 1.1.3, the effective stress is the symmetric tensor, ˜ σij = σkl(I-D)-1 klij , (1.12) which may also be written as ˜ σij = Mijkl σkl , with Mijkl =(I - D)-1 klij . (1.13) Back to a second order damage tensor, there are several possibilities to write a restriction of the fourth order formulation but only one fulfills the following conditions: -- Symmetry of the effective stress (note that ˜ σij = σik(1 - D)-1 kj is not symmetric!). -- An effective stress independent of the strain behavior and, in par- ticular, independent from the Poisson ratio (˜ σij = Eijkl ˜ E-1 klrsσrs may depend on the Poisson ratio). -- Compatibility with the thermodynamics framework: existence of strain potentials and principle of strain equivalence. The symmetrization ˜ σij=1 2 σik(1 - D)-1 kj +(1 - D)-1 ik σkj is not derived from a po- tential (J.P. Cordebois and F. Sidoroff 1979). -- Different effect of the damage on the hydrostatic behavior represented by the stress (σH) and on the deviatoric part (σD ij)bymeansofahy- drostatic sensitivity parameter (η) that is easy to identify. This restriction is represented by ˜ σij =(Hik σD klHlj)D + σH 1-ηDHδij, withHij =(1-D)-1/2 ij , (1.14) whereDH= 1 3 Dkk is the hydrostatic damage and H is the effective damage tensor. The corresponding fourth order tensor Mijkl is Mijkl = HikHlj - 13 H2 klδij + H2 ijδkl + 19H2 ppδijδkl + 1 3(1 - ηDH)δijδkl . (1.15) For the uniaxial case, the effective von Mises stress (˜ σeq)differsfromthe effective tensile stress (˜ σ1) (assumed here in direction 1) as follows: ˜ σeq=23 σ 1-D1+13 σ 1-D2 ˜ σ1=49 σ 1-D1+29 σ 1-D2+13 σ 1-ηDH , (1.16) where D3 = D2. The coefficient η does not depend very much on the materials as most often η ≈ 3. The isotropic damage case corresponds to Dij=Dδijandη=1. The effective stress taking into account the quasi-unilateral conditions of microdefects closure is formulated in Sect. 1.2.4.

1.2 Thermodynamics of Damage 7 1.1.5 Effects of Damage Damage by the creation of free surfaces of discontinuities reduces the value of many properties: • It decreases the elasticity modulus • It decreases the yield stress before or after hardening • It decreases the hardness • It increases the creep strain rate • It decreases the ultrasonic waves velocity • It decreases the density • It increases the electrical resistance Some of these effects are used to evaluate the damage by inverse methods (see Sect. 1.3). Furthermore, the effects on mechanical strength and stiffness are different in tension and in compression due to microcracks opening under tension and their closure under compression. 1.2 Thermodynamics of Damage The thermodynamics of irreversible processes allows for the modelling of different materials' behavior in three steps: 1. Definition of state variables, the actual value of each defining the present state of the corresponding mechanism involved 2. Definition of a state potential from which derive the state laws such as thermo-elasticity and the definition of the variables associated with the internal state variables 3. Definition of a dissipation potential from which derive the laws of evolu- tion of the state variables associated with the dissipative mechanisms These three steps offer several choices for the definitions, each chosen in accordance with experimental results and purpose of use. Then, the second principle of the thermodynamics must be checked for any evolution. The two potential functions introduce parameters which depend on the material and the temperature. They must be identified from experiments in each case. 1.2.1 General Framework The state variables, observable and internal, are chosen in accordance with the physical mechanisms of deformation and degradation of the material (Table 1.1). Taking small deformations into consideration, the total strain is split into a thermo-elastic part e and a plastic part p: ij= eij+ p ij. (1.17)

8 1 Background on Continuum Damage Mechanics Ta b l e 1 . 1 . State and associated variables (J. Lemaitre 1978) Mechanisms Type State variables Associated Observable Internal variables Thermoelasticity Tensor ij σij Entropy Scalar Ts Plasticity Tensor p ij -σij Isotropic hardening Scalar rR Kinematic hardening Tensor αij Xij Damage Scalar (isotropic) D -Y Tensor (anisotropic) Dij -Yij The Helmholtz specific free energy taken as the state potential of the material is a function of all the state variables. Written as ψ( eij ,D or Dij ,r, αij ,T), some qualitative experimental results on the possibility of couplings show that the state potential is the sum of thermo-elastic (ψe), plastic (ψp), and purely thermal (ψT) contributions. Here, it is more convenient to con- sider the potential as the Gibbs specific free enthalpy (ψ ) deduced from the Helmholtz free energy by a partial Legendre transform on the strain: ψ =sup 1 ρ σij ij - ψ (1.18) or ψ =sup e 1 ρσij eij -ψe + 1 ρσij p ij -ψp -ψT, (1.19) where ρ is the density and where ψp and ψT do not depend on the total strain. It is finally expressed as ψ =ψ e+1 ρσij p ij-ψp-ψT, (1.20) where • The elastic contribution ψ e is affected by damage to model the experimen- tally-observed coupling between elasticity and damage through the effec- tive stress concept ˜ σ associated with the principle of strain equiva- lence (J. Lemaitre 1971). It states that the strain constitutive equations of a damaged material is derived from the same formalism as for a non- damaged material except that the stress is replaced by the effective stress. • Thepartψp=1 ρ r 0Rdr+1 3 Cαij αij is the contribution due to plas- tic hardening. When multiplied by ρ,itistheenergy stored (ws)in the RVE. The material parameter C accounts for the linear part of the kinematic hardening. • The extra contribution ψT is a function of the temperature only. It par- tially defines the heat capacity of the material.

1.2 Thermodynamics of Damage 9 First, the state laws are derived from the state potential. They are the laws of thermoelasticity, ij =ρ∂ψ ∂σij =ρ∂ψ e ∂σij + p ij -→ eij =ρ∂ψ ∂σij s=∂ψ ∂T. (1.21) The other derivatives define the associated variables as follows: R = -ρ∂ψ ∂r, Xij = -ρ∂ψ ∂αij , -Y = -ρ∂ψ ∂D or -Yij= -ρ∂ψ ∂Dij . (1.22) The second principle of thermodynamics, written as the Clausius-- Duhem inequality is satisfied when the damage rate is positive: σij ˙ p ij- ˙ ws+Yij ˙ Dij - qiT,i T≥0 (1.23) This means the dissipation sum of the dissipation due to plastic power (σij ˙ p ij), minus the stored energy density rate (˙ ws =R˙ r+Xij˙ αij), plus the dissipation due to damage (Yij ˙ Dij), and plus the thermal energy ( q is the thermal flux), is transformed into heat. Finally, the kinetic laws governing the evolution of the internal variables are derived from a dissipation potential (F ) which is a convex function of the associated variables to ensure fulfillment of the second principle: F = F(σ,R,Xij,Y or Yij;D or Dij,T). (1.24) The state variables representing the temperature and the damage may act, but only as parameters. Introducing the plastic criterion function (f), the nonlinear kinematic hardening term (FX) and the damage potential (FD), according to qualitative experiments on the possibilities of coupling, F is the sum F = f + FX + FD . The evolution laws are formally written as ˙ p ij=- ˙λ ∂F ∂(-σij) = ˙λ ∂F ∂σij , ˙ r=- ˙λ ∂F ∂R, ˙ αij=- ˙λ ∂F ∂Xij , ˙ D=- ˙λ ∂F ∂(-Y) = ˙λ∂F ∂Yor˙ Dij=- ˙λ ∂F ∂(-Yij) = ˙λ ∂F ∂Yij . (1.25) This is the normality rule of generalized standard materials.

10 1 Background on Continuum Damage Mechanics For phenomena which do not depend explicitly on time, such as plasticity, the potential F is not differentiable and ˙λ is the plastic multiplier, calculated from the consistency condition, f =0, ˙f = 0. The first condition, f =0, means that the state of stress is on the actual yield condition; the second, ˙f = 0, means that an increase of the state of stress induces an increase of the yield stress. Elastic unloading occurs when f<0or ˙f<0, the internal variables then keeping a constant value ( ˙ p ij =˙ r=˙ αij= ˙ Dij = 0). The com- plete loading or unloading conditions are called the Kuhn--Tucker conditions: ˙λ≥0,f≤0, ˙λf=0. For phenomena like visco-plasticity which depends explicitly upon time, ˙λ is the viscosity function ˙λ(f). To complete the formal description of elasto-(visco-)plasticity coupled with damage, the accumulated plastic strain rate (˙ p)isdefin edina c - cordance with the yield criterion considered. For the von Mises criterion it is ˙p = 23 ˙ p ij˙ p ij. (1.26) In 1D (uniaxial tension-compression case), it simply means ˙p = | ˙ p|. 1.2.2 State Potential for Isotropic Damage According to the principle of strain equivalence, the strain potential for linear isotropic thermo-elasticity and isotropic damage (D)is ρψ e =1+ν 2E σij σij 1-D- ν 2E σ2 kk 1-D+α(T-Tref)σkk, (1.27) where E is the Young's modulus, ν the Poisson ratio, α the thermal expansion coefficient, and Tref a reference temperature. The thermo-elasticity law is derived from this potential as eij =ρ∂ψ e ∂σij = 1+ν E˜ σij-ν E˜ σkkδij + α(T - Tref)δij , (1.28) where the effective stress is ˜ σij = σij 1-D. The energy density release rate (Y ), the associated variable with the damage variable, is also derived from the state potential and may be written as (J.L. Chaboche 1976) Y=ρ∂ψ ∂D= ˜ σ2 eqRν 2E, (1.29)

1.2 Thermodynamics of Damage 11 introducing the triaxiality function Rν = 23(1 + ν)+3(1- 2ν) σH σeq 2 (1.30) where σH = σkk/3isthehydrostatic stress, σeq = 3 2σD ij σD ij the von Mises equivalent stress,a ndσD ij = σij - σHδij the stress deviator. The ratio σH/σeq is the stress triaxiality denoted by TX. If we is the elastic strain energy density defined by dwe = σij d eij ,then Y= we 1-D andY=1 2 dwe dD σ = const T = const . (1.31) At this level, an interesting concept is the damage equivalent stress (σ ) (J. Lemaitre 1981) defined as the uniaxial stress which gives the same amount of elastic strain energy (we) as a multiaxial state of stress. For linear isothermal isotropic elasticity, we = ρψ e or in terms of the stress deviator (σD) for shear energy and the hydrostatic stress (σH) for the hydrostatic energy, ρψ e =1+ν 2E σD ij σD ij 1-D+3(1-2ν) 2E σ2 H 1-D= σ2 eqRν 2E(1 - D) . (1.32) Writing the equality between the uniaxial case, for which Rν =1,a ndthe multiaxial case, σ 2 2E(1-D)= σ2 eqRν 2E(1-D), (1.33) yields σ = σeqR1/2 ν. (1.34) 1.2.3 State Potential for Anisotropic Damage In accordance with the principle of strain equivalence, with the definition of the effective stress (1.14) of Sect. 1.1.4 and with P. Ladev` eze's (1983) framework for the description of an anisotropic state of damage, the state potential ρψ e represented by the tensor D is ρψ e =1+ν 2E Hij σD jkHklσD li+3(1-2ν) 2E σ2 H 1 - ηDH + α(T - Tref)σkk , (1.35) where Hij =(1 - D)-1/2 ij (1.36)

12 1 Background on Continuum Damage Mechanics The law of elasticity is derived from the Gibbs potential and as expressed in (1.28) still introduces the symmetric effective stress tensor defined in Sect. 1.1.4: ˜ σij =(Hik σD klHlj)D + σH 1-ηDHδij. (1.37) The associated variable with D is the energy density release rate tensor, Y , which is also derived from the Gibbs energy, Yij = ρ∂ψ /∂Dij .This derivative needs some care due to possible variation of the damage principal directions. Using Hik ˙ Hkj+˙ HikHkj = H2 ik˙ DklH2 lj and Aijkl ˙ Hkl=H2 ip˙ DpqH2 qj, with Aijkl=1 2 (Hikδjl+Hjlδik +Hilδjk+Hjkδil) , (1.38) where the symmetrization is due to Hkl = Hlk ,onegets: Yij = 1+ν EσD kp Hpq σD ql A-1 klmn H2 mi H2 jn+η(1-2ν) 2E σ2 H (1 - ηDH)2 δij . (1.39) It is possible to verify that the dissipation Yij ˙ Dij is positive or zero at least for practical cases. By chance, the law of damage evolution in Sect. 1.4 will not be a function of Y but it will be a function of the effective elastic energy density,the scalarY = ˜ σij d eij , as in the isotropic case. Y can be written as a function of the effective stress, Y=1 2 Eijkl ekl eij = 1 2˜ σij eij = ˜ σ2 eq˜ Rν 2E, (1.40) with the effective triaxiality function ˜ Rν = 23(1 + ν)+3(1- 2ν) ˜ σH ˜ σeq 2 , (1.41) where ˜ σeq = HσDH eq = 32 HσDH D ij HσDH D ij 1/2 ˜ σH= σH 1-ηDH . (1.42) 1.2.4 Quasi-Unilateral Conditions of Microdefects Closure For most materials under certain conditions of loading, the microdefects may close during compression. This is more often the case for very brittle mate- rials. The phenomenon of partial closure of microcracks increases the area

1.2 Thermodynamics of Damage 13 which effectively carries the load in compression and the stiffness may then be partially or fully recovered. For most materials, considering ˜ E+and˜ E- as the effective elasticity modulus in tension and in compression, the ratio (E- ˜ E-)/(E - ˜ E+) has a constant value close to 0.2 when the damage models of Sects. 1.2.2 and 1.2.3 give a value equal to 1. This phenomenon is referred to as quasi-unilateral conditions, the term "quasi" standing for "initial elasticity partially recovered in compression." From a theoretical point of view, the damage state due to the presence of microdefects is represented by the internal variable D or D.Beingathermo- dynamical state, it is independent of both the intensity and the sign of the loading at constant internal variables (metals, concretes, composites, poly- mers . . . do not physically recover from their wounds!). This means that • No extra damage variable has to be introduced to model the mi- crodefects closure effect • D or D act differently in tension and in compression For unidimensional states of stress, a solution is to define an effective stress such as • σ 1 - D in tension with D the relative reduction of the resisting area in tension identified by D =1- ˜ E+/E and • σ 1 - hD in compression with hD, the relative reduction of the resisting area in compression identified by hD =1- ˜ E-/Eorh=(E- ˜ E-)/ (E- ˜ E+), where h is a microdefects closure parameter that is material-dependent (but most often h ≈ 0.2). For 3D states of stress, the difficulty is to recognize what is compres- sion and what is tension! The theoretical background needed to handle such a problem mostly concerns the definition and use of positive and negative parts of tensors built with their three principal values. The positive part s + , also written as s + ij (with negative part s - or s - ij respectively), of a symmetric tensor s is built from its positive (negative) eigenvalues sK and the corresponding normalized eigenvectors qK ,asin s + ij= 3 K=1 sK qK iqK j and s - ij = sij - s + ij , (1.43) where · stands for the positive part of a scalar: x = x if x ≥ 0, 0i fx<0. Using the property s + ij s - ij = 0, it is easy to demonstrate that skk 2 = skk 2 + -skk 2 sij sij = s + ij s + ij + s - ij s - ij. (1.44)

14 1 Background on Continuum Damage Mechanics The products skk 2, s + ij s + ij ,and s - ij s - ij may be continuously differen- tiated as follows: ∂ ∂sij 1 2 skk 2 = skk δij , ∂ ∂sij 1 2 s + rs s + rs = s + ij, ∂ ∂sij 1 2 s - rs s - rs = s - ij. (1.45) 1.2.4.1 Quasi-Unilateral Conditions for Isotropic Damage (P. Ladev` eze and J. Lemaitre 1984) The microdefects closure parameter h operates by (1-hD)-1 on the negative part of the principal stresses and by (1 - D)-1 on the positive principal stresses. For isotropic damage, the isothermal state potential ρψ eis ρψ e =1+ν 2E σ + ij σ + ij 1-D + σ - ij σ - ij 1-hD - ν 2E σkk 2 1-D + -σkk 2 1 - hD . (1.46) The elasticity law is still derived from eij = ρ∂ψ e /∂σij , eij = 1+ν E σ + ij 1-D+ σ - ij 1-hD - ν E σkk 1-D- -σkk 1 - hD δij . (1.47) It defines an effective stress as ˜ σij = σ + ij 1-D+ σ - ij 1-hD +ν 1 - 2ν δkl σ + kl - σkk 1-D +δkl σ - kl + -σkk 1-hD δij. (1.48) The energy density release rate Y = ρ∂ψ /∂D now strongly depends on h as Y=1+ν 2E σ + ij σ + ij (1-D)2 +h σ - ij σ - ij (1 - hD)2 - ν 2E σkk 2 (1-D)2+h -σkk 2 (1 - hD)2 . (1.49) 1.2.4.2 Quasi-Unilateral Conditions for Anisotropic Damage (P. Ladev` eze 1983, R. Desmorat 1999) As for the isotropic case, the scalar parameter ha , different from h in general, is introduced in order to model the different effects of D on tension and compression. We define

1.2 Thermodynamics of Damage 15 Hp ij =(1 - D)-1/2 ij ,H n ij =(1 - haD)-1/2 ij , (1.50) where p stands for positive and n for negative, as it will be exhibited by their use.The isothermal state potential that can model quasi-unilateral anisotropic damage is ρψ e =1+ν 2E Hp ij σD +jkHp klσD +li+Hn ij σD +jkHn klσD +li +3(1-2ν) 2E σH 2 1-ηDH+ -σH 2 1 - haηDH , (1.51) where σD + is built with the eigenvalues λK and the corresponding eigen- vectors ( T K) of the non-symmetric matrix (H pσD)ins u c haw a ytha t (HpσD +HpσD +) may be continuously differentiated. This means d 1 2Hp ij σD +jkHp klσD +li = Hp ij σD +jkHp kldσD li+σD +liHp ij σD +jkdHp kl , (1.52) where T K and λK are given by the eigenvalue problem σD ijTj = λ(Hp)-1 ij Tj (without summation) (1.53) and the normalization T I i (H p)-1 ij TJ j = δIJ is made. Be careful: the scalar product TI· T J = δIJ as (H pσD) is non-symmetric. The eigenvalues λK are real because σD is symmetric and (H p)-1 is positive-defined and symmetric. The deviatoric stress tensor may then be rewritten as σD ij= 3 K=1 λK (Hp)-1 ik TK k (Hp)-1 jl TK l (1.54) and the special positive part σD + is therefore defined as σD +ij = 3 K=1 λK (Hp)-1 ik TK k (Hp)-1 jl TK l . (1.55) The same procedure is followed for the negative part σD - with Hn and with the eigenvectors and the negative eigenvalues of (H nσD). The elasticity law is derived from the state potential, eij =ρ∂ψ e ∂σij = 1+ν E (Hp ik σD +klHp lj)D +(Hn ikσD -klHn lj)D +1-2ν E σH 1-ηDH - -σH 1 - ηhaDH δij eij = 1+ν E˜ σij-ν E˜ σkkδij , (1.56)

16 1 Background on Continuum Damage Mechanics and defines the effective stress, ˜ σij =(H p ik σD +klHp lj)D +(Hn ikσD -klHn lj)D + σH 1-ηDH - -σH 1 - ηhaDH δij , (1.57) which takes into account the quasi-unilateral effect. The effective energy den- sity is also a function of the microdefects closure parameter. It is expressed as Y=1+ν 2E tr HpσD +Hp 2 + ha HnσD -Hn 2 +3(1-2ν) 2E σH 2 (1 - ηDH)2 + ha -σH 2 (1 - ηhaDH)2 . (1.58) In order to keep the possibility to differentiate the state potential, the pos- itive and negative parts are taken with respect to the deviatoric stress tensor. This means that the parameter ha affects both tension and compression (σD has positive and negative components in any uniaxial case), therefore the model is quite complex even for the tensile test. Furthermore, the value of the microdefects closure parameter depends on the model itself: for a given material, h for the isotropic damage model is different from ha identified for the anisotropic damage model. The good thing is that the common value for many materials, h ≈ 0.2, for the isotropic damage model corresponds to ha ≈ 0 for the anisotropic damage model. Finally, the law of elasticity may be written as (ha =0) eij = 1+ν E (Hp ikσD +klHp lj)D + σD - D ij +1-2ν E σH 1 - ηDH - -σH δij (1.59) and the effective energy density is Y=1+ν 2E tr HpσD +Hp 2 + 3(1 - 2ν) 2E σH 2 (1-ηDH)2 . (1.60) 1.3 Measurement of Damage The direct measurement of damage as the surface density of microdefects is difficult to perform and is used only in laboratories well equipped for microg- raphy from both the human and microscopy points of view. It is easier to take advantage of the coupling between damage and elasticity (or plasticity) to evaluate the damage by inverse methods.

1.3 Measurement of Damage 17 1.3.1 Isotropic Elasticity Change In the case of isotropic damage, the uniaxial law of elasticity in tension cou- pled with damage reduces to e= σ E(1-D)= σ ˜ E, (1.61) where E is the Young's modulus of undamaged elasticity and ˜ E is the actual modulus of damaged elasticity. The damage is then expressed as the loss of stiffness, D =1- ˜ E E. (1.62) To evaluate the damage as a function of the accumulated plastic strain, p = t 0|˙ p|dt, it is advised to perform a very low cycle test at a constant strain range on a tension-compression specimen (rupture for 10 to 100 cycles) and to measure the elastic strain by means of small-strain gauges during unloadings (Fig. 1.4, J. Dufailly 1976). If Δ p is the plastic strain range over a cycle, the accumulated plastic strain for N cycles is simply p ≈ 2Δ pN . Fig. 1.4. Measurement of damage by means of elasticity change The evaluation of the elasticity modulus needs much care because an absolute accuracy of about 10-6 is needed on the measurement of the strain. Furthermore the damage is almost always very localized on a small volume and it looses its continuous signification as soon as a mesocrack appears. In tension, this is before the whole fracture, when the elasticity modulus decreases rapidly, an instant which corresponds to a quick change of the curvature in the graph of D =1- ˜ E/E as a function of the accumulated plastic strain p (Fig. 1.4). 1.3.2 Isotropic Elasticity Change by Ultrasonic Waves A wave's speed is related to the density ρ and to the elastic properties of the considered medium. Considering the longitudinal waves in a linear, isotropic,

18 1 Background on Continuum Damage Mechanics elastic, long cylindrical specimen with Young's modulus E and a Poisson ratio ν , the wave speed is determined by υ = E ρ 1-ν (1+ν)(1-2ν). (1.63) If the material is damaged mainly by microcracks, the density remains almost unchanged and if they are randomly oriented to make the damage isotropic, the Poisson ratio also remains constant. The wave speed becomes ˜ υ = ˜ E ρ 1-ν (1+ν)(1-2ν), (1.64) from which the damage may be determined as D =1- ˜ E E-→ D =1- ˜ υ2 υ2. (1.65) This method requires the measurement of the propagation time of the waves. The accuracy is higher when the distance covered by the waves is large. Unfortunately, due to the localization of the damage, the distance available for an uniform field of damage is always small, often too small for metals, but the method works nicely for concrete with a frequency of 0.1 to 1 MHz (Y. Berthaud 1988). 1.3.3 Anisotropic Elasticity Change When anisotropic damage is considered, the damage tensor has six com- ponents or three if the principal orthotropic frame is known, through, for example, an independent measurement of the plastic strains. Considering the case D = D1 00 0D2 0 00 D3 , H = H1= 1 √1-D1 00 0H2= 1 √1-D2 0 00 H3= 1 √1-D3 , (1.66) with elastic strains corresponding to an uniaxial tension σ1 in the direction 1 of a previously damaged material, the elasticity law (1.28) with the effective stress (1.37) of Sect. 1.2.3 can be expanded as e 100 0 e 20 00 e3 = 1+ν E H1 00 0H20 00H3 2σ1 300 0 -σ1 30 00 -σ1 3 H1 00 0H20 00H3 D +1-2ν 3E σ1 1 - ηDH 100 010 001 . (1.67)

1.3 Measurement of Damage 19 The damaged elasticity modulus in the direction 1 and the associated con- traction ratios also measured by strain gauges are defined by ˜ E1=σ1 e1 , ˜ ν12 = - e2 e1 ,and˜ ν13 = - e3 e1 . (1.68) This leads to three expressions for the elastic properties as functions of the damage: E ˜ E1 = 1+ν 9 4 1-D1+ 1 1-D2+ 1 1-D3 + 1-2ν 3(1 - ηDH) , (1.69) ˜ ν12 E ˜ E1 = 1+ν 9 2 1-D1+ 2 1-D2- 1 1-D3 - 1-2ν 3(1 - ηDH) , (1.70) ˜ ν13 E ˜ E1 = 1+ν 9 2 1-D1- 1 1-D2+ 2 1-D3 - 1-2ν 3(1 - ηDH) . (1.71) For a tensile loading in direction 2 (or 3), the equations remain the same with subscripts 1 and 2 (or 1 and 3) inverted. Then uniaxial tensions applied in the directions 2 and 3 give 6 additional equations to determine the 3 components of the damage (D1, D2, D3), plus the coefficient η if it is unknown, with a verification of the symmetries: ˜ νij ˜ Ei = ˜ νji ˜ Ej (no summation) . (1.72) If a uniformly damaged cube is available to machine 3 tensile specimens in the 3 principal directions, 3 elasticity tests (with measurement of the elastic- ity modulus and contraction ratios) allow for the calculation of the damage components, D1 =1- ˜ E1 E (1 + ν) 2+˜ ν12 - ˜ E1 ˜ E2 -1 , D2 =1- ˜ E2 E(1+ν) 2-(1- ˜ ν12) ˜ E2 ˜ E1 -1 , D3 =1- ˜ E3 E (1 + ν) 2+˜ ν32 - ˜ E3 ˜ E2 -1 , and ηDH =1- ˜ E1 E 1-2ν 1-2˜ ν12 , (1.73) withDH =13(D1+D2+D3). Due to the required size of the specimens, this procedure is not possible most of the time. Nevertheless, a cube smaller than the classical tension spec- imens may be analyzed by ultrasonic waves in the three principal directions. In this case, the transversal wave speed must be also measured.

20 1 Background on Continuum Damage Mechanics 1.3.3.1 Damage Induced by Uniaxial Tension From the previous general expressions, approximate formulae may be derived for damage induced by uniaxial tension (in direction 1). Using experiments of ductile damage with repeated unloadings for which only the elasticity modulus ( ˜ E1) and the contraction coefficient (˜ ν12)aremeasured, D1≈1- ˜ E1 E (1.74) D2=D3≈1- ˜ E1 E 1+ν 1+3˜ ν12-2ν . (1.75) For the extremal values 1 2≤˜ ν ν≤1a nd3 4≤˜ E E ≤ 1, this corresponds to a maximal relative error of 15% when compared with the exact formulae. The last expression of (1.73) for ηDH remains valid as only ˜ E1and˜ ν12 are needed. 1.3.3.2 Damage in Thin Sheets Practical applications often concern thin sheets in which it is possible to machine small tension specimens in two perpendicular directions and in the direction at 45 degrees, as shown in Fig. 1.5. Careful measurements made on the small specimens give ˜ E1, ˜ E2, ˜ Eπ 4 and ˜ ν12,˜ ν21 ,˜ νπ 4 ,fr o mwhichD1 and D2 are determined. The parameter η is obtained as the slope of 1 - ˜ E1 E 1-2ν 1-2˜ ν12 as a function of the hydrostatic Fig. 1.5. Uniaxial tension and plane tension in three specimens machined in anisotropic damaged sheets

1.3 Measurement of Damage 21 damage DH = 1 3 (D1 + D2 + D3). A hypothesis concerning the damage created in direction 3 has to be made for the calculation of DH.ItisD2 = D3 for damage induced by uniaxial tension loading; D2 =0andD3 = D1 for damage induced by plane tension loading (large plates). Such choices have an influence on the measurement of η only. They are consistent with the consideration of the damage evolution law of Sect. 1.4. The data at 45 degrees may be used as complementary data for the iden- tification of the damage or to check the quality of the measurements, ˜ Eπ 4 =4 1 ˜ E1+1 ˜ E2+ 1 ˜ G12 -2˜ ν12 ˜ E1 -1 (1.76) ˜ νπ 4= ˜ Eπ 4 4 2˜ ν12 ˜ E1+1 ˜ G12 -1 ˜ E1 -1 ˜ E2 , (1.77) with the damaged shear modulus being ˜ G12 =G (1-D1)(1-D2), and G= E 2(1 + ν) . (1.78) Two examples are given for anisotropic ductile damage created in uniaxial tension and plane tension in the direction 1 of thin sheets of ARCELOR steel SOLDUR 355. The results are given in Fig. 1.6 for two values of the plastic strain applied on the big samples in order to produce the damage. In both cases, the ratio D2/D1 is close to the ratio | p 2|/| p 1| as D2/D1 ≈ 1/2inthe case of uniaxial tension and D2/D1 ≈ 0 in the case of plane tension. The valu e of η is in the range of many other experiments for which it has been found: 2.1 ≤ η ≤ 3.5. Fig. 1.6. Damage anisotropy in uniaxial tension and plane tension in polar coor- dinates (M. Sauzay 2000)

22 1 Background on Continuum Damage Mechanics 1.3.4 Hardness Change Hardness or, better for damage evaluation, microhardness is influenced by the softening effect of damage. The process of inserting a diamond indenter in the material where the load (F ) and the projected indented area (S)are measured defines the hardness as H=FS. (1.79) The material around the mark is loaded in 3D, proportional plasticity which avoids the consideration of a kinematic hardening (see Sect. 2.1.2). In the case of isotropic damage with the same effect on tension and compression, the plastic potential is written with the effective von Mises equivalent stress, the isotropic hardening stress R, and the yield stress σy, f= σeq 1-D-R-σy =0, (1.80) which means that the actual plastic yield stress corresponding to a plastic strain in the material is σs =(R+σy)(1-D). (1.81) Theoretical analyses and many experiments have proved that this actual yield stress is related to the hardness H linearly, H=kσs. (1.82) • If a microhardness test is performed on a virgin part of a piece of material where there is no hardening (or only the small hardening due to the micro- indentation), H=kσy. (1.83) • If a microhardness test is performed on a damaged part of the same piece of material, as the damage occurs for quasi-saturated hardening R+σy ≈σu, onehas ˜ H=kσu(1-D). (1.84) with σu being the ultimate stress. From the two last equations the damage is evaluated as D =1- ˜ H Hσy σu . (1.85) This method gives about the same results as the elasticity changes but, with some care, it allows for the measurement of surface damage fields with in situ measurements (R. Billardon and J. Dufailly 1987). Nevertheless the method does not take into consideration eventual internal stresses, which

1.3 Measurement of Damage 23 sometimes exist in zones subjected to high gradients of plastic strains and which may artificially increase or decrease the hardness. The damage here is measured in compression by use of the coupling be- tween plasticity and damage. Good comparisons with damage measurements in tension prove that the yield criterion does not depend much on the micro- defects closure phenomenon. This non-dependency is due to the mechanism of plasticity itself produced by slips in shear. 1.3.5 Elasticity Field Change (D. Claise, F. Hild and S. Roux 2002) The microhardness technique allows for the measurement of damage fields, but in discrete values for each indentation. More powerful is the measurement, by digital image correlation, of the displacement field of the damaged structure loaded in its elastic range, associated with a finite element analysis (FEA) in which the loading and the displacement fields are given and the local elastic properties related to the damage field are unknown. This technique is described for plane stress or plane strain problems but its extension to 3D problems is possible. Digital image correlation consists of correlating a small image of the sur- face of a deformed body with the image of the same zone in its initial state, by a translation that represents the displacement of its center. It needs: • Some preparation (or not) of the surface in order to obtain a texture heterogeneity that can be observed by a camera. • A CDD camera which is the key point for the resolution of the method. A 12-bit camera allows for a displacement resolution of 10-2 pixel or 5 × 10-5 as the absolute value of the strain, but a 16-bit camera is likely to allow for the measurement of strains with absolute values as low as 10-6, with a relative accuracy of 5% and a gauge length of 1024 pixels. • A fast acquisition set up to record the amount of information defining the images. • A standard Personal Computer. • Software for the image data processing by multiscale correlation (for ex- ample, the software CORRELI developed by F. Hild at LMT-Cachan). • A special finite element code giving directly the damage field whose prin- ciple is explained below. This technique is applied to real damaged struc- tures loaded in such a way that the strain in the most damaged zone remains elastic, with the largest possible value. 1.3.5.1 Damage Field from Displacements Measurements The equilibrium condition σij,j = 0 for elasticity coupled with damage con- stitutive equation (λ and μ are Lam´ e elasticity parameters of the undamaged material),

24 1 Background on Continuum Damage Mechanics σij =2μ(1 - D) eij + λ(1 - D) ekkδij , (1.86) is 2μ eij + λ ekkδij (1 - D),j + 2μ eij + λ ekkδij ,j (1 - D) = 0 (1.87) or 2μ eij + λ ekkδij (1 - D),j 1 - D + 2μ eij + λ ekkδij ,j =0, (1.88) which is rewritten with (1 - D),j 1-D =[ln(1-D)],j: 2μ eij + λ ekkδij [ln(1 - D)],j + 2μ eij + λ ekkδij ,j =0. (1.89) The continuity of the stress vector across interfaces or element boundaries for finite element analyses leads to (with here a boundary oriented by a nor- mal ex) (1 - D){λ( e xx+ eyy+ e zz)+2μ e xx} =0, (1 - D)μ e xy =0, [[(1 - D)μ e xz]]=0, (1.90) where [[ ]] denotes the jump of a quantity . Similar expressions are obtained for normals ey, ez ,or n. In equations (1.89) and (1.90), the displacement field u(x) and therefore the elastic strain field e(x) are known (assumed equal to the strain (x) determined by image correlation in the elastic range). These equations allow for the determination of the field (1 - D(x)) up to a multiplicative factor only since no load measures are considered. If the critical damage Dc is known, the observed crack initiation condition corresponds to (1 - D)=(1- Dc) and gives the multiplicative factor. Based on the FEA, a weak formulation of the problem may be built, assuming a spatial discretization by 2D quadratic elements and a damage constant per element (D = D(p) for element p). The strain energy W (p) eof an element p classically depends on the elastic properties and of the nodal displacements {U e} (see Sect. 2.2). It is linear in (1 - D). In the absence of applied load on each middle node k between two elements p and q,the derivative of the strain energy W (pq) e = W(p) e +W(q) e of both elements with respect to the displacement uk of node k vanishes, so that ∂W (pq) e ∂uk i =0. (1.91) Due to the linearity with respect to (1 - D(p))inelementp and to (1 - D(q)) in element q, one obtains two equations per middle node. These equations

1.3 Measurement of Damage 25 are written in the synthetic form g(p) ik ({U (p)})(1 - D(p))=g(q) ik ({U (q)})(1 - D(q)) , (1.92) where the functions g(p or q) ik are generic and only depend on the nodal dis- placements {U (p)}, {U (q)} of elements p and q. Taking the logarithm of (1.92) yields ln(1 - D(p)) - ln(1 - D(q))=ln|g(p) ik ({U (p)})|-ln |g(q) ik ({U (q)})| (1.93) and leads to the overdetermined linear system [M]{d}={q}, (1.94) where the vector {d} of components the logarithm of (1-D)overeachelement is the unknown, {d} = ln(1 - D(1)) . . . ln(1 - D(p)) . . . ln(1 - D(N)) , (1.95) and where the matrix [M] is filled up with 0, 1 and -1 only. The second member {q} is due to the terms ln |g(p) ik |-ln |g(q) ik | and is function of the measured nodal displacements. The system is solved by the use of the least square method: ([M] {d}-{q})T [Wcor]([M] {d}-{q}) minimum gives {d} , (1.96) where [Wcor] is a diagonal weight matrix. We specify one component of {d} and define {δ} as the new unknown vector {δ} = {d}-{d}0 where {d}0 = 0. . .0 ln(1 - D)i0 0. . .0 . (1.97) The damage field is finally obtained as the solution of [M]T[Wcor][M] {δ} = [M ]T[Wcor] {q}- [M ]T[Wcor][M] {d}0 .(1.98)

26 1 Background on Continuum Damage Mechanics 1.3.5.2 Example of a Cross-Shaped Specimen As an example, Fig. 1.7 shows a cross-shaped specimen that is loaded bi- axially in the triaxial testing machine ASTREE of LMT Cachan and also the lens of the camera. The material is a vinylester-glass fibers composite considered as isotropic since a random distribution of the fibers is observed (Fig. 1.7). The size of the analyzed square is 36.5 × 36.5 mm and it is 2.5 mm thick. The displacement measured just before failure by a mesocrack is also shown in the figure and the corresponding damage field is given in the third picture. Three highly damaged elements are visible on the top left corner and correspond to the initiation of a mesocrack precursor of the final failure of the specimen. Fig. 1.7. Sample in the ASTREE machine with its microstructure (a), displace- ment field (b), damage field of the central zone (c) (D. Claise, F. Hild and S. Roux 2002) 1.4 Kinetic Laws of Damage Evolution According to the thermodynamics framework of Sect. 1.2.1, the evolution law for damage derives from the potential of dissipation and particularly from the function FD : ˙ D = ˙λ∂FD ∂Yor˙ Dij = ˙λ∂FD ∂Yij . (1.99) There are many possible choices for the analytical form of the function FD , depending on the knowledge of experimental results, the purpose of use and the ability of the model maker! The best is the simplest with the domain of validity required, where simplest means the smallest possible number of material parameters.

1.4 Kinetic Laws of Damage Evolution 27 1.4.1 Damage Threshold and Mesocrack Initiation All measurements of damage during plastic loadings, creep, or fatigue show that no mechanical damage occurs before a certain irreversible or accumu- lated plastic strain (pD) is reached, on a meso- or microscale. This threshold pD depends on the material but also encounters strong variations with the type of loading. This is because the damage initiation is in fact related to the amount of energy needed for the incubation of defects, as the stored energy threshold (wD)ofthematerial. According to the formalism of elasto-(visco-)plasticity with isotropic and kinematic hardening of Sect. 1.2, the stored energy is ws = t 0 (R˙ r+Xij˙ αij)dt. (1.100) The ws vs p curve obtained is drawn in Fig. 1.8. It is also shown that the isotropic hardening saturates at the value R = R∞ for large p and recall that p = r as long as there is no damage. With the consideration of the state law Xij=2 3 Cαij , one has then ws =ρψp≈R∞p+ 3 4CXijXij as long as D =0. (1.101) For nonlinear kinematic hardening, the contribution 3 4C Xij Xij reaches a sat- uration value for monotonic loadings and becomes a positive periodic function of time for cyclic loadings. This last expression then exhibits a linear depen- dency in p for large values of the accumulated plastic strain and values for ws much larger than what can be measured when the observed tendency is to reach a constant value asymptotically. Fig. 1.8. Stored energy and damage threshold in pure tension (exponential isotropic hardening with b = 80) .

28 1 Background on Continuum Damage Mechanics For the above purpose, the classical framework needs to be corrected (A. Chrysochoos 1987). A new set of thermodynamics variables, (Q, q), is considered to represent isotropic hardening which introduces the correction function z(r)= A m r(1-m)/m (A and m are material parameters), leading to new expressions such as ws = t 0(Q˙q+Xij˙ αij)dt = t 0 (R(r)z(r)˙ r+Xij˙ αij)dt. (1.102) Within the thermodynamics framework, the change of variables is written as Q(q)=R(r)a n dd q = z(r)dr (1.103) so that ws increases much less with p, as shown in Fig. 1.8: ws ≈AR∞p1/m+ 3 4CXijXij as long as D =0. (1.104) Nothing else in the constitutive equations is modified. One considers then that damage is initiated when the corrected stored energy reaches the threshold value and wD is considered as a material pa- rameter. This allows us to represent the loading dependency of the damage threshold in terms of accumulated plastic strain pD (Fig. 1.9). Fig. 1.9. Stored energy defining the damage thresholds in monotonic and in cyclic loadings For practical applications, approximate expressions for pD may be derived. In the monotonic case, the kinematic hardening may be considered as an additional isotropic hardening (see Sect. 2.1.2) and with p = p and r = p as long as there is no damage. The threshold is defined by reference to the true

1.4 Kinetic Laws of Damage Evolution 29 limit of irreversibility taken as the asymptotic fatigue limit σ∞ f, wD = pD 0 (σu-σ∞ f)A m 1-m m p d p or wD=A(σu-σ∞ f ) 1/m pD , (1.105) with σu as the ultimate stress and pD as the damage threshold in pure tension. • For monotonic loadings, pD= pD. (1.106) • For cyclic or fatigue loadings between σmin ≤ 0a ndσmax > 0, the stored energy due to kinematic hardening is small and may be neglected. An approximation of perfect plasticity at the maximum stress in tension and at the minimum stress in compression allows us to write wD=1 2 pD 0 (σmax-σ∞ f)A mp1-m mdp+1 2 pD 0 (|σmin|-σ∞ f)A mp1-m mdp = A σmax + |σmin| 2 -σ∞ f p1/m D, (1.107) with a stress range, Δσ = σmax -σmin = σmax+|σmin| > 2σ∞ f , correspond- ing to a plastic strain range, Δ p. Equation (1.107) gives the threshold pD as a loading-dependent function of the threshold in pure tension ( pD): pD= pD σu-σ∞ f σmax + |σmin| 2 -σ∞ f m = pD σu - σ∞ f Δσ 2 -σ∞ f m . (1.108) For 3D cyclic loadings such as (Δσ)eq = σeq max + σeq min > 2σ∞ f ,itcan be written as pD= pD σu-σ∞ f (Δσ)eq 2 -σ∞ f m . (1.109) But the most accurate expression for any loading is of course to calculate the stored energy ws and to write max ws = wD at damage initiation . (1.110) One needs then to identify the correction parameters A, m, and the stored energy at damage initiation (wD). Two experiments with damage mea- surements give the threshold of monotonic tension ( pD)a ndinfatigu e

30 1 Background on Continuum Damage Mechanics (pD) for a known plastic strain range (Δ p). The stored energy in mono- tonic tension is ws =A m pD 0 R(p)p(1-m)/mdp + X 2( pD) 2C = wD (1.111) and is ws =A m pD 0 R(p)p(1-m)/mdp + X 2 max 2C =wD (1.112) in fatigue with (see Sect. 1.5.1): -- for exponential isotropic hardening: R(p)=R∞(1 - exp (-bp)) -- for linear kinematic hardening: X( pD)=C pD in monotonic loading, Xmax = C pm a x = CΔ p/2 in alternate fatigue loading σmin = -σmax -- for nonlinear kinematic hardening: X( pD)=X∞(1 - exp (-γ pD)) in monotonic loading, Xmax = X∞ tanh γΔ p 2 in alternate fatigue loading σmin = -σmax where R∞ , b, C, γ and X∞ = C/γ are the hardening parameters. The exponent m is determined by (1.108) such that m= lnpD pD ln σu - σ∞ f Δσ 2 -σ∞ f (1.113) and A is identified by a comparison between (1.111) and (1.112). For nonlinear kinematic hardening, A= mX∞ 2γR∞ [1 - exp (-γ pD)]2 - tanh2 γΔ p 2 pD pD (1 - exp(-bp))p 1 m -1dp (1.114) or, with the hypothesis of saturated hardening at damage initiation in monotonic tension, A≈ X∞ 2γR∞ 1 - tanh2 γΔ p 2 p1/m D - 1/m pD . (1.115) If possible, take A as the average value given by different tests where the plastic strain range Δ p and the damage threshold pD are measured.

1.4 Kinetic Laws of Damage Evolution 31 Finally, still for nonlinear kinematic hardening, wD=AR∞ m pD 0 (1 - exp (-bp)) p(1-m)/mdp +X2 ∞ [1 - exp (-γ pD)]2 2C . (1.116) • For cyclic or fatigue loadings that are periodic by blocks,e a ch level or block i is a cyclic loading between σ(i) eq min and σ(i) eq max . Damage will be initiated during the nB-th block when the stored energy density reaches its threshold, i.e. as soon as ws = wD , or in an equivalent manner when the accumulated plastic strain reaches the loading-dependent threshold pD deduced from: σ(nB) eq min + σ(nB) eq max 2 -σ∞ f p1/m D - (pnB -1)1/m + nB-1 i=1 σ(i) eq min + σ(i) eq max 2 -σ∞ f (pi)1/m - (pi-1)1/m =(σu - σ∞ f) 1 m pD (1.117) where pi is the value of the accumulated plastic strain reached at the end of the i-th block. This equation generalizes equation (1.109) to multilevel fatigue loadings. An example of application is given in Sect. 4.4.1. At the other end of the damage evolution, a mesocrack is initiated when the density of defects reaches the value for which the process of localiza- tion and instability develops (see Sect. 1.6), that is D = Dc in the plane where D( n) is maximum. The critical damage Dc is a material parameter. A way to evaluate Dc is to apply the concept of effective stress at fracture: in a pure tensile test when damage develops at saturated hardening, the stress decreases from the ultimate stress σu to the rupture stress σR in such a way that for isotropic damage: ˜ σR=σu or σR 1-Dc =σu (1.118) from which Dc =1- σR σu (1.119) leading to values of the critical damage between 0.2 and 0.5 for many mate- rials. For anisotropic damage, ˜ σeq=2 3σ1 1-D1+1 3σ1 1-D2 with D2 ≈ D1/2inten - sion. Writing again ˜ σeqR = σu and D1 = Dc gives values of the critical damage of the same order of magnitude.

32 1 Background on Continuum Damage Mechanics 1.4.2 Formulation of the Isotropic Unified Damage Law The thermodynamics approach ensures that the main variable governing the damage evolution or the damage rate ( ˙ D) is its associate variable (Y ), the energy density release rate. Then the dissipative damage potential func- tion (FD) is primarily a function of Y . Many observations and experiments show that the damage is also governed by the plastic strain which is intro- duced through the plastic multiplier ( ˙λ)as ˙ D = ˙λ∂FD ∂Y if p>pD or max ws >wD , (1.120) with ˙λ calculated from the constitutive equations of (visco-)plasticity coupled with the damage deduced from the dissipative potential function (F ), F=f+FX+FD. (1.121) The (visco-)plasticity loading function f is determined by the von Mises criterion (see also Sect. 1.5), f= σ 1-D-X eq -R-σy=σv, (1.122) where • σ 1-D-X eq = 3 2 σD ij 1-D - Xij σD ij 1-D - Xij • σv is the viscous stress for viscoplasticity, σv = 0 for plasticity The normality rule, ˙ p ij= ˙λ∂F ∂σij= ˙λ∂f ∂σij = 32 σD ij 1-D-Xij σ 1-D-X eq ˙λ 1-D, (1.123) coupled with the definition of the accumulated plastic strain rate, ˙p = 2 3˙ p ij˙ p ij , and of the evolution law for the variable r, ˙ r=- ˙λ ∂F ∂R= - ˙λ ∂f ∂R= ˙λ, (1.124) leads to ˙p= ˙λ 1-D. (1.125)

1.4 Kinetic Laws of Damage Evolution 33 Many experimental results show also that FD must be a nonlinear function of Y . Then a simple (good !) choice is FD= S (s + 1)(1 - D) YS s+1 , (1.126) from which ˙ D = YS s ˙p. (1.127) S and s are two material parameters that are functions of the temperature. The full damage constitutive equation is (J. Lemaitre 1987) ˙ D = YS s ˙p if maxws>wD orp>pD, ˙ D =0 ifnot, D = Dc → mesocrack initiation , (1.128) where • Y= ˜ σ2 eqRν 2E Rν=2 3(1 + ν)+3(1- 2ν) σH σeq 2 in the simplest case • Y=1+ν 2E σ + ij σ + ij (1-D)2 +h σ - ij σ - ij (1 - hD)2 - ν 2E σkk 2 (1-D)2+h -σkk 2 (1 - hD)2 if quasi-unilateral conditions are considered • ws= t 0 (R(r)z(r)˙ r+Xij˙ αij)dt and wD is a material parameter (related to pD) • pD = pD for monotonic loading, pD= pD σu-σ∞ f σeq max + σeq min 2 -σ∞ f m for cyclic loading • Dc is a material parameter This law unifies many particular models: • Ductile damage if ˙p is governed by plasticity (see Chap. 3) • Creep damage if ˙p is given by a viscosity law such as Norton power law (see Chap. 5) • Fatigue damage if ˙p is calculated from cyclic plasticity (see Chaps. 4 and 6) • Quasi-brittle damage if ˙p is at a microscopic level (see Chaps. 6 and 7)

34 1 Background on Continuum Damage Mechanics 1.4.3 Formulation of the Anisotropic Damage Law (J. Lemaitre, R. Desmorat and M. Sauzay 2000) It is a "simple" extension of the isotropic case if the following damage dissi- pation potential is considered: FD = Y( e) S sYij d p dr ij , (1.129) where |.| applied to a tensor means the absolute value in terms of the principal components. The term Y is the effective elastic energy density which can be written as a function of the effective stress, Y=1 2 Eijkl ekl eij = 1 2˜ σij eij = ˜ σ2 eq˜ Rν 2E, (1.130) introducing the effective stress triaxiality function, ˜ Rν=2 3(1 + ν)+3(1- 2ν) ˜ σH ˜ σeq 2 , (1.131) where ˜ σeq =(HσDH)eq and ˜ σH= σH 1-ηDH . (1.132) Then ˙ Dij= ˙λ∂F ∂Yij with ˙λ =˙ r (1.133) ˙ Dij =˙ r YS s d p dr ij . (1.134) Or finally, ˙ Dij = YS s |˙ p|ij if max ws >wD or p>pD ˙ Dij =0 ifnot, (1.135) an equation written in the principal frame of the plastic strain rate tensor ˙ p which shows that the principal directions of the damage rate tensor coincide with those of the plastic strain rate. As an example, the pure tensile test reads σ = σ 100 000 000 , p = p 10 0 0-1 20 00- 1 2 , and D=D 100 01 20 001 2 . (1.136) Andasintheisotropiccase, ˙ Dij=0 if ws<wD or p<pD. (1.137) The condition of a mesocrack initiation is fulfilled when the intensity of the damage in one plane reaches the critical value Dc . According to the physical

1.4 Kinetic Laws of Damage Evolution 35 definition of the damage, this occurs when the norm of the damage vec- tor Dij nj or when the largest principal value of the damage DI reaches Dc : max DI = Dc → mesocrack initiation. (1.138) nI(max DI) gives the orientation of the plane on which lies the mesocrack. 1.4.4 Fast Identification of Damage Material Parameters As already stated in Sect. 1.3, the best set of data on damage evolution comes from very low cycle tests, at constant strain range on tension-compression specimens, from which the damage is deduced using the elasticity modu- lus change. Unfortunately, these tests are not commonly available. We will describe here a method to obtain the values of the material parameters for a specific material from usual properties listed in catalogues or hand- books, or derivations using only a few usual tests as tensile and fatigue data: • The damage law itself needs E, ν, S, s • The damage threshold needs pD, σ∞ f,σuandm • The condition of mesocrack initiation needs Dc • The quasi-unilateral conditions need h for isotropic damage or ha for anisotropic damage but most often h =0.2orha =0 • anisotropic damage needs η but a good candidate is η =3 1.4.4.1 Partial Identification from a Simple Tensile Test A simple uniaxial tension test, as shown in Fig. 1.10, gives: • The Young modulus E and the Poisson ratio ν • The yield stress σy , the conventional yield stress σy02 = σ( p =0.210-2) and the ultimate stress σu • The rupture stress σR and the rupture plastic strain pR • The necking parameter Z = S0 - SR S0 with S0 the initial section of the specimen and SR its rupture minimal section Considering the uniaxial, isotropic, unified damage law in monotonic loading with the hardening saturated at σu gives ˙ D= σ2 u 2ES s ˙ p (1.139) or, by integration with D =0if p ≤ pD, D= σ2 u 2ES s ( p - pD) . (1.140)

36 1 Background on Continuum Damage Mechanics The damage usually starts to grow when the plastic strain reaches the value corresponding to the ultimate stress σu , pD ≈ p(σ = σu). (1.141) As introduced in Sect. 1.4.1, the critical value of the damage is given by Dc =1- σR σu (1.142) and 0.2 ≤ Dc ≤ 0.5 in general. Upon fracture, the local rupture strain in the necking region ( pR) is again estimated from the necking parameter Z =(S0 - SR)/S0 considering plastic incompressibility ( p kk =0): pR =2 1-√1-Z . (1.143) Then, Dc = σ2 u 2ES s pR- pD . (1.144) This relation allows us to determine the 3 remaining parameters: S, s,and m. To go further, another type of test is needed. Fig. 1.10. Material parameters from a tension test on ferritic steel at room tem- perature 1.4.4.2 Final Identification from Fatigue Tests Usually it is not too difficult to obtain some information about fatigue! That is at least the case for the engineering fatigue limit (σf) corresponding to

1.4 Kinetic Laws of Damage Evolution 37 a number of cycles to rupture of 106 (or 107), or better, the asymptotic fatigue limit (σ∞ f ) and some low fatigue tests results (Fig. 1.11). The unified damage law can be easily applied to low cycle fatigue if we make the assumption that the material is perfectly plastic for each level of stress, i.e., ˙ D= σ2 max 2ES(1 - D)2 s ˙p. (1.145) As ˙p=|˙ p|, the integration of (1.145) over one cycle N , neglecting the vari- ation of D during the cycle, is simply δD δN = 1cycle ˙ Ddt = σ2 max 2ES(1 - D)2 s 2Δ p , (1.146) where Δ p is the plastic strain range corresponding to σmax or the stress range Δσ =2σmax through the cyclic stress-strain behavior. Using ND as the number of cycles corresponding to the damage threshold and NR as the number of cycles corresponding to a mesocrack initiation when D = Dc , a second integration of (1.145) over the whole fatigue process gives Dc 0 (1 - D)2sδD = σ2 max 2ES s 2Δ p NR ND δN (1.147) or 1 2s +1 1 - (1 - Dc)2s+1 = σ2 max 2ES s 2Δ p (NR - ND) , (1.148) with ND given by pD =2Δ pND = pD σu - σ∞ f σmax - σ∞ f m . (1.149) The number of cycles needed to initiate a mesocrack is finally expressed as NR= pD 2Δ p σu - σ∞ f σmax - σ∞ f m+1-(1-Dc)2s+1 2(2s +1)Δ p 2ES σ2 max s , (1.150) with (2ES)s taken from (1.144) of the tensile test results (2ES)s = σ2s u pR- pD Dc (1.151) so that NR= pD 2Δ p σu - σ∞ f σmax - σ∞ f m+1-(1-Dc)2s+1 2(2s +1)DcΔ p σu σmax 2s pR- pD . (1.152)

38 1 Background on Continuum Damage Mechanics This equation written for two "good" results of low cycle fatigue tests, NR1(σmax 1, Δ p1)andNR2(σmax 2, Δ p2) leads to two equations for the un- knowns s and m which can be solved by substitution by any mathematical software, for example. If the threshold is written in terms of stored energy, we also need the valu e of A to calculate wD according to (1.114) or (1.115) of Sect. 1.4.1: A≈ X∞ 2γR∞ 1 - tanh2 γΔ p 2 p1/m D - 1/m pD and wD=AR∞ m pD 0 (1 - exp (-bp)) p(1-m)/mdp + X 2 ∞ (1 - exp (-γ pD))2 2C , (1.153) where R∞ , C, γ, X∞ = C/γ are the hardening parameters (see Sect. 1.5.1). The word "fast" in the title of this section means a procedure of a few hours once one has the tensile curve and the W¨ ohler curve, but obtaining these experimental results can take a few days or even months! For anisotropic damage, the same procedure gives material parameters close to those obtained for the isotropic law when using damage data with D<0.2. Fig. 1.11. Material parameters from a W¨ ohler curve of ferritic steel at room tem- perature

1.4 Kinetic Laws of Damage Evolution 39 1.4.4.3 Example of Identification for Ferritic Steel The experimental tensile and W¨ ohler curves are shown in Figs. 1.10 and 1.11 but the identification is made only with the coordinates of the 6 points marked by "•" on the figures, that is: σu( pu), σR( pR), σR( pR)a ndσ∞ f, NR1(σmax 1, Δ p1)andNR2(σmax 2, Δ p2). 1. From the tensile curve you can obtain the following: -- Elasticity modulus E = 200000 MPa. -- Poisson ratio measured ν =0.3. -- Yield stress σy = 375 MPa. -- Conventional yield stress σy02 = 380 MPa. -- Ultimate stress: σu = 474 MPa. -- p(σu)=0.15, then pD =0.15. -- σR=330MPathenDc =0.3. -- Z =0.5then pR =0.6. 2. The W¨ ohler curve yields -- Asymptotic fatigue limit σ∞ f = 180 MPa. If the asymptotic fa- tigue limit cannot be estimated take the engineering fatigue limit σf instead. -- Low cycle fatigue tests corresponding to NR ≈ 10 and NR ≈ 1000 cycles: 1. σM1 = 450 MPa, Δ p1 =0 .027, mean value NR1 =1 0c y - cles, 2. σM2 = 340 MPa, Δ p2 =0 .0035, mean value NR2 = 984 cy- cles, from which s =2.4, m =6.Thev alu eofS can then be calculated using (1.144): S= σ2 u 2E pR- pD Dc 1/s =0.665 MPa . (1.154) 3. Finally, take h =0.2, ha =0,andη = 3. If the two scale damage model is applied (see Sect. 1.5.5), Cy = σu - σy pu = 660 MPa and be happy. 4. Last, but most important, is to check how close the above values return the starting curves. The graphs given by the model are shown by the dotted lines in Figs. 1.10 and 1.11: -- for the tensile curve with D ≈ σ2 u 2ES s p - pD , --f o r t h e W ¨ ohler curve in the range of low cycle fatigue. Considering the small number of input information, the comparison with the experimental data is "not bad." The range of high cycle fatigue is the domain of application of the two-scale damage model of Sect. 1.5.5.

40 1 Background on Continuum Damage Mechanics 1.4.4.4 Case of Anisotropic Damage If now the same work is performed with the anisotropic formulae, the only change is in the damage law where ˜ Rν is now different from unity, even in the uniaxial case: σ = σ 00 000 000 , D = D 100 01 20 001 2 , (1.155) and ˜ Rν=2 3(1 + ν)+3(1- 2ν) ˜ σH ˜ σeq 2 , (1.156) with ˜ σH= σH 1-ηDH = σ 1- 2η 3D ˜ σeq = 32 (HσDH)D :(HσDH)D 1/2 =23 σ 1-D+13 σ 1-D 2 . (1.157) Then, ˜ Rν = 23(1 + ν)+3(1- 2ν) (1 - 2η 3D) 2 1-D+ 1 1-D 2 -2 (1.158) in tension. With ν =0.3andη = 3, the maximum value of ˜ RνforD≤0.2is1.12, which is 12% more than the isotropic damage value Rν = 1. As the uniaxial law turns into ˙ D = σ2 max ˜ Rν 2ES s ˙p, (1.159) this changes the value of S and Dc by an amount which remains in the order of magnitude of the experimental discrepancy or the hypothesis of perfect plasticity. In practice, keep s as identified for the isotropic damage model and update S and Dc on the monotonic tensile curve. For more accurate predictions, the "fast identification" results may be used as the starting values of an optimization process to fit all available data that can be obtained on a specific material. This numerical optimiza- tion process, the least square method, consists of finding the set of param- eters to minimize the difference between experiments and predictions. Nu- merical methods for precise identification are described in Sect. 2.4 with an exampley. The end of Sect. 1.5.5 offers a more precise identification of the asymptotic fatigue limit.

1.4 Kinetic Laws of Damage Evolution 41 1.4.5 Generalization of the Unified Damage Law For materials which do not exhibit meso-plasticity, it is not possible to con- sider the damage as governed by the accumulated plastic strain rate. The damage law ˙ D =(Y/S)s ˙p is then useless. A damage law D = D(Y ) cannot be considered either as it does not lead to damage growth in fatigue. For such materials the idea is to relate the damage rate to the main dissipative mechanism, often internal sliding and friction, and to consider damage as governed by a cumulative measure of the internal sliding. This may ap- ply to metals for which internal slips are mainly due to dislocations creation and evolution, as well as many non-metallic materials such as elastomers (Sect. 4.4.3), concretes, and composites. We then use a framework that is similar to elasto-(visco-)plasticity cou- pled with damage and define π , α, q,andD as internal variables associated with -σπ , X, Q,and-Y (see Table 1.2). The physical meaning of the ther- modynamic variables depends on the type of material and of the physical dis- sipative mechanisms. It will be discussed for the case of metals, elastomers, and concrete later (Sect. 1.4.5.3). Nevertheless, • π is an internal inelastic strain which can be recovered • X is a residual microstress of kinematic nature • Q defines the size increase of the reversibility domain in the σπ stress space • D is the damage variable (D if induced anisotropy is considered) Ta b l e 1 . 2 . State and associated variables Mechanisms Type State variables Associated Observable Internal variables Elasticity Tensor σ Internal Tensor π -σπ sliding Tensor αX Scalar qQ Damage Scalar D -Y Next we consider the small strain hypothesis with isotropy of the dis- sipative mechanisms, including damage. For the finite strain framework see Sect. 4.4.3. The general form of the state potential canbeexpressedas ρψ =(1- D)[w1( )+w2( - π)] + ws(q, α) , (1.160) where w1 and w2 define the strain energy density and ws is the stored energy density as a function of the scalar variable q and the tensorial variable α. The state laws are

42 1 Background on Continuum Damage Mechanics σij=ρ∂ψ ∂ ij =(1- D)∂(w1 + w2) ∂ ij , σπ ij= -ρ∂ψ ∂ π ij =(1- D) ∂w2 ∂ ij , Xij=ρ∂ψ ∂αij = ∂ws ∂αij , Q=ρ∂ψ ∂q=∂ws ∂q, Y=-ρ∂ψ ∂D=w1+w2. (1.161) They naturally define the effective stresses (˜ σ,˜ σπ) such that the elasticity law written in terms of strains and effective stresses does not depend on D (strain equivalence principle): ˜ σ =∂(w1+w2) ∂ , ˜ σπ=∂w2 ∂ . (1.162) The dissipation potential is defined as F=f+FX+FD, (1.163) where •f= σπ 1 - D - X -Q - σs < 0 defines the reversibility domain, . is a norm in the stresses space (not necessarily von Mises norm), and σs is the reversibility limit • the functions FX = γ 2CX Xij Xij and Q = Q(q) model the internal sliding nonlinearity • FD= S (s + 1)(1 - D) YS s+1 is the damage potential The evolutions laws can then be derived from the dissipation potential (nor- mality rule) ˙ π ij =˙ μ∂F ∂σπ ij, ˙ αij=- ˙μ∂F ∂Xij , ˙q= - ˙μ∂F ∂Q, ˙ D=˙ μ∂F ∂Y, (1.164)

1.4 Kinetic Laws of Damage Evolution 43 where ˙μ is the internal sliding multiplier equal to a norm of the inelastic strain rate: ˙μ 1-D= ˙ r 1-D= ˙ π . (1.165) This defines the cumulative measure of the internal sliding as π = t 0 ˙ π dt. (1.166) The multiplier ˙μ is given by the consistency condition, f =0and ˙f =0,for non-viscous materials or by a viscosity law such as the generalized Norton law, ˙ π = f/KN N = σv/KN N , for viscous materials undergoing a viscous stress σv . The generalized damage evolution law is derived from (1.164), leading to ˙ D = YS s ˙ π if π>πD D=Dc -→ mesocrack initiation, (1.167) which corresponds to the damage governed by the main dissipative mecha- nisms through ˙ π and where S and s are the damage material parameters and πD is the damage threshold. 1.4.5.1 Positivity of the Intrinsic Dissipation As in the previous thermodynamics framework, the generalized damage model satisfies the positivity of the intrinsic dissipation, D = σij ˙ ij-ρ˙ψ, as D=σπ ij˙ π ij-Q˙q-Xij˙ αij+Y˙ D = σπ ij ∂F ∂σπ ij +Q∂F ∂Q+Xij ∂F ∂Xij +Y∂F ∂Y ˙λ ≥ 0 (1.168) at constant temperature when the dissipation potential F (σπ ,Q,X,Y; D) is a non-negative convex function of its arguments σπ , R, X,andY ,where F (0, 0, 0, 0; D) = 0 and the damage D acts as a parameter. Using the evolu- tion laws, the intrinsic dissipation may also be rewritten as D= σs+σv+ γ CX Xij Xij (1 - D) ˙ π +Y ˙ D≥0. (1.169) This condition requires the damage rate to be positive or zero ( ˙ D≥0, an eventual recovery of damage needs a new variable) and the stored energy rate ˙ ws =Xij˙ αij + Q ˙q to remain smaller or equal to the inelastic strain power (σπ ij˙ π ij).

44 1 Background on Continuum Damage Mechanics 1.4.5.2 Extension to Induced Anisotropy Note that the generalization of previous damage evolution extension to in- duced damage anisotropy is also possible. It is ˙ Dij = YS s |˙ π|ij , (1.170) with |.| as the absolute value of a tensorfor ductile materials such as metals (with then π = p), or ˙ Dij = YS s ˙ π + ij, (1.171) with . + as the positive part of a tensor for quasi-brittle materials such as concrete for (J. Mazars, Y. Berthaud and S. Ramtani 1990): D = D 00 000 000 in tension D = 000 0D0 00D in compression (1.172) when the loading direction is e1. 1.4.5.3 Application to Metals, Concrete and Elastomers To conclude, this section (Sect. 1.4.5) can be considered a synthetic presen- tation of constitutive models for metals, elastomers, concrete: • Fo r m e t a l s , w1 =0,Q(q)=R(r) is the isotropic hardening, X is the kinematic hardening, . is the von Mises norm (.)eq, π is the plastic strain p, and the generalized damage law (1.167) recovers ˙ D =(Y/S)s ˙p where π equals the accumulated plastic strain p. • For filled elastomers, and anticipating the choices made in Sect. 4.4.3 for the model of hyperelasticity with internal friction coupled with damage, w1 is an hyperelasticity density such as Mooney or Hart--Smith densities, R =0,a ndw2 and FX are quadratic functions. The variable X stands for the residual microstresses due to internal sliding with friction of the macromolecular chains on themselves and the black carbon filler parti- cles. The internal inelastic strain π represents the average displacements incompatibilities due to friction on a microscale. • For concrete, w1 , w2 ,andFX are quadratic, Q and X model the growth and the translation of the reversibility domain f<0intheσπ space, and π represents the average slip discontinuities of the cracked media on amicroscale.

1.5 Elasto-(Visco-)Plasticity Coupled with Damage 45 1.5 Elasto-(Visco-)Plasticity Coupled with Damage The whole set of constitutive equations is derived from the dissipation po- tential as explained in the general thermodynamics framework of Sect. 1.2.1. The different models differ by the choice of analytic forms of the functions f , FX ,andFD for the potential F=f+FX+FD. (1.173) 1.5.1 Basic Equations without Damage Coupling Both plasticity and visco-plasticity introduce a yield criterion (f) by defin- ing the elastic domain of the material by f<0, and the plastic and visco- plastic states by f =0, ˙f =0 plasticity f=σv>0, visco-plasticity (1.174) respectively. The term σv is the viscous stress given by the law of viscosity. More often, the von Mises criterion is used with isotropic hardening, f=σeq-R-σy, (1.175) where σeq is the von Mises equivalent stress. When isotropic and kinematic hardening are taken into consideration, f=(σ-X)eq-R-σy, (1.176) with (σ - X)eq = 3 2(σD ij-XD ij)(σD ij-XD ij ). The isotropic hardening R is related to the density of dislocations or flow arrests and it represents the growth in size of the yield surface. Expo- nential isotropic hardening is considered to ensure a quasi-saturation of the strain hardening when damage occurs, i.e., R = R(r)=R∞ [1 - exp (-br)] , (1.177) with R∞ and b as temperature-dependent material parameters. The variable r is equal to the accumulated plastic strain p as long as there is no damage. ApowerlawR = Kpr1/M or a linear law (M =1)mayalsobe used. The kinematic hardening governed by the back stress X is related to the state of internal microstress concentration. It represents the translation of the yield surface as X defines the center of the current elastic domain in the stress space. Nonlinear kinematic hardening is modelled by the function potential FX, FX=3γ 4CXijXij , (1.178)

46 1 Background on Continuum Damage Mechanics with C and γ temperature-dependent material parameters. As long as there is no damage, the classical evolution laws for the back stress are Xij = 23C p ij for linear kinematic hardening d dt Xij C = 2 3˙ p ij-γ C Xij ˙p for nonlinear kinematic hardening. (1.179) The last equation is the non-isothermal form of the Armstrong--Frederick law which is often used with X∞ = C/γ for easier identification, as in monotonic uniaxial loading X = X∞ [1 - exp(-γ p)]. The back stress X governed by the plastic strain is a deviatoric tensor (Xkk =0andX = XD). For Prager linear hardening, Xij = 2 3 C p ij can be recovered by setting γ =0. A strong effect of the temperature (T ) is observed as there is a transition from visco-plastic time-dependent (viscous) behavior at high temperature, such as creep, to plastic time-independent behavior at lower temperature. The constitutive equations can be derived from (1.25) as follows: ˙ p ij= ˙λ∂F ∂σij , ˙ r=- ˙λ ∂F ∂R, ˙ αij=- ˙λ ∂F ∂Xij , ˙ D= ˙λ∂F ∂Y,or˙ Dij= ˙λ∂F ∂Yij , (1.180) provided that • For plasticity, the multiplier is determined by the consistency condition f=0, ˙f=0, ˙λ= ∂f ∂σij ˙ σij+23dC dT αij ∂f ∂Xij ˙ T dR dT ∂f ∂R ∂F ∂R+23C ∂f ∂Xij ∂F ∂Xij - ∂f ∂Dij ∂F ∂Dij . (1.181) • For viscoplasticity, the multiplier is a function of the accumulated plastic strain rate ( ˙p = 2 3˙ p ij˙ p ij) given by a viscosity law. Different choices are possible: - Norton power law σv =KN˙p1 N or ˙p= f KN N , (1.182)

1.5 Elasto-(Visco-)Plasticity Coupled with Damage 47 - Exponential law to ensure saturation at large plastic strain rate, σv = K∞ 1 - exp - ˙p n or ˙p=ln 1- f K∞ -n , (1.183) where KN, K∞, N,a ndn are material parameters that depend on the temperature. There are many possibilities in modelling plasticity and viscosity, depend- ing on whether or not the yield stress, kinematic hardening, and isotropic hardening are equal to zero. The model must be chosen carefully because the material parameters for a given material have values that are specific to each model. To be as clear as possible, the notations adopted in the book for the (visco-)plasticity parameters have an extra "0" in superscript or lowerscript when a zero yield stress is considered. They have an extra "y" in superscript or lowerscript when (visco-)plasticity is modelled with a non-zero yield stress but with one hardening only, either isotropic or kinematic. This is illustrated in the uniaxial case as: • Yieldfunctionin monotonictensionf=σ-X-R-σy --I f σy =0andX =0,R = K0 p 1/M0 p --I f σy =0andX =0,R = Ky p 1/My p orR=Ry ∞ (1 - exp(-by p)) --I f σy =0andR=0,X=Cy p orX=Xy ∞ (1 - exp(-γy p)) --I f σy =0,X =0andR =0, R = Kp 1/M p orR=R∞(1- exp(-b p)), X=C p or X = X∞(1- exp(-γ p)), • Viscosity law --I f σy =0,X =0andR =0, ˙ p = σ K0 N N0 --I f σy =0,X =0andR =0, ˙ p= σ-σy Ky N Ny --I f σy =0,X =0andR =0, ˙ p= σ-X-R-σy KN N or˙ p =ln 1- σ-X-R-σy K∞ -n . 1.5.1.1 Fast Identification of (Visco-)Plasticity Material Parameters An accurate value of the (visco-)plasticity material parameters is necessary for practical applications and may be obtained independently from the dam- age parameters if p<pD. Altogether, there are 5 (+2) characteristic parame- ters of (visco-)plasticity to determine for each material and each temperature:

48 1 Background on Continuum Damage Mechanics • Yield stress: σy . • Isotropic hardening: R∞ and b (or Kp and M). • Kinematic hardening: C (linear) or X∞ and γ (nonlinear). • Viscosity: KN and N or K∞ and n. 1.5.1.1.1 Hardening parameters For hardening, a direct and fast identification is possible from a tension test or tension-compression low cycles tests that are strain controlled, at increasing amplitude below the damage threshold, as R and X may be directly measured on the graph σ( p). • From a monotonic tensile curve it is only possible to identify one harden- ing which is either -- An isotropic hardening by · ApowerlawR=σ-σy=Ky p 1/My p · AnexponentiallawR=σ-σy=Ry ∞ [1 - exp(-by p)] -- Or a kinematic hardening by · AlinearlawX=σ-σy=Cy p · An exponential law X = σ-σy = Xy ∞ [1 - exp(-γy p)] with Xy ∞= Ry ∞,γy=by. From the example of Fig. 1.12 for an Inconel alloy at room temperature with a yield stress depending upon the chosen hardening law: Fig. 1.12. Tension curve for identification of either isotropic or kinematic hardening parameters (Inconel alloy at room temperature, J. Dufailly 1987)

1.5 Elasto-(Visco-)Plasticity Coupled with Damage 49 σy = 920 MPa,Ky p = 810 MPa,My =4.5 for the power R law σy = 1120 MPa,Cy =(σA - σy)/ pA = 3800 MPa for the linear X law σy = 1040 MPa,Ry ∞ =Xy ∞ = 315 MPa,by = γy =55fortheexp.laws • From a tensile curve with repeated unloadings and compressions until the yield stresses in compression are reached, we can identify both isotropic and kinematic hardenings acting together as the back stress X is the ordinate of the middle of the elasticity straight line. The test should be performed at very low strain rate if the material exhibits viscosity. From the example of Fig. 1.13 on the same material used for Fig. 1.12, a curve fitting procedure gives the following for isotropic and kinematic hardenings considered altogether: a) Kp = 280 MPa, M =5.5 for the isotropic hardening power law, or R∞ = 165 MPa, b = 80 for the isotropic hardening exponential law b) C = 7140 MPa and γ = 0 for linear kinematic hardening, or X∞ = 450 MPa, γ =60(andC = γX∞ = 27000 MPa) for nonlin- ear kinematic hardening Fig. 1.13. Tension test with repeated unloadings up to a plastic strain offset of 10-5 for the identification of both isotropic and kinematic hardenings parameters (Inconel alloy at room temperature, J. Dufailly 1987) • From the stabilized cycles of tension-compression experiments performed at different plastic strain ranges Δ p, it is possible to identify the nonlinear kinematic hardening parameters C, γ, X∞ = C/γ.

50 1 Background on Continuum Damage Mechanics The integration of the nonlinear law (1.179) over each half cycle leads to Δσ 2 -k=X∞ tanh γΔ p 2 , (1.184) where Δσ is the stress range of the considered cycle and 2k is the size of the elastic domain measured on each cycle unloading for each strain range(k= σy+Rifthereis no viscosity,k= σy+R+σv ifthereis).We can identify X∞ as the asymptote of the curve Δσ 2 -kvsΔ pandthen determine γ using a curve fitting procedure. 1.5.1.1.2 Viscosity parameters The more accurate way to determine viscosity parameters is to perform re- laxation tests after saturating both isotropic and kinematic hardenings. The saturation values R∞ and X∞ can be found from a very slow tensile test: σ=σy+R∞+X∞+σv, (1.185) where σv is the viscous stress. At constant strain, = e + p, the strain rate ˙ =0,and ˙ p=- ˙ σ E (1.186) coupled with the viscosity law leads to a nonlinear differential equation whose solution is the σ(t)curve. The graph of σv = σ -σy -R∞ -X∞ as a function of˙ p=-˙ σ/E allows then for the identification of either Fig. 1.14. Relaxation test for identification of viscosity parameters of an Inconel alloy at T = 627◦C (J. Dufailly 1987)

1.5 Elasto-(Visco-)Plasticity Coupled with Damage 51 • The Norton law ˙ p = σv KN N • The exponential law σv = K∞ 1 - exp - ˙ p n From the example of Fig. 1.14 with E = 160000 MPa, a curve fitting procedure gives KN = 75000 MPa·s1/N , N =2.4; K∞ =107 MPa, and n =1.410-2s-1. For better accuracy, the results of this fast identification may be taken as the starting solution of a numerical procedure of optimization if other tests are available (see Sect. 2.4). 1.5.1.2 Concerning the Choice of a Damage Model Different possibilities arise corresponding to the physical effects really needed for the application in mind, the quantitative information available in the experimental data base and different levels of mathematical and numerical complexity. The following advice may be considered as guidelines: • Fo r proportional loading and more generally when simplicity is the most important issue, the isotropic damage models are preferred. When analytical solutions are needed, this choice is necessary and compatible with the consideration of the microdefects closure effect. • Fo r numerical computations, the use of the anisotropic damage models is encouraged as they do not introduce additional material parameters, except maybe the coefficient η which is equal to 3 in most cases. The difficulty related to the consideration of induced anisotropy is mostly nu- merical but Sect. 2.2 is devoted to the subject. • Fo r non-proportional loading (difficult to handle in closed form), choose the anisotropic damage models as they reproduce in a more re- alistic way the accumulation of the damages due to loadings applied in different directions. • Fo r fatigue applications, we advise using the models that include the microdefects closure effect as they lead to an evolution of the damage different in tension than in compression and then to a mean stress effect. Last, choose a proper damage threshold criterion (see Sect. 1.4.1): • Fo r monotonic applications use the criterion p = pD, • Fo r fatigue applications use the criterion p = pD. It is possible to consider pD = constant as long as no overloading occurs and then usually pD pD. The preferred way to calculate pD for each loading amplitude is using pD= pD σu-σ∞ f σmax + |σmin| 2 -σ∞ f m . (1.187)

52 1 Background on Continuum Damage Mechanics • Fo r numerical analysis with a complex history of loading, use the stored energy criterion max ws = wD. It is then necessary to consider both non- linear isotropic and kinematic hardenings with the thermodynamics cor- rection of Sect. 1.4.1. The material parameters for the damage initiation are either wD , A, m or pD, A, m,withA and wD given by (1.114) and (1.116). If the fatigue limit σ∞ f and the plasticity parameters are known, use the approximate formula (1.153) to calculate A. 1.5.2 Coupling with Isotropic Damage , The damage is represented by the scalar D. Its law of evolution is (see Sect. 1.4) ˙ D = YS s ˙p, if r>pD or maxws>wD, (1.188) where the damage threshold is written in terms of stored energy or in an equivalent manner of accumulated plastic strain (see Sect. 1.4.1). The full sets of constitutive equations for elasto-(visco-)plasticity coupled with isotropic damage with nonlinear isotropic and kinematic hardening are given in the following tables, where the case of linear kinematic hardening is recovered by setting γ =0. 1.5.2.1 Isotropic Damage without Microdefects Closure Effect (Table 1.3) The coupling of damage with elasticity as well as plasticity is made through theuseoftheeffectivestress ˜ σ instead of σ in the elasticity law, eij = 1+ν E˜ σij-ν E˜ σkkδij , ˜ σij = σij 1-D, (1.189) and in the von Mises criterion, f =(˜ σ-X)eq-R-σy. (1.190) The plasticity remains incompressible and p, X,a n dα are deviatoric tensors.

1.5 Elasto-(Visco-)Plasticity Coupled with Damage 53 Ta b l e 1 . 3 . Elasto-(visco-)plasticity coupled with isotropic damage Strain partition ij= e ij+ p ij Thermo-elasticity e ij=1+ν E˜ σij-ν E˜ σkkδij + α(T - Tref)δij ˙ p ij = 32(˜ σD ij - Xij) (˜ σ-X)eq ˙ r 1-D (Visco-)plasticity ˙p= ˙ r 1-D R = R∞(1- exp(-br)) d dt Xij γX∞ = 23(1 - D)˙ p ij-Xij X∞ ˙ r ˙ D = YS s ˙pifr>pDor maxws>wD uptoDc Damage Y = 12Eijkl e ij ekl = ˜ σ2 eqRν 2E Rν = 23(1 + ν)+3(1- 2ν) σH σeq 2 Plastic multiplier ˙ r= ˙λgivenbyf=0and˙f=0 Visco-plastic multiplier ˙p= f KN N Norton law ˙p=ln 1- f K∞ -n exponential law

54 1 Background on Continuum Damage Mechanics 1.5.2.2 Isotropic Damage with Microdefects Closure Effect (Table 1.4) The coupling of damage with elasticity is made through the use of the effective stress, ˜ σij = σ + ij 1-D+ σ - ij 1-hD +ν 1 - 2ν δkl σ + kl - σkk 1-D +δkl σ - kl + -σkk 1 - hD δij , (1.191) defined in Sect. 1.2.4 in the elasticity law, but not in the von Mises criterion in which σ/(1 - D) is used. The justification is in the mechanism of plasticity itself controlled by slips and produced by shear stresses in the same manner regardless of their signs. Furthermore, as mentioned in Sect. 1.3.4, damage measurements mainly in compression by microhardness give the same values as those obtained by elasticity change in tension: f= σ 1-D-X eq -R-σy. (1.192) The plasticity remains incompressible and p, X,a n dα are deviatoric tensors.

1.5 Elasto-(Visco-)Plasticity Coupled with Damage 55 Ta b l e 1 . 4 . Elasto-(visco-)plasticity coupled with isotropic damage and with microdefects closure effect Strain partition ij= e ij+ p ij Thermo-elasticity e ij=1+ν E˜ σij-ν E˜ σkkδij + α(T - Tref)δij ˙ p ij=32 σD ij 1-D-Xij σ 1-D-X eq ˙ r 1-D (Visco-)plasticity ˙p= ˙ r 1-D R = R∞(1- exp(-br)) d dt Xij γX∞ = 23(1 - D)˙ p ij-Xij X∞ ˙ r Damage ˙ D = YS s ˙pifr>pDor maxws>wD uptoDc Y=1+ν 2E σ + ij σ + ij (1-D)2 +h σ - ij σ - ij (1 - hD)2 -ν 2E σkk 2 (1-D)2 +h -σkk 2 (1 - hD)2 Plastic multiplier ˙ r= ˙λgivenbyf=0and˙f=0 Visco-plastic multiplier ˙p= f KN N Norton law ˙p=ln 1- f K∞ -n exponential law

56 1 Background on Continuum Damage Mechanics 1.5.3 Coupling with Anisotropic Damage , The damage is represented by the second order tensor D.Itse v olutio nis governed by the law (see Sect. 1.4) ˙ Dij = YS s |˙ p|ij if r>pD or max ws >wD , (1.193) where the principal directions of the damage rate coincide with the absolute value (in terms of principal values) of the plastic strain rate. The damage threshold is written in terms of stored energy or in an equivalent manner of accumulated plastic strain (see Sect. 1.4.1). The full sets of constitutive equations for elasto-(visco-)plasticity coupled with anisotropic damage with nonlinear isotropic and kinematic hardening are given in the following tables, where the case of linear kinematic hardening is recovered by setting γ =0. 1.5.3.1 Anisotropic Damage without Microdefects Closure Effect (Table 1.5) The coupling of damage with elasticity is made through the use of the effective stress, ˜ σij =(Hik σD klHlj)D + σH 1-ηDHδij, (1.194) in the elasticity law as well as in the von Mises criterion, f =(˜ σ-X)eq-R-σy. (1.195) The plasticity remains incompressible and p, X,andα are deviatoric ten- sors.Writing the following set of equations in terms of effective stress makes it fully similar to the set obtained in the case of isotropic damage.

1.5 Elasto-(Visco-)Plasticity Coupled with Damage 57 Ta b l e 1 . 5 . Elasto-(visco-)plasticity coupled with anisotropic damage Strain partition ij= e ij+ p ij Thermo-elasticity e ij=1+ν E˜ σij-ν E˜ σkkδij + α(T - Tref)δij ˙ p ij =[Hik ˙ ep klHlj]D (Visco-)plasticity with ˙ ep ij=32 ˜ σD ij-Xij (˜ σ-X)eq ˙ r ˙p = H(˜ σD - X)H eq (˜ σ-X)eq ˙ r R = R∞(1- exp(-br)) d dt Xij γX∞ = 23 ˙ ep ij-Xij X∞ ˙ r ˙ Dij = YS s|˙ p|ij if r>pD or max ws >wD uptoDc Damage Y = 12Eijkl e ij ekl = ˜ σ2 eq˜ Rν 2E ˜ Rν = 23(1 + ν)+3(1- 2ν) ˜ σH ˜ σeq 2 ˜ σeq = HσDH eq,˜ σH= σH 1-ηDH Plastic multiplier ˙ r= ˙λgivenbyf=0and˙f=0 Visco-plastic multiplier ˙p= f KN N Norton law ˙p=ln 1- f K∞ -n exponential law

58 1 Background on Continuum Damage Mechanics 1.5.3.2 Anisotropic Damage with Microdefects Closure Effect (Table 1.6) The coupling of damage with elasticity is made through the use of the effective stress, ˜ σij =(H p ik σD +klHp lj)D +(Hn ikσD -klHn lj)D + σH 1-ηDH - -σH 1 - ηhaDH δij , (1.196) defined in Sect. 1.2.4 in the elasticity law, where Hp ij =(1 - D)-1/2 ij and Hn ij =(1 - haD)-1/2 ij. (1.197) The full (HpσDH p)D is introduced in the yield criterion, not affected by the closure effect, f= HpσDHp-X eq-R-σy. (1.198) The plasticity remains incompressible and p, X,a ndα are deviatoric tensors.

1.5 Elasto-(Visco-)Plasticity Coupled with Damage 59 Ta b l e 1 . 6 . Elasto-(visco-)plasticity coupled with anisotropic damage and with microdefects closure effect Strain partition ij= e ij+ p ij Thermo-elasticity e ij=1+ν E˜ σij-ν E˜ σkkδij + α(T - Tref)δij ˙ p ij = Hp ik˙ ep klH p lj D (Visco-)plasticity with ˙ ep ij = 32(Hp ikσD klHlj)D - Xij (HpσDHp - X)eq ˙ r ˙p = Hp (HpσDHp)D - X Hp eq (HpσDHp - X)eq ˙ r R = R∞(1- exp(-br)) d dt Xij γX∞ = 23 ˙ ep ij-Xij X∞ ˙ r ˙ Dij = YS s|˙ p|ij if r>pD or max ws >wD uptoDc Damage Y=1+ν 2E tr H pσD +Hp 2 + ha HnσD -H n 2 +3(1-2ν) 2E σH 2 (1 - ηDH)2 + ha -σH 2 (1 - ηhaDH)2 Plastic multiplier ˙ r= ˙λgivenbyf=0and˙f=0 Visco-plastic multiplier ˙p= f KN N Norton law ˙p=ln 1- f K∞ -n exponential law

60 1 Background on Continuum Damage Mechanics 1.5.4 Non-Isothermal Behavior The constitutive equations in the preceding tables are written for anisother- mal cases and all the material parameters are functions of the temperature. If an incremental numerical procedure is used, the state laws must be prop- erly differentiated with respect to the time. This is particularly important for the law of thermo-elasticity, in which appears an extra term when the temperature varies. ˙ eij = 1+ν E˙ ˜ σij-ν E˙ ˜ σkkδij+α ˙ T + d dT 1+ν E ˜ σij-d dT ν E ˜ σkkδij + dα dT (T - Tref)δij ˙ T. (1.199) There are no such temperature derivatives in the laws of (visco-)plasticity and damage as they are derived from the dissipation potential that is written in terms of powers. Note that the evolution law for nonlinear kinematic hardening is simpler for anisothermal loading if it is written in terms of α,aswiththestatelaw Xij=2 3 Cαij . We can then obtain ˙ αij =(1- D)˙ p ij-γαij˙ ror˙ αij =˙ ep ij-γαij˙ r, (1.200) with ˙ ep ij =˙ p ijand˙ r=˙ p as long as there is no damage. This avoids taking into account the supplementary thermal term due to the derivative of C = γX∞ with respect to T in the Armstrong--Frederick law, as d dt Xij γX∞ = 23 ˙ ep ij-Xij X∞ ˙ r (1.201) becomes ˙ Xij=23C˙ ep ij-γXij˙ r+Xij CdC dT˙ T (1.202) Note also that in plasticity, the expression (1.181) for the multiplier ˙λ introduces a ˙ T term. 1.5.5 Two-Scale Model for Damage at Microscale (J. Lemaitre and I. Doghri 1988, R. Desmorat and J. Lemaitre 2000) The damage threshold criterion max ws = wD or p = pD states that damage occurs for a given amount of plasticity. In the same spirit, the damage evolu- tion and its anisotropy are both governed by the plastic strains. The damage model previously described applies then only when plastic strains are sensi- ble on a mesoscale, i.e. mostly for ductile failure, low cycle fatigue, and creep (Chaps. 3, 4, 5). For brittle failures with no permanent strains, other damage

1.5 Elasto-(Visco-)Plasticity Coupled with Damage 61 models are necessary (see Chap. 7). For quasi-brittle failures or high cycle fatigue, for which the loading is below the conventional yield stress, plastic- ity (or dissipation) and damage occur but at a scale much smaller than the RVE scale. A multiscale approach is thus necessary (see also Sects. 6.2.3 and 7.2.4). Two scales are defined in accordance with the growth of microscale dam- age in a mesoscopic RVE: • The mesoscale or the classical scale of continuum mechanics. • The microscale or the scale of microdefects present inside the RVE but whose effects on the mechanical properties are not measurable, except for monotonic and fatigue supture properties. From the mechanical point of view of the homogenization procedures, such defects are considered altogether as a "weak" inclusion in a meso-RVE, the matrix (see Fig. 1.15). Fig. 1.15. Microelement embedded in an elastic (plastic) RVE 1.5.5.1 Constitutive Equations The overall elasto-(visco-)plasticity material behavior is the same on the two different scales but as the inclusion is "weak," it will be subjected to damage, with the matrix remaining undamaged. On a mesoscale, the full set of elasto-(visco-)plasticity constitutive equa- tions with a yield stress of σy and with both isotropic and kinematic hard- ening may be considered. For quasi-brittle failure or high cycle fatigue ap- plications (with a state of stress under the yield stress) only elasticity is considered. On a microscale, the behavior is modeled by elasto-(visco-)plasticity cou- pled with damage. The weakness of the inclusion is related to its yield stress σμ y taken equal to the asymptotic fatigue limit σ∞ f of the material, below which no plasticity exists and then no damage can occur. The yield criterion is written as fμ= σμ 1-Dμ -Xμ eq -σ∞ f, (1.203)

62 1 Background on Continuum Damage Mechanics where Xμ is the microscale back stress. To simplify, only linear kinematic hardening is assumed on the microscale but with the same plastic modu- lus Cy as the modulus measured on the mesoscale. The microscale damage is assumed to be isotropic and its evolution law is written in terms of mi- crostress, micro-energy density release rate, and micro-accumulated plastic strain, i.e., ˙ Dμ =(Y μ/S)s ˙pμ. As the mean stress effect needs to be repre- sented in fatigue, the micro-energy density rate Y μ takes into account the different behaviors in tension and in compression through the parameter h. Finally, the plastic multiplier, ˙λ =˙ pμ(1 - Dμ), is calculated from • The consistency condition f μ =0and ˙f μ = 0 for micro-plasticity or • The Norton law ˙pμ = fμ KN N for micro-viscoplasticity. The full set of equations is given in Table 1.7. The variables in the inclu- sion (stress tensor σμ , total strain tensor μ, elastic strain tensor μe and plastic strain tensor μp, damage Dμ ...) have a "μ"-superscript to denote microscale when the variables at the mesoscale are simply represented by σ, , e , p ... with no superscripts. Note that damage being considered only on the microscale, the "μ"-superscript is omitted by setting Dμ ≡ D. 1.5.5.2 Scale Transition The scale transition for inner defects is made by use of the Eshelby--Kr¨ oner localization law: the total and plastic strains at microscale level are related to the strains at the mesolevel as in μ ij = ij +β( μp ij - p ij), (1.204) where β is given by an Eshelby analysis of a spherical inclusion: β=2 154-5ν 1-ν . (1.205) For surface defects, due to free edge conditions the localization law must be changed (see Sect. 6.4.6). 1.5.5.3 Use of the Two-Scale Model The mesostresses (σ(t)) and strains ( (t), ( p(t))) are determined from a clas- sical structure calculation (made in elasticity for quasi-brittle and high cycle fatigue applications). Their history are the inputs for the post-processing cal- culation of the strains, stresses, hardening, and damage at microscale. Their values are obtained from the time integration of the constitutive equations at microlevel coupled altogether with the Eshelby--Kr¨ oner law of localization. When the damage (D) reaches the critical value (Dc) there is initiation of a crack in the inclusion which corresponds to a mesocrack in the RVE if

1.5 Elasto-(Visco-)Plasticity Coupled with Damage 63 Ta b l e 1 . 7 . Two-scale damage model equations Mesoscale General case Elasto-(visco-)plasticity constitutive equations σ , e , p Quasi-brittle failure Elasticity ij = 1+ν Eσij-ν E σkkδij X,R High cycle fatigue with σ∞ f <σeq <σy Scale Eshelby--Kr¨ oner μ ij = ij+β( μp ij - p ij) transition localization law Microscale (Visco-)plasticity coupled with isotropic damage μe ij=1+ν E σμ ij 1-D-ν E σμ kk 1-Dδij σμ fμ =(˜ σμ -Xμ)eq -σ∞ f with˜ σμ ij= σμ ij 1-D μ, μe, μp ˙ μp ij=32 ˜ σμD ij -Xμ ij (˜ σμ - Xμ)eq ˙λ 1-D Xμ ˙ Xμ ij=23Cy˙ μp ij(1-D) D ˙ D= Yμ S s ˙pμ if pμ >pD anduptoDc with pD = pD σu-σ∞ f σμ max eq +σμmin eq 2 -σ∞ f m Yμ=1+ν 2E σμ + ij σμ + ij (1 - D)2 + h σμ - ij σμ - ij (1-hD)2 -ν 2E σμ kk 2 (1-D)2+h -σμ kk 2 (1 - hD)2 its size is comparable to the value of the mesocrack initiated (δ0)calculated using (1.252) in Sect. 1.6.3. All the material parameters at the mesoscale are identified with large plastic strain. Nevertheless, we advise adjusting s and m on a test where fracture occurs in quasi-brittle conditions.

64 1 Background on Continuum Damage Mechanics The numerical procedure to solve the set of equations is described in Sect. 2.3. Some approximations allow for closed-form solutions in particular cases described in Chaps. 6 and 7. 1.5.5.4 More Precise Identification of the Asymptotic Fatigue Limit (S. Calloch and C. Doudard 2003) In the two-scale damage model the asymptotic fatigue limit (σ∞ f )playsanim- portant role as the yield stress at the microlevel. A definition as the asymptote of the W¨ ohler curve is mathematically appealing but difficult to practice be- cause to reach points close to this limit, we may need experiments of months, years, centuries and more duration! Fortunately, there is an other way by evaluating the dissipation through an elevation of temperature in cyclic tests (M.P. Luong 1998, A. Galtier 2002). Damage (and fatigue in particular) is always related to plastic strain, at microlevel for high cycle fatigue. In cyclic tests, the corresponding dissipation σij ˙ p ij induces an elevation of temperature which can be measured if the tests are performed at a frequency large enough to compensate the heat lost by conduction. The ideal would be adiabatic tests. Then, if several successive increasing levels of periodic stresses are applied on one specimen and the stationary temperature T is recorded, σ∞ f corresponds to the level for which an elevation of temperature is just detected. Of course this value depends on the accuracy of the temperature measurement but, with thermocouples and some elementary precautions, an offset of 0.05◦C may be detected, thus providing a good accuracy for σ∞ f. Fig. 1.16. W¨ ohler curve of a dual phase steel and asymptotic fatigue limit detected by temperature elevation (S. Calloch and C. Doudard 2003) In the following example of dual-phase steel, the successive stress levels at 10 Hz are 25, 50, 75, 100, 105, 120, 125, 130, 135, 140, and 145 MPa for about 1000 cycles each.

1.6 Localization and Mesocrack Initiation 65 The graph of the elevation of temperature T -T0 as a function of the stress level in Fig. 1.16 allows us to consider the asymptotic fatigue limit σ∞ f =105 MPa when the engineering fatigue limit is σf = 130 MPa at NR =106 cycles. 1.6 Localization and Mesocrack Initiation The aim of this section is to give an answer to difficult questions concerning a mesocrack initiation: what is a crack initiation from a continuum mechanics point of view? What is the size and the direction of the crack initiated? A theoretical difficulty is encountered as continuum mechanics defines its scale of application as the scale of the Representative Volume Element, in which the mechanical fields are homogeneous and continuous, whereas the free surface creation of a crack is a geometrical, non-homogeneous process. 1.6.1 Critical Damage Criterion The simplest and most practical solution to model a crack initiation is to use the critical damage criterion which states that a mesocrack is initiated when the damage reaches a critical value Dc . • For isotropic damage, this occurs when D = Dc (see Sect. 1.4.1). • For anisotropic damage with principal damage components DI , I =1, 2, 3, this takes place when the maximum principal damage reaches Dc , i.e., when max DI = Dc as already stated in Sect. 1.4.3. The term Dc is considered as a material constant, which is not so easy to measure. For most materials, 0.2 ≤ Dc ≤ 0.5. 1.6.2 Strain Damage Localization Criterion One may consider the mesocrack initiation as the ultimate state of the strain localization process which occurs in softening materials. Due to severe load- ing, localization bands occur in which strain and damage are strongly local- ized and in which microcracks develop and then degenerate into a mesocrack (R. Billardon, I. Doghri, A. Benallal and G. Geymonat 1989). This is a realistic criterion for a mesocrack initiation in its physical defi- nition but it has two main drawbacks: 1. Such a criterion needs tough calculations and is difficult to use in finite element computations. 2. It is strongly dependent on the damage evolution law as well as the plastic or visco-plastic behavior of the materials, such as anisotropy, ratcheting, and non-proportional loading effects.

66 1 Background on Continuum Damage Mechanics Nevertheless, at least for the uniaxial tensile case, it allows for the theoret- ical calculation of the value of the critical damage Dc without any need for experiments. Two main approaches are available for the study of the instabilities related to the phenomenon of localization: the bifurcation approach which applies to time-independent constitutive laws; the perturbation approach which applies to both time-independent and time-dependent constitutive laws. The con- sideration of viscosity effects makes the solution of the mechanical problem unique in general but instabilities may still occur. 1.6.2.1 Bifurcation Approach of Localization (R. Hill 1962, J.R. Rice 1973, J.R. Rice and J.W. Rudnicki 1975) The bifurcation approach consists of the analysis of the loss of uniqueness in the rate mechanical problem. It is is written in terms of velocity field v, strain rate ˙ and stress rate ˙ σ. In the quasi-static case, ˙ σij,j+ ˙fi=0 in the structure, ˙ ij=1 2 (vi,j + vj,i) in the structure, ˙ σijNj = ˙ F given i on the given load boundary, vi = ˙U given i on the given displacement boundary, and ˙ σij = Lijkl ˙ ij in the structure, (1.206) with f as the body force, U given as the applied displacements, F given as the applied loads, and N as the outward normal of the boundary. The last equa- tion is the rate form of the time-independent constitutive laws. Its introduces the fourth order tensor tangent operator L which will be introduced later for elasto-plasticity coupled with damage (1.216). Let us consider a homogeneous infinite body with a known homogenous solution v(1) and let us assume that at a given loading time, a second possi- ble solution of the rate problem v(2) exists. Two bifurcation modes may be exhibited: 1. A harmonic eigenmode (j is the pure imaginary number j = √-1), [vi]=v(1) i -v(2) i = gi exp(jξnkxk) (1.207) which, if reported within the equilibrium, leads exactly to the loss of ellipticity of the equilibrium equations, ξ2 ( nL n)ij gj =0 and det( nL n)=0, (1.208) where ξ is an arbitrary wave number of mode g and ( nL n) is the acous- tic tensor related to the localization plane with a normal n:( nL n)ij = nkLikjl nl. 2. A bifurcation mode involving discontinuous velocity gradient.Ifthesub- scripts (1) and (2) stand now for the fields in each side of the discontinuity surface (or planar band) of normal n, the continuity of the normal stress

1.6 Localization and Mesocrack Initiation 67 and Maxwell compatibility equations read ˙ σ(1) ijnj=˙ σ(2) ij nj and v(1) i,j - v(2) i,j = ginj , (1.209) with ˙ σ(1) ij = L(1) ijkl v(1) k,l and ˙ σ(2) ij = L(2) ijkl v(2) k,l due to the usual symmetry Lijkl = Lijlk . One ends up with nL(1) n ij gj + nj L(1) ijkl - L(2) ijkl v(2) k,l =0. (1.210) The first case of continuous bifurcation corresponds to a material still plas- tifying (and damaging) on both sides of the discontinuity surface: L(1) ijkl = L(2) ijkl = Lijkl given by (1.216) and det ( nL n)=0. (1.211) The vector g is then the eigenvector associated with a vanishing eigenvalue of the acoustic tensor. If g is orthogonal to n, one gets a shear band. If g is parallel to n, an opening mode results instead. The second case of discontinuous bifurcation corresponds to a body still loaded with L(1) ijkl = Lijkl at one side of the planar band but unloaded in elasticity at the other side (L(2) ijkl= ˜ Eijkl). This leads to the condition det ( nL n)<0. The condition det ( nL n) ≤ 0isanecessary and sufficient condition for strain localization to occur in homogeneous, non-viscous bodies. 1.6.2.2 Critical Damage from the Bifurcation Analysis The tangent stiffness operators may be derived from the full sets of elasto- plasticity coupled with the damage constitutive equations of Sect. 1.5. No kinematic hardening and no unilateral effect are considered here in order to keep the calculation simple! The constitutive equations are written in a concise way, as in ˙ p ij =aij˙p with aij =32(Hik˜ σD klHlj)D (H˜ σDH)eq , (1.212) ˙ r=˙ pΔw i t hΔ = ˜ σeq H˜ σDH eq , (1.213) ˙ Dij=dij˙p with dij= YS s δij , isotropic damage, YS s |a|ij , anisotropic damage, (1.214)

68 1 Background on Continuum Damage Mechanics and where Hij =(1 - D)-1/2 ij for anisotropic damage and Hij = δij/√1 - D for isotropic damage. The accumulated plastic strain rate is determined by the consistency con- dition ˙f =0: ˙p= bij˙ ˜ σij R (r)Δ , with bij = 32 ˜ σD ij ˜ σeq . (1.215) For both isotropic and anisotropic damage models, Lijkl = ˜ Eijkl - 2G R Δ+2Gamnbmn ˜ Eijpq apqbkl + M-1 ijpq ∂˜ σpq ∂Drs drsbkl , (1.216) with ˜ Eijkl = M-1 ijpq Epqkl as the elastic effective tensor and Mijkl is given by (1.15). Readers can refer to Sect. 2.2.4 for details concerning the calcula- tion of the tangent operator. For isotropic damage, the strain localization condition, det ( nL n)=0, written for uniaxial tension leads to the expression of a critical damage which depends on the normal of the planar localization band, Dc( n)≈1-κ(θ) σ2 u 2ES s σu G, (1.217) with n =[cosθ, sin θ, 0]T and κ(θ)= 2-4ν+(5-4ν)sin2θcos2θ 3-6sin2θcos2θ+(1-2ν)(2sin2θ-cos2θ). (1.218) This allows for the determination of the normal to the localization plane: for ν =0.3, θ =42◦ . In fact, the ratio of the ultimate stress to the shear modulus (σu/G) remains very small for any material such that κ is of the order of magnitude of unity and Dc in tension is found to be close to 1. For anisotropic damage in pure tension, the result "a critical damage al- most equal to 1" is also obtained but in terms of hydrostatic effective damage: strain localization occurs when ηDHc ≈ 1orDHc ≈ 1/η, i.e., in tension when D1c =2D2c =2D3c ≈ 3 2η. (1.219) With η =3,thisgiv e sD1c ≈ 0.5. This value is in accordance with the critical damages often measured in experiments with poor accuracy due to the difficulty in defining the initiation of a mesocrack in practice! The stress at strain localization has a non-vanishing value, σ= 3σu 2 1-D1+ 1 1-D2 , (1.220) which is σR = σu/2forη = 3. In the absence of any measurements, Dc =0.5 is a good candidate for all applications.

1.6 Localization and Mesocrack Initiation 69 1.6.2.3 Perturbation Analysis -- Stability (A. Molinari 1985, A. Benallal 1988) To check the possibility of bifurcation toward solutions that are different from the homogeneous one, a way to proceed is to slightly perturb the reference solution ( v 0). If the evolution of the perturbed solution ( v= v0+δ v)remains close to v 0, one expects stability. If not, instability occurs. From a mathematical point of view, this practical approach applied to mechanical problems is fully similar to the study of the stability of a set of first order differential equations written as ∂U ∂t = G(U, μload) , (1.221) where G is in general a nonlinear differential operator, μload is a parameter (for example, representing the loading intensity), and U is the vector solution (for example, made of the velocity and all the necessary variables to describe the material behavior). Different perturbation and stability analyses are possible: • Study of the decay (or lack of decay) in the linearized perturbation δU : ∂ ∂t(U 0 + δU)=G0(U, μload)+ ∂G ∂U (U 0)δU (1.222) or ∂ ∂t(δU)=AδU A = ∂G ∂U(U0). (1.223) If one of the eigenvalues (λA) of the operator A has a positive real part, the perturbation δU will grow. • Study of the decay (or lack of decay) in a relative perturbation defined as Z= δU U0 , (1.224) and ∂Z ∂t = ∂G ∂U(U0)- 1 U0 ∂ ∂t U 0 Z, (1.225) with 1 as the identity operator. This set of differential equations leads to a different value for λA from that in the previous case. If the perturbations are sought in the form δU = U exp (λAt)a ndδZ = Z exp (λrelt), λrel compared to λA yields λrel=λA- 1 U0 ∂ ∂t U 0 (1.226) and the "relative" instability occurs when Re(λA) ≥ 1 U0 ∂ ∂t U 0 (1.227) instead of Re(λA) ≥ 0.

70 1 Background on Continuum Damage Mechanics The perturbation and stability analysis applies to rather complex problems such as elasto-plasticity or elasto-visco-plasticity coupled (or not coupled) with damage, quasi-static or dynamic loadings, temperature and heat con- duction, or any other diffusive phenomenon. 1.6.2.4 General Thermo-Mechanical Case (A. Benallal and V. Cano 1996) Let us consider the general case of structures made of generalized standard materials submitted to dynamic loadings. The thermodynamics description of such material behaviors is given in Sect. 1.2. It introduces the Helmholtz free energy potential, ρψ, written in terms of strains and internal variables VK (the damage D or D is one of those), a yield criterion f , and a dissipation potential F . The equilibrium equations are represented by σij,j +fi = ρ∂2ui ∂t2 , (1.228) with u as the displacement, f as the body force, and ρ as the density. The compatibility equations are of the form ij=1 2 (ui,j + uj,i) . (1.229) The energy conservation principle (first principle of thermodynamics) reads as -qi,i+ω=ρC ˙ T-AK ˙VK+T ∂AK ∂T ˙VK - ∂σij ∂T˙ ij , (1.230) with ω as the heat source, C = -T ∂2ψ ∂T2 as the heat capacity, and AK as the associated variables. The constitutive equations are the elasticity law σij=ρ∂ψ ∂ ij , state laws AK = -ρ ∂ψ ∂VK , evolution laws ˙VK=- ˙λ ∂F ∂AK , conduction law qi = -kT,i , (1.231) where k is the conductivity and ˙λ =˙ r is the Lagrange multiplier in addition to the boundary and initial conditions. In order to derive the differential operator G for the general thermo- mechanical problem, let us set

1.6 Localization and Mesocrack Initiation 71 U = ui vi T σij VK with vi=∂ui ∂t, (1.232) with a set of equations to be solved: ˙ ui=vi ˙ vi=1 ρ (σij,j + fi) ˙ T=k ρC T,kk+ T C ∂2ψ ∂ ij∂T vi,j - 1 C ∂ψ ∂VK -T ∂2ψ ∂VK∂T ˙VK + ω ρC ˙ σij=ρ ∂2ψ ∂ ij ∂T ˙ T+ρ ∂2ψ ∂ ij∂ kl vk,l + ρ ∂2ψ ∂ ij ∂VK ˙VK ˙VK=-˙ r∂F ∂AK (1.233) For an infinite homogeneous body we take the Fourier transform of this set of equations or, in an equivalent manner, seek the perturbed solution of the form U(x,t)=U 0(t)+ ˆ U(t)exp(jξnk xk)a n dˆ U = ˆ ui ˆ vi ˆ T ˆ σij ˆ VK , (1.234) where ξ acts as a wave number. We then linearize the previous differential equations, identify the differential operator A and solve for the solution as ˆ U = U exp(λAt), (1.235) where λA is the stability parameter to be determined (Re(λA) < 0 implies stability). We will then obtain a set of linear equations and after some sub- stitutions, we can formally express them as λAu p=v p, ρλ2 Au p =jξσpq nq , V K =jξCλ Kpqnq u p+Rλ KT , σ pq =jξLλ pqrsnsu r+Mλ pqT , ρC + kξ2 λA +ρCλ VK T =jξPλ pqnqu p, (1.236)

72 1 Background on Continuum Damage Mechanics where the 4 tensors Lλ ijkl, Cλ Kij, Mλ ij ,andP λ ij , the vector Rλ K ,andthescalar ρCλ VK introduced depend on the stability parameter λA but not the wave number ξ. They are temperature-dependent and are affected by viscosity and inertia. • The fourth order tensor Lλ ijkl generalizes the expression for the tangent operator Lijkl to viscous materials loaded in dynamics at constant tem- perature as the rate law ˙ σpq = Lpqrs ˙ rs = Lpqrs ˙ ur,s . (1.237) Coupled with the consideration of the perturbed fields, σpq=σ0 pq+σ pq exp (λAt)exp(jξnk xk) , ur=u0 r+u r exp (λAt)exp(jξnk xk) (1.238) lead to σ pq =jξLpqrs nsu r. (1.239) Note that Lλ ijkl is not a material property as it depends on λA . • The tensor Mλ ij stands for the thermal effect on stresses and M λ ijT rep- resents the perturbation of the thermal stress, • The tensor Cλ Kij and Rλ K represent the contributions in terms of internal variables due to the mechanical and the thermal loadings, respectively. • The heat capacity contribution (Cλ VK ) is due to the consideration of in- ternal variables to model the material behavior and P λ ij models the heat source due to the material deformation. Finally, we obtain a set of two equations of the two unknowns u andT ρλ 2 A δik +ξ2npLλ ipkq nq -jξMλ ip np -jξρPλ kq nq 1+ kξ2 ρC λA + Cλ VK C u k T = 0 (1.240) and the parameter λA is a solution of the polynomial equations, det ( nL n)=0, (1.241) Lijkl = ρλ2 Aδikδjl + ξ2 Lλ ijkl + Mλ ijPλ kl ρC + kξ2 λA +ρCλ VK . (1.242) When Re(λA) ≥ 0(o rRe(λA) ≥ 1 U0 ∂ ∂t U 0 ) the perturbation (or the relative perturbation) starts to grow. The adiabatic, isothermal, and static cases are limiting cases of this per- turbation analysis. They are solved by mathematically setting: • k = 0 for the adiabatic case • ρC →∞for the isothermal case

1.6 Localization and Mesocrack Initiation 73 • ρ = 0 for the quasi-static case except in the heat equation in which ρC is kept constant For elasto-visco-plastic materials (without damage), the parameter λA is bound and the question of when the localization process takes place has not been clearly answered. For constitutive equations coupled with dam- age, the strain damage localization criterion λA = λc = ∞ coincides with det( n˜ E n) = 0 (inertia effects neglected) and therefore with ηDH ≈ 1 as well. One ends up with η = 3 to the 3D strain-damage localization criterion trD≈1 (1.243) which corresponds in tension to D1c =2D2c =2D3c ≈ 1 2. (1.244) 1.6.2.5 Effects of Viscosity, Temperature, and Inertia Qualitatively, • Viscosity has a regularizing effect. • Heat conduction may have a destabilizing effect. The smaller the wave number is, the larger is the destabilization. • Dynamics has a stabilizing effect which is much more important for the large wave numbers than for the lower ones. Inertia effect may usually be neglected. 1.6.3 Size and Orientation of the Crack Initiated Based on the principles of Continuum Damage Mechanics, the size of the mesocrack is the size on which the constitutive equations operate, i.e., the size of the Representative Volume Element: infinitely small for a mathematician but something concrete for an engineer! If the question asked is whether or not a crack is initiated, the answer is given by information on the loading conditions for which the damage reaches its critical value. If the damage analysis must be followed by a fracture analysis based on an existing initial finite crack, its size and orientation has to be determined. One way is to consider that the mesocrack initiated by Continuum Dam- age Mechanics involving a dissipated energy φDp can also be described by a process of Fracture Mechanics involving the same amount of dissi- pated energy φF = φDp (J. Mazars 1984). This bridges the gap between damage mechanics and fracture mechanics at least in the sense of energy. Since δ0 is the linear size of the mesocrack, also the size of the RVE for this

74 1 Background on Continuum Damage Mechanics purpose, the energy φDp involved in the process of initiation by damage of a mesocrack is composed of two energies: • The energy dissipated in the damage process itself, including isotropic damage, φD=δ3 0 Dc 0 YdD. (1.245) Assuming saturated hardening and a triaxiality function of Rν =1asthe crack is often initiated at the surface where the state of stress is also often uniaxial, we have φD≈δ3 0σ2 u 2EDc . (1.246) • The energy dissipated in the associated plasticity process is φp=δ3 0 fracture 0 σij d p ij. (1.247) Assuming either proportional loading or uniaxial loading leads to φp=δ3 0 pR 0 σeq(p)dp, (1.248) where pR is the accumulated plastic strain at rupture (for which σeq ≈ σu and pR = pR in pure tension). Then φDp =φD+φp≈δ3 0 σ2 u 2EDc + σu pR . (1.249) The first term is preponderant for brittle materials as the second term is dominant for ductile materials. On the same RVE, the energy φF is evaluated through the concepts of classical fracture mechanics dealing with a crack area A0 = δ2 0 and a strain energy release rate G: φF = A0 0 GdA. (1.250) For simplicity, let us consider the upper bound on φF given by the maximum valu e Gc of G, the material toughness. This approximation is close to reality for brittle materials and is a step function of the R-curve for ductile materials. Then, φF ≈ Gcδ2 0. (1.251) Writing the energy balance φDp = φF gives the length δ0 which matches Continuum Damage Mechanics and fracture mechanics: δ0≈ Gc σ2 u 2E Dc + σu pR . (1.252)

1.6 Localization and Mesocrack Initiation 75 This formula gives values generally obtained by metallurgy or physics con- siderations, as shown below: • δ0 ≈ 0.1to0.2 mm for light alloys • δ0 ≈ 0.2to0.5 mm for steels • δ0≈0.1to1mmforceramics • δ0 ≈ 0.5to1mmforpolymers • δ0 ≈ 10 to 100 mm for concretes Concerning the orientation of the plane in which lies the initiated mesocrack, its normal n is the result of the localization analysis of Sect. 1.6.2, det( nL n)=0. (1.253) If no localization analysis has been performed, the anisotropic damage evo- lution gives the orientation of the mesocrack as the plane with normal n (in which lies the maximum value of the damage vector D n which corresponds to the maximum principal value of the damage (see Sect. 1.4.3)): n= n(max DI). (1.254) If only an isotropic damage analysis has been performed, we use the orienta- tion of the maximum principal stress, n= n(max σI). (1.255) To conclude, Table 1.8 gives the possible choices in modelling the damage threshold, critical damage, size, and orientation of the mesocrack initiated.

Ta b l e 1 . 8 . Conditions for initiation of damage and mesocrack Damage threshold Monotonic p = pD pD= p(σ=σu) loading Cyclic p=pD pD = pD σu-σ∞ f σmax eq + σmin eq 2 -σ∞ f m loading Numerical max ws = wD wD given by (1.116) prediction Critical damage Isotropic D = Dc Dc =1- σR σu damage Anisotropic max DI = Dc Dc =0.5 damage Numerical det( nL n)=0 ηDH≈1 prediction Direction of the crack plane Isotropic Max principal σ n damage Anisotropic Max principal D n damage Numerical Localization n prediction Size of the mesocrack Checking RV E A0(mm)2 ≈ (0.2)2 metals (1)2 polymers (100)2 concrete initiation Checking Equivalence with A0 = G2 c σ2 u 2E Dc + σu pR 2 propagation Fracture Mechanics

2 Numerical Analysis of Damage Damage is essentially a nonlinear phenomenon often coupled with (visco-) plasticity, also a nonlinear phenomenon. Therefore we can not expect sim- ple closed-form solutions of mesocrack initiation problems except for rough approximations of simple cases. For early design of mechanical components, the coupling of the strain behavior with the damage may be neglected and a post-processing of dam- age evolution is possible after a classical structure analysis (D. Hayhurst and F.A. Leckie 1974). This approach is the uncoupled analysis based on a reference (visco-)plastic computation. For localized (visco-)plasticity and damage, this reference computation can even be purely elastic with a local energetic correction (such as the Neuber method) to estimate the plastic strain. Fast! For accurate engineering applications and when the coupling between strains and damage is strong, (visco-)plasticity, damage, and possible cracks distributed over the whole structure deem a fully coupled analysis nec- essary. The constitutive equations need to be implemented within a finite element computer code and the numerical analysis encounters the classi- cal difficulties of convergence of linearized schemes. It needs special algo- rithms, much care, and large computer times (A. Benallal, R. Billardon and I. Doghri 1988). When the damage is localized on the mesoscale, there is the possibility to use the two-scale damage model of Chap. 1 in which damage occurs on a microscale only (J. Lemaitre and I. Doghri 1992). This locally coupled analysis mainly applies to high cycle fatigue (fatigue in the elastic range), eventually with initial plastic strain and damage. The analysis can be per- formed by post-processing an elastic computation for "elastic" fatigue or a (visco-)plastic computation if the process of creation of non-trivial initial conditions has been modelled. Another area that requires numerical analysis is the precise identifica- tion of the material parameters. Even if a fast, rough identification is

78 2 Numerical Analysis of Damage possible using simple methods, an adjustment or updating of the parameters from more complex tests or similar studies needs numerous iterations and robust optimization techniques based on sensitivity analyses. A table at the end of the chapter gives values of damage parameters for several materials. In order to make the expressions simpler, intrinsic notations are used in this chapter when describing the schemes for the numerical implementation of the constitutive equations. 2.1 Uncoupled Analysis Structure calculations performed with nonlinear material behavior become very costly in time very quickly. Their use is therefore difficult to perform for designs in which the geometry of the structure and the choice of the materials are the results of an optimization process. A fast way to evaluate the damage is by post-processing classical calcula- tions of elasticity or elasto-(visco-)plasticity in order to perform a posteriori time integration of the damage evolution law of Sect. 1.4 (see Fig. 2.1): D = t tD Y (t) S s ˙p(t)dt or D = t tD Y (t) S s|˙ p(t)|dt, (2.1) where tD is the time taken for damage initiation, corresponding to the damage threshold pD = tD 0 ˙p(t)dt (see Sect. 1.4.1). Fig. 2.1. Uncoupled approach to structural damage analysis The time histories of the plastic strain, the energy density release rate Y for isotropic damage, and the effective strain energy Y for anisotropic damage are the necessary inputs for the damage post-processing. They may

2.1 Uncoupled Analysis 79 come directly from an elasto-(visco-)plastic computation or indirectly from an elastic computation followed by an initial post-processing of (visco-)plasticity. Note that the material parameters depend on the temperature which may vary during the loading. In that case, their time dependencies have to be taken into account when integrating the damage law. The procedure for the uncoupled analysis of damage is then: • Perform a structure calculation to obtain the histories of Y or Y and p • Evaluate D or D by means of the time integration of Eq. (2.1) • Estimate the time or the load corresponding to the critical damage Dc • Define a safety margin on the most appropriate parameter: the plastic strain p, the number of cycles N ,thetim et, or the damage equivalent stress σ , through a safety factor Saf (larger than unity) in order to ensure p≤ pR SaforN≤NR Safort≤tR Saf or σ ≤ σ R Saf (2.2) as a safe non-failure design criterion. Most of the time, neglecting the coupling of the damage with the strain behavior yields an upper bound on these parameters. The integration of the damage rate equation (2.1) concerns any kind of loading: monotonic, cyclic, multi-level, random . . . Examples are given in the next chapters. 2.1.1 Uniaxial Loading , Let us first consider the 1D case of tension or tension-compression with a state of stress σ = σ 00 000 000 ,σ = σ(t) (2.3) and a state of plastic strain p = p 00 0- p 20 00- p 2 , p = p(t). (2.4) The accumulated plastic strain is then p = p(t)= t 0|˙ p(t)|dt, (2.5) the von Mises stress is σeq = |σ|, and the stress triaxiality has the value 1/3. The damage calculated by means of the isotropic model is D = t tD Y (t) S s|˙ p(t)|dt. (2.6)

80 2 Numerical Analysis of Damage For the anisotropic model, the same expression is obtained on D1 (the com- ponent in the loading direction) as for tension such that D = D1 100 01 20 001 2 (2.7) and then D1 = t tD Y (t) S s|˙ p|dt. (2.8) The expressions for the functions Y (t)o rY (t) depend on whether or not we consider the microdefects closure effect (quasi-unilateral conditions) through the value of the microdefects closure parameter h or ha of Sect. 1.2.4. 2.1.1.1 Damage without Microdefects Closure Effect For both isotropic and anisotropic damage models, the effective energy den- sity release rate functions have the same expression if written in terms of the uniaxial elastic strain e : Y=1 2 E 2 e(t)o rY=1 2 E 2 e(t). (2.9) From a reference elasto-(visco-)plastic computation, the knowledge of the time history of the elastic strain allows for the determination of Y (t)orY (t) and the damage, as follows: D = t tD E 2 e(t) 2S s|˙ p(t)|dt or D1 = t tD E 2 e(t) 2S s|˙ p(t)|dt. (2.10) Due to the uncoupled analysis where the stress and the strain are calcu- lated without the softening effect of damage, Y and Y written in terms of stresses are preferred as they give an upper bound on D. In order to keep the post-processing simple enough for design purposes, the preferable case of isotropic damage is considered for which Y= σ2(t) 2E(1-D)2 . (2.11) If the stress and plastic strain histories are known, we have D 0 (1-D)2sdD = t tD σ2(t) 2ES s |˙ p(t)|dt (2.12) or D =1- 1-(2s+1) t tD σ2(t) 2ES s |˙ p(t)|dt 1 2s+1 . (2.13)

2.1 Uncoupled Analysis 81 The anisotropic case is similar, with an effective triaxiality function ˜ Rν now that depends on the damage (Eq. (1.41) of Sect. 1.2.3). For uniaxial tension, it is a function of D1 alone because D2 = D3 = D1/2a ndDH = 2D1/3, leading to ˜ Rν(D1)= 23 (1+ν)+3(1-2ν) (1 - 2η 3D1) 2 1-D1+ 1 1- D1 2 -2 (2.14) and the evolution of the damage is obtained as an implicit function of D1, which is easy to solve by use of mathematics software: D1 0 ˜ R-s ν dD1 = t tD σ2(t) 2ES s |˙ p(t)|dt. (2.15) 2.1.1.2 Damage with Microdefects Closure Effect Considering the quasi-unilateral conditions is important when dealing with compressive loading and cyclic or fatigue applications as they lead to a dam- age rate that is much smaller in compression than in tension. The represen- tation of the mean stress effect in fatigue then follows. Microdefects closure material parameters h or ha are introduced within the expressions for the Y and Y functions. This makes the models more difficult for closed-form solutions. We advise using the approximation Y (σ, D,ha) ≈ Y (σ, D =0,h =0.2) if damage anisotropy needs to be taken into account. For the resolution with the exact Y function for anisotropic damage with microdefects closure effect, please refer to Sect. 2.1.2 on pro- portional loading. For the uniaxial tension-compression case, one has Y=1 2E σ 2 (1-D)2+h -σ 2 (1 - hD)2 , (2.16) which may be written in terms of elastic strain Y=E 2 e 2 + h - e 2 . (2.17) Then, D = t tD YS s |˙ p|dt with Y = Y+= σ2(t) 2E(1 - D)2 in tension, Y- =h σ2(t) 2E(1 - hD)2 in compression. (2.18)

82 2 Numerical Analysis of Damage 2.1.2 Proportional Loading , Uniaxial loading is a particular case of proportional loading for which the stress tensor at a given point M of a structure remains proportional to a time-independent tensor Σ such that σij(M, t)=σΣ(t)Σij(M) . (2.19) The main sufficient condition for a structure to be considered as proportion- ally loaded is when there is only one applied load or when all the loads vary proportionally to one parameter. With the normalization Σeq = 3 2ΣD ij ΣD ij = 1, the scalar σΣ is the signed von Mises stress and |σΣ| = σeq. In tension-compression, Σ = 100 000 000 , ΣD = 2 300 0-1 30 00- 1 3 , and σΣ = σ. (2.20) For elasto-(visco-)plasticity that is coupled (or not coupled) with isotropic damage, the plastic strain tensor remains proportional to the deviatoric part of Σ,asin p ij(M, t)= 32 pΣ(t)ΣD ij(M)a n dΣ D ij =Σij - 13 Σkkδij , (2.21) introducing the scalar signed equivalent plastic strain pΣ such as | pΣ| = 2 3 p ij p ij . Due to the 3/2 term in (2.21), the accumulated plastic strain has the same expression as for the uniaxial tensile case: ˙p=|˙ pΣ| or p = p(t)= t 0|˙ pΣ|dt. (2.22) The anisotropic damage case is more complex and the previous equation p ij=3 2 pΣΣD ij of proportional loading in terms of plastic strains may be seen as an approximation for the general anisotropic 3D case but it strictly applies for tension-compression and for shear. 2.1.2.1 Kinematic Hardening as an Additional Isotropic Hardening in Monotonic Proportional Loading For elasto-(visco-)plasticity with isotropic and kinematic hardenings R and X, one has σD ij = σΣΣD ij, p ij=3 2 pΣΣD ij and Xij = X(t)ΣD ij ,X eq = 32XijXij = |X|. (2.23)

2.1 Uncoupled Analysis 83 The yield criterion is f=(σD-X)eq-R-σy = (σΣ-X)ΣD eq-R-σy, (2.24) with (σΣ - X)ΣD eq = 3 2(σΣ -X)2ΣD ij ΣD ij =|σΣ -X|Σeq =|σΣ -X|. (2.25) In cases of increasing monotonic proportional loadings (σΣ > 0, X>0, X<σΣ) one ends up with f=|σΣ-X|-R-σy =σeq-(Xeq+R)-σy, (2.26) which shows that kinematic hardening may be considered in these cases as an additional isotropic hardening. This remark is consistent with the consideration of one hardening only (either kinematic or isotropic) for com- putations of structures undergoing monotonic loadings. 2.1.2.2 Damage Post-processing Without Microdefects Closure Effect For both isotropic and anisotropic damage, the effective elastic energy density functions have the same expression if written in terms of elastic strain e : Y=1 2Eijkl eij ekl or Y = 1 2 Eijkl eij ekl . (2.27) As for the uniaxial case, information on the time history of the elastic strains allows for the determination of Y (t)orY (t) and the damage. Expressions written in terms of stresses are preferred. For isotropic dam- age, Y= σ2 eqRν 2E(1-D)2 = σ2 ΣRν 2E(1-D)2 , (2.28) where the triaxiality function Rν only depends on the tensor Σ and has a constant value: Rν = 23(1 + ν)+13(1 - 2ν)(Σkk)2 = const . (2.29) The possibilities for the time integration of the damage evolution law are D = t tD Eijkl eij ekl 2S s|˙ pΣ|dt. (2.30) If the elastic and plastic strains are known or (the most conservative choice),

84 2 Numerical Analysis of Damage then D 0 (1-D)2sdD=Rs ν t tD σ2 eq 2ES s | ˙ pΣ|dt ⇔ D =1- 1 - (2s +1)Rs ν t tD σ2 eq(t) 2ES s|˙ pΣ(t)|dt 1 2s+1 . (2.31) If the von Mises stress σeq = |σΣ|, the stress triaxiality TX = σH σeq =ΣH = 13 Σkk and the accumulated plastic strain rate ˙p = | ˙ pΣ| are known, or D=Rs ν t tD σ2 eq 2ES s | ˙ pΣ|dt (2.32) as an approximation of the last formula. Thecaseofanisotropic damage is similar but is made more difficult for closed-form solutions because of the dependency of the triaxiality function on the damages D1, D2,andD3. Nevertheless, it may always be worked out by using Dij = 32|ΣD|ij t tD YS s|˙ pΣ|dt, (2.33) whereY=1 2 Eijkl eij ekl and |ΣD| denotes the absolute value of the deviatoric tensor ΣD in terms of principal components. 2.1.2.3 Damage Post-processing with Microdefects Closure Effect For the isotropic damage model, the only change in the damage law is the expression of Y , which now introduces the microdefects closure parameter h (1.49): Y=1+ν 2E σ + ij σ + ij (1-D)2 +h σ - ij σ - ij (1 - hD)2 - ν 2E σkk 2 (1-D)2+h -σkk 2 (1 - hD)2 , (2.34) with h ≈ 0.2formetals. By considering the definition σij = σΣ Σij of proportional loading and by neglecting the effects of the damage on Y ,onegets Y≈σ2 Σ(t)Rνh 2E, (2.35)

2.1 Uncoupled Analysis 85 if σΣ>0,R νh=R+ νh =(1+ν) Σ + ij Σ + ij + h Σ - ij Σ - ij - ν Σkk 2 + h -Σkk 2 = const , (2.36) if σΣ<0,R νh=R- νh =(1+ν) Σ - ij Σ - ij + h Σ + ij Σ + ij - ν -Σkk 2 + h Σkk 2 = const . (2.37) For the anisotropic damage model the microdefects closure parameter ha is introduced. It is different from h, with ha ≈ 0 in most cases (1.60). The effective elastic energy density is then Y=1+ν 2E tr HpσD +Hp 2 + 3(1 - 2ν) 2E σH 2 (1 - ηDH)2 (2.38) so that R+ νh =(1+ν) ΣD + ij ΣD + ij+1 3(1 - 2ν) Σkk 2 = const (2.39) R- νh =(1+ν) ΣD - ij ΣD - ij + 13(1 - 2ν) -Σkk 2 = const . (2.40) 2.1.3 Post-processing a (Visco-)Plastic Computation A classical elasto-(visco-)plastic computation without any damage gives the time histories of the von Mises stress σeq, the hydrostatic stress σH ,the stress triaxiality TX = σH/σeq, the elastic energy density 1 2 Eijkl eij ekl,the accumulated plastic strain rate ˙p, and the stored energy density ws .The s e quantities are used directly as inputs for the time integration of the damage evolution law, providing an estimation of the damage as a function of the time, the accumulated plastic strain, or the number of cycles for fatigue applications. To make the post-processing procedure fast, the time integration of the damage law may be performed only at the most loaded point location where the damage equivalent stress σ = σeqR1/2 ν has the largest value in the whole structure. Such a criterion takes the stress triaxiality effect into ac- count through the function Rν . In that case the hypothesis of a proportional loading may often be made, allowing for the use of the analytical expressions of Sects. 2.1.1 and 2.1.2. The post-processing procedure may also be automatically applied at each Gauss point of the structure. Then the most loaded point simply is the point where the damage is the largest. The advantage is that one obtains maps of the damage field, while the drawback is of course a longer computer time. If the loading is periodic, it is only necessary to run the elasto-(visco-) plastic computation up to the stabilized cycle (10 to 50) as the information collected for the time integration of the damage law will be sufficient. For large numbers of cycles, a "jump" in cycles procedure may be applied to avoid the calculation of too many cycles (see Sect. 2.1.5).

86 2 Numerical Analysis of Damage 2.1.4 Post-processing an Elastic Computation Often, the plasticity is localized so that the stresses and the strains of the entire structure may be first calculated in elasticity. This has many advan- tages including reduced computational time cost and the possibility to use the main linearity property to obtain the stress and strain fields for many other applied loadings. The results depend only on the Young's modulus and Poisson ratio. The (visco-)plastic quantities p, ws and the quantities strongly dependent on the (visco-)plastic behavior σeq, σH, Y ,orY need to be estimated from an initial post-processing procedure as those quantities are required for the time integration of the damage law. Examples of these caculations include the Neuber method or the Strain Energy Density (SED) method fully de- scribed in Sects. 3.2.4, 4.2.4 and 5.2.4. These methods are based on a local energy equivalence at the stress concentration points between an elastic and an elasto-plastic computation of the same structure with the same loading history. Applied as post-processors of an elastic computation, the Neuber and SED methods allow for the determination of the von Mises stress and the ac- cumulated plastic strain where plasticity is localized (small scale yielding). The damage post-processing is then carried out as described in Sects. 2.1.1 or 2.1.2, yielding closed-form expressions for the mesocrack initiation condi- tions with an explicit dependence on plasticity and damage material param- eters. The knowledge of the stress triaxiality TX is of first importance as it partly governs the damage growth through the triaxiality function: Rν = 23(1 + ν)+3(1- 2ν)T2 X, where TX=σH σeq . (2.41) It is not given by the Neuber or SED methods. Nevertheless some analytical results may be obtained for plane deformation problems: • Fo r a plane stress state, the points located along free edges are exposed to pure tension (or compression). The value of the triaxiality ratio is simply 1/3. • Fo r a plane strain state in elasticity, the triaxiality ratio evaluated at points located along free edges only depends on Poisson ratio, TX= 1+ν 3√1-ν+ν2, (2.42) where TX depends on neither the loading type nor its intensity. For ν =0, TX =1/3 for some composite materials. For ν =1/3, TX =0.5. For ν ≈ 0.5, TX =1/√3 ≈ 0.58 for rubber-like materials. • Fo r a plane strain state in (visco-)plasticity, the closed-form expres- sion of the stress triaxiality may be derived analytically for points located along free edges.

2.1 Uncoupled Analysis 87 In plasticity with linear hardening the yield function is f = σeq -Cyp- σy, where Cy is the plastic "tangent" modulus and Cy ≈ (σu - σy)/ pu .The boundary conditions (free edges of normal e1: σi1 = 0), the plane strain condition i3 = 0, and the elasto-plastic behavior considered altogether lead to ˙ 33 = ˙ σ33-ν˙ σ22 E + (2σ33 - σ22)˙ p 2σeq =0. (2.43) With the notations, χ=Cy(1-2ν) 2(Cy+E),u 0= 1 √1-ν+ν2, W= 2√3χ 3+4χ2 1 - 2χ 1-2ν , and ω= 2χ 1-2ν+ 2χ2 3+4χ2 1 - 2χ 1-2ν , (2.44) and without any assumption about the loading, the closed-form expression for the TX(p) law is then governed by the parametric representation TX(u)= u 2-16 4-3u2, p(u)= σy Cy 1 - 3u2 0 4 -χ·u0 1- 3u2 4 -χ·u ω · exp W· arcsin √3u 2 u u0 - σy Cy, (2.45) which may be seen as a law TX = TX(p)orasTX = TX(σeq): the triaxiality ratio on a free edge depends on the von Mises stress only. For Poisson ratios larger than 0.3, there is a slight difference between TX evaluated in elasticity and TX evaluated in plasticity: the triaxiality re- mains between 0.5 and 0.58 but its variation shows that the plane strain loadings are not truly proportional. As soon as elastic strains are negli- gible, TX reaches a saturation value TXsat. Table 2.1 gives the values of the triaxiality at saturation as a function of the ratio Cy/E for different Poisson ratios. For metals, it is TXsat =0.58. Ta b l e 2 . 1 . Triaxiality in plane strain condition Cy/E 10-6 0.1 0.25 0.5 TXsat(ν = 0) 0.58 0.56 0.54 0.50 TXsat(ν =0.3) 0.58 0.57 0.56 0.55 TXsat(ν =0.5) 0.58 0.58 0.58 0.58 If the hardening law is not linear, one has to fit a linear law in the plas- tic strain range under consideration and apply the parametric expres- sion (2.45) as well.

88 2 Numerical Analysis of Damage Consideration of the viscosity effects introduces the viscous stress σv func- tion of the loading rate. For strain rates at which the viscosity effects are important, the yield stress has to be replaced by σy +σv but the saturation value is independent of the loading rate. To conclude, TX =0.58 at a free edge point is a good value to consider in order to evaluate Rν and to achieve plane strain Neuber or SED method. • Fo r 3D cases, the hypothesis of a stress triaxiality in plasticity equal to the (known) stress triaxiality in elasticity can be made. This may be seen as a weak form of proportional loading. 2.1.5 Jump-in-Cycles Procedure in Fatigue (R. Billardon and I. Doghri 1988) For loadings that are periodic or periodic by blocks in fatigue, the step by step computation in time becomes prohibitive when the number of cycles becomes large (104,106,108, ...). Therefore a simplified method which allows the program to "jump" full blocks of ΔN cycles is necessary. The time integration is performed over one cycle once in a while and the computation time may be reduced by a factor of almost ΔN . This "jump"-in-cycles procedure is as follows: 1. Before any damage growth, i.e., up to ws = wD or p = pD,r u nthe computation until reaching a stabilized cycle Ns and let δp δN Ns be the accumulated plastic strain increment over this single cycle. Assume then that during the next ΔN cycles, p remains linear versus the number of cycles N and calculate the number of cycles to be advanced by ΔN cycles as ΔN= Δp δp δN Ns , (2.46) where Δp is a given value which determines the accuracy of the procedure and Δp ≈ pD/50 is a good compromise between accuracy and time cost. The accumulated plastic strain is updated as p(Ns + ΔN)=p(Ns)+Δp (2.47) and is equal to r(Ns + ΔN) as long as there is no damage. The stored energy density is updated as ws(Ns + ΔN)=ws(Ns)+ p(Ns+ΔN) p(Ns) A m R(p)p 1 m -1dp. (2.48) The stresses, strains, plastic strains, kinematic hardening at the end of the cycle Ns , the accumulated plastic strain p(Ns + ΔN), and the stored

2.1 Uncoupled Analysis 89 energy density ws(Ns + ΔN) are then the initial values for the computa- tion of the first time increment of the cycle (Ns + ΔN +1). Repeat the jumps until damage occurs. 2. Once damage occurs, first run the computation at constant damage until a new stabilized cycle Ns is reached. Then • Calculate the accumulated plastic strain increment δp δN Ns . • Calculate the damage increment δD δN Ns or δDH δN Ns over this cycle. • Assume again that during the next ΔN cycles, p and D (or DH) remain linear versus N and calculate the number of cycles to be ad- vanced as ΔN =min Δp δp δN Ns ,ΔD δD δN Ns , (2.49) where ΔD is a given value which determines the accuracy on the damage. Here again ΔD ≈ Dc/50 is a good compromise between accuracy and time cost and take Δp = S Ymax s ΔD with Ymax as the maximum value of functions Y or Y over the cycle Ns . The accumulated plastic strain and the damage are finally updated as p(Ns + ΔN)=p(Ns)+ δp δN Ns ΔN, r(Ns + ΔN)=r(Ns)+ δr δN Ns ΔN, D(Ns + ΔN)=D(Ns)+ δD δN Ns ΔN for isotropic damage, and Dij(Ns + ΔN)=Dij(Ns) 1+ 1 DH(Ns) δDH δN NsΔN for anisotropic damage, (2.50) and the stored energy density as ws(Ns + ΔN)=ws(Ns)+ r(Ns+ΔN) r(Ns) A m R(r)r 1 m -1dp. (2.51) The stresses, strains, plastic strains, kinematic hardening at the end of the cycle Ns , the accumulated plastic strain p(Ns + ΔN), the stored energy density ws(Ns + ΔN), and the damage D(Ns + ΔN)orD(Ns + ΔN)are then the initial values for the computation of the first time increment of the cycle (Ns + ΔN +1).

90 2 Numerical Analysis of Damage 2.2 Fully-Coupled Analysis For complex loadings, such as non-proportional or anisothermal, or for severe loadings leading to large scale yielding, the stress and damage states cannot be determined from an uncoupled analysis. Stress redistribution and stress triaxiality changes enhanced by the damage may be a major accelerating factor towards structural failure. It is then necessary to solve the continuum mechanics equilibrium equa- tions in a fully coupled manner with the elasto-(visco-)plasticity coupled with damage laws (see Fig. 2.2). This is in general a difficult task as the problem is strongly nonlinear and the computation of strain localization gives rise to non-unique, mesh-dependent solutions. Fig. 2.2. Fully coupled approach to structural damage analysis Based on both time and space discretizations, the finite element anal- ysis (FEA) is commonly used to solve complex engineering structure prob- lems. The FEA is briefly described here for nonlinear material behavior. The main part of this section concerns the description of the implicit numerical schemes used for the implementation of the damage models of Chap. 1 as subroutines of commercial finite element computer codes. Temperature-dependent loadings and behaviors are considered. As the in- fluence of the mechanical behavior on heat transfer remains small in many situations (be careful with contact problems and high speed dynamic ef- fects ...), one assumes that the history of the temperature field is deter- mined from an initial thermal computation. It affects the mechanical prob- lem through the temperature dependency of the material parameters and the thermal strain th = α(T - Tref)1. The schemes described remain the same whether or not the viscosity effect is taken into account. They allow

2.2 Fully-Coupled Analysis 91 us to represent the continuous transition plasticity/visco-plasticity due to temperature variation. One considers here the quasistatic case. The acceleration quantities and the inertia effect are not taken into account. 2.2.1 Nonlinear Material Behavior FEA (J.J. Moreau 1974, Q.S. Nguyen 1977, J.C. Simo and R.L. Taylor 1986) The finite element analysis uses a mesh of the considered structure in ac- cordance with both the computation option (2D, axisymmetric, 3D) and the degree of approximation for the elementary displacement field (linear or quadratic shape functions in general). The approximations for the displacement u(M)oneachelementVe have the general expression u ≈{u}={u(M)}=[N]{Ue}, (2.52) where shape functions Nij(M) are introduced. The vector {U e} represents the nodal unknowns (displacements) of an element; it is part of the nodal displacements vector {U} for the whole structure. For 2D problems with n-node elements, {U e} has 2n components and [N]isa2× (2n)m atrix . For 3D problems with n-node elements, {Ue} has 3n components and [N]is a3× (3n)matrix. The Voigt vectorial representation for the strain tensor { } and the stress tensor {σ} may be considered: { } = 11 22 33 √2 23 √2 31 √2 12 , {σ} = σ11 σ22 σ33 √2σ23 √2σ31 √2σ12 . (2.53) The strains are calculated from information on the displacements by use of classical differential operators [D]and[B], such that { } =[D]{u} =[B] {U e} and [B]=[D][N] . (2.54) The virtual work principle allows us to derive the global matricial form for the equilibrium equations, {RGE}≡ all elements Ve [B]T {σ} dV -{F } =0, (2.55) where the vector {F } accounts for the applied loading. This last equation also defines the global FE residual {RGE} which vanishes for the equilibrated solution.

92 2 Numerical Analysis of Damage The local nonlinear constitutive equations are often linearized and solved by use of iterative methods (Newton--Raphson or Quasi-Newton methods . . . or others). The consistent tangent operator Lc and its matricial representa- tion [Lc] are then defined as Lc=∂Δσ ∂Δ or [Lc]= ∂{Δ } ∂{Δσ} , (2.56) where {Δσ} is the stress increment obtained for the strain increment {Δ }. [Lc] will be used to build a FE tangent matrix (see next section), ensuring good convergence of the iterative scheme for the resolution of the global equilibrium (2.55). To sum up, the full mechanical problem is made of a global equation concerning the whole structure and two local equations: • The global equilibrium {RGE} =0, • The compatibility equation { } =[B] {U e}, • The constitutive equations considered at each Gauss (or integration) point. Of course the boundary conditions and the initial conditions are included as well.Due to the nonlinearity in material behavior and the loading dependency of the tangent operator, it is difficult to ensure both global equilibrium and local behavior simultaneously. An iterative process takes place which con- sists of each instant tn+1 in iterations made of a global equilibrium resolution, followed by local integrations (see Fig. 2.3): • The global FE resolution of the structure equilibrium is made with tan- gent operators [Lc(M)]. The initial value for [Lc] is the effective elasticity matrix [ ˜ E]. The solution obtained called "elastic predictor"isafir st estimate {U 1 n+1} for the nodal displacements vector at time tn+1 and for the strains { 1 n+1}. • The local time integrations of the nonlinear behavior equations called "plastic corrector" are performed in order to satisfy the state and the evolution laws ("local" means "performed at each Gauss point"). Practi- cally, this integration is made through the use of subroutines -- whose inputs are the first estimate for the strains { 1 n+1} and the values of the state and internal variables at time tn and -- whose outputs are the updated estimates for the state and internal variables at time tn+1, the updated value of the consistent tangent operator (if possible), or any good approximation. A global convergence criterion is checked at the end of the local time integra- tion of the constitutive equations, such as the absolute convergence, written in terms of residuals {RGE} < admitted error, or the relative convergence,

2.2 Fully-Coupled Analysis 93 Fig. 2.3. FEA algorithm for nonlinear constitutive equations

94 2 Numerical Analysis of Damage written in terms of relative residuals {ΔRGE} {F } < admitted error.Whensat- isfied, the estimate for {U q n+1}, for the state and internal variables, is kept as the FE solution at time tn+1 . If the convergence is not easily reached, the time step is reduced and the whole process is restarted with a smaller tn+1. The computation of the structure response at time tn+2 is made follow- ing the same procedure. The relative criterion is usually preferred because dimensionless but it is inapplicable when unloadings with {F } = 0 occur. 2.2.2 FE Resolution of the Global Equilibrium The global equilibrium equations at time tn+1 are RGE({Un+1})=0, (2.57) with {Un+1} as the FE solution (to be determined) of the mechanical problem at time tn+1. If this nonlinear equation is solved iteratively by use of the Newton method, solutions {U q+1 n+1} are calculated at each q-th global iteration such as RGE({U q n+1})+KT|q n+1 · {U q+1 n+1}-{U q n+1} =0. (2.58) The previous equation introduces the tangent stiffness matrix KT built from the knowledge at each point of the consistent tangent matrix [Lc]: KT|q n+1 = ∂RGE ∂{U} q n+1 = all elements Ve [B]T[Lc]q n+1[B]dVe . (2.59) Despite its expected rapid convergence, the Newton--Raphson process solving the global equilibrium equations can be expensive and inconvenient because its main disadvantage for non-associated plasticity coupled with dam- age models is that [Lc]a ndKT are not symmetric, so specific solvers are required. In fact, any approximations for [Lc]andKT may be used as these matrices only affect the convergence rate of the iterative process (Fig. 2.4). Modified Newton methods use, for instance, the tangent matrix calculated at the first iteration. It is even possible to use the elasticity matrix [E] or the effective elasticity matrix [ ˜ E] as a constant iterative matrix over a time increment. Quasi-Newton methods use a secant approximation KS of KT. Last, note that the arc-length methods (G.A. Wempner 1971, E. Riks 1972, 1979, M.A. Crisfield 1980) can converge when classical displacement control methods fail. Nevertheless, the capture of instabilities such as se- vere strain localization may demand specific enhanced arc-length algorithms (M.A. Crisfield 1996). In any case, most robust algorithms are available in the commercial FE computer codes. Do not hesitate to switch from one method to another when convergence difficulties are encountered!

2.2 Fully-Coupled Analysis 95 Fig. 2.4. Iterative process for nonlinear FEA To initiate the process, the resolution starts with a (thermo-)elastic com- putation (the elastic predictor)with[Lc]1 t=tn+1 =[˜ E]t=tn (the effective elasticity matrix) locally and gives {U 1 n+1} as the initial first estimate. The corresponding first estimate for the strain at time tn+1 needed for the local time integrations is { 1 n+1} = { n} + {Δ } and {Δ } =[B] {U 1 n+1}-{Un} . (2.60) After each q-th global resolution, a q-th local time integration (the plastic corrector) gives the value of the tangent operator, [Lc]q n+1 ,an e wfir ste s - timate for the FE solution, {Un+1} = {U q+1 n+1},a nd{ n+1} = { q+1 n+1} is set with { q+1 n+1} = { n} + {Δ q} and {Δ q} =[B] {U q+1 n+1}-{Un} . (2.61) Remark on dynamics -- Taking dynamic effects into consideration does not change the numerical resolution of the mechanical problem by too much. From a the- oretical point of view a matrix Kdyn (built with the acceleration terms of dynamics equilibrium not explicited stated above) has to be added to the previous tangent matrix KT . As for the damage models of Chap. 1, the density remains constant and Kdyn does not depend on the damage behavior. From a practical point of view, the expression for Kdyn depends on the numerical scheme chosen for the time dis- cretization of the acceleration quantities and explicit algorithms may be needed for

96 2 Numerical Analysis of Damage the local integration of the constitutive laws. Such a work needs much care and is not described here. 2.2.3 Local Integration Subroutines After each resolution of the global structure equilibrium, the value of the stress {σn+1}, the thermodynamics internal variables, the accumulated plas- tic strain, the stored energy, and the value of [Lc] are updated. This is made by performing the local time integration of the constitutive laws of Sect. 1.5 at the structure's Gauss points for which f>0 (a negative yield criterion f<0 corresponds to an elastic state and does not need any correction). The inputs for the local integration subroutine are the values at current time tn+1 of the strain tensor n+1 (represented by the previous { n+1}), the thermodynamics variables σn , n , e n, p n, rn,Rn, αn, Xn,Dn,orDn at time tn , as well as the values of the accumulated plastic strain pn and the stored energy wsn . The calculation of p is not strictly necessary as it is replaced by the variable r, but is useful for comparisons with measures and fitting of experimental data. Recall that, as long as there is no damage, the equality r = p stands and the damage threshold p = pD is equivalent to r = pD. The outputs are the same variables as above but calculated at time tn+1 and the updated consistent tangent operator (previous matrix [Lc] or any good approximation for [Lc]). If the damage model does not exist in the chosen FE code, it has to be implemented as a subroutine (such as ABAQUS UMAT FORTRAN subrou- tines) written in the adequate language of programming. The corresponding implicit algorithms are fully described in Sects. 2.2.4 and 2.2.5. Due to the strong nonlinearity of the behavior and the possible occurrence of instabilities, implicit schemes are preferred. During the same computation, they allow switching between plasticity models at low temperature to visco- plasticity models at higher temperature (and reciprocally) as the Norton parameters vary with T . For high-temperature, visco-plastic damage computations, explicit schemes (very sensitive to the time step) may be used with shorter com- putation times if the value of Dc is not too large (≤ 0.3). The algorithms for the time integration of the constitutive equations are simpler: the values at time tn+1 of the accumulated plastic strain and the state variables are calculated from the explicit discretization of a nonlinear system of first or- der differential equations (use of Runge--Kutta schemes, for example). This makes the computation of structures undergoing visco-plasticity/plasticity transition more difficult. Plasticity is then numerically recovered by setting N →∞ and the numerical convergence is difficult. Finally, do not use explicit schemes for states of damage close to the occurrence of strain localization as instabilities are expected.

2.2 Fully-Coupled Analysis 97 2.2.4 Single Implicit Algorithm for Damage Models (R. Desmorat and J. Besson 2001) The damage models of Tables 1.3 and 1.5, Sect. 1.5, use the effective stress for damage coupling with both elasticity and plasticity. This feature allows for the use of the existing schemes developed for elasto-(visco-) plasticity (A. Benallal, R. Billardon and I. Doghri 1988). The algorithm described here applies to anisothermal computations, the temperature maps being determined for each time increment by a previ- ous heat transfer computation. In order to make the presentation as well as the programming synthetic, both isotropic and anisotropic damage vari- ables are represented by the second order tensors D and H =(1 - D)- 1 2. Isotropy represents the limiting case where D = D 1, H = 1/√1 - D,and η =1. The evolution laws for the internal variables are derived from the nor- mality rule applied to the potential F = f + FX + FD,whe ref is the yield criterion, FX stands for the nonlinearity of the kinematic hardening and FD stands for the damage evolution. Remember that f =(˜ σ-X)eq-R-σy, and FX=3γ 4CX:X, (2.62) with (.)eq = 3 2 (.)D :(.)D the von Mises norm. We will define the normals as nX=∂F ∂˜ σ=-∂f ∂X=3 2 ˜ σD-X (˜ σD - X)eq , n=∂F ∂σ = HnXH D , m= -∂F ∂X=nX-γα. (2.63) The evolution laws for the plastic strain and the kinematic hardening then become ˙ p = ˙λ∂F ∂σ =˙ rnand˙ α=- ˙λ ∂F ∂X =˙ rm (2.64) and the accumulated plastic strain rate is ˙p= 23n:n ˙ r, (2.65) which reads ˙p =˙ r/(1 - D) for isotropic damage. With the state laws ˜ σ =E:[ e -α(T-Tref)1]a n dX = 23Cα (2.66)

98 2 Numerical Analysis of Damage and with the definition of H, the normals nX, n,andm may be expressed at given T as functions of e , α,andD only: nX = nX( e, α), n = n( e,α,D), m = m( e, α). (2.67) A set of 4 nonlinear equations of the 4 independent variables W = { e , α,r,D} then has to be solved in a coupled manner, as follows: ˙ -˙ e- ˙ rn =0, ˙ α-˙ rm =0, f-σv =(˜ σ-X)eq-R-σy-σv =0, ˙ D - YS s ˙p 1 = 0 isotropic damage, ˙ D - YS s |n|˙ r = 0 anisotropic damage, (2.68) where |n| means the absolute value of n in terms of principal components and where • R=R(r) • σv= KN˙p1 N = KN 2 3n:n˙ r 1 N Norton law K∞ 1 - exp - 1 n 2 3n:n˙ r exponential law • Y ( e)=Y ( e)= 1 2E: e: e For the sake of relative simplicity, the dilatancy terms are dropped out next. Keeping them does not yield any particular difficulties. 2.2.4.1 Discretization by the θ-method The previous set of nonlinear equations is discretized in time by considering the resolution variables at the intermediate time, tn+θ = tn + θΔt,withθ as the numerical parameter of the so-called θ-method. • The value 0 ≤ θ ≤ 1 is used for the 3 differential equations. • In plasticity, it is of first importance to ensure the validity of the yield cri- terion at each computation time tk .Thev alueθ = 1 (Euler fully implicit scheme) is set for the nonlinear equation fn+1 = 0 and the incremental form of the plasticity loading/unloading conditions is Δr ≥ 0, fn+1 ≤ 0, and Δrfn+1 =0. Any value 0 <θ≤ 1 can be used in visco-plasticity.

2.2 Fully-Coupled Analysis 99 In plasticity coupled with damage, the local residual is then defined as {Rloc} = {R e , Rα ,Rr ,,RD}T , {Rloc} = R e =Δ e -Δ +Δr nn+θ, Rα =Δα-Δr mn+θ, Rr = fn+1 =(˜ σn+1 - Xn+1)eq - R(rn+1) - σy , RD= ΔD - Y ( e n+θ) S s Δr 1 - Dn+θ 1 , for isotropic damage, ΔD - Y ( e n+θ) S s|nn+θ| Δr, for anisotropic damage, (2.69) where for any of the 4 variables e , α, r,andD, the subscript n + θ means "variable at time tn + θΔt": Wn+θ = Wn + θΔW , i.e., e n+θ= e n+θΔ e , αn+θ=αn+θΔα, (2.70) rn+θ =rn+θΔr, Dn+θ =Dn+θΔD, and for any function g of those variables, gn+θ = g e n+θ, αn+θ ,rn+θ , Dn+θ . (2.71) In visco-plasticity coupled with damage, the residual Rr is changed to Rv r, Rv r =Δr- Δt 2 3 nn+θ : nn+θ fn+θ KN N . (2.72) Performing the time integration of the constitutive law consists of reaching the local convergence {Rloc} < admitted error at a given strain { } = { n+1} or = n+1 by correcting the variables e , α, r and D.TheNewton iterative scheme may be used again and one has then to solve {R q loc n+1} + ∂{Rloc} ∂ΔW q n+1 · Wq +1 n+1 -Wq n+1 =0, (2.73) where the expression for the jacobian matrix [∂{R}/∂ΔW]q n+1 (or any good approximation) of the partial derivative of each discretized equation with re- spect to each variable increment ΔW = {Δ e , Δα, Δr, ΔD} is needed for convergence reasons. The convergence of the Newton scheme for the local

100 2 Numerical Analysis of Damage integration is not guaranteed in general. For the damage models under con- sideration, the convergence is enhanced by using Amarthe derivatives derived in next subsection and 3D computations have proven the method efficient. At convergence, Δ e =Δ e q +1,Δα =Δαq +1,Δr =Δrq +1,andΔD = ΔDq +1 is set and e n+1= e n+Δ e, αn+1 =αn+Δα, rn+1 = rn +Δr, Dn+1 =Dn+ΔD. (2.74) 2.2.4.2 Closed-form expression of the Jacobian matrix The derivatives of {R} taken with respect to ΔW define the Jacobian matrix as [Jac] = ∂{R} ∂ΔW . For any function g one has ∂g ∂ΔW=∂g ∂W:∂W ∂ΔW=θ∂g ∂W (2.75) and all the necessary ∂ ∂ΔW terms are given thereafter. First, let us consider e , α, r,andD as independent variables such that ∂nX ∂˜ σ=-∂nX ∂X= 1 (˜ σ-X)eq 32I-1 21⊗1-nX⊗nX , ∂nX ∂r =0, and ∂nX ∂D =0, (2.76) where (˜ σ-X)eq = E: e -23Cα eq . To calculate the derivatives of n, a fourth order tensor Q is defined such thatn=(HnXH)D =Q:nX and Q=H⊗H-131⊗H2, (2.77) where the special tensorial product H⊗H applied on the symmetric second order tensor H stands for (H ⊗H)ijkl = Hik Hjl, leading to ∂n ∂˜ σ=-∂n ∂X =Q:∂nX ∂˜ σ ∂n ∂r =0. (2.78)

2.2 Fully-Coupled Analysis 101 Ta b l e 2 . 2 . Jacobian terms for isotropic and anisotropic damage models Derivatives of R e with respect to ΔW ∂R e ∂Δ e =I+θΔrQn+θ : ∂nX ∂˜ σ n+θ :E ∂R e ∂Δα = 23CθΔrQn+θ : ∂nX ∂X n+θ ∂R e ∂Δr = nn+θ ∂R e ∂ΔD=θΔr ∂n ∂D n+θ Derivatives of Rα with respect to ΔW ∂Rα ∂Δ e = -θΔr ∂nX ∂˜ σ n+θ :E ∂Rα ∂Δα =(1+γθΔr) I - 23 CθΔr ∂nX ∂X n+θ ∂Rα ∂Δr = -mn+θ ∂Rα ∂ΔD = -θΔr ∂nX ∂D n+θ Derivatives of Rr with respect to ΔW (take θ = 1 for the plastic case) ∂Rr ∂Δ e =θnX n+θ:E ∂Rr ∂Δα = -23CθnX n+θ ∂Rr ∂Δr = -θR (rn+θ) ∂Rr ∂ΔD =0 Derivatives of RD with respect to ΔW Isotropic damage Anisotropic damage ∂RD ∂Δ e = - sθYs-1 n+θ Δr Ss(1-Dn+θ)1⊗E: e n+θ ∂RD ∂Δα =0 ∂RD ∂Δr = - Yn+θ S s 1 1-Dn+θ1 ∂RD ∂ΔD = I - Yn+θ S s × θΔr (1-Dn+θ)2131⊗1 ∂RD ∂Δ e ≈-sθY s-1 n+θ Δr Ss |nn+θ|⊗E : e n+θ ∂RD ∂Δα ≈0 ∂RD ∂Δr = - Y n+θ S s |nn+θ| ∂RD ∂ΔD≈I

102 2 Numerical Analysis of Damage The differentiation of the property H 2(1 - D)=(1 - D)H2 = 1 allows for the calculation of the derivatives of H 2 and H with respect to D: ∂H2 ∂D =H2⊗H2, ∂H ∂D =A-1 : H2⊗H2 , (2.79) where A is the fourth order tensor A = H⊗1 + 1⊗H or its symmetric part already introduced in Chap. 1 (Eq. (1.38) of Sect. 1.2.3). The expression for ∂n ∂D is finally derived from the knowledge of ∂(HnXH) ∂H = 1⊗ HnX + HnX ⊗1 (2.80) as ∂n ∂D = ∂(HnXH) ∂H :∂H ∂D-1 31⊗nX : H2⊗H2 . (2.81) Table 2.2 gives an abstract of all the Jacobian terms for plasticity coupled with damage. When the viscosity effects are taken into account, one needs the terms ∂Rv r ΔW at time tn+θ .ForΔr, we consider the Norton law (2.72) here so that ∂Rv r ∂Δr =1- NΔtfN-1 n+θ KN N ∂Rr ∂Δr . (2.82) Fo r Δ Wi =Δ e , Δα, ΔD,wehave ∂Rv r ∂ΔWi = - NΔtfN-1 n+θ KN N 2 3 nn+θ : nn+θ ∂ΔRr ∂ΔWi - ΔtfN n+θ KN N 2 3θ nn+θ 2 3 nn+θ : nn+θ :∂n ∂Wi n+θ . (2.83) 2.2.4.3 Updating the Thermodynamics Variables Once e n+1, αn+1, rn+1 ,andDn+1 are known, the remaining thermodynamics variables are updated explicitly: • Effective stress tensor ˜ σn+1=E: e n+1 • Plastic strain tensor p n+1= n+1- e n+1 • Strain hardening variables Rn+1 = R(rn+1), Xn+1 = 2 3Cαn+1 • Accumulated plastic strain pn+1 = pn + 2 3 nn+θ : nn+θ Δr equivalent to pn+1 = pn +Δr/(1 - Dn+θ) for isotropic damage

2.2 Fully-Coupled Analysis 103 • Stored energy (Be careful for the integration: the correction term z(r)= A m r(1-m)/m of Sect. 1.4.1 is singular in r =0) ws n+1 = AR(rn+1)r1/m n+1+13Cαn+1:αn+1- ˆ ωn+1 , ˆ ωn+1 =ˆ ωn+A 2 R (rn)r1/m n + R (rn+1)r1/m n+1 Δr, with R (r)=bR∞ exp(-br) for exponential isotropic hardening. • Damage H n+1 =(1 - Dn+1)- 1 2,Yn+1=Yn+1=1 2E: e n+1: e n+1 • Stress tensor σn+1 = M -1 n+1:˜ σn+1 = σD n+1 +˜ σH n+11 (see Eq. (2.91)), also written as σD n+1 = H-1 n+1 ˜ σn+1H-1 n+1 -(1-Dn+1):˜ σn+1 3(1-DH n+1) (1 -Dn+1), σH n+1 =(1- ηDH n+1)˜ σHn+1. (2.84) Note that for isotropic damage, the last equation simply recovers σn+1 =(1- Dn+1) ˜ σn+1. 2.2.4.4 Consistent Tangent Operator (J.C. Simo and R.L. Taylor 1985, J. Besson 1999) One of the advantages of the implicit integration by Newton methods is the direct calculation of the consistent tangent operator Lc or its matrix representation [Lc]. Let us break down the residual {Rloc} into 2 parts, {Rloc} = {Ri}-{Re} and {Re} = Δ 000 (2.85) where {Ri} corresponds to the contribution due to the internal variables and {Re} to the contribution due to the applied loading. Once the convergence is reached, we perform a perturbation of (2.85), δ{Rloc} = δ{Ri}-δ{Re} = {0}. With the definition of the Jacobian matrix, we have δ{Ri} =[Jac]δΔW . (2.86) One has then δΔ e δΔα δΔr δΔD =[Jac]-1 δΔ 000 , (2.87)

104 2 Numerical Analysis of Damage which shows that the first column of the inverse of the Jacobian matrix at convergence is the vector [Jac]-1 e , e [Jac]-1 α, e [Jac]-1 r, e [Jac]-1 D, e = ∂Δ e ∂Δ ∂Δα ∂Δ ∂Δr ∂Δ ∂ΔD ∂Δ (2.88) whose value at time tn+θ is calculated within Newton iterative resolution. The tensorial definition of the effective stress ˜ σ=M:σwith M=H⊗H-13 H2⊗1+1⊗H2 +19 trH2 1⊗1+ 1 3(1-ηDH)1⊗1 (2.89) gives back ˜ σ = HσDH D+ σH 1-ηDH1, (2.90) and may be inverted in σ=M-1:˜ σ=H-1˜ σH-1-(1-D):˜ σ 3(1 - DH) (1 - D)+(1- ηDH)˜ σH1 , (2.91) with H -1 =(1 - D)1/2 and M-1 =H-1⊗H-1-(1-D)⊗(1-D) 3(1-DH) +13(1-ηDH)1⊗1. (2.92) Then, δΔσ=M-1:δΔ˜ σ+˜ σ:∂M-1 ∂D :δΔD (2.93) and finally with δΔ˜ σ=E:δΔ e =E:[Jac]-1 e, e :δΔ δΔD =[Jac]-1 D, e :δΔ , (2.94) the expression for the consistent tangent operator is: Lc = M-1 : E :[Jac]-1 e, e+˜ σ:∂M-1 ∂D :[Jac]-1 D, e . (2.95)

2.2 Fully-Coupled Analysis 105 2.2.5 Damage Models with Microdefects Closure Effect (R. Desmorat and J. Besson 2001) For the damage models with the microdefects closure effect (consideration of the material parameters h or ha of Chap. 1), the effective stress defined in elasticity by ˜ σ=E:[ e - α(T - Tref)1] is not used for the coupling with plasticity. For the isotropic damage model, ˜ σ is given by Eq. (1.48) of Sect. 1.2.4 but now f=(s-X)eq-R-σy with s= σD 1-D = ˜ σD , (2.96) where (.)eq = 3 2 (.)D :(.)D is the von Mises norm. For the anisotropic dam- age model ˜ σ is given by (1.57) and f =(s-X)eq -R-σy with s =(1-D)-1/2σD(1-D)-1/2 = ˜ σD . (2.97) Again, isotropic and anisotropic damage may be represented by the single second order tensor D, with isotropy being the limiting case D = D1. As the yield criterion remains unchanged, the normals nX, n and m have the same expressions as for the case without the microdefects closure effect: nX=32 sD-X (s-X)eq , n = (1 - D)-1/2nX(1 - D)-1/2 D , m=nX-γα, (2.98) and can be considered as functions of α, D and σ only. A set of 5 nonlinear equations function of the 5 independent variables { e , α,r,D, σ} has to be solved in a coupled manner: ˙ -˙ e- ˙ rn =0, ˙ α-˙ rm =0, f-σv =(s-X)eq-R-σy-σv =0, ˙ D - YS s ˙p 1 = 0 for isotropic damage, ˙ D - YS s|n|˙ r = 0 for anisotropic damage, e-E-1:˜ σ-α(T-Tref)1=0, (2.99)

106 2 Numerical Analysis of Damage with •˜ σ astheeffectivestresssuchastheelasticitylaw.Forisotropicdamage, e-1+ν E σ + 1-D+ σ - 1-hD +ν E tr σ 1-D- -trσ 1 - hD 1-α(T -Tref)1 =0 (2.100) and for anisotropic damage, e-1+ν E (HpσD +Hp)D +(HnσD -Hn)D -1-2ν E σH 1-ηDH - -σH 1 - ηhaDH 1 - α(T - Tref)1 =0, (2.101) with Hp =(1 - D)-1/2 and Hn =(1 - haD)-1/2. • X = 23Cα, R = R(r)for hardening. • σv=KN˙p1 N or σv =K∞ 1-exp - ˙p n for the viscosity law. • Y =Y(D,σ), Y =Y(D,σ). For isotropic damage, Y=1+ν 2E σ + : σ + (1-D)2 +h σ - : σ - (1-hD)2 -ν 2E tr σ 2 (1-D)2+h -tr σ 2 (1 - hD)2 (2.102) and for anisotropic damage, Y=1+ν 2E tr HpσD +Hp 2 + ha HnσD -Hn 2 +3(1-2ν) 2E σH 2 (1 - ηDH)2 + ha -σH 2 (1 - ηhaDH)2 . (2.103) Still for the sake of relative simplicity, the dilatancy terms are dropped out next. 2.2.5.1 Discretization by the θ-method The previous set of nonlinear equations is discretized by use of the θ-method (with θ = 1 for the yield criterion). This defines the local residual for plasticity coupled with damage as

2.2 Fully-Coupled Analysis 107 {Rloc} = R e =Δ e -Δ +Δr nn+θ, Rα =Δα-Δr mn+θ, Rr = fn+1 =(sn+1 - Xn+1)eq - R(rn+1) - σy , RD= ΔD - Yn+θ S s Δr 1 - Dn+θ 1 for isotropic damage, ΔD - Y n+θ S s |nn+θ| Δr for anisotropic damage, Rσ= e n+θ-E-1:˜ σn+θ (2.104) and the incremental form of the plasticity loading/unloading conditions still reads as Δr ≥ 0, fn+1 ≤ 0, and Δrfn+1 =0. The main difference with the case without the microdefects closure effect is that the relationship σ( e , D) is now implicit and given by the numerical inverting of the elasticty law. For visco-plasticity coupled with damage, we consider the Norton law for the residual Rv r defined by (2.72) instead of Rr . 2.2.5.2 Jacobian Matrix The Newton iterative scheme is used again here and the derivatives of the residuals with respect to the increments Δ e ,Δα,Δr,ΔD,a ndΔσ are needed. First, we have ∂nX ∂s = -∂nX ∂X= 1 (s - X)eq 3 2I-1 21⊗1-nX⊗nX , ∂nX ∂ e =0, ∂nX ∂r =0, ∂nX ∂α = 23C∂nX ∂X, ∂nX ∂D=∂nX ∂s :∂s ∂D, ∂nX ∂σ =∂nX ∂s :∂s ∂σ, (2.105) with ∂s ∂D = ∂HpσDHp ∂Hp : ∂Hp ∂D ∂s ∂σ =Hp⊗Hp-13Hp2⊗1, (2.106)

108 2 Numerical Analysis of Damage where ∂HpσDHp ∂Hp and ∂Hp ∂D are defined by (2.79) with H changed into Hp and nX into σD. Again, we set up n =(HpnXHp)D = Q : nX with Q and ∂(Hp nXHp) ∂Hp obtained by replacing H by H p in (2.77) and (2.79). Then, we obtain ∂n ∂s=-∂n ∂X =Q:∂nX ∂s, ∂n ∂ e =0, ∂n ∂r =0, ∂n ∂α=2 3C ∂n ∂X =Q:∂nX ∂α, ∂n ∂D=Q:∂nX ∂D + ∂(Hp nXHp) ∂Hp : ∂Hp ∂D - 13 1 ⊗ nX : Hp2⊗Hp2 , ∂n ∂σ =Q:∂nX ∂σ. (2.107) Finally, the derivatives of Y and Y are needed. For isotropic damage, closed-form expressions are obtained: ∂Y ∂D =1+ν E σ + : σ + (1-D)3 +h2 σ - : σ - (1-hD)3 1 -ν E tr σ 2 (1-D)3+h2 -trσ 2 (1 - hD)3 1 ∂Y ∂σ =1+ν E σ + (1-D)2+ h σ - (1 - hD)2 -ν E tr σ (1-D)2 - h -tr σ (1 - hD)2 1 . (2.108) For anisotropic damage, only the hydrostatic terms (those responsible for strain localization) can be obtained in a closed-form. For an estimation of the last Jacobian terms, let us consider the approximation Y≈1+ν 3E σ2 eq (1-DH)2+3(1-2ν) 2E σH 2 (1 - ηDH)2 + ha -σH 2 (1 - ηhaDH)2 , (2.109) which leads to ∂Y ∂D ≈ 2(1 + ν) 9E σ2 eq (1-DH)3+η(1-2ν) E σH 2 (1-ηDH)3+ h2 a -σH 2 (1 - ηhaDH)3 1 ∂Y ∂σ ≈1+ν E σD (1-DH)2+1-2ν E σH (1 - ηDH)2 - ha -σH (1 - ηhaDH)2 1 (2.110)

2.2 Fully-Coupled Analysis 109 Table 2.3 gives a summary of the Jacobian terms. For visco-plasticity, the derivatives for ∂Rv r ∂ΔW are still given by (2.82) and (2.83) as in the case without microdefects closure effects. Note that in last equation of Table 2.3, H is the Heaviside function, H(x)=1forx ≥ 0, H(x)=0forx<0. Ta b l e 2 . 3 . Jacobian terms for damage models with microdefects closure effect Derivatives of R e ∂R e ∂Δ e =I ∂R e ∂Δα = 23CθΔrQn+θ : ∂nX ∂X n+θ ∂R e ∂Δσ =θΔrQn+θ : ∂nX ∂σ n+θ ∂R e ∂Δr = nn+θ ∂R e ∂ΔD=θΔr ∂n ∂D n+θ Derivatives of Rα ∂Rα ∂Δ e =0 ∂Rα ∂Δα =(1+γθΔr) I - 23 CθΔr ∂nX ∂X n+θ ∂Rα ∂Δσ = -θΔr ∂nX ∂σ n+θ ∂Rα ∂Δr = -mn+θ ∂Rα ∂ΔD =0 Derivatives of Rr (take θ = 1 for the plastic case) ∂Rr ∂Δ e =0 ∂Rr ∂Δα = -23CθnX n+θ ∂Rr ∂Δσ =θnn+θ ∂Rr ∂Δr = -θR (rn+θ) ∂Rr ∂ΔD=θnX n+θ:∂s ∂D n+θ (continue next page) 2.2.5.3 Updating the Thermodynamics Variables Once e n+1 , αn+1, rn+1 , Dn+1,andσn+1 are known, the remaining thermo- dynamics variables are updated explicitly: • Plastic strain tensor: p n+1= n+1- e n+1

110 2 Numerical Analysis of Damage Table 2.3. (continued) Derivatives of RD Isotropic damage Anisotropic damage ∂RD ∂Δ e =0 ∂RD ∂Δα =0 ∂RD ∂Δr = - Yn+θ S s 1 1-Dn+θ1 ∂RD ∂ΔD = I - Yn+θ S s × θΔr (1-Dn+θ)2131⊗1 - sθY s-1 n+θ Δr Ss(1 - Dn+θ)1 ⊗ ∂Y ∂D n+θ ∂RD ∂Δσ ≈-sθY s-1 n+θ Δr Ss |nn+θ|⊗ ∂Y ∂σ n+θ ∂RD ∂Δ e ≈-sθY s-1 n+θ Δr Ss |nn+θ|⊗ ∂Y ∂ e n+θ ∂RD ∂Δα ≈0 ∂RD ∂Δr = - Y n+θ S s |nn+θ| ∂RD ∂ΔD≈I - sθY s-1 n+θ Δr Ss |nn+θ|⊗ ∂Y ∂D n+θ ∂RD ∂Δσ ≈-sθY s-1 n+θ Δr Ss |nn+θ|⊗ ∂Y ∂σ n+θ Derivatives of Rσ ∂Rσ ∂Δ e =θI ∂Rσ ∂Δr =0 ∂Rσ ∂Δα =0 ∂Rσ ∂ΔD ≈-θ(1 + ν) E I-131⊗1 : ∂s ∂D n+θ -ηθ(1-2ν) 3E σH n+θ (1 - ηDH n+θ)2 - ha -σH n+θ (1 - ηhaDH n+θ)2 1 ⊗ 1 ∂Rσ ∂Δσ ≈-θ(1 + ν) E I-131⊗1 : ∂s ∂σ n+θ -θ(1-2ν) 3E H(σH n+θ) 1-ηDHn+θ+ H(-σHn+θ) 1-ηhaDHn+θ 1⊗1 • Strain hardening variables: Rn+1 = R(rn+1), Xn+1 = 23 Cαn+1 • Accumulated plastic strain: pn+1 = pn + 2 3nn+θ : nn+θΔr • Stored energy:

2.2 Fully-Coupled Analysis 111 ws n+1 = AR(rn+1)r1/m n+1+13Cαn+1:αn+1- ˆ ωn+1 , ˆ ωn+1 =ˆ ωn+A 2 R (rn)r1/m n + R (rn+1)r1/m n+1 Δr, with R (r)=bR∞ exp(-br) for exponential isotropic hardening • Damage: Hp n+1 =(1 - Dn+1)- 1 2, Hn n+1 =(1 - haDn+1)- 1 2 and Yn+1 = Y (Dn+1, σn+1)o rY n+1 = Y (Dn+1, σn+1). 2.2.5.4 Consistent Tangent Operator The variables { e , α,r,D, σ} have been considered for the local integration of the constitutive equations. The consistent tangent operator is then a block of the Jacobian matrix at the convergence of the local Newton scheme as Δσ =[Jac]-1 σ, e Δ =⇒ Lc =[Jac]-1 σ, e . (2.111) 2.2.6 Performing FE Damage Computations Once the damage models are available as part of the FE code material li- brary, their use is identical to the use of elasto-(visco-)plasticity models. The material parameters need to be supplied in an input data file with eventually tables of the temperature dependency information. Users prefer the anisotropic damage model because it demands the same computation effort than the isotropic model but takes into account the in- duced anisotropy and gives good results for the strain-damage localization with a realistic mesh size. Recall that due to the strong nonlinearity encoun- tered, the computations are costly in time. When a whole structure is under consideration, we advise starting with a purely elasto-(visco-)plastic analysis before running the fully coupled computation (set for example, the dam- age threshold to a very large value) and performing an uncoupled analysis of damage as detailed in Sect. 2.1.3. Systematic comparisons between both uncoupled and coupled analysis are encouraged to build up the engineering experience. The outputs of a fully coupled damage analysis are the history of the nodal displacements and, at each Gauss point, the stresses, strains, and state and internal variables, particularly the damage field history. The damage maps identifies the structure's weak points. There is crack initiation when the damage reaches the critical value Dc . Different options are then possible • To stop the computation when strain-damage localization takes place. This is the most commonly used option as the FE solution is mesh- independent up to this point.

112 2 Numerical Analysis of Damage • To continue the continuum mechanics computation with a given mesh size in the zone of intense damage. The strain-damage localization pat- tern gives an idea of the further development of cracks. The FE solution is mesh-dependent and should only be used to compare different design solutions. • To continue the computation with a given mesh size and releasing nodes to model the crack initiation and propagation (see Table 1.8 of Sect. 1.6.3 for the orientation and the size of the initial mesocrack). This option needs the difficult operation of release of the adequate nodes to create a crack with the right size and orientation. The FE solution is still mesh- dependent; it has no absolute value but has again a relative value for the comparison of different design solutions. • To initiate and propagate mesocracks with sizes and orientations inde- pendent of the mesh nodes by use of enriched finite elements with em- bedded displacements discontinuities. New classes of efficient methods emerged recently: manifold method (G. Shi 1992) or more generally the partition-of-unity method (J.M. Melenk and I. Babuska 1996, N. Mo¨ es, J. Dolbow, and T. Belytschko 1999). But the extension to damage behav- ior with softening, strain localization and mesh dependency is still under study. 2.2.7 Localization Limiters When performing the FE analysis of a structure made of damageable ma- terials, the instabilities encountered are due to the numerical representation of the physical occurrence of shear bands where the initial fracture mechan- ics mesocrack will initiate. The good thing is that damage mechanics re- produces such a phenomenon. As we just pointed out, the drawback is the mesh dependency of the solution and the shear band thickness. This empha- sizes that there is missing information in the formulation. For an arbitrary small mesh size, the computed shear band may be much too thin, corre- sponding to a non-physical, unlimited, strain localization. Localization lim- iters are then necessary to introduce by a way or another a characteristic length. Initially proposed for the crack band model (S.T. Pietruszczak and Z. Mroz 1981, Z.P. Baˇ zant and B.H. Oh 1983), the simplest localization limiter is to set the mesh size to a constant value. Some authors propose considering the mesh size as a material parameter (and identifying it) in or- der to compute the crack propagation within damage mechanics framework (G. Rousselier 1987). The characteristic length introduced may be seen as the size of the RVE. But the "correct" mesh size for a good quality computation seems to be related to the shape, the size of the whole structure and to the loading!

2.2 Fully-Coupled Analysis 113 As 21st century localization limiters, a material internal length is intro- duced directly into the constitutive laws, the main idea being that plasticity and/or damage evolution at a structure point x depend on the value of the thermodynamics variables at the considered point as well as a small domain around it. One speaks then of non-local constitutive models. 2.2.7.1 Strongly-Non-local Theories (Z.P. Baˇ zant and G. Pijaudier-Cabot 1987) Each local thermodynamics variable V (or some of them) may be replaced by an "average" V nl of the variable around the considered point. The delo- calization of V is described by Vnl=1 Vr V W(x - s)V(s)dV and Vr = V W(x - s)dV, (2.112) where W (x - s) is a generalized weight function and V is the structure volume. The non-local weight function is a new parameter of the model, chosen as the Gauss distribution function for instance: W (x)=W0 exp - x 2 2δ2 c (2.113) or the polynomial bell-shaped function with finite support (Z.P. Baˇ zant and J. Oˇ zbolt 1990): W(x)=W 0 1 - x 2 δ 2 c 2 , (2.114) with W0 and W 0 as the normalization factors and δc , δ c as "the" internal lengths of the medium. To perform the variables delocalization makes the numerical implemen- tation of the constitutive equations difficult in classical FE computer codes. The local integration subroutines now need the value of the thermodynamics variables at many Gauss points, eventually located far outside the considered element. 2.2.7.2 Gradient Theories (E. Aifantis 1987) An alternative way that is easier to implement is to consider gradient theories for which plasticity and/or damage evolution at a structure point depend on the value of the thermodynamics variables as well as their first, second, . . . n-th gradients. Replace then each local variable V by the expansion Vnl =V+c1· V+c2 2V+..., (2.115)

114 2 Numerical Analysis of Damage often with c2 as the only non-vanishing term (second gradient theories). It is also possible to define V nl as the implicit solution of Vnl-c1· Vnl-c2 2Vnl- ...=V, (2.116) where the "internal lengths" are introduced through the parameters ck . Note that the gradients theories are recovered by introducing the Taylor expansion V(x+s)=V(x)+ V·s+ 1 2! (2)V·(s ⊗ s)+... (2.117) in the average integrals of the non-local theories. Many non-local or gradient models may be constructed, depending then on the choice of the variables to be delocalized and the delocalization proce- dure (T. Belytschko 1988, Z.P. Baˇ zant and F.B. Lin 1988, R. de Borst and H.B. Mulhaus 1991, S. Forest and E. Lorentz 2004). They all introduce an internal length. We will present in the next section a simple way to make the damage models of Chap. 1 non-local. 2.2.7.3 Simple Non-local Damage Model One possible way to study damage models is to delocalize the damage variable and use Dnl=1 Vr V W (x - s)D(s)dV (2.118) instead of D in the constitutive equations. But from the remark of Sect. 1.6 that the strain localization is strongly related to the value of the parameter η, which defines an hydrostatic damage dH (fully acting when strain localization occurs) as dH=ηDH where ˜ σH= σH 1-dH , (2.119) the simplest is to make the previous relationship non-local and to calculate dH as dH=1 Vr V W (x - s)ηDH(s)dV, still with ˜ σH= σH 1-dH , (2.120) or to consider the gradient form dH - cD 2dH = ηDH,withcD as a material parameter. The last equation written either in an integral or a gradient form is the only change when compared to the local damage model. 2.3 Locally-Coupled Analysis In quasi-brittle failure and high-cycle fatigue applications, the damage is very localized in such a way that the damaged material occupies a small

2.3 Locally-Coupled Analysis 115 volume in comparison with the macroscale of the structural component and even with the mesoscale of the RVE. This is due to the high sensitivity of dam- age to stress concentrations at the mesoscale and defects at the microscale. According to the hypothesis of a weak, damageable inclusion embedded in a meso-RVE, such a state of localized damage is represented by the two-scale damage model of Sect. 1.5.5 (see also Fig. 2.5). Fig. 2.5. Locally-coupled approach to structural damage analysis By considering damage on the microscale only, the two-scale model pre- dicts crack initiation when the microdamage reaches the critical value Dc . The crack initiation condition D = Dc on the microscale coincides with the initiation of a mesocrack. The model is 3D and applies to complex loadings under isothermal conditions. It needs robust algorithms of resolution and an implicit scheme for its numerical implementation is described here. 2.3.1 Post-Processing a Reference Structure Calculation The damage is determined by post-processing a reference structure calcu- lation, performed in elasticity for quasi-brittle and high-cycle fatigue appli- cations and in elasto-plasticity for more ductile conditions. The reference

116 2 Numerical Analysis of Damage calculation provides information on the history of the stresses, strains, and plastic strains with no damage at the mesolevel of classical continuum me- chanics. Considered altogether with the Eshelby--Kr¨ oner localization law and isotropic elasticity, μ = +β( μp- p)a n dβ= 2 154-5ν 1-ν , (2.121) are inputs for the time integration of elasto-(visco-)plasticity fully coupled with damage constitutive equations on the microscale. The numerical scheme used to solve those equations is the one described in Sect. 2.2.4 for the local integration of the fully-coupled analysis with only slight differences: • For the fully-coupled damage analysis, the full calculation is performed by iterations made of global FE resolutions followed by local integrations at the structure Gauss points. Here, the time integration of the consti- tutive equations is performed only one time as a post-processor of the reference calculation. It may then be performed at the most loaded point only. • In nonlinear FE computations, the local time integrations are made at constant strain. Here, the localization law has to be considered and the calculation is made at constant ( μ - β μp). • The microscale constitutive equations are those of elasto-(visco-)plasticity coupled with damage, but with linear kinematic hardening and isotropic damage only. At points where f μ > 0, a set of 4 nonlinear differential equations is solved in the same manner as in Sect. 2.2.4 (μ-superscripts standing for "microscale" are added): ˙ μe +(1- β)˙ rμnμ- ˙ +β˙ p =0, ˙ αμ- ˙ rμ mμ =0, fμ-σμ v =(˜ σμ-Xμ)eq-σ∞ f -σμ v =0, ˙ D- Yμ S s ˙pμ=0 if pμ>pD, (2.122) where ˜ σμ = σμ/(1 - D) is the microscale effective stress, the yield stress σμ y is equal to the fatigue limit σ∞ f,σμ v , if needed, is given by a viscosity law and where (isothermal case) mμ=32 ˜ σμD-Xμ (˜ σμD - Xμ)eq , nμ= mμ 1-D, ˜ σμ= σμ 1-D=E: μe,

2.3 Locally-Coupled Analysis 117 Xμ = 23Cyαμ , Yμ=1+ν 2E σμ + : σμ + (1 - D)2 + h σμ - : σμ - (1-hD)2 -ν 2E tr σμ 2 (1 - D)2 + h -tr σμ 2 (1 - hD)2 . (2.123) 2.3.2 Implicit Scheme for the Two-Scale Model (I. Doghri and R. Billardon 1988) The reference computation gives the history of stresses, strains, and plastic strains on the mesoscale as discrete values at every instant t =0,...,tk ,...tn , tn+1,... With the microscale variables at time tn , the mesoscale variables at times tn ,a ndtn+1 being known, the microscale variables at time tn+1 are determined following a two step procedure: 1. A local elastic prediction, which assumes an elastic behavior with constant plastic strains μp = μp n , constant kinematic hardening Xμ = Xμ n , and constant damage D = Dn , gives a first estimate of the strains, elastic strains, and effective stresses on a microscale at time tn+1 : μ = +β μp n - p n+1 , μe = μ- μp n, ˜ σμ =E: μe =σ-2G(1-β) μp n - p n+1 . (2.124) 2. A local plastic correction of the state and internal variables μ, μe , and ˜ σ made at constant μ -β μp = -β p gives the strain μ n+1 , elastic strain μe n+1 , plastic strain μp n+1,stressσn+1, kinematic hardening X n+1, and damage Dn+1 at time tn+1. To detail the second step, consider that the elastic predictor has given ˜ σμ, μ,and μe as initial estimates of the stresses, strains and elastic strains. If the yield condition f μ ≤ 0 is satisfied, then ˜ σμ n+1= ˜ σμ, μ n+1 = μ,a nd μe n+1 = μe is set. If not, the Newton iterative process starts. For simplicity, the damage is assumed to remain constant over a time increment (in fatigue it may even be assumed constant over a whole cycle) and it is then the same as to integrate a law of elasto-plasticity with linear kinematic hardening only. The nonlinear equations to be solved in a coupled manner are (implicit Euler scheme is used) Δ μe +(1- β)Δrμ nμ n+1 -Δ +βΔ p =0, Δαμ-Δrμ mμ n+1 =0, fμ n+1 = ˜ σμ n+1-Xμ n+1 eq - σ∞ f. (2.125)

118 2 Numerical Analysis of Damage They may be solved straightforwardly by use of the Newton iterative scheme as in Sects. 2.2.4 and 2.2.5 for the fully-coupled analysis, but it is advan- tageous here to write them first in terms of the plastic strain pμ and the variable sμ = ˜ σμ - Xμ as a set of two equations, as follows: Rs=sμ n+1+2 3Gmμ n+1Δpμ - E : +2Gβ p +2G(1 - β) μp n +Xμ n =0, Rp =(sμ n+1)eq - σ∞ f =0, (2.126) where G =3G(1 - β)+Cy(1 - Dn), mμ = 3 2 sμD sμ eq , and the mesoscale strains = n+1and p= p n+1 are known from the initial FE analysis. For each iteration q of the Newton scheme, the solution sμ(q+1) and pμ(q+1), or in an equivalent manner, the "corrections" Cs = sμ(q+1) - sμ(q), Cp = pμ(q+1) - pμ(q) to be applied at each step to the previous iterated sμ(q) and pμ(q) are given by Rs+∂Rs ∂sμ :Cs+∂Rs ∂p Cp =0, Rp+∂Rp ∂sμ :Cs =0, (2.127) where Rs , Rp, and their partial derivatives are taken at time tn+1 and the iteration q. The starting solution sμ(0) = ˜ σμ-Xμ n andpμ(0)=pμ n corresponds to the elastic predictor (2.124). The set of equations (2.127) are then written as Rs + I + 2 3GΔpμ ∂mμ ∂sμ :Cs+2 3 GmμCp =0, Rp+mμ:Cs =0, (2.128) where I is the fourth order identity tensor and ∂mμ ∂sμ=1 sμ eq 32I - 1 21⊗1-mμ⊗mμ . (2.129) Sincemμ:mμ=32andmμ:∂mμ ∂sμ = 0, the system explicitly gives the corrections for pμ and sμ as Cp=Rp-mμ:Rs G Cs =23(mμ:Rs -Rp)m-Rssμ eq+2 3 GΔpμ(mμ : Rs)mμ sμ eq + GΔpμ . (2.130) For the solution to any system of equations, the procedure is then an implicit scheme with the advantage of an explicit one: the unknowns are updated explicitly by use of the closed-form formulae (2.130) for Cp and Cs . Once the convergence is reached, pμ n+1 = pμ(q+1) and sμ n+1 = sμ(q+1) is set and the remaining variables are updated as

2.3 Locally-Coupled Analysis 119 • Normalmμ:mμ=32 sμD n+1 σ∞ f • Plastic strain: μp n+1 = μp n + mμΔpμ • Kinematic hardening: Xμ n+1 = 23 Cy(1 - Dn) μp n+1 • Effective stress: ˜ σμ n+1=sμ n+1+Xμ n+1 • Elastic strain: μe n+1=E-1:˜ σμ n+1 • Damage: Dn+1 = Dn + Y μ n+1 S s Δpμ if p>pD,with Yμ n+1 = 1+ν 2E ˜ σμ n+1 + : ˜ σμ n+1 ++h 1-Dn 1-hDn 2 ˜ σμ n+1 - : ˜ σμ n+1 - -ν 2E tr ˜ σμ n+1 2+h 1-Dn 1-hDn 2 -tr ˜ σμ n+1 2 (2.131) • Stress tensor: σμ n+1 =(1- Dn+1)˜ σμ n+1 2.3.3 DAMAGE 2000 Post-processor The locally-coupled analysis of damage is made as a post-processing compu- tation of an initial elastic or elasto-(visco-)plastic analysis. For simple geome- tries and/or loading types (such as uniaxial or proportional), the most loaded point is simply determined as the point where the damage equivalent stress σ = σeqR1/2 ν is maximum (see also Sect. 2.1.3). It is sufficient to perform the post-processing at this single point to calculate the failure condition by the mesocrack initiation condition D = Dc . For complex geometries and/or loading types (such as non-proportional), the most loaded point may vary from one time increment to another or from one cycle (or block of cycles) to another. The calculation of the damage accumulation at the possibly weak points of the structure must be han- dled properly. This includes post-processing at all structure Gauss points and drawing damage maps. The result of the locally-coupled analysis will be the numerical prediction of a mesocrack initiation at the point where D = Dc is reached for the corresponding time tR or number of cycles NR to supture. The computer code DAMAGE 2000 allows us to solve the two-scale model constitutive equations on the basis of the numerical scheme of Sect. 2.3.2. The input data are the material parameters and the history of the strain components ij and p ij . The outputs are the evolutions of the damage D,the accumulated plastic strain pμ, and the microscale stress components σμ ij up to crack initiation. DAMAGE 2000 can handle any kind of proportional (or

120 2 Numerical Analysis of Damage non-proportional), monotonic or fatigue loading, fatigue periodic by block, or random fatigue. For the fatigue loadings, the jump-in-cycles procedure of Sect. 2.1.5 may be activated in order to save much computer time. Examples are given in Sects. 6.4.1 and 6.4.2. To finish, note that: • The caseβ=0a ndσ∞ f = σy corresponds to the single-scale damage post-processing with the uncoupled analysis of Sect. 2.1. • The case β = 0 corresponds to the use of the Lin--Taylor localization law (instead of the Elshelby--Kr¨ oner law). Coupled with the consideration of Cy =0,m =1,a nds = 1 it corresponds to the initial two-scale damage model described in the book A course on Damage Mechanics by J. Lemaitre, in which the FORTRAN 77 listing of the DAMAGE 90 post-processor is given. • The effect of free edges and free surfaces on mesocrack initiation in fa- tigue may be represented by considering an adequate localization law (see Sect. 6.4.6) programmed as a possible option of DAMAGE 2000. 2.4 Precise Identification of Material Parameters Contrary to linear elasticity for which the Young's modulus and Poisson ra- tio have almost the same value for each class of materials (steel, aluminum alloys, concrete ...), nonlinear behaviors introduce parameters whose val- ues strongly depend on the material. Due to the diversity of the engineer- ing materials and the strong influence of the microstructure on the failure properties, the material parameters need to be identified directly from spe- cific experiments despite the existence of handbooks of parameters. The ta- ble in Sect. 2.6 gives only the order of magnitude of parameters for some materials. This section deals with precise identification procedures. They require computer tools which at least allow for the calculation of the material re- sponse in uniaxial tension-compression under isothermal conditions. They are • Mathematical softwares that perform the time integration of the con- stitutive laws. • FE computer codes that may include numerical optimization proce- dures. • Specific identification by optimization softwares such as SIDOLO (P. Pilvin 1983). Three levels of tests are generally used: • Qualitative tests to choose the proper state variables to measure, to determine how they act, and to determine the couplings between the phenomena represented.

2.4 Precise Identification of Material Parameters 121 • Quantitative tests to identify the numerical values of the material pa- rameters for each material at each temperature considered. • Tests of validation to check the ability of the constitutive equations to represent more complex situations than those used for the parameters identification. This section completes the fast procedures of Sect. 1.4.4 used to obtain an approximate initial set of parameters to be improved. If anisothermal constitutive equations are considered, the identification procedure consists of identifying the material parameters at each temperature and considering by interpolation all the parameters as functions of the temperature. 2.4.1 Formulation of an Identification Problem Identifying the parameters of a model consists of finding the set of material parameters which gives the best representation of a maximum volume of experimental data and information on a given material. The data comes from • Simple laboratory tests as monotonic (with repeated unloadings) or cyclic tension and compression experiments, monotonic or cyclic shear experi- ments in torsion on tubes, as well as creep and relaxation experiments performed after either a monotonic loading or a cyclic loading. • More elaborate laboratory tests in the bending of beams, in bi-axial load- ing on cross-shaped specimens or in tri-axial loading on pseudo-cubic spec- imens. As the damage is not uniform over the whole geometry, such ex- periments need structure computations to determine the history of stress and strain on the RVE where the mesocrack is initiated. • Any failure of a component, provided the structure calculation is available. An inverse method is not advised at this level because the damage is always localized and has an effect that is too small on control global variables. It may be possible only if local and very accurate measurements are performed. • Any qualitative or quantitative information from the "state of the art" of experienced engineers and technicians! Note that as damage governs the mesocrack initiation, it is essential to run all the laboratory tests up to the point of failure. Never interrupt a test which runs too long. Increase the applied load or the applied strain range instead in order to break the specimen more quickly. The corresponding data may then be used to validate the identification. The database is then a finite set of load-displacement or stress-strain charts, or it could be a set of load, displacement, stress or strain versus time charts. The first thing to do is to extract as much information as possible from each test and to determine the history of all the state variables (plastic strain, accumulated plastic strain, hardenings, damage . . . ) or at least some

122 2 Numerical Analysis of Damage components of the internal variables. This operation defines for each exper- iment an array, Z exp(t), of the collected history at discrete times, ti ,ofthe variables. The identification problem consists of determining the material param- eters denoted formally as A = {E, ν, σy ...} which minimize the difference between the observations Z exp(t) and the numerical simulation of the model that is denoted as Z(t, A). From a classical mathematical point of view, a functional L(A) is introduced to measure the accumulated error between observations and simulations. The term L is the sum of functionals Lk for each test k such that L= kLk andLk= 1 N exp k i Zexp k (ti) -Zk(ti, A) 2 , (2.132) where N exp k is the number of experimental points considered for the k-th experiment. At this stage, one would expect the precise identification to end (L≈0) because such a formulation may be handled automatically by use of numer- ical minimization procedures such as the Simplex method (not described in this book), the Newton or Quasi-Newton methods, the Levenberg--Marquardt method, or the Sequential Quadratic Programming (SQP or Projected La- gragian Method), using evolution or genetic algorithms or combinations of different minimization procedures (e.g., the identification software SIDOLO or FE computer code optimizers). In fact, the question concerning the choice of the norm on the space of thermodynamics variables is somewhat subjective. It depends on the relative accuracy the experimental results and the domains of application in which a good accuracy is necessary. Note that a ponderation (weight) matrix P needs to be defined in order to make Zexp(t) -Z(t, A) dimensionless (P. Pilvin 1988): Zexp(t) -Z(t, A) 2 = {Zexp(t) -Z(t, A)}TP {Zexp(t) -Z(t, A)} . (2.133) One may refer to Sect 2.4.6 on "Sensitivity Analysis" of the following chapters as an aid to avoid an arbitrary choice of the ponderation coefficients. In order to avoid giving too much weight to the comparison times ti (for non-regular time discretization, for instance), the expression Lk= 1 T exp k Texp k Zexp k (t) -Zk(t, A) 2dt (2.134) may be used instead of (2.132) for some experiments or some part of ex- periments (with T exp k as the observation time of the k-th experiment). The integral is numerically calculated, for example by use of trapezes method. An example of precise identification is given in Sect. 2.4.3. Some numerical minimization procedures for least squares nonlinear prob- lems are described in next section. Due to the strong nonlinearity of the

2.4 Precise Identification of Material Parameters 123 identification problem, local minima may be obtained and as in general, the solution of the optimization problem is not unique. It is of first importance to have a starting solution A0 that is "not too far" from "the" solution. When the convergence fails or becomes slow, it is important to be able to switch automatically from one method to another. 2.4.2 Minimization Algorithm for Least Squares Problems The optimum set of material parameters Aopt minimizes the error L(A)that is mathematically called the objective function. The term L may generally be written as L(A)= 1 2 j r2j(A)=1 2 r(A) 2 , (2.135) where the residuals rj or their vector form r are defined according to (2.132) and (2.134). This is a least squares problem that is strongly nonlinear for the nonlinear constitutive equations considered and is non-convex that is with possibly several local minima. The mathematical tools to handle such a problem exist and are well de- scribed in the applied mathematics literature. For further details, readers can refer, for instance, to the book Numerical optimization by J. Nocedal and S.J. Wright (1999). There are two classes of procedures: • The unconstrained optimization procedures with no conditions (con- straints) on the material parameters. From this class the Newton method, Gauss--Newton method, BFGS method, and Levenberg--Marquardt method are described below. • The constrained optimization procedures with conditions (constraints) on the material parameters to force them to remain bound by some "reason- able" values: see for instance the SQP method described below. For the identification problems, it is often efficient to disregard the constraints and assume that they have no effect on the optimal solution, or to replace them by additional penalization terms in the objective function (use loga- rithmic penalization for inequality constraints). These terms have the effect of discouraging constraints violation. One can then use the unconstrained optimization procedures that are simpler to implement. For all the methods (except for the genetic algorithms), the gradient of the objective function is needed. For the least squares problem (2.135), we need L(A)=J T(A) r(A) ; (2.136) for some of them the Hessian is needed: 2L(A)=J(A)J T(A)+ j rj(A) 2 rj , (2.137)

124 2 Numerical Analysis of Damage where the Jacobian of r, J(A)= ∂rj ∂Ai , is introduced. Note that knowing the Jacobian allows us to compute the first part of the Hessian for free. Near convergence, the second term in (2.137) may be neglected and the approxi- mation 2L(A) ≈ J(A)J T(A) (2.138) may be used. 2.4.2.1 Generalities on Iterative Minimization Procedures The numerical minimization procedures for nonlinear problems are iterative. The solution at the iteration k is calculated as Ak+1 =Ak+ρkwk, (2.139) where wk is the search direction and ρk the step length. The expressions for the search direction depend on the method and wk is usually calculated first. The step length is initially taken to be equal to unity but one may optimize its value in order to get a substantial reduction, L(Ak) -L(Ak+1), of the objective function. The idea is to minimize at low cost L(Ak + ρwk)with respect to ρ and an iterative process may again take place. An efficient possibility for convergence reasons is to choose ρk which sat- isfy the Armijo--Wolfe condition L(Ak + ρk wk) ≤L(Ak)+c1ρk LT kwk, LT(Ak + ρk wk)wk ≥ c2 LT kwk, (2.140) with 0 <c1 <c2 < 1 as constants of the method. For the sake of simplicity the expression, L(Ak)= Lk , has been set up and we shall also denote rk= r(Ak)and 2L(Ak)= 2Lk .Withs u ch notations, equations (2.136) and (2.138) stand as Lk=JT k rk and 2Lk ≈ JkJT k. (2.141) 2.4.2.2 Newton Method The search direction is the solution of 2Lk wN k=-JT k rk (2.142) and ρN k =1. 2.4.2.3 Gauss--Newton Method The search direction is the solution of JkJT k wGN k =-JT k rk (2.143) where the approximation (2.138) of the Hessian is used. We then find a step length ρGN k which satisfies the Armijo--Wolfe condition (try ρGN k =1first).

2.4 Precise Identification of Material Parameters 125 2.4.2.4 Broyden--Fletcher--Golfarb--Shanno or BFGS Method The search direction is wBFGS k = -HkJT k rk, (2.144) with Hk the approximation of the inverse of the Hessian calculated iteratively, Hk+1 = I - skyT k yT k sk Hk I - yksT k yT k sk + sksT k yT k sk , (2.145) where sk = Ak+1 -Ak, yk = Lk+1 - Lk,a ndI is the identity matrix. Set the initial H0 to be equal or proportional to the identity matrix or set it to the inverse of an approximate Hessian 2L-1 at A = A0 (calculated, for example, by finite differences). The step length ρBFGS k is chosen to satisfy the Armijo--Wolfe condition. 2.4.2.5 Levenberg--Marquardt Method The Levenberg--Marquardt method is a robust, first order method especially meant for least squares optimization. The search direction is the solution of JkJT k + λkI wLM k=-JT k rk, (2.146) which corrects the possible rank deficiency of the Jacobian. The scalar λk may be interpreted as a Lagrange multiplier. Take ρLM k =1.Aslo nga sL(Ak + wk) ≥L(Ak), multiply the previous try for λk by a factor of 10 (λk ← 10λk). When L(Ak + wk) < L(Ak), take λk+1 = λk/10. 2.4.2.6 Sequential Quadratic Programming (SQP) The SQP method explicitly handles equality and inequality constraints. 2.4.2.6.1 Equality Constraints Minimization To set up the SQP framework, consider first the problem: min L(A) subject to gi(A)=0 where i =1,...m, (2.147) which allows us to define the Lagrangian as L(A,λ)=L-λTg. The minimization problem at the k-th iteration is written as the mini- mization of a quadratic problem under linear constraints: min w1 2wTWkw + LT kw subject to Ak w + gk =0, (2.148)

126 2 Numerical Analysis of Damage where Wk = 2AAL(Ak,λk), gk = g(Ak), and gi = gi(Ak), Ak = [ g1,..., gm]T .Thetermλk is the Lagrange multiplier vector of the k-th iteration. The solution set Ak+1 = Ak + wk and λk+1 = λk + wλ solves the Karush-- Kuhn--Tucker (KKT) system, Wk -AT k Ak 0 wk wλ = - Lk + AT kλk -gk , (2.149) which may also be written as Wk -AT k Ak 0 wk λk+1 = - Lk -gk . (2.150) 2.4.2.6.2 Inequality Constraints Minimization The nonlinear minimization problem, min L(A) subject to gi(A) ≥ 0w h e r ei =1,...m, (2.151) defines the linearized problem at the k-th iteration, min w1 2wTWkw + LT kw subject to Akw +gk ≥ 0, (2.152) which is solved iteratively. The method defines then the auxiliary equality constraints sub-problem: min xw 1 2xT wWkxw +[Wkw(r) + Lk]Txw subject to A(r) k xw =0, (2.153) wherexw =w-w(r)isset. The SQP method proceeds as follows: 1. Set C0 as the subset of the active constraints at A = A(0) = Ak (if gi is active gi(A)=0). 2. In order to find xw , solve the auxiliary KKT problem associated with (2.153) with the equality constraints gT i xw =0(i ∈Cr) rewritten as A(r) k xw =0: Wk -A(r) k T A(r) k 0 xw λ = -Wkw(r) - Lk -g(r) , (2.154) with g(r) as a vector with components gi(Ak), i ∈Cr . 3. a) If xw = 0, compute the auxiliary step length as ρr =min 1, min (i/∈Cr , gT i xw <0) - gT i w(r)+gi gT i xw (2.155)

2.4 Precise Identification of Material Parameters 127 and try for the new search direction w(r+1) = w(r) + ρrxw . (2.156) Take then first Cr+1 = Cr. If there are blocking constraints (i.e., con- straints i for which the minimum in (2.155) is achieved), update Cr+1 by adding one of these constraints to the subset of the active con- straints Cr+1. b) If xw = 0, the current value ˆ w of w(r) minimizes the objective func- tion over the current working set ˆ C = Cr . Compute the Lagrange multipliers that satisfy i∈ˆ C giˆλi=Wkˆ w+ Lk. (2.157) If all the ˆλi are positive, stop with the solution wk =ˆ w.Ifsomeˆλj are strictly negative, subtract the constraint j corresponding to the larger |ˆλj| from the subset of the active constraints ( ˆ C = Cr+1 ←Cr \{j}). 4. Take ρSQP =1andAk+1 = Ak + wk. Note that the calculation of Wk needs the calculation of the second deriva- tives of L. The method is then similar to a Newton scheme. Again, approx- imate expressions for 2L may be used, the most popular being the BFGS approximation of the Hessian. 2.4.3 Procedure for Numerical Identification Consider that the constitutive laws are available in a computer code which of- fers optimization facilities. The identification is then performed automatically by the minimization of the functional L(A) but some practical (convergence) difficulties may be encountered. As a guide to optimize the full identification process, a 5-step procedure may then be followed: 1. Choose the plasticity, visco-plasticity and damage models, bearing in mind the experimental data available and the considered application. For example considering both isotropic and kinematic hardenings is useless for a monotonic application, considering classical plasticity models (those described in this book) gives a poor accuracy in modelling the ratcheting effect. And it is no secret that for low cycle fatigue applications, the best choice is to perform the model identification on low-cycle fatigue tests. In general, the identification is better as the identification tests are close to the cases of the application! 2. Perform the fast identification procedure of Sect. 1.4.4 to determine an initial set of material parameters.

128 2 Numerical Analysis of Damage 3. Estimate qualitatively and quantitatively the sensitivity of the simu- lation to each parameter (see Sect. 2.4.6). This allows for a qualitative understanding of the model and a way to find out in which experiment or in which stage of the experiment each material parameter has a minor or major effect. 4. Build a chart of the experimental values of all the possible variables for discrete values of the time. The chart will compare the experimen- tal values with the numerical simulation in order to calculate the error Zexp k (ti) -Zk(ti , A) 2 or the integral T exp k Zexp k (t) -Zk(t, A) 2dt. 5. Use the set of initial parameters to perform the numerical minimiza- tion of the functional L. Some FE codes propose this option. For better convergence, proceed step by step and try to identify first the plastic- ity parameters, second the viscosity parameters, and last the damage parameters. In a last step, perform a numerical identification of all the parameters at the same time. Let us detail each point of this identification procedure on an example: 1. The whole set of operations is described here for the elasto-(visco-) plasticity coupled with the damage model of Table 1.3 for which the one-dimensional isothermal constitutive equations are recalled below for the Norton viscosity law: = e+ p e= σ E(1-D) f= σ 1-D-X -R-σy =σv ˙ p =sgn(σ - X)˙ p=sgn(σ-X) ˙ r 1-D R = R∞ (1 - exp(-br)) ˙ X=C(1-D)˙ p-γX˙ r withC=γX∞ ˙ D = YS s ˙p if p>pD, mesocrack initiation if D = Dc Y= σ2 2E(1 - D)2 ˙p = σv KN N = f KN N (2.158) 2. The initial set of material parameters is determined according to the fast identification procedures of Sects. 1.4.4 and 1.5.1. The precise identifi-

2.4 Precise Identification of Material Parameters 129 cation is performed for the steel alloy 2-1/4CrMoatate mpe r atu r eof 580◦C and from the following initial data: • Fatigue limit σ∞ f =60MPa • Yield stress σy02 =95MPa • Ultimate stress (at ˙ =10-3 s-1) σu = 187 MPa for an ultimate plastic strain pu =0.2 • Rupture stress (at ˙ =10-3 s-1) σR = 150 MPa for a rupture plastic strain pR =0.3 • A few tension-compression tests at very low strain rate ˙ =10-6 s-1 give for the yield thresholds σ+ s in tension and σ- s in compression: p =0,σ + s = σy =80MPa,σ - s = -80MPa, p =0.110-2 ,σ + s =87MPa,σ - s = -77MPa, p =0.410-2 ,σ + s =99MPa,σ - s = -69MPa, p =1.410-2 ,σ + s =105MPa,σ - s = -65MPa. (2.159) They are used for the determination of both kinematic and isotropic hardenings as the laws R = R∞[1 - exp(-b p)] and X = X∞[1 - exp(-γ p)] for monotonic tension fit the discrete values X = X( p)= σ+ s +σ- s 2 and R = R( p)=σ+ s -σy-X.(2.160) • A few creep tests at different constant values of stress give the sec- ondary plastic strain rate: σ=110MPa, ˙ p =10-6 s-1 , σ=120MPa, ˙ p =210-5 s-1 , σ=150MPa, ˙ p =210-4 s-1 . (2.161) They are used to identify the Norton parameters KN and N (with the hypothesis in of saturated hardenings) in ˙ p= σ-σy-R∞-X∞ KN N . (2.162) As the linear regression ln˙ p =Nln(σ-σy-R∞ -X∞)-lnKN N (2.163) fits the experimental points in (2.161) in the ln ˙ p vsln(σ-σy-R∞- X∞) diagram. • Furthermore, the thermo-elasticity parameters are known as -- Elasticity modulus E = 134000 MPa -- Poisson ratio ν =0.3

130 2 Numerical Analysis of Damage -- Dilatation coefficient α =1.3 · 10-5/◦C Finally, the fast identification leads to the following set (A0)ofmaterial parameters: • Thermo-elasticity: E = 134000MPa, ν =0.3, α =1.3 · 10-5/◦C • Yield stress: σy =80MPa • Isotropic hardening: R∞ =5MPa,b = 300 • Kinematic hardening: X∞ =20MPa,γ = 270 • Damage: S =0.113 MPa, s =5,Dc =0.2 • Damage threshold: pD =0.2, σu = 187 MPa at ˙ =10-3 s-1, σ∞ f= 60MPa,m=4 • Viscosity: KN = 1450 MPa s1/N , N =2.4 3. For this didactic example we assume that all the parameters have the same sensitivity. Each particular case is examined in the following chap- ters. 4. The experiments used to improve the set of initial parameters are those of Fig. 2.6: two low cycle fatigue tests up to rupture, a cyclic hardening curve, and a relaxation test. Fig. 2.6. Additional experiments for parameters identification of the 2-1/4 CrMo steel at 580◦C (J.-P. Sermage 1998)

2.4 Precise Identification of Material Parameters 131 The charts Z exp k of the state variables needed to apply a numerical opti- mization procedure are: • One file for each fatigue test σmax(N) curve with the following columns: Col. 1: The time tN corresponding to the maximum of the N -th cy- cle (T =2Δ / ˙ is the period of the loading). For the practical application, choose the points N = 100, 200, 300, 400, 500, 550, and 600 cycles for the curve at strain range Δ =1.210-2,a nd N = 100, 200, 300, 350, 400, and 425 cycles for Δ =210-2. Col. 2: The accumulated plastic strain at t = tN and p ≈ 2N Δ p. The plastic strain range Δ p is known either from the experiment or calculated as Δ p(tN )=Δ - 2σmax(N)/E(1 - D(N)). Col. 3: The damage D(tN )=D(N) calculated from the decrease of the maximum stress, D(N)=1- σmax(N)/σmax(N = 100). The corresponding charts (or arrays of data) are used for a point to point comparison (application of eq. (2.132)). • One file per strain range for the cyclic stress-strain curves of Fig. 2.6 at constant strain rate ˙ =10-3 s-1. Use enough points as these files are used for the integral comparison (2.132) over each stabilized cycle, the observation time for the cycle with strain range Δ k where T exp k =2Δ k/ ˙ . Place in columns: Col. 1: Time ti corresponding to the point i of the stress-strain sta- bilized cycle, Col. 2: Stress σ(ti), Col. 3: Strain (ti), Col. 4: Plastic strain (measured by fictitious unloadings) p(ti), Col. 5: Accumulated plastic strain p(ti)=pA + | p(ti) - A p | during plastic unloading, p(ti)=pB + p(ti) - B p during plastic loading with pA ≈ 2N Δ p and pB ≈ (2N +1)Δ p after a number of cycles N large enough to reach stabilization, Col. 6: Isotropic hardening R(ti), Col. 7: Kinematic hardening X(ti), Col. 8: Damage D(ti). • One two-column file σ(ti) for the relaxation test of Fig. 2.6. The last but not the least practical point concerns the choice of the pon- deration matrix P which allows us to make some experiments prepon- derant over some others but also to make some parameters more sensible than some other. Unfortunately, many choices are possible. As proposed by P. Pilvin (1988) take the ponderation matrices for each variable as the inverse of the square of the accuracy times identity, i.e., • For the stresses, Pσ = 1 (1 MPa)2 1 • For the strains or the plastic strains, P = 1 (10-5)2 1

132 2 Numerical Analysis of Damage • For the accumulated plastic strain (fatigue applications), Pp= 1 (10-4)2 1 • Forthedamage,PD= 1 (10-2)2 1 • Forthehardening,PR=PX= 1 (2 MPa)2 1 5. The numerical optimization is finally performed with SIDOLO optimizer by keeping unchanged the thermo-elasticity parameters E, ν , α,andthe damage threshold in pure tension pD. The final set of parameters for the 2-1/4 CrMo steel at 580◦Cisthen: • Thermo-elasticity: E = 134000 MPa, ν =0.3, α =1.3 · 10-5/◦C • Fatigue limit: σ∞ f =60MPa • Yield stress: σy =85MPainsteadof80 • Isotropic hardening: R∞ =30MPainsteadof5,b = 2 instead of 300 • Kinematic hardening: X∞ = 22 MPa instead of 20, γ = 250 instead of 270 • Damage: S =0.6 MPa instead of 0.113, s =2insteadof5,Dc =0.2 • Damage threshold: pD =0.2, σu = 200 MPa (at ˙ =10-3 s-1) instead of 187, σu = 137 MPa at ˙ ≈0,m=4, • Viscosity: KN = 1220 MPa s1/N instead of 1450, N =2.5 instead of 2.4, • If necessary, the parameters A and wD for the damage threshold are determined from the knowledge of the plastic strain range Δ p and the corresponding threshold pD by use of (1.114)--(1.116). The example has been derived for isotropic damage. If the anisotropic damage model is considered, apply the same procedure but change the D-columns to D1-columns. The damage measurement on the maximum stress for cyclic loading is: σmax(N)= 3σmax(N = 100) 2 1-D1+ 1 1-D1 2 -→ D1(N) . (2.164) 2.4.4 Cross Identification of Damage Evolution Laws For each application, different laws may model the damage evolution with either a phenomenological, thermodynamical, or micromechanical basis. One can consider: • Damage as a function of the energy density release rate, i.e., D = D(Y ) • Damage as a function of the accumulated plastic strain, i.e., D = D(p) • Damage as a function of the damage equivalent stress D = D(σ ), in which the von Mises stress and triaxiality apply

2.4 Precise Identification of Material Parameters 133 • Damage as a function of the accumulated plastic strain and the triaxiality Note that the previous laws D(Y )a ndD(σ ) do not apply to fatigue. The law D(p) may apply, but with different values of the damage parameters than for ductile failures!! The initial difficulty for the numerical analysis of a structure is then the choice of a damage law and its material parameters. Each set of parameters is related to the damage law considered and even if the different models are available in a FE code, it may not be a small task to switch from one to an other. A solution may then be: 1. To build a new data base by numerical simulation with the law for which the numerical values of the parameters are known 2. To apply the identification procedures of Sects. 1.4.4 and 2.4 on this new database in order to find the values of the parameters related to the new law used. An example of such a cross identification is given in Sect. 3.4.5 where the damage parameters pD, S, s,andDc are determined from the Gurson model parameters by a fastened procedure. 2.4.5 Validation Procedure Any (good!) model must be able to represent situations other than those used for the identification of the material parameters. Furthermore, it is essential to know its domains of validity for safety reasons. This is why it is important to check the model against special tests designed for the validation. It can be: • 2D or 3D state of stress measurements to check the criteria used • Non-proportional tests to check the validity of the anisotropy representa- tion • Complex history of stress to check the representation of the damage ac- cumulation • Non-isothermal tests to check the temperature dependence • Tests with gradient of stress to check the stress redistribution due to the coupling between damage and strain behaviors As an example, the elasto-(visco-)plasticity coupled with the damage model identified on the 2-1/4 CrMo steel at 580◦C in Sect. 2.4.3 has also been identified at room temperature, 300, 400, and 500◦C. From the results, two series of validation have been performed: 1. One-dimensional non-isothermal cyclic tests are described in Figs. 2.7 and 2.8. The history of strain (or stress) and temperature are given for both tests. They are introduced as inputs for the calculation of the stress (or strain) and damage for comparison with the experiments. The graphs

134 2 Numerical Analysis of Damage correspond to the first cycle. The relative difference of about 25% on the strain, stress or number of cycles to rupture is on the order of magnitude expected in this kind of prediction. Fig. 2.7. Thermal stress cyclic test on 2-1/4 Cr steel (J.-P. Sermage 1998). The solid line represents the calculation and the dots represent experimental results Fig. 2.8. Thermomechanical cyclic test on 2-1/4 Cr steel (J.-P. Sermage 1998). The solid line represents the calculation and the dots represent experimental results

2.4 Precise Identification of Material Parameters 135 2. Bidimensional non-isothermal cyclic tests up to crack initiation on Mal- tese cross-shaped specimens for which the numerical simulation are de- scribed in detail in Sect. 5.4.3 which is devoted to creep-fatigue damage. The difference between the number of cycles predicted and obtained by experiments is on the order of 25% to 100% depending on the method of calculation used. The final set of temperature-dependent material parameters is available in the Table 5.1 in Sect. 5.4.3. 2.4.6 Sensitivity Analysis The accuracy of a structure failure prediction depends very much on the accuracy of the material parameters, but not all of the parameters have the same effect on the model predictions concerning the strain-stress response and the rupture of a Representative Volume Element. The sensitivity of the calculated response to slight or main changes in each variable and material parameter value is of first importance at different stages of the mechanical analysis: • At the stage of parameters identification, one has to minimize the error (L(A)) between the numerical response of the model and the ex- perimental database with respect to the set of material parameters (A). The sensitivity of the functional L with respect to the material parame- ters is in fact the gradient ( ∂L ∂A ) or its numerical approximation ( ΔL ΔA). In general, it is necessary to efficiently apply the minimization procedures leading to the best set of parameters. The expression for ∂L ∂A is quite complex and is numerically and automatically derived within the identi- fication procedure. It is however a mathematical definition which has no clear mechanical meaning. It is difficult to properly handle the contribution to the functional L due to damage. Following the work of G. Amar and J. Dufailly (1993), it is thus preferable to define the sensitivity to the material parameters as the relative sensitivity of the engineering variable considered for each specific application to the relative changes of each material parameter A =[A1 , A2,...An] such as the plastic strain at failure pR, the stress to failure σR, the number of cycles to failure NR, or more generally the time- to-failure tR . A dimensionless sensitivity matrix may then be introduced, such as δpR pR δσR σR δNR NR δtR tR = SpR A1 SpR A2 ... SpR An SσR A1 SσR A2 ... SσR An SNR A1 SNR A2 ... SNR An StR A1 StR A2 ... StR An δA1 A1 δA2 A2 ... δAn An . (2.165) Each line of the sensitivity matrix corresponds to a given case: mono- tonic loading for SpR Ak or SσR Ak terms, fatigue loading for SNR Ak terms, more

136 2 Numerical Analysis of Damage complex loading for StR Ak terms. A few other lines may be added for ex- periments performed at different strain rates or at different temperatures, for example. • At the early stage of design of mechanical components,thechoice of the materials may not be definitive. A sensitivity analysis made on the failure properties may help for such a choice. Performed on the FE analysis of the components with real loading conditions, it will tell if it is better to -- Choose a material with better plasticity properties through the hard- ening parameters σy , R∞ , b, X∞ ,andγ -- Choose a material with better creep properties through the viscosity parameters KN , N . • At the stage of component manufacturing, the previous sensitivity matrix may tell if a change of material supplier will have minor or ma- jor consequences for the component design and if further complementary studies are necessary to ensure the safety conditions. Quantitative results of this method of sensitivity analysis are given for specific applications in the following chapters (see Sects. 3.2.3, 4.2.3, 5.2.3, 6.2.4, 7.2.5). Note finally that if the expressions of the material parameters are known as (smooth) functions of the temperature (Ak = Ak(T )) or the microstructure through a few parameters μ1 ,μ2 ..., the knowledge of the sensitivity matrix allows us to determine the sensitivity of the failure properties with respect to a change in temperature as ∂pR ∂T = k SpR Ak pR Ak dAk dT, ∂σR ∂T = k SσR Ak σR Ak dAk dT, ∂NR ∂T = k SNR Ak NR Ak dAk dT, ∂tR ∂T = k StR Ak tR Ak dAk dT, (2.166) or with respect to a change in microstructure as ∂pR ∂μi = k SpR Ak pR Ak dAk dμi , ∂σR ∂μi = k SσR Ak σR Ak dAk dμi , ∂NR ∂μi = k SNR Ak NR Ak dAk dμi , ∂tR ∂μi = k StR Ak tR Ak dAk dμi . (2.167)

2.5 Hierarchic Approach and Model Updating 137 In anticipation of the sensitivity analyses made in the following chapters for the accumulated plastic strain, stress, time, or number of cycles to rupture, we can make the following general conclusions: • The most important parameter is the loading for which a relative error on the stress δσ σ influences the relative error on the results by a factor S... σ of 5 to 10. If the loading is expressed in terms of strain,thefa ctorS... may be reduced to 1. • The material parameters which do not need a high degree of accuracy are the damage threshold in tension pD and the critical damage Dc because their sensitivity factor S... pD and S... Dc are only of the order of 0.5. • Due to the nonlinearities, all the sensitivity factors for the other param- eters are larger than 1 and of the order of 1 to 5. • Finally, if all the parameters are known with a relative accuracy of a few percent one may expect or fear (who knows?) an accuracy on the order of: -- ±20% on the accumulated plastic strain to rupture in ductile failures --0 .5to2× on the number of cycles to rupture in low cycle fatigue failures --0 .5to2× on the time-to-rupture in creep failures --0 .2to5× on the number of cycles to rupture in creep-fatigue failures --0 .1to10× on the number of cycles to rupture in high cycle fatigue fail- ures -- ±5% on the stress to rupture in brittle failures Large numbers indeed! This explains why the job of designers or engineers is still, at least partially, an art! 2.5 Hierarchic Approach and Model Updating , "It is always easy to make things complicated," tells a chinese proverb! This is particularly true when modelling materials and structures with computers which may give a multitude of useless output data. To understand well what can happen on a structure in service, we strongly advise beginning predictions with simple models and increasing the accuracy with more sophisticated models progressively. This is the hierarchic approach (D. Marquis 1990). It is developed at the end of each applications chapter but some general conclusions are: • σ = σu is a good rupture criterion to begin with • Isotropic hardening is sufficient for monotonic proportional loading • Kinematic hardening is necessary to represent cyclic loading • Linear kinematic hardening is often sufficient for damage purposes • The energy density release rate Y = constant in the damage law is a good approximation when the strain hardenings are large • The damage threshold pD = constant is a good approximation in ductile failures

138 2 Numerical Analysis of Damage • But it is necessary to take into account the variation of pD with the stress in low or high cycle fatigue • An elastic calculation followed by the Neuber correction is a good approx- imation in small scale yielding Updating a model consists of changing the model or the value of the material parameters each time new information is available. It can be • More information concerning the material as the choices in early designs progress • More accurate values of the damage parameters as a test program progress • New phenomena which may take place during validation tests on samples or structures • New in situ tests results on the structure itself to check if the real structure is made of exactly the same material as the one used for the laboratory identification tests • Aging in service • Injuries due to overloading or accident in service which may affect the state of strain hardening and damage governing the residual strength In order to be prepared for model updating of a structure in service, two important points to remember are: • Keep the initial calculations and the possibilities to change the inputs in proper archives. Unfortunately, it is not so simple over several decades with the change of computers and persons every few years! • The possibility to practice in situ tests: the microhardness test and the digital image correlation are good candidates! 2.6 Table of Material Damage Parameters To end this chapter, let us give sets of the numerical values of damage pa- rameters for some materials. You should take the numbers only as an order of magnitude because the name of a material does not fully identify all the properties. Be careful to always check the values using appropriate tests or information in each particular case. Fortunately, you are clever and you know that most often you only need qualitative results or relative values to compare different design solutions for which approximate results are sufficient.

2.6 Table of Material Damage Parameters 139 Material TEν σy σu σ∞ fCyS s Dc pDmhη ◦C GPa MPa MPa MPa MPa MPa SOLDUR 355 steel 20 230 0.3 375 474 3000 0.57 4 0.5 0.025 2.5 ha 1 2.8 0.43 ha0 Weldox 460 E steel 20 200 0.33 490 1 0.3 0 - Steel 2-1/4 CrMo 20 200 0.3 180 450 140 6000 2.8 2 0.20.1220.2- 580 134 0.3 85 137 60 0.6 2 0.2 0.2 4 0.2 AISI 316 20 200 0.3 260 700 180 7 1 0.15 0.1 0.2 - 600 140 0.32 6 3 0.2 1 0.5 0 0.5 - AISI 1010 20 190 0.28 320 700 200 2.4 1 0.2 0.44 0.2 - Refr. alloy IN 100 827 170 0.3 30 0.2 1 0.3 0.005 - Al alloy 2024 20 72 0.32 300 500 250 1.7 1 0.23 0.03 0.2 - Al alloy 6014 T7 20 70 0.33 240.6 275 1.22 2 0.36 0.05 - Copper 20 100 0.33 190 300 100 0.4 1 0.85 0.35 0.6 - Concrete 20 42 0.2 σ+ y2.1σ+ u4 Aa 0.99 κ0 3 σ- y7.4σ- u38 5 103 2.93 10-4 510-5 Al ceramic 20 400 0.2 306 500 300 6 1 0.99 0.1 0.2 - Carbon-epoxy E1 311 ν12 0.35 1760 1760 MPa1/2 ply composite 20 E2 6.35 ν13 0.35 τy 17 ST 1.96 0.5 0.99 YDT 0- E3 20 ν23 0.48 SS 2.55 YDS 0 SB rubber 20 2 10-3 0.5 1.16 5.6 5 0.2 0 -

3 Ductile Failures With this chapter, we begin our discussion of the applications of damage mechanics to specific structure failures classified by a phenomenon: here we are focusing on ductile failures which may occur in structures due to over- loading and also during metal forming. Ductile damage without any rup- ture may also be produced by forming or mechanical processes and may modify the mechanical properties which must be taken into account in the constitutive equations used to evaluate the further strength of structures in service. From the physical point of view, ductile damage is essentially atomic de- cohesions following dislocations piling in metals or growth and coalescence of cavities induced by large deformations in the vicinity of inclusions in both metals and polymers. From the micromechanical point of view, this is the growth of a spheric or elliptic hole in a plastic medium subjected to large strains and the problem can be solved analytically (F.A. Mac Clintoch 1968, J.R. Rice and D.M. Tracey 1969) or numerically (V. Tvergaard and A. Needleman 1982). From the Continuum Damage Mechanics point of view, this is a reduction of the resisting area in any plane of a Representative Vol- ume Element that is governed by the elastic energy and the accumulated plastic strain, as explained in Chap. 1. All of the following chapters on applications have the same format: some engineering considerations; description of "fast methods"whichcanbeused in early design where the hypothesis of proportional loading and small scale yielding apply, with indications on the sensitivity analysis and possible safety margin; closed-form solutions of simple problems currently found in en- gineering such as structures with holes or notches, pressurized cylinders, and forming limits and post-buckling behavior; specific cases treated by nu- merical analysis, such as finite strains, porous materials, forming pro- cesses such as deep drawing and extrusion and frames analysis using Lumped Damage Mechanics. All applications are considered on materials at room temperature and low strain rates (the domain of application of plastic-

142 3 Ductile Failures ity). A ductile damage model for elastomers which also applies in fatigue is described in Chap. 4. Creep effects and also "dynamic plasticity" are relevant to visco-plasticity and are treated in Chap. 5. Problems of elas- tomers or polymers involving strain rate effects are approached at the end of Chap. 5. 3.1 Engineering Considerations Ductile failures are most often related to large deformations, plastic strains in metals, and irreversible strains in polymers. These conditions can arise locally in the vicinity of notches or severe bendings. They can also occur on a large scale during forming processes but they are always associated with instabilities and the phenomenon of localization of strains and damage. Fortunately these phenomena occur at the latest stage of failures, allowing us to only look into their initiation. The "in service" security of pressure vessels or mechanical members with holes or notches needs to be checked against ductile failures in case of over- loads. The case of cyclic loadings is treated in Chap. 4 for low cycle fatigue and in Chap. 5 for elevated temperatures. Another area of applications is analyzing the forming processes in order to choose the proper machine, to optimize the processes for economical energy consumption, avoid trouble such as necking and cracks, and determine the modifications of the constitutive equations after forming. Be careful when reading values of material parameters in a metallurgy catalog because they characterize materials in the state of the products sold (e.g., sheets) but not the products after metal forming (e.g., deep drawing). The sequences of machining like stamping may take advantage of non-proportional loadings to increase the forming limits. In post-buckling analysis of crash problems, the energy involved is much dependent on the damage which reduces the strength and the energy ab- sorbed. The dynamic case, which needs to take into account the strain rate effect, is described in Sects. 5.3.1 and 5.4.4. 3.2 Fast Calculation of Structural Failures Fast calculation means obtaining the desired result using closed-form solu- tions or mathematical softwares on personal computers which do not need large finite element computations on big computers. Often, taking time for a clever qualitative analysis of the problem allows you to consider a simplified geometry of the structure together with a simplified loading, which then al- lows for a "fast calculation." For such cases, we advise using isotropic damage without the quasi-unilateral condition of microdefects closure.

3.2 Fast Calculation of Structural Failures 143 3.2.1 Uniaxial Behavior and Validation of the Damage Law The basic uniaxial test is the "simple" tension test which is not so simple in the range of large deformation where necking occurs. Figure 3.1 is an example of the same test represented in the engineering stress-strain reference of small strain theory and in the local "true" stress-"true" strain reference (σtr = σ(1 + ), tr =ln(1+ )) of large strain theory. The difference in stress may reach 50% for strains around 0.5. Fig. 3.1. Engineering and true stress-strain curves of Cu/Al at room temperature (J. Dufailly 1995) Ductile properties of the material must take into consideration this big difference. The easiest way is to use the simple tension test only up to the strain corresponding to the ultimate stress (σ = σu) and to explore the damage during a low cycle fatigue test for which no necking appears. The ultimate stress (σu) is the true stress (Fu/S where S is the necking section) if a large deformation theory is used; it is the engineering stress otherwise (Fu/S0 where S0 is the initial section of the specimen). The method of iden- tification of material parameters advised is the one discussed in Sect. 1.4.4 for a fast identification, improved with a numerical optimization if other tests are available as described in Sect. 2.4. Due to large deformations which corre- spond to saturated strain hardening at the ultimate stress σu , the plasticity criterion for monotonic tension is f=σ 1-D-σu =0, (3.1) the energy density release rate Y is almost constant: Rν=1andY≈σ2 u 2E ≈ const, (3.2)

144 3 Ductile Failures and the unified damage law reduces to ˙ D = YS s ˙p= σ2 u 2ES s | ˙ p| if p> pD. (3.3) A simple integration gives a relation between the critical value of the damage Dc at mesocrack initiation and the plastic strain at rupture pR: Dc = σ2 u 2ES s ( pR - pD) . (3.4) This expression may be used to decrease the number of material parameters in the damage law, as then ˙ D= Dc pR - pD|˙ p| if p> pD, (3.5) or by an obvious integration in monotonic loading: D=Dc p- pD pR - pD . (3.6) The ductile damage is a linear function of the plastic strain. Checking this property by experiments is a validation of the damage law to be added to the procedures of identification of Sects. 1.4.4 and 2.4. An approximate order of magnitude of the damage is obtained with Dc ≈ 0.5, pD ≈ pR/2, yielding D ≈ p pR-1 2 (3.7) (recall that x denotes the positive part of x). 3.2.2 Case of Proportional Loading As defined in Sect. 2.1.2, the proportional loading condition for a structure is when the loading induces principal directions of the stresses which are constant in time but which are eventually different in each point of the struc- ture, σij(M, t)=σΣ(t)Σij(M) , (3.8) with the von Mises norm for easy applications 3 2ΣD ij ΣD ij =1. (3.9)

3.2 Fast Calculation of Structural Failures 145 Let us recall that the main sufficient condition for a structure to be con- sidered proportionally loaded is when there is only one applied load or when all the loads vary proportionally to one parameter. The simplification which arises is the possible a priori integration of the damage law and the plastic constitutive equations as all the tensors are col- inear: σD ij = σΣΣD ij ⇒ σeq =|σΣ| σH=σΣΣH ⇒ TX=σH σeq =ΣH · sgn(σΣ)= 13 Σkk · sgn(σΣ) ≈ TXelas . (3.10) The value of the stress triaxiality in elasto-plasticity is usually close to the value obtained in a pure elastic calculation. Using the isotropic damage law together with a monotonic loading, we have ˙ D= σ2 eqRν 2ES(1 - D)2 s ˙p if p>pD, (3.11) where Rν = 23(1 + ν)+3(1- 2ν)Σ2 H=const and σeq=σΣ. (3.12) Considering natural initial conditions of no damage (D = 0 at the beginning of the loading), we have D 0 (1-D)2sdD = Rν 2ES s t tD σ2s Σ (t)˙ p(t)dt (3.13) D =1- 1 - (2s +1) Rν 2ES s t tD σ2s Σ (t)˙ p(t)dt 1 2s+1 , (3.14) where tD is the time for which the accumulated plastic strain is equal to the damage threshold p = pD, i.e., for monotonic loading pD = pD. This integration may be performed once the time histories σΣ(t)a nd p(t) are determined, from an elasto-plastic computation or from the ini- tial post-processing of an elastic computation using the Neuber method (see Sects. 2.1.4 and 3.2.4, respectively.) If a saturated hardening is considered it is possible to simply relate the accumulated plastic strain at mesocrack initiation (pR)totheuniaxial plastic strain to rupture ( pR): ˙ D = σ2 uRν 2ES s ˙p if p>pD. (3.15)

146 3 Ductile Failures Integrating with the natural initial conditions and with pD = pD in mono- tonic loading leads to Dc = σ2 uRν 2ES s (pR - pD) (3.16) and dividing by the same equation in the uniaxial case gives pR- pD pR- pD =R-s ν and Rν = 23(1 + ν)+3(1- 2ν)Σ2 H , (3.17) with ΣH = TX (the triaxiality). 3.2.3 Sensitivity Analysis Following the general method of Sect. 2.4.6, the sensitivity to loading condi- tions and material parameters is determined here on the predicted plastic strain to rupture using its closed-form expression in proportional loading (3.16), Dc = σ2 uRν 2ES s (pR - pD)o rpR = pD + σ2 uRν 2ES -s Dc , (3.18) withRν =2 3(1 + ν)+3(1- 2ν)T 2 X. The logarithmic derivative allows us to determine the relative error on all the variables and parameters in order to build the scheme of the qualitative importance of each of them: ln(pR - pD)=lnDc+s(ln2+lnE+lnS-2lnσu -lnRν). (3.19) With the notation δx = |dx| to ensure upper bounds on the errors (of un- known signs), δ(pR - pD) pR- pD =δpR pR pR pR- pD-δ pD pD pD pR- pD (3.20) and δRν Rν =δν ν |6T2 X-2 3|ν Rν +δTX TX 6(1-2ν)T2 X Rν , (3.21) writing δpR pR = k SpR Ak δAk Ak where SpR Ak are the coefficients of the sensitivity matrix of Sect. 2.4.6, we obtain SpR TX =pR- pD pR 6s(1 - 2ν)T 2 X Rν , SpR σu =pR- pD pR 2s,

3.2 Fast Calculation of Structural Failures 147 SpR E =pR- pD pR s, SpR ν =pR- pD pR |6T2 X-2 3 |νs Rν , SpR pD = pD pR, SpR S =pR- pD pR s, SpR s =pR- pD pRs ln 2ES σ2 uRν , SpR Dc =pR- pD pR. (3.22) Finally, the scheme of Fig. 3.2 gives an example of the values of the sensi- tivity parameters and shows the relative importance of each parameter given by the height of the frames around each sensitivity coefficient. It has more or less a general qualitative value for ductile failures as it has been obtained for mean values of the parameters: TX =1,Rν =2.07, σu = 500 MPa, E = 200000 MPa, ν =0.3, pR/ pD =2,S = 2 MPa, and s =5. Fig. 3.2. Relative importance of each parameter in ductile failures The loading is represented here by the triaxiality ratio TX and by the stress through σu . Their influences are larger than those of the material pa- rameters. The parameters which do not need a large accuracy are pD and Dc . Nevertheless, if all the parameters were known with an error as small as 1%, the error on the accumulated plastic strain at failure could be of the order of 10 to 20%. Fortunately, in practice some errors are positive and some negative! 3.2.4 Stress Concentration and the Neuber Method The case of small scale yielding allows us to avoid a whole elasto-plastic calculation of the structure by setting up a plastic correction of an elastic

148 3 Ductile Failures structure analysis. Small scale yielding refers to the cases where plastic strain is limited in energy and in geometrical space. To give a quantitative criterion, it is in the domain where σeq >σ yisbelow≈1%ofthevolumeofthe structure. This corresponds to the zones of stress concentrations as those close to holes or notches. To evaluate the risk of a failure the proposed procedure is as follows: • First, perform an elastic structure calculation • Second, do a Neuber local plastic analysis as a correction of the elastic analysis. Other local energetic methods may be used. For instance, the strain energy density (SED) method described in Chap. 4 applies better at free edge points if the plasticity remains very localized. This is the case for cyclic loadings. For monotonic loadings, the Neuber method is generally preferred. • Third, calculate the damage based on the results of the elastic and plastic analysis. The time integration of the damage evolution law is performed by using (3.6) or (3.14). The Neuber method looks like an energy equivalence between the elastic and the elasto-plastic calculations of the same geometry submitted to the same loading but it is a heuristic. For unidimensional states of stress, the product (stress × strain) calculated in elasticity is assumed to be locally identical to the same product calculated by means of an elasto-plastic analysis, σ =(σ )elas at the stress concentration point, (3.23) where (.)elas means "value determined from a strictly elastic computation," even if the stress is above the yield limit. The plastic state is then deter- mined as the matching of the constitutive equation = σ/E + g(σ)with the equation of the hyperbole (stress × strain = the constant determined by the elastic calculation), where for monotonic loading isotropic harden- ing R( p) alone has to be considered (Fig. 3.3). The function g(σ)=p is g(σ)= σ-σy Ky p My for the hardening power law. One may introduce the stress concentration coefficient in elasticity, KT = σelas σn = elas n , (3.24) whose value may be found in handbooks (see bibliography) for common engi- neering geometries. The nominal stress σn is the nominal uniform stress field calculated from the external loading by the simple consideration of loads at equilibrium (see Fig. 3.4), elas = σelas/E,and n = σn/E. This allows us to write the Neuber heuristic as σ =K2 Tσn n = K2 T Eσ2 n. (3.25)

3.2 Fast Calculation of Structural Failures 149 Fig. 3.3. The Neuber method Fig. 3.4. Nominal stress (σn) and elastic stress concentration coefficient (KT)for an applied load (F )

150 3 Ductile Failures The result of the post-processing is the stress σ and the plastic strain p determined graphically (Fig. 3.3) or analytically: use, for instance, (3.36) for linear hardening and solve (3.38) with Rν = 1 for nonlinear hardening. This defines the ratio kNeuber = σ σelas (3.26) and the stress concentration coefficient in plasticity as σ σn = kNeuberKT . (3.27) For three-dimensional states of stress, Neuber fundamental hypo- thesis may be written as σij ij =(σij ij)elas for monotonic loading, (3.28) where the quantity (σij ij)elas may also be written in terms of von Mises stress σelas eq and stress triaxiality TXelas coming from the elastic reference computation, (σij ij)elas = (σelas eq )2Relas ν E and Relas ν = 23(1+ν)+3(1-2ν)T 2 Xelas . (3.29) The plastic behavior is described by an integrated Hencky--Mises law for monotonic loading , σij = Eijkl kl -3GσD ij σeqp and p = R-1(σeq - σy), (3.30) where G is the shear modulus and R(p) is the isotropic hardening law. For the power law, we have p= σeq-σy Ky p My . (3.31) Again, the values of the stress triaxiality TX and the triaxiality function Rν=2 3(1 + ν)+3(1- 2ν)T 2 X are needed in order to properly apply the Neuber method. Use the proportional loading assumption TX ≈ TXelas for general 3D cases. Use TX =1/3andRν = 1 for stress concentration points located on free edges in plane stress. Use TX ≈ 0.58 and Rν ≈ 1.27 for stress concentration points located on free edges in plane strain (see Sect. 2.1.4). 3.2.4.1 Neuber Method with Linear Hardening, R = Cyp Assume that an elastic computation gives the product (σij ij)elas as well as the von Mises stress σelas eq at a stress concentration point. The application of the Neuber method (3.28) leads to

3.2 Fast Calculation of Structural Failures 151 σij ij = σ2 eqRν E + σeq σeq - σy Cy =(σij ij)elas (3.32) and then the evaluation of the von Mises stress in plasticity σeq if Rν is known. The relationship σeq(σelas eq ) is explicit: σeq = E Cy σy + E Cy σy 2 +4E Rν + E Cy (σij ij)elas 2 Rν+E Cy , (3.33) wherewedefine kNeuber = σeq σelas eq from the Neuber method (3.34) and the accumulated plastic strain is p=σeq-σy Cy. (3.35) This method has the main advantage of being fully explicit and giving closed-form expressions for σeq and p. The hardening parameters σy and Cy need to be identified from the tensile stress-strain curve within a range in accordance with the value of the plastic strain finally estimated. For the 1D case, σ = σnKTkNeuber = σnKT 1+ 1+4 Cy E+C2 y E2 σ2 elas σ2 y 2 Cy E +1 σelas σy , (3.36) with σelas = KTσn. 3.2.4.2 Neuber Method with Nonlinear Hardening, R=Ry ∞ (1 - exp (-byp)) The accumulated plastic strain is p(σeq)=g(σeq)=- 1 by ln Ry ∞+σy-σeq Ry ∞ (3.37) and the Neuber method now reads (Rν known): σij ij = σ2 eqRν E + σeqp(σeq)=(σij ij)elas , (3.38) an equation which has to be solved numerically to estimate the von Mises stress in plasticity σeq, and then the accumulated plastic strain p and the auxiliary function kNeuber = σeq/σelas eq.

152 3 Ductile Failures Considering a nonlinear hardening gives better results but a mathematical software is needed to solve the nonlinear equation (3.38). 3.2.4.3 Neuber Method Coupled with Damage When damage occurs, the Neuber method can still be used but with the stress replaced by the effective stress, ˜ σeq = σeq/(1 - D). Equation (3.33) for linear hardening becomes ˜ σeq = E Cy σy + E Cy σy 2 +4E Rν + E Cy (σij ij)elas 2 Rν+E Cy (3.39) and equation (3.38) for nonlinear hardening becomes ˜ σ2 eqRν E+˜ σeqp(˜ σeq)=(σij ij)elas , (3.40) with the accumulated plastic strain p=p(˜ σeq)=R-1(˜ σeq - σy)=g σeq 1-D-σy . (3.41) The damage is equal to Dc at crack initiation. 3.2.5 Safety Margin and Crack Arrest The main parameter which allows us to evaluate how far or close a loaded structure is to a ductile mesocrack initiation is the maximum accumulated plastic strain p resulting from a structure analysis. The plastic strain corresponding to a mesocrack initiation is given by the damage analysis: pR =pD+Dc σ2 uRν 2ES -s = pD +( pR - pD)R-s ν . (3.42) If the number Saf ≥ 1 is the safety factor to take into consideration in engineering, the safety margin is defined by p< pR Saf , (3.43) with Saf = 5, 2, or 1.1 depending on the compromise adopted between secu- rity and weight design.

3.2 Fast Calculation of Structural Failures 153 Once the mesocrack is initiated, it is often important to check its rate of growth. As a finite crack exists, the simple Continuum Damage Mechanics is not appropriate any more and the concepts of Fracture Mechanics by cracking can be applied. The behavior of a ductile crack is approximately governed by a resistant curve (or R-curve) that depends on each material: an energy which depends on the area of the crack A, Rc =Rc(A-A0), (3.44) where the function Rc(A - A0) is known from experiments (Fig. 3.5) and where A0 is the area of the mesocrack initiated by damage (see Sect. 1.6.3), A0= G2 c σ2 u 2E Dc + σu pR 2 . (3.45) The energy available for the crack growth is determined by the structure strain energy release rate (G) that depends on the geometry of the structure and the far field loading (σ∞), G = G(A, σ∞). (3.46) It can be calculated from the Fracture Mechanics concepts and has the general form of G=κσ2 ∞ πA1/2 E, (3.47) with κ a dimensionless shape parameter. Fig. 3.5. Ductile crack growth governed by the R-curve

154 3 Ductile Failures The strain energy release rate G is compared to the resistant curve (Fig. 3.5) as the fracture behavior is determined by G(A, σ∞)=Rc(A - A0) . (3.48) • If this equality is satisfied, the intersection I of the two curves exists, there will be a crack arrest for the value of σ∞ considered and a stable growth of the crack if σ∞ increases. • If this equality is not satisfied, which means G>Rc , there will be a fast crack propagation by instability as soon as the tangent point Ic is reached: ∂G ∂A=∂Rc ∂A atIc. (3.49) If the R-curve for the considered material is not available, there is always the possibility to compare the strain energy release rate for the value A0 of the crack area with the toughness Gc :doe sκσ2 ∞ πA1/2 0 /E remain much smaller than Gc?Ifyes,behappy! 3.3 Basic Engineering Examples Some basic geometries and loadings are very common in engineering. For plates with holes or notches, for cylinders or for some plane stress prob- lems there are approximate solutions which allow for fast calculations of the mesocrack initiation conditions. Furthermore, some results can be expressed in non dimensional form for use in large problem sets. Here again, the damage is considered isotropic without the quasi-unilateral condition of microdefects closure. 3.3.1 Plates or Members with Holes or Notches These are all cases where the critical RVE is submitted to a stress concen- tration, inducing a small scale local plasticity. Assume that the local elastic stress, ignoring the plasticity, is known for a monotonic loading either from a structure calculation or through the stress concentration coefficient (KT) which may be found in handbooks (see bibliography): σelas eq =KTσn. (3.50) with σn the nominal stress. When the load (σ∞) increases, small scale local plasticity develops which decreases the stress concentration determined now from the 1D Neuber correction (as the stress concentration lies on a free surface, see Sect. 3.2.4). Then σeq = kNeuberσelas eq = kNeuberKTσn . (3.51)

3.3 Basic Engineering Examples 155 This stress is used to calculate the accumulated plastic strain p which ensures the mesocrack initiation when it reaches pR or pR given by the critical damage condition of Sect. 3.2.1, Dc = σ2 uRν 2ES s ( pR - pD)o r pR = pD + Dc 2ES σ2 uRν s (3.52) with Rν = 1 for thin plates with the hypothesis of plane stresses and Rν =1.27 for thick plates with the hypothesis of plane strains (stress tri- axiality TX =0.58 from Sect. 2.1.4). 3.3.1.1 Linear Hardening kNeuber = E Cy σy + E Cy σy 2 +4E Rν + E Cy (σij ij)elas 2 Rν+E Cy σelas eq , (3.53) with Cy the plastic modulus such that p= σeq 1-D-σy Cy . (3.54) Writing the rupture condition as pR = σeq 1-Dc -σy Cy = pD + Dc 2ES σ2 uRν s , (3.55) from which σeq =(1- Dc) σy + Cy pD + Dc 2ES σ2 uRν s (3.56) and the failure condition is σn= ˜ σeq kNeuberKT , ˜ σeq = σeq 1-Dc . (3.57) 3.3.1.2 Exponential Hardening, R = Ry ∞ (1 - exp (-byp)) kNeuber =˜ σeq/σelas eq is determined by the Neuber method (3.38), with p= -1 by ln Ry ∞+σy- ˜ σeq Ry ∞ . (3.58)

156 3 Ductile Failures Writing the rupture condition p= -1 by ln Ry ∞+σy- σeq 1-Dc Ry ∞ = pD + Dc 2ES σ2 uRν s , (3.59) from which σeq =(1- Dc) σy + Ry ∞ 1 - exp -by pD + Dc 2ES σ2 uRν s , (3.60) the failure condition is σn= ˜ σeq kNeuberKT , ˜ σeq = σeq 1-Dc . (3.61) 3.3.2 Pressurized Shallow Cylinders A pressurized cylinder may explode if a crack is initiated through the phe- nomenon of ductility. It may happen in pipes or during the process of hy- droforming. If the cylinder is considered long enough, with a thin thickness (tcyl) compared to the mean radius (Rcyl, Fig. 3.6), the state of stress derives simply from overall equilibrium equations. Fig. 3.6. Pressurized circular cylinder In cylindrical coordinates (r, θ, z)withP as the internal pressure, we have σ = ≈00 0 0 PRcyl tcyl 0 00PRcyl 2tcyl , (3.62) from which it is easy to determine

3.3 Basic Engineering Examples 157 • The von Mises equivalent stress σeq = √3 2 PRcyl tcyl , • The hydrostatic stress σH = PRcyl 2tcyl • The triaxiality ratio TX = σH σeq=1 √3 • The triaxiality function Rν = 23(1 + ν)+3(1- 2ν)T2 X=5-4ν 3 (3.63) or Rν =1.27 for ν =0.3 A rough approximation consists of writing the condition of brittle fracture of Chap. 7 through the damage equivalent stress σ de riv edinSe ct.1.2.2 (1.34), using σ = σu or σeqR1/2 ν =σu, (3.64) where σu is the ultimate stress in tension. The term Pc is the critical pressure at mesocrack initiation, where √3 2 PcRcyl tcyl 5-4ν 3 =σu (3.65) gives Pc= 2 √5-4νσutcyl Rcyl . (3.66) The critical pressure is linear with the ultimate stress and the thickness-radius ratio. A better analysis consists of the resolution of the unified damage law together with the plastic constitutive equations for which the hypothesis of linear hardening is sufficient: p= σeq 1-D-σy Cy . (3.67) Since the loading is proportional and monotonic, considering the saturated strain hardening allows us to use the result of Sect. 3.2.5 (3.42): pR =pD+Dc σ2 uRν 2ES -s = pD +( pR - pD)R-s ν . (3.68) There will be a mesocrack initiation for the pressure corresponding to the accumulated plastic strain value equal to pR, such that √3PcRcyl 2tcyl(1 - Dc)Cy - σy Cy = pD+ 5-4ν 3 -s ( pR - pD) (3.69)

158 3 Ductile Failures or Pc=2 √3 tcyl Rcyl(1 - Dc) σy + Cy pD + 5 - 4ν 3 -s ( pR - pD) . (3.70) The critical pressure is still linear with the ratio tcyl/Rcyl but depends on the damage properties. Example of a Pipe For a pipe made of ferritic steel at room temperature: E = 200000 MPa, ν =0.3, σy = 375 MPa, σu = 474 MPa, pu =0.15, Cy≈σu-σy pu = 660 MPa, pD =0.15, pR =0.32, Dc =0.3, s =2.4. Equation (3.70) gives Pc = 435 tcyl Rcyl (MPa). The condition of brittle frac- ture (3.66) leads to Pc = 486 tcyl Rcyl (MPa) which overestimates the pressure by a factor of 12%. 3.3.3 Post-Buckling in Bending A situation which often occurs in accident evaluation is a post-buckling de- formation following an instability due to buckling. The purpose here is to evaluate the energy absorbed by plastic deformation, taking into account the damage up to a mesocrack initiation for an elementary volume loaded in pure bending at slow strain rate. The problem reduces to the analysis of a beam element of length l,height h and width b, loaded in circular bending of radius of curvature ρ up to a maximum plastic strain pR or pR (Fig. 3.7). The elementary beam theory is used together with the Bernoulli hypothe- sis applied on the plastic strain as the elastic strain can be neglected, yielding p = pM2y h, (3.71) where pM is the maximum uniaxial plastic strain reached in the cross sec- tion and pM = pR at mesocrack initiation. The density of energy to create a tension defined by a plastic strain p is w = p 0 σd p. (3.72) For a material subjected to a power law hardening (with the yield stress taken as σy = 0) and the unified damage law (3.6) of Sect. 3.2.1 (with the damage threshold taken equal to pD =0), wehave

3.3 Basic Engineering Examples 159 Fig. 3.7. Elementary bending of a rectangular beam p= σ (1 - D)K0 p M0 and D=Dc p pR . (3.73) Then, w = p 0 1-Dc p pR K0 p 1/M0 p d p =M0 M0 +1K0 p M0 +1 M0 p - DcK0 p pR M0 2M0 +1 2M0 +1 M0 p . (3.74) At this stage it is interesting to compare the energy involved without any damage at crack initiation ( p = pR, w = wR): w0 = p 0K0 p 1/M0 p d p= M0 M0 +1K0 p M0 +1 M0 p (3.75) and wR=w0 1-DcM0+1 2M0 +1 . (3.76) This shows that a calculation made without consideration of damage leads to an overestimation of about w0Dc/2, a relative error of 10 to 25%. Back to the bending problem, w has to be integrated in the whole volume with the linear variation of p in height p = pM 2y h:

160 3 Ductile Failures W =2bl h/2 0 p(y) 0 1-Dc p pR K0 p 1/M0 p d pdy (3.77) or W = bhlK0 pM0 2M0 +1 M0 +1 M0 p M0 M0+1-Dc M0 3M0 +1 pM pR . (3.78) If the damage is not taken into consideration, then W0 = bhlK0 p M2 0 (2M0 +1)(M0 +1) M0 +1 M0 p (3.79) and for the mesocrack initiation condition ( p = pR, W = WR), WR=W0 1-DcM0+1 3M0 +1 . (3.80) When damage is not taken into account, the result is again an overestimation of the energy. The relative difference is slightly smaller and of about Dc/3, that is 7 to 17%. For the practical applications of bar structures collapsing with nh identical plastic hinges, we estimate the bending length as a full bending: l = πh/2 (see Fig. 3.7) and take the following as a rough estimation of the energy absorbed: WR(nh)=nhb πh2 2K0 p M2 0 (2M0 +1)(M0 +1) M0 +1 M0 pR 1-DcM0+1 3M0 +1 (3.81) or with pR = σR (1 - Dc)K0 p M0 ≈ σu K0 p M0 , W (nh)=nhb πh2 2 M2 0 (2M0 +1)(M0 +1)σu pR 1 - Dc M0 +1 3M0 +1 , (3.82) which only needs the knowledge of the geometry b, h, and the material pa- rameters σu , pR, M0,andDc . 3.3.4 Damage Criteria in Proportional Loading The case of proportional loading allows us to derive the mesocrack initiation condition as a function of the state of stresses or strains with the need of only a few material parameters. Equation (3.17) derived in Sect. 3.2.2 for saturated hardening is used here but its application is limited to positive stresses as the damage is considered isotropic, without any effect of microdefects closure in compression: pR- pD pR- pD =R-s ν. (3.83)

3.3 Basic Engineering Examples 161 3.3.4.1 Three-Dimensional Loading The large effect of the triaxiality ratio TX = σH/σeq on the accumulated plastic strain at mesocrack initiation pR is shown in Fig. 3.8. The value of pR may be deduced from the graphs if the values of the damage threshold pD, the damage exponent s, the plastic strain to rupture in pure tension pR,and the triaxiality ratio from a structure calculation are known. Fig. 3.8. Triaxiality makes materials more brittle! 3.3.4.2 Case of Plane Strains The case of plain strains applies to thick sheets for which the strain within the thickness 3 is considered negligible in comparison to the in-plane principal strains 1 and 2: = 1 00 0 20 000 and σ = σ1 00 0σ20 00σ3 . (3.84) Neglecting the elastic strains, the condition of plastic incompressibility gives 2= - 1. (3.85) The plastic constitutive equations integrated in case of proportional loading gives back the Hencky--Mises law with p = g(σeq,D):

162 3 Ductile Failures 3 = 32 g(σeq,D)σD 33 σeq , (3.86) from which σD 33 =0, 1 = 32 g(σeq,D)σD 11 σeq , 2 = 32 g(σeq,D)σD 22 σeq . (3.87) As 2=- 1,σD 22=-σD 11, it follows that σ3=1 2(σ1+σ2), σH=1 2(σ1+σ2), σeq=√3 2|σ1-σ2|. (3.88) The accumulated plastic strain is p = 23( 2 1+ 2 2)= 2 √3 | 1| (3.89) and the crack initiation criterion becomes 2 √3 | 1|- pD pR- pD =R-s ν (3.90) or | 1| = | 2| =√3 2 pD +( pR - pD) 23 (1 + ν)+(1- 2ν) σ1 + σ2 σ1 - σ2 2 -s . (3.91) The case σ1 = σ2 corresponds to a pure hydrostatic state of stress σ1 = σ2 = σ3 for which there is no plastic strain and no damage since it would need infinite strains. 3.3.4.3 Case of Plane Stresses The case of plane stresses applies to thin sheets for which the stress within the thickness σ3 is considered as negligible in comparison to the in-plane principal stresses σ1 and σ2 .

3.3 Basic Engineering Examples 163 With the condition of incompressibility kk = 0, and neglecting the elastic strains, σ = σ1 00 0σ20 000 , = 1 00 0 2 0 00-( 1 + 2) (3.92) To use the condition of mesocrack initiation (3.17) pR- pD pR- pD =R-s ν (3.93) one needs the accumulated plastic strain and the triaxiality function ex- pressed either as functions of the strains or of the stresses. 3.3.4.3.1 Plane Stress Criterion as a Function of the Strains p = 23 D ij D ij=2 √3 2 1+ 2 2+ 1 2 (3.94) The triaxiality ratio σH/σeq may be derived from the plastic constitutive equations (3.87). Both σH and σeq may be expressed as a function of σ1 and 2/ 1. First of all 2 1=σD 22 σD 11 , (3.95) with σD 11 =σ1-13(σ1+σ2)a n dσD 22 = σ2 - 13(σ1 +σ2). (3.96) It follows that σ2=σ1 2 2 1 +1 2+ 2 1 . (3.97) Then, σH =13(σ1+σ2)=σ1 3 1+2 2 1 +1 2+ 2 1 , (3.98) σeq=1 √2 (σ1 - σ2)2 + σ2 1+σ2 2=σ1 2 2 1 +1 2+ 2 1 2 - 2 2 1 +1 2+ 2 1 +1, (3.99) and TX=σH σeq = 2 1 +1 √3 2 1 2 + 2 1 +1 . (3.100)

164 3 Ductile Failures Finally at rupture, we have 2 √3 2 1+ 2 2+ 1 2- pD pR - pD = 23(1 + ν)+(1- 2ν) 2 1 +1 2 2 1 2 + 2 1 +1 -s . (3.101) A resolution by any mathematics software with pD = 0 gives the graphs of Fig. 3.9 where the proportional loading is always a straight line in the plot of 2/ pR vs 1/ pR. The admissible domain for the couple of strains 1 and 2 is smaller and smaller as the damage exponent s increases. Fig. 3.9. Strain limit curves in plane stresses ( pD =0) 3.3.4.3.2 Plane Stress Criterion as a Function of Stresses σH =13(σ1+σ2) σeq=1 √2 (σ1 - σ2)2 +(σ2 - σ3)2 +(σ3 - σ1)2 = σ2 1+σ2 2-σ1σ2 (3.102) The plastic strain needs to be expressed as a function of the stresses. Using again the integrated plastic constitutive equations again, but with a zero yield stress, allows us to obtain a simple expression for the ratio pR/ pR.

3.3 Basic Engineering Examples 165 The hardening law reads: p = g(σeq,D)= σeq (1 - D)K0 p M0 . (3.103) Close to crack initiation the hardening is close to saturation, leading to pR = σeq (1 - Dc)K0 p M0 and pR = σR (1 - Dc)K0 p M0 ≈ σu K0 p M0 . (3.104) Then pR pR = σeq σu(1 - Dc) M0 , (3.105) where pR pR = R-s ν gives σ2 1+σ2 2-σ1σ2 (1 - Dc)σu = 23(1 + ν)+13(1 - 2ν) (σ1 + σ2)2 σ2 1+σ2 2-σ1σ2 - s M0 . (3.106) Fig. 3.10. Stress limit curves in plane stresses ( pD =0)

166 3 Ductile Failures If the damage threshold is considered as pD = 0, the stress condition of mesocrack initiation depends only on the ultimate stress σu , the critical damage Dc , and the ratio of the damage and plastic exponents s/M0,a s shown in Fig. 3.10. In the same figure, the von Mises criterion is plotted to show which mis- take may be made in using it as a rupture criterion when the triaxiality ratio differs from ≈ 1/3. The damage equivalent stress criterion σ = σeqR1/2 ν =σR corresponds to the curve s/M0 =0.5. 3.4 Numerical Failure Analysis For complex geometries and loadings, closed-form solutions for the stress, strain, and damage fields usually do not exist and the loading is often non- proportional at most Gauss points of finite element analyses. No simplifying assumptions can be made, except the earlier hypothesis of localized plasticity (small scale yielding) which gives the possibility to efficiently use the Neuber method as described in Sect. 3.2.4. When plasticity takes place in a non- negligible domain of the structure (one speaks then of large scale yielding), stress redistribution occurs. It may have an accelerating effect on the failure conditions as it enhances the phenomenon of strain and damage localiza- tion.We then use computer codes and perform FE analyses with the fully- coupled damage constitutive equations of Chap. 1. For ductile failures we use the damage initiation criterion written in terms of plastic strain where pD = pD (see Sect. 1.4.1). For monotonic loading, we use the single isotropic hardening R with either the exponential law R = Ry ∞ (1 - exp(-byr)), the powerlawR=Ky p r1/My , or the linear law R = Cyr. When a numerical analy- sis is performed, there is no more reason to consider the unified damage law reduced to isotropy. We strongly advise using the anisotropic law to obtain a better accuracy. It requires only one additional material parameter which in practice may be taken as η = 3. The consideration of the quasi-unilateral conditions of microdefects closure is not necessary as far as monotonic loading is applied. For more details see for instance Sect. 2.2.6 for the use of the fully-coupled scheme and more generally Sect. 2.2 for its numerical implementation, as well as Sects. 1.4.4 and 2.4 for the material parameters identification. Other models concern ductile failures: an anisotropic plasticity model with the Hill yield surface that is compatible with the effective stress concept is described at the end of this chapter; the model extension to finite strains is briefly exposed in next section; and the Gurson model specific to ductile failure of porous materials is summarized in Sect. 3.4.5 and used for the cross identification of the unified damage law. Frames may be analyzed by limit analysis incorporing damage through Lumped Damage Mechanics of Sect. 3.4.6.

3.4 Numerical Failure Analysis 167 3.4.1 Finite Strains When ductile failure occurs, the strains often become too large for the small strain perturbation hypothesis to remain valid: for metals the plastic strain at rupture is usually larger than 0.1 (and most of the time smaller than 1); for polymers it may reach much larger values corresponding sometimes to a few hundred percent. The large deformations framework has to be used and this can be done only with the help of computer codes. Different solutions exist to extend nonlinear small strain constitutive equations to finite strains, mainly related to the material behavior description in either the reference initial configuration C0 or in the deformed or actual configuration C(t)attimet. The link between C0 and C(t) is the gradient of the transformation F and F T is its transpose. One may consider different strain tensors, such as the Green--Lagrange tensor (E) in the reference configuration, the Euler--Almansi tensor (A) in C(t), E=1 2 FTF-1 and A=1 2 1 -F-TF-1 , (3.107) and even different strain rate tensors such as the velocity gradient L or its symmetric part: the strain rate tensor Δ, L=˙ FF-1 and Δ=1 2 L+LT . (3.108) But considering one definition instead of another does not provide an equiv- alent description and leads to different theories. Their use is also related to stress tensors definitions: • The second Piola--Kirchhoff tensor S associated with E (defined in the reference configuration C0), • The Cauchy stress tensor σ associated with Δ (defined in C(t)), and • The first Piola--Kirchhoff stress tensor τ associated with F . The tensors F and τ are not symmetric. The following relations stand: (detF)σ = τFT =FSFT, (3.109) and one has the energetic equivalence 1 ρσ:Δ=1 ρ0τ:˙ F=1 ρ0S: ˙ E, (3.110) with ρ0 as the initial density in C0 and ρ = ρ0/ det F as the actual density in C(t). There are also theoretical difficulties concerning the objectivity and frame- work independency of the time derivative of the stress tensor, the main ques- tion being, "In which framework or configuration do we take the derivatives?"

168 3 Ductile Failures Different answers to this question lead to different definitions of the derivative (called objective), the most "popular" being the Jaumann derivative, dJ dtσ= ˙ σ-Wσ+σW with W=1 2 L-LT . (3.111) The Truesdell derivative is also considered; it corresponds to the reactu- alized Lagrangian formulation, dTr dtσ= ˙ σ-Lσ-σLT+tr(L)σ, (3.112) but other good (better?) definitions exist. We briefly present here three pos- sible formulations and further details about objectivity or about plasticity and thermodynamics within the large deformation framework given in the books by G. Maugin (1992) and P. Ladev` eze (1996). The thermodynamics framework of Chap. 1 then applies strictly if the constitutive equations are written in a "rotated" configuration. In order to keep the presentation simple, only isotropic hardening (vari- ables R, r) and isotropic damage (variables Y , D) are considered here. 3.4.1.1 Additive Split of the Strain Rate Tensor The strain rates ˙ ,˙ e ,and ˙ p of small deformation formulation are replaced by Δ, Δe , Δp, and the stress rate by Jaumann objective derivative (3.111). The strain rate partition reads Δ=Δe+Δp. (3.113) The elasticity law is written in the rate form dJ dtσ=a:Δe, (3.114) with a an objective elasticity tensor. The yield criterion is written in terms of the von Mises invariant of the Cauchy stress, f= σeq 1-D-R-σy with R=R(r) (3.115) and the normality rule Δp = ˙λ∂f ∂σ with ˙λ =˙ r=˙ p(1 -D), ˙p = 2 3Δp:Δp (3.116) which ensures the plastic incompressibility. The damage evolution remains the same as for the small strain formulation of Chap. 1: ˙ D = YS s ˙p if p> pD . (3.117)

3.4 Numerical Failure Analysis 169 3.4.1.2 Multiplicative Decomposition of F The multiplicative decomposition F=FeFp (3.118) defines an intermediate relaxed configuration which in small strain plasticity corresponds to the linearly-unloaded state. It defines an elastic strain tensor, Ee=1 2 FeTFe -1 , (3.119) associated with the stress tensor Se in order to derive the elasticity law as Se=ρi ρ Fe-1σFe-1T = ρi ∂ψ ∂Ee , (3.120) with ρi the density for the relaxed configuration. The yield criterion is written as f= Σeq 1-D-R(r)-σy with Σ= 1 ρiFeTFeSe (3.121) and the normality rule of standard generalized materials gives ˙ FpFp-1 = ˙λ∂f ∂Σ with ˙λ =˙ r=˙ p(1-D) ˙p = 2 3 ˙ FpFp-1 : ˙ F pF p-1 , ˙ D = YS s ˙p if p> pD . (3.122) 3.4.1.3 Reactualized Lagrangian Formulation This formulation extends the rate formulation ˙ σ=L:˙ of small strain problems to large deformations • By considering C(t) permanently as the reference configuration: take F(t)=1 at any time t (but ˙ F =0)and • By still considering the rate formulation, but on the deformed structure. Itisthenequivalentto ˙S=L: ˙ E,withS and E defined with respect to C(t). From (3.109) and (3.110), one can see that S and E are in fact replaced by σ and Δ and after some calculations that ˙S is replaced by the Truesdell derivative of the Cauchy stress tensor dTr dt σ. For numerical finite element analysis, the extension to finite strains is in- cremental and for the computation of the solution at time tn+1, the deformed mesh C(t)=C(tn)isused.

170 3 Ductile Failures 3.4.2 Deep Drawing Limits During deep drawing or forming processes to induce large plastic deforma- tion of thin sheets, there are limitations in strains due to instabilities at small scale, instability of the phenomenon of strain localization, and crack initiation. The first limitation governs the appearance of the surfaces. The second governs the local reduction of thickness; it appears sooner in the process of hydro-forming than in classical deep drawing. The third limitation is the lo- cal rupture of the sheet. 3.4.2.1 Forming Limits by Strain Localization Knowing the loading path, the limit may be predicted by the strain damage localization criterion of Sect. 1.6.2: det( nL n)=0, (3.123) where L is the fourth order tangent operator derived from the elasto-plastic constitutive equations that may or may not be coupled with damage and n is the normal to the plane of localization. Considering the problem of plane stress in proportional loading of Sect. 3.3.4, but without any simplified hypothesis here, it is possible to find at each increment the minimum of the criterion det( nL n) with respect to any normal n and to check when det( nL n) = 0 is satisfied. Working with uniform fields of stresses and strains, we have σ = σ1 00 0σ20 000 , = 1 00 0 2 0 00-( 1 + 2) . (3.124) and Fig. 3.11 gives an example for steel with the following parameters: E = 200000 MPa, ν =0.3, σy = 200 MPa, K y p = 10000 MPa, My =1.66, pD =0, s =1,a ndS =0.5 MPa. Numerical simulations show that the shape of the curve is very sensitive to the value of the plastic exponent My of the hardening law R = K y pr1/My . 3.4.2.2 Forming Limits by Mesocrack Initiation The problem of plane stress has already been solved in Sect. 3.3.4 but with a set of simplifications to yield a closed-form solution: proportional load- ing, elastic strain neglected, hardening saturated, and damage considered as isotropic. With numerical simulations it is possible to be closer to reality where the forming processes are executed in several steps eventually on different

3.4 Numerical Failure Analysis 171 Fig. 3.11. Strain localization limit curves of deep drawing (I. Doghri 1989) machines which correspond to non-proportional loadings, inducing effects of anisotropy. Furthermore, it can be interesting to beneficiate from particu- lar loading paths to minimize the damage in order to increase the limit of forming. Let us consider again the case of a plane stress problem and look for the strain forming limits in the plane ( 1, 2). The limits are defined by the anisotropic critical damage criterion maxDI =Dc (3.125) for different proportional and non-proportional loading paths represented in Fig. 3.12 as thin lines finishing by the point of mesocrack initiation. The material is ARCELOR steel SOLDUR 355. The constitutive equa- tions are those of elasto-plasticity coupled with anisotropic damage and microdefects closure effect of Table 1.6 (Sect. 1.5). A single isotropic harden- ing is considered with an exponential law R = Ry ∞ (1 - exp (-byr)). Tensile tests performed on small specimens cut inside large plates damaged either in uniaxial tension or in plane tension, giving both the η-parameter and the anisotropic damage evolution for different stress triaxialities (see Sect. 1.3.3). The set of material parameters is: E = 230000 MPa, ν =0.3, σy = 375 MPa, Ry ∞ = 120 MPa, by = 25, pD =2.5 · 10-2, ha =0,S =0.43 MPa, s =4,η =2 .8, and Dc =0.5. Note that this corresponds to the same stress-strain response in tension as with ha =1a ndS =0.57 MPa for the model without microdefects closure effect. The computations are per- formed with the ZeBuLon FE code using the numerical implicit scheme of Sect. 2.2.5. The numerical results for many monotonic proportional loading paths allow us to build the crack initiation limit curve of deep drawing (solid curve of Fig. 3.12) in which are also reported the results for some non-proportional paths (points •).

172 3 Ductile Failures Fig. 3.12. Computed crack initiation limit curve and points of deep drawing of SOLDUR 355 (R. Desmorat and J. Besson 2004) • It is seen that very large strains may be obtained for loadings close to pure shear 2 = - 1. This is the case of hydroforming of tube-like structures with axial compression added to pressure. • The reality taking into account both localization and damage is a curve below the crack initiation curve of Fig. 3.12, with a flatter part for 1 > 0 due to easier strain localization conditions. • Some computed non-proportional loading paths exhibit a crack initiation below the proportional limit curve. Some specific non-proportional load- ings increase the limit of forming as shown by F. Moussy and J.P. Corde- bois (1990). This is mainly the case for the path 2 =2 1 up to 1 =0.1, followed by ˙ 2=-˙ 1/2 (parallel to the tensile path) up to 2 =0.29 which is found to be very beneficial. This kind of calculations offers the possibility to optimize loading paths to reach a state of strain with a minimum value of the damage. 3.4.3 Damage in Cold Extrusion Process (K. Saanouni 2002) Another important difficulty concerning the forming processes is the exis- tence and then the determination of possible local instabilities. The global instabilities are well predicted from elasto-plastic structure computations. The local instabilities leading to damage initiation and to microcrack growth can only be studied by use of the damage mechanics constitutive equations. They correspond to the reach of the critical damage Dc for the local damage

3.4 Numerical Failure Analysis 173 as in the following example or to the strain damage localization det( nL n)=0 as in the example of Sect. 3.4.4. The forward cold extrusion process consists of obtaining a bar or a wire of diameter d from a bigger bar of diameter d0 by pushing the material through a die. The quality of the result depends on several parameters: the ratio of the diameter d/d0, the angle of the die α, the lubrication, and of course the ductility of the material. The optimization of the process consists of choosing these parameters in order to obtain bars with adequate properties and to avoid large damage leading to chevrons as in Fig. 3.13. Fig. 3.13. Picture (M. Grange) and numerical simulations of damage and inside chevrons cracking during forward cold extrusion It is possible to catch this periodic phenomenon using the finite strains framework and the constitutive equations of elasto-plasticity coupled with damage of Sect. 1.5.2, Table 1.3, or something similar. The corresponding finite element analysis does not ensure the convergence regarding the mesh size but in the following example, the smallest mesh size was adjusted to correctly fit a simple tensile test calculated by an axisymmetric FEA in the softening range up to failure. For the extrusion of the circular bar of diam- eter d0 = 35 mm reduced to a diameter d = 31 mm, the meshing consists of 1312 triangular linear elements. The material is a ductile steel of yield stress σy = 300 MPa, ultimate stress σu = 390 MPa, and rupture strain R =0.7. It is represented by the damage law ˙ D =(Y/S)s1 ˙p/(1 - D)s2 , withS=500MPa,s1=2 .5, and s2 =7.5. The axisymmetric calcula-

174 3 Ductile Failures tion of the extrusion process corresponding to the picture of Fig. 3.13 was performed with FORGE 2 code using the reactualized Lagrangian formula- tion, the elements being removed when the damage reaches its critical value. The result is given in Fig. 3.13, with a close similitude with the experi- ment. The discrete appearance of the chevrons is due to the redistribution of stresses, a consequence of the coupling of damage with elasticity -- if this coupling is neglected, the damaged zone is continuous all along the axis of the specimen. As far as the specimen goes in the die, there is a large gradient of damage mainly governed by the stress triaxiality with a loss of rigidity. As the material moves on, a chevron crack forms at an angle determined by the angle of the die. At the same time the relaxation of stresses in the ligament behind the chevron does not produce any more damage until the material has moved on a certain distance to recover a damaging stress level. A new chevron crack theninitiates. . . andsoon. . . From this kind of analysis performed on many cases, the following quali- tative observations can help to decrease the risk of such damage and obtain a small damage state without any chevron: • A small diameter reduction (e.g., 16%) needs a small die angle (≈ 4◦) • A large diameter reduction (e.g., 30%) may be obtained in good conditions with a large die angle (≈ 15◦) which decreases the contact surface • A large ductility of the material is better, of course • A large friction (e.g., a friction coefficient of 0.2) can prevent the formation of chevrons but it increases the load to perform the process and damage may occur at the surface of the material due to the heavy contact with the die. Nevertheless, these results may be helpful in the preparation of a precise numerical procedure of optimization of any extrusion process. 3.4.4 Crack Initiation Direction (R. Billardon and I. Doghri 1989) The question of the direction in which a mesocrack initiates is of first im- portance if a Fracture Mechanics analysis must be performed afterwards to determine the conditions of crack growth (see Sect. 3.2.5). An example is given below using the localization criterion of Sect. 1.6.2 for which the math- ematical problem consists of determining the normal n (and the tangent operator L)whichmakes det( nL n)=0. (3.126) Consider the notched specimen of Fig. 3.14 with an out-of-axis hole of di- ameter φ = 1mm, inducing a stress concentration area which may model an initial macroscopic defect of non-negligible size at the scale of the structure. The material is an aluminum alloy 2024 at room temperature.

3.4 Numerical Failure Analysis 175 Fig. 3.14. Notched plate with a hole and iso-damage curves with the strain local- ization directions (R. Billardon and I. Doghri 1989) A monotonic displacement u(t) is applied. Before any crack initiates, the small hole ovalizes strongly and the specimen bends (without any buckling). The first crack initiates on the hole edge and propagates quickly toward the notched edge. A second crack initiates also on the hole and propagates through the whole specimen up to complete failure. The direction of the first crack is not easily guessed as it does not coincide with the shortest distance between the hole and the notch. Furthermore, the two possible directions for the crack initiated are observed on each side of the specimen, with the crack finally taking an intermediate direction. The numerical simulation of this experiment has been performed in elasto- plasticity coupled with isotropic damage with ABAQUS code. The mesh is made of 8-node isoparametric elements with reduced integration. Plane stress conditions apply. The material parameters of the 2024 aluminum alloy con- sidered are: • E = 72000 MPa, ν =0.33 for elasticity • σy = 273.5 MPa for the yield stress • R∞ = 275 MPa, b =1.86 for the exponential isotropic hardening law • C = 4950 MPa, γ =37.2 for the nonlinear kinematic hardening law • pD = pD =0,S =1.3MPa,s = 1 for damage evolution Figure (3.14) also gives the iso-damage curves around the hole at strain- damage localization where det( nL n) = 0. In agreement with the experiments,

176 3 Ductile Failures two normals of localization ( n1and n2) are obtained showing the ability of the criterion to predict the direction of the cracks initiated drawn in solid lines on the figure. 3.4.5 Porous Materials -- the Gurson Model (A.L. Gurson 1977, V. Tvergaard and A. Needleman 1984) Porous materials submitted to heavy loadings are subjected to volume or density change. Furthermore, the cavities can grow due to a ductile damage process. This is the case for geomaterials, powders, and also for certain steels where cavities may nucleate at the neighborhood of defects, grow by plastic deformation, and finally give a mesocrack by coalescence. The early Gurson model mathematically describes mainly the second mechanism. The Gurson-- Tvergaard--Needleman (GTN) model describes the three mechanisms. This model may be used in numerical structure simulations to predict flow local- ization or final failure. It is restricted to proportional loading and applies badly when the loading induces mainly shear. The basic micromechanics cell of Gurson analysis contains a hollow sphere and the damage variable is the volume fraction of cavities or the porosity fv . At microlevel the material surrounding the cavities is considered elasto-plastic with isotropic hardening R andayieldstressσs = σy + R. At mesolevel the homogenized behavior is plasticity with volume change (i.e., p kk =0). The plastic potential FGurson is obtained for proportional loading by con- sidering an appropriate velocity field in the matrix, FGurson = σ2 eq σ2 s +2q1f v cosh 3 2q2σH σs - 1 -(q1f v )2 , (3.127) with q1 and q2 as the two material parameters added by V. Tvergaard and A. Needleman to avoid an overestimation of the rupture strain which occurs for fv = fR < 1. Introduced by the same authors, the effective porosity f v models the fast coalescence of voids once a threshold fc is reached: f v= fv, iffv<fc, fc+δGTN ·(fv -fc)i ffv≥fc , (3.128) where δGTN = q-1 1 -fc fR - fc is also a material parameter. When f v = fv = 0, the plastic potential (3.127) reduces to the von Mises criterion σeq - (σy + R)=0. Remark -- The Rousselier model (1981) uses the plastic potential coupled with porosity damage fv : FRousselier = σeq ρ - R(p)- σy + dRfvσ1 exp σH ρσ1 =0, (3.129)

3.4 Numerical Failure Analysis 177 withρ= 1-f 1-f0 as the relative density and f0 as the initial porosity, and where dR and σ1 are material parameters. The normality rule applied on FGurson gives the plastic strain rate as ˙ p ij = ˙λ 3σD ij σ2 s + q1q2f v σs sinh 32 q2 σH σs δij , (3.130) where the plastic multiplier ˙λ is determined from the consistency condition FGurson =0a nd˙ FGurson = 0. The hardening law in the yield criterion is a power or exponential law function R(p) of the equivalent plastic strain p defined by the energetic equivalence σij ˙ p ij =(1- fv)σs ˙p (3.131) and p differs from the von Mises accumulated plastic strain 23 ˙ p ij˙ p ij dt. Next, the porosity evolution law ˙fv =(1- fv)˙ p kk+˙fn (3.132) states that the porosity rate is the sum of the void growth rate (1 - fv)˙ p kk determined by the plastic incompressibility of the material surrounding the cavities and the voids nucleation rate ˙fn . Phenomenological evolution laws are used to model the nucleation phenomenon assumed either controlled • by the stress, ˙fn =Aσ˙ σs+Bσ ˙ σkk 3, (3.133) • or by the plastic strain, ˙fn =An ˙p, (3.134) with Aσ, Bσ,a ndAn as material constants to be identified or, better, functions of the strains and of the stress triaxiality. The second law ( ˙fn = An ˙p) is often used with the statistically-based expres- sion An=fN SN√2π exp - 1 2 p- N SN 2 (3.135) proposed by C.C. Chu and V. Tvergaard in 1980. Three additional material parameters are introduced: • fN is the volume fraction of voids which may nucleate, fN = ∞ -∞ An(p)dp ≈ pR 0 An(p)dp 1 (3.136)

178 3 Ductile Failures • N is the mean strain at nucleation • SN is the standard deviation of the rupture strain Finally, the conditions of ductile failure are obtained through a numerical analysis of elasto-plasticity coupled with porosity. It gives the condition of localization of plastic strain together with the final rupture by coalescence of cavities and initiation of a mesocrack for f v =1/q1 that is for a poros- ity: fR=fc+ 1 δGTN 1 q1 -fc . (3.137) 3.4.5.1 Material Parameter Identification of the GTN Model Each application with a specific material needs: • The elasticity parameters E and ν . • The yield stress σy and either the power hardening parameters K y p and My or the exponential hardening parameters Ry ∞ and by (see Sect. 1.5.1) determined on specimens without any damage. • The parameters q1 and q2 governing the voids' growth are determined from numerical micromechanics analysis. In most cases good results for metals are obtained with q1 ≈ 1.5andq2 ≈ 1. • It is the same for the coalescence parameters fR and fc where estimations from numerical simulations and experiments on metals are fR =0.25 and fc =0.09 (δGTN =3.6). • The initial void volume fraction and the nucleation parameters fN, N,and SN can be estimated only from micrographs analysis at different states of deformation. N =0.3andSN =0.1 are reasonable values for metals. 3.4.5.2 Cross Identification of the Unified Damage Law ˙ D(Y, ˙ p) It is the purpose here to determine the material parameters of the damage law(˙ D =(Y/S)s ˙p) from the knowledge of the GTN parameters following the method described in Sect. 2.4.4. It is also the purpose to estimate the damage threshold in monotonic tension ( pD). Recall that for Continuum Damage Mechanics, the isotropic damage (D) may either be evaluated on unloading through the elasticity change or on the stress softening part of the stress- strain curve. As for porosity damage, the GTN model neglects the coupling of elasticity with damage, allowing us to use the stress softening effect to make a link between both theories up to a fast identification procedure based on the expressions of the yield surfaces of the damaged material. For the GTN model, the plastic potential is rewritten as FGurson = σ2 eq (σy + R)2 +2q1f v cosh 3 2q2TX - 1 -(q1f v )2 =0, (3.138)

3.4 Numerical Failure Analysis 179 with TX as the stress triaxiality 13 σkk σs . For the damage model of Chap. 1, the yield criterion is (isotropic damage) f= σeq 1-D-R-σy=0 (3.139) so that for saturated hardening σy +R = σu (the ultimate stress), the damage D measured in tension is directly related to the void volume fraction fv by simple substitution of (3.139) in (3.138), D =1- 1+(q1f v)2 - 2q1f v cosh 32 q2TX . (3.140) Next, we plot the damage D versus the accumulated plastic strain p calculated from the GTN model. As D = σ2 uRν 2ES s (p - pD) for a monotonic tensile loading, a curve fitting gives, for a given s, both the damage threshold pD and the ratio σ2 u/2ES. If no other information is available, take s = 1. If results for different stress triaxiality are available, plot dD dp vslnRν(withRν = 2 3(1 + ν)+3(1- 2ν)T 2 X). As ln dD dp =ln σ2 u 2ES s+slnRν , (3.141) s is the slope of the curve obtained. To illustrate the procedure, consider here that f v = fv (acceleration factor δGTN = 1) and the porosity remains small. With the additional assumption of a constant stress triaxiality TX (equal to 1/3 in tension), a closed-form expression may be derived from the GTN model for D vs p.Thepo r o sity evolution law becomes then ˙fv ≈ 32 q1q2fv sinh 32 q2TX + An(p) ˙p, (3.142) where ˙p is nearly the von Mises accumulated plastic strain rate. The solution for fv is fv =exp 32 q1q2 sinh 32 q2TX p · p 0 An(p)exp - 32 q1q2 sinh 32 q2TX p dp (3.143) and the damage D is calculated by use of (3.140). The D(p) curves obtained for the nucleation law An(p) (3.135) are plotted in Fig. 3.15 for different values of the parameter fN. Note that these curves could be plotted with a better accuracy (and also for larger values of the acceleration factor δGTN)fr o m computations using Gurson or GTN model implemented in a finite element code.

180 3 Ductile Failures Linear regressions of the D(p) curves correspond to the integrated unified damage law D = σ2 uRν 2ES s(p - pD). (3.144) With Rν = 1 in tension, they give for each fN the damage threshold pD and the slope σ2 uRν 2ES s . The damage exponent is determined from the stress triaxiality effect on damage growth ((3.141) with D given by (3.140)): the derivative dD dp is performed numerically and linear regression on ln dD dp |p=pgiven vs ln Rν gives s as the slope of the curve (a given accumulated plastic strain p = pgiven is considered: pgiven =0.25 for fN =0.01, 0.05, 0.1, and 0.2). TheresultsaresummarizedinTable3.1.Aninterestingpoint,adamage threshold of 0.15 is found for metals: physical existence of porosity at very small strains does not correspond to mechanical damage occurrence. Knowing the ultimate stress and the Young's modulus finally gives S. Fig. 3.15. Cross identification of the unified damage law ( N =0.3, SN =0.1). Damage D in thick line, porosity fv in thin line, damage law in dotted line

3.4 Numerical Failure Analysis 181 Ta b l e 3 . 1 . Results of cross identification for q1 =1.5, q2 =1,δGTN =1, N =0.3, and SN =0.1 fN 0.01 0.05 0.1 0.2 pD 0.15 0.15 0.15 0.15 s22.52.52.5 σ2 u 2ES 0.25 0.62 0.83 1.13 Last, consider that the reach of the critical damage Dc in tension corre- sponds to the rupture porosity f v = fR.WithTX ≈ 1/3, the critical damage is then Dc =1- 1+(q1fR)2 - 2q1fR cosh q2 2 (3.145) and ranges between 0.1 and 0.5 (nothing new!) as fR =0.1givesDc =0.17, fR =0.2givesDc =0.36, and fR =0.25 gives Dc =0.46. Example : for the values of the GTN parameters of Table 3.1 for fN =0.1and fR =0.2, the unified damage law reads: ˙ D=(0.83·Rν)2.5 ˙p if pD >0.15, Dc =0.36 -→ mesocrack initiation. (3.146) Now we have a law which can be adopted to obtain results for steel when material data are ignored! 3.4.6 Frame Analysis by Lumped Damage Mechanics (J. Fl´ orez-L´ opez 1998) The analysis of inelastic frames is an important subject in civil engineering for metallic as well as concrete reinforced structures. The plastic hinge con- cept and limit analysis are efficient tools to design metallic frames and the conventional theory is based on perfect-plasticity. The extension to damage is possible by concentrating the damage in the hinges and is called Lumped Damage Mechanics. It applies to ductile monotonic failures as well as to cyclic and dynamic (seismic) loadings. The model of a frame member between nodes i and j is made of two in- elastic hinges i and j and an elastic column whose shape and size depend on the structure studied (but of elastic behavior Fig. 3.16). Generalized stresses {M} =(Mi,Mj ,N)T and deformations {Φ} =(φi ,φj ,δ)T are used to write the frame behavior instead of stress and strain tensors in continuum mechan- ics. For instance, elasticity reads {Φ} =[S]{M} where [S] is the symmetric compliance matrix. (3.147)

182 3 Ductile Failures Fig. 3.16. Frame and lumped dissipation model of a frame member We define the complementary energy for a damaged frame member as W =1 2{M}T[˜ S]{M} and [˜ S]= S11 1-di S12 0 S21 S22 1-dj 0 00S33 1-dn (3.148) where the components of {d} = {di,dj ,dn}T are the lumped damage vari- ables. Note that the form for W is fully similar to the form for the complen- tary strain energy for anisotropic composite layers (see Sect. 7.4.1). Inelastic frame deformation {Φp} occurs due to plasticity and damage in the hinges so that the generalized state laws for elasticity coupled with damage are {Φe}={Φ-Φp}= ∂W ∂{M} , {y} = ∂W ∂{d} (3.149) or φei =φi -φp i =S11 Mi 1-di+S12Mj, φej =φj-φpj =S22 Mj 1-dj +S21Mi, δe =δ-δp=S33 N 1-dn . (3.150) For the generalized strain energy release rates, the state laws are

3.4 Numerical Failure Analysis 183 yi = S11M2 i 2(1-di)2 , yj = S22M2 j 2(1-dj)2 , yn = S33N2 2(1-dn)2 . (3.151) To complete the model and write the generalized evolution laws, we will neglect the inelastic axial effect (δ ≈ δe , dn ≈ 0). The yield function for the damaged plastic hinge i is then simply written as fi= Mi 1-di -xi -my≤0, (3.152) where my is the yield momentum and xi stands for linear kinematic hardening (parameter c): ˙ xi = c(1-di)˙φp i (no summation). (3.153) Finally, the generalized damage evolution law is ˙di = yi S s ˙ πi if πi>πD, (3.154) where π = t 0 | ˙φp|dt is the generalized accumulated plastic deformation and πD , S,ands are the frame member damage parameters. Remark -- For reinforced concrete frames, use the damage framework of Sect. 7.4.1, and consider the following as damage law: di = κ-1(yi max) and yi max =s u p τ ∈[0,t] yi(τ ) (3.155) instead of (3.154). J. Fl´ orez-L´ opez proposes modelling the crack-resistance-like phe- nomenon by using κ(di)=yi max and κ(d)=A + B ln(1 - d) 1-d (3.156) with A and B as frame member damage parameters. The frame analysis is then performed by assembling the frame members (use beam boundary conditions) and by computing the structure response to ap- plied nodal loads or displacements in case of ductile failures or to inertia forces in case of dynamic failures. There are not many nodal quantities for a real structure and the method is usually of low cost (cheaper than the mul- tifiber beam modelling of Sect. 7.4.3). Some difficulty may be encountered in the identification of the frame members parameters: S11, S12 = S21 , S22,and S33 for elasticity; my and c for plasticity; πD, S,ands for damage (or A and B for quasi-brittle damage). These parameters depend on the cross section

184 3 Ductile Failures of the member, which can have any shape, size, or reinforcement. The good thing is that damage is localized at the ends of the member frames and no in- stabilities are encountered, such as strain-damage localization in Continuum Damage Mechanics. As an illustration, Fig. 3.17 shows the kind of results expected on a frame subjected to seismic loadings. The location and size of the dots represent the damage field. A design criterion such as D<Dc or D<Dgiven tells us when and where to repair the structure. Following conventional engineering criteria, the damages encountered in frame (b) have very high values and the frame should not be repaired. Fig. 3.17. Damage distribution in a frame (M.E. Marante and J. Fl´ orez-L´ opez 1998) (a) after a low intensity shake and (b) after a severe shake 3.4.7 Predeformed and Predamaged Initial Conditions (R. Billardon 1988) The initial state of a material is a question with several answers! Most of the time, it is the state in which the material is received, but it can be before a forming process in order to calculate the process or after the process to determine the component's strength in service. It can be also the state of the material after an accident in service in order to determine the residual strength. In all cases of structure calculation, the initial state is the state corre- sponding to the specimens used for the identification of the material pa- rameters. A question arises immediately: how do we modify the constitutive

3.4 Numerical Failure Analysis 185 equations to take into account a change without performing a completely new identification procedure? This is the power of the thermodynamics approach to work with differ- ential evolution laws of state variables which may have initial values. If an identification of a set of an elasto-(visco-)plastic coupled with damage consti- tutive equations has been performed on a material in its origin state (plane sheet for example), the initial conditions to use in a structure calculation after a forming process (a deep drawing for example), or any rheological modifica- tion, are the values of the internal variables at the end of the process: • The accumulated plastic strain p0 • The corresponding isotropic hardening R0 • The corresponding kinematic hardening X 0 ij • The eventual damage D0 or, better, D0 ij Introducing these initial values in a numerical analysis consists of adding to the set of constitutive equations of Sect. 1.5 the fields of initial conditions: R(t =0,M)=R0(M) , Xij(t =0,M)=X 0 ij(M), p(t =0,M)=p0(M) in accordance with R0 and X 0 ij, D(t =0,M)=D0(M)o rDij(t =0,M)=D0 ij(M). (3.157) In a finite element analysis they must be considered at each Gauss point, which is not a major problem. The main difficulty is to know that their values are often perturbed by an other initial condition coming from a structural effect: a field of residual self-equilibrated stresses, described by σij(t =0,M)=σ0 ij(M). (3.158) The only way to properly determine these fields of initial conditions is to numerically simulate the process of their creation. Some experiments like the in situ microhardness or an X-ray analysis or a digital image correlation qmay give some indications but never enough information. Concerning the ductile failure, the influence of non-zero initial conditions in proportional loading are: • A modification of the yield stress (an increase if the original damage was zero or small), σ0 y =(σy+R0+X0 eq)(1 - D0) with X0 eq = 32X0 ijX0 ij (3.159) • A decrease of the plastic strain to rupture pR: Back to the unified damage law of ˙ D = σ2 uRν 2ES s ˙p if p>pD, (3.160)

186 3 Ductile Failures the integration with zero initial conditions gives Dc = σ2 uRν 2ES s(pR - pD). (3.161) The integration with initial conditions D0 and p0 >pD gives Dc -D0 = σ2 uRν 2ES s(pR - p0) (3.162) from which the remaining plastic strain to rupture is pR-p0 =(pR-pD)Dc -D0 Dc . (3.163) • Therefore some anisotropy can also be observed. As an example, we will describe here the method used for the determination of the remaining strength of a pressurized gas pipe that has been damaged by a shock from a digging machine (Fig. 3.18): Fig. 3.18. Injured gas pipe and "equivalent" flat specimen 1. Careful measurement of the local geometry of the indented pipe in order to make a flat specimen ready for microhardness tests (Fig. 3.18) from the same material. Its notch is made as identical as possible to the accident notch by an indentation process.

3.4 Numerical Failure Analysis 187 2. Careful measurement of the microhardness all around the notch in order to determine the damage field and the extra hardening field induced by the indentation ((1.85) and (1.81) of Sect. 1.3.4): D0 =1- ˜ H H σy σu and R0= σs 1-D0 -σy. (3.164) The accumulated plastic strain field is deduced from the plastic consti- tutive equation: p0 = R0 Ky p My . (3.165) 3. These fields are given in Fig. 3.19 for the following notch geometry and material parameters corresponding to a low carbon laminated steel: • A notch with a depth of 2 mm made by an indenter with an angle of 60◦ • Parameters of the low carbon laminated steel determined from the initial virgin material: σy = 575 MPa, K y p = 552 MPa, and My =2.04 Fig. 3.19. Fields of accumulated plastic strain and damage in the neighboring of the notch (R. Billardon 1988) 4. Assuming these fields are representative of what happened in the gas pipe, they are introduced as initial conditions by interpolation at each Gauss point in a finite element analysis performed with the code ABAQUS in elasto-plasticity coupled with damage. The analysis corresponds to the in-service pressure increased up to crack initiation at the notch. In comparison to the strength of the undamaged gas pipe, the result is

188 3 Ductile Failures a reduction of the pressure at crack initiation by an amount of about 50%. Regarding the fatigue strength due to a cyclic variation of the pressure the reduction is a factor of about 100 on the number of cycles to crack initiation. 3.4.8 Hierarchic Approach up to Full Anisotropy , From the simplest analysis that require a low level of calculation and a small number of material parameters to advanced numerical methods with the highest degree of accuracy involving a large set of experimental data, the possibility to prevent ductile failures are as follows: • Knowing only the sate of stress, use the damage equivalent stress criterion σ <σu. (3.166) • Knowing the state of the accumulated plastic strain, use the result ob- tained in Sect. 3.2.2 in proportional loading with the triaxiality deduced from an elastic calculation, p<pR with pR = pD +( pR - pD)R-s ν . (3.167) • For plane strain or plane stress problems use the damage criteria of Sect. 3.3.4. • For small scale yielding, use Neuber plastic correction of an elastic anal- ysis in order to obtain the local stress and plastic strain. Then make an integration of the unified damage law which can be either its simplest form deduced from the Gurson model in Sect. 3.4.5, ˙ D =(0.83 · Rν)2.5 ˙p if p>0.15,D c =0.36 , (3.168) its expression with saturated hardening, ˙ D = σ2 uRν 2ES s ˙p if p> pD , (3.169) or the original unified law, ˙ D= σ2 eqRν 2ES(1 - D)2 s ˙p if p> pD . (3.170) • For large scale yielding, we advise using an elasto-plastic coupled with damage numerical analysis with the anisotropic unified damage law of Sect. 1.4.3, ˙ Dij = YS s |˙ p|ij if p> pD , (3.171)

3.4 Numerical Failure Analysis 189 -- without or with the effects of microdefects closure of Sect. 1.4.3, -- without or with initial conditions of plasticity and damage as discussed in Sect. 3.4.7. • Finally, the more advanced ductile analysis within the scope of Chaps. 1 and 2 is an elasto-plastic coupled with damage analysis, including aniso- tropic damage, microdefects closure effects, non-natural initial conditions, and plastic anisotropy by use of the Hill criterion whose coupling with damage may be obtained as follows. Damage anisotropy is modelled through the use of the second order dam- age variable D, the associated tensor H =(1 - D)-1/2, and the effective stress ˜ σ = HσDH D+ σH 1-ηDH1. (3.172) For ductile failures, modelling the elastic anisotropy is not of main im- portance as elasticity may often be neglected, but modelling the plastic anisotropy can be necessary as in the case of rolling sheets, for example. A possible approach simply consists of generalizing the use of the effective stress concept: -- Keep the elasticity law unchanged: e=1+ν E˜ σ-ν Etr ˜ σ1 (3.173) -- Use the Hill anisotropic yield criterion: f= ˜ σ:h:˜ σ-R-σy (3.174) where h is the Hill fourth order tensor with minor and major symme- tries, hijlk = hijkl = hjikl = hklij , and where the hardening R follows the same anisotropy -- Keep the damage evolution law: ˙ D = YS s|˙ p| if p> pD (3.175) The only changes concerning the plasticity evolution laws are ˙ p = ˙λ∂f ∂σ = ˙λ∂f ∂˜ σ:∂˜ σ ∂σ, (3.176) which for incompressible plasticity (h such as h : σ = h : σD =(h : σ)D) gives ˙ p= ˙λ[H(h: ˜ σ) H]D √˜ σ:h:˜ σ, (3.177) with the plastic multiplier ˙λ calculated by means of the consistency con- dition f =0, ˙f =0andwhereR = R(r)andr = t 0˙ rdt= t 0 ˙λdt.

190 3 Ductile Failures In non-proportional loading, plastic anisotropy may also result from the distorsion of the yield surface which features a smooth corner with an opposite flat end in the stresses space (Fig. 3.20). Such an "egg" effect may have an influence in metal forming, as in spring back prediction in deep drawing. Adequate (complex!) 3D models can be found in the literature (T. Kurtyka and M. Zyczkowski 1985, N.K. Gupta and A. Meyers 1994, M. Fran¸ cois 2000, L. Vincent, S. Calloch and D. Marquis 2003 . . . ). To add the damage coupling, simply replace in the expressions for f the stress by the effective stress; the evolution law of the plastic strain coupled with damage is obtained by use of (3.176). Fig. 3.20. Yield surface of a 2024-T4 aluminum alloy for non-proportional loadings (Lines: model after M. Fran¸ cois (2000); small circles: experiments with an offset of δ p =10-5 (M. Rousset 1985))

4 Low Cycle Fatigue This second chapter on applications concerns the phenomenon of fatigue dam- age which occurs when materials are subjected to cyclic loadings. The clas- sical way to describe fatigue consists of splitting the domain of the numbers of cycles to rupture into three parts corresponding to different strain behav- iors and also different fields of applications: elasticity corresponds to relatively small stress amplitudes which induce large numbers of cycles to failure (larger than 105), this is "high cycle fatigue" treated in Chap. 6; elasto-plasticity corresponds to stresses above the yield stress which induce lower numbers of cycles to failure (smaller than 104), this is "low cycle fatigue;" elasto- visco-plasticity also corresponds to small number of cycles to failure (smaller than 104), but with time effects induced by creep, it is generally called "creep fatigue interaction" and is treated in Chap. 5. From a physical point of view, the repeated variations of stress induce in metals alternate plastic strains which produce internal microstresses re- sponsible of microdecohesions by slip band arrests. The microcracks initiated grow either inside the crystals or along the grains boundaries, depending on the materials and the loadings, up to coalescence corresponding to ini- tiation of a mesocrack. Plastic strain and stress both participate in this phenomenon. This is the reason the unified damage law is able to model the low cycle fatigue and in 3D directly through the concepts of accumulated plastic strain and elastic energy. Nevertheless, the main variable is the plastic strain range as it was pointed out independently in 1954 by S.S. Manson and L.F. Coffin in a famous empir- ical law called now the Manson--Coffin law. Many improvements followed (J.D. Morrow 1964, G.R. Halford 1975, A. Pineau 1980, D. Socie 1991) up to Continuum Damage Mechanics for which the difficulty to define a cycle is solved by a time integration of the damage law on the full time history of the loading. The specific items of this chapter are the cyclic elasto-plastic stress con- centration analysis, the effects of loading history, and the application to multiaxial fatigue and elastomers.

192 4 Low Cycle Fatigue 4.1 Engineering Considerations Low cycle fatigue failures may occur when structures are subjected to heavy cyclic loadings which induce irreversible strains on small or large scale, giving rise to damage up to crack initiation and propagation. To avoid this phenomenon, a careful assessment of information on the development of dam- age is needed in order to quantify a safety margin. What is called here a cycle is most often the service time between the start and the stop of a plant operation or the repetition of a heavy loading. The number of cycles to rup- ture (NR), corresponding to states of stress which induces plastic strains, is relatively small or "low": • It can be on the order of 10 to 100 for aerospace rockets where some tests are necessary before launching or for metal forming by forging. The state of stress lies between the ultimate stress and the yield stress, σu >σ>σy . • It can be on the order of 100 to 1000 for nuclear or thermal power plants, chemical plants, and many domestic apparatus as the butt hinges of poly- meric boxes! The state of stress is somewhat higher than the yield stress, σy. • It can be on the order of 1000 to 10000 for aircraft engines or car engines where, on some parts, the state of stress induces plastic strain on the order of the elastic strain, p ≈ σy/E. • NR > 105 corresponds to high-cycle fatigue where the mesoscopic strains may be considered elastic, but not the microscopic ones. It is described in Chap. 6. • Fo r 1 0 4 <NR < 105, low- or high-cycle fatigue may be considered de- pending on the case and, moreover, on the degree of accuracy needed. Low cycle fatigue is mainly governed by the dissipative strain at mesolevel and it is essentially encountered in metals, polymers,andelastomers. 4.2 Fast Calculation of Structural Failures In low cycle fatigue, if the steady state of plastic strain is known at the critical point of a structure that is loaded periodically, there is no need to perform a complicated calculation to determine an approximative value of the number of cycles leading to a mesocrack initiation. Furthermore, if the plasticity is localized, there is a possibility to obtain the plastic strain range from a purely elastic calculation and a correction which is an extension of the Neuber method of Sect. 3.2.4. "Fast" also means "simple" here and the dam- age is considered isotropic and equally produced in tension and compression. 4.2.1 Uniaxial Behavior and Validation of the Damage Law The basic low cycle fatigue characteristic of a material is its Manson--Coffin curve which gives the number of cycles to rupture of uniaxial specimens

4.2 Fast Calculation of Structural Failures 193 periodically loaded in tension-compression, at constant range of total strain Δ , and as a function of the range of plastic strain. An example is given in Fig. 4.1. Fig. 4.1. Manson--Coffin curve of UDIMET 700 alloy at room temperature (J. Lemaitre and J.L. Chaboche 1985) As in a log-log graph, the curve is close to a straight line. It can be represented by the empirical law of Manson--Coffin, NR = CMC Δ p γMC , (4.1) where CMC and γMC are material parameters: CMC depends on the temper- ature but γMC is close to 2 regardless of the material and the temperature. Furthermore, an extrapolation of the curve to NR = 1 corresponds to a test for which the range of plastic strain is close to two times the rupture plastic strain pR in a monotonic tension test. Then CMC≈2 pR. (4.2) When no fatigue tests are available for a given material, a rough estimation for an early design purpose is NR = 2 pR Δ p 2 . (4.3) Let us recall that this Manson--Coffin curve, also called the "W¨ ohler curve in the range of low cycle fatigue" in Sect. 1.4.4, is one of the main data source for the identification of the unified damage law

194 4 Low Cycle Fatigue ˙ D = YS s ˙p if p>pD. (4.4) In the following, we assume that the damage parameters S, s, pD, m, and Dc defined in Sect. 1.4 are known for each application. Nevertheless, we strongly advise checking each time it is possible with new tests results or informations that their values give good low cycle fatigue results (particularly for s and m). For more details, you should read Sects. 1.4.4 and 2.4 again. Both sections are devoted to the difficult problem of material parameters identification. 4.2.1.1 Case of Periodic Loading Consider an uniaxial periodic loading of strain range Δ at zero mean stress (Fig. 4.2) for the applied stress ±σM. Fig. 4.2. Schematic low cycle fatigue Beyond the damage threshold, the increment of damage per cycle ( δD δN) comes from a first integration of the uniaxial damage law, in which, for sim- plicity, the damaged material is considered as perfectly plastic at σ 1-D ≈ σM = const: ˙ D= σ2 2ES(1 - D)2 s |˙ p| if p>pD =⇒ δD δN = 1cycle ˙ Ddt = σ2 M 2ES s 2Δ p . (4.5) A second integration gives the number of cycles to rupture (NR) correspond- ing to the critical value of the damage Dc for the initial condition: N=ND= pD 2Δ p → D=0, (4.6)

4.2 Fast Calculation of Structural Failures 195 with (see Sect. 1.4.1): pD= pD σu-σy σeq max + σeq min 2 -σy m = pD σu - σy σM - σy m . (4.7) Then, NR=ND+ Dc 2Δ p 2ES σ2 M s . (4.8) The number of cycles to rupture is a power function of the stress range and is a linear function of the plastic strain range. Just to compare with the Manson--Coffin law, consider σM as a power function of Δ p given by the cyclic tension-compression curve Δσ =2σM = KcΔ 1/Mc p. (4.9) Then, NR ≈ const + const Δ p 2s Mc +1, (4.10) which shows that the value of the exponent s is on the order of Mc/2, at least for steels, to make 2s Mc +1≈ 2 as in the Manson--Coffin law. Before using any of the unified damage law identified as explained in Sects. 1.4.4 and 2.4, we advise checking if the values of the materials in the formula (4.8) give the proper number of cycles to rupture in comparison with some available test data and eventually adjusting the most sensitive parameters (see Sect. 4.2.3). 4.2.1.2 Case of Non-Periodic Loading When the range of stress varies as a function of the number of cycles, the problem of accumulation of damage arises. The Palmgreen--Miner rule (1924, 1945) consists of the simple summation of damages supposed to be proportional to the number of cycles for a given constant range. If ni is the number of cycles of an applied strain range Δ i and NRi is the number of cy- cles to rupture corresponding to this range constant all along the process, the corresponding damage is supposed to be niDc/NRi. Then for many loadings, the linear rule of summation is simply niDc NRi =Dc → ni NRi =1 (4.11) and ni = NR is the number of cycles to rupture corresponding to the entire sequence of Δ i.

196 4 Low Cycle Fatigue In fact, this rule is a property of any differential equation, linear or non- linear, representing the damage evolution. But unfortunately, materials do not wish to obey mathematics! The accumulation of damage is most often nonlinear. Let us show it with the continuous damage law applied to two-level fatigue loadings. Fig. 4.3. Two level fatigue loading Consider the loading represented in Fig. 4.3 and assume that the dam- age initiates (at ND1 cycles) during the first level (n1 >ND1). Using (4.5) together with σM1 = Δσ1 2 and Δ 1 = const, the damage D(n1)attheendof the first level is D(n1)=(n1 - ND1) σ2 M1 2ES s 2Δ p1 , (4.12) or together with eq. (4.8), D(n1)=Dc n1 - ND1 NR1-ND1 . (4.13) The damage at the end of the second level n2 is equal to the mesocrack initiation condition Dc .Withn1 + n2 = NR, Dc(NR)=D(n1)+n2 σ2 M2 2ES s 2Δ p2 , (4.14) or Dc(NR)=Dc n1 - ND1 NR1-ND1+Dc n2 NR2-ND2 , (4.15) or n1 NR1+n2 NR2 1-ND1 NR1 1-ND2 NR2 =1. (4.16) This shows that

4.2 Fast Calculation of Structural Failures 197 •n1 NR1+n2 NR2 < 1ifthehighlevelisfirst ND1 NR1 > ND2 NR2 •n1 NR1+n2 NR2 > 1 if the low level is first ND1 NR1 < ND2 NR2 • The Miner rule n1 NR1+n2 NR2 = 1 of linear accumulation is generally not recovered as it corresponds to the particular case ND1 NR1 = ND2 NR2 Fig. 4.4. Bilinear damage accumulation in two-level fatigue loadings In fact, the rule obtained is a bilinear rule in the diagram n2/NR2 vs n1/NR1 because (a) If n1 >ND1, the damage initiates during the first loading level. The number of cycles to rupture, NR = n1 + n2 (with n1 known), is given by (4.16). (b) If n1 <ND1, the damage initiates during the second loading level. The number of cycles to rupture, NR, is given by the damage equation, NR -ND NR2 -ND2 =1,whereND is determined by the stored energy balance: wD = ND1Δws1 = ND2Δws2 = n1Δws1 +(ND - n1)Δws2 (4.17)

198 4 Low Cycle Fatigue or ND = n1 +(ND1 - n1)Δws1 Δws2 with Δws1 Δws2 = ND2 ND1 . (4.18) As NR = n1 + n2 the final relationship is: n1 NR1 ND2 ND1 NR1 NR2+n2 NR2 =1. (4.19) An angular point corresponds to the case ND1 = n1 of damage initiating at the exact time of the level transition. An example is given in Fig. 4.4 for ND/NR =0.225 and 0.58. 4.2.2 Case of Proportional Loading The case of proportional loading is somewhat similar to the uniaxial case as all the tensors are colinear due to the fixed principal directions of the stress tensor (see Sect. 2.1.2). This is the case at all points of a structure if the applied loads vary proportionately with one parameter. If the loading is periodic, the number of cycles to rupture is obtained from two integrations of the damage law: ˙ D= σ2 eqRν 2ES(1 - D)2 s ˙p if p>pD. (4.20) • A first integration over one cycle: the material is again considered per- fectly plastic for each maximum stress σeq 1-D ≈ σeqmax = const;the triaxiality function Rν is also constant due to the loading proportionality, δD δN = σ2 eq maxRν 2ES s 2Δp if p>pD , (4.21) where Δp is the accumulated plastic strain increment over half of acycle. • A second integration over the whole process with the initial condition N=ND= pD 2Δp → D=0, (4.22) with pD= pD σu-σy σeq max - σy m . (4.23) Then NR=ND+ Dc 2Δp 2ES σ2 eq maxRν s . (4.24)

4.2 Fast Calculation of Structural Failures 199 It is interesting to compare this number of cycles to rupture to the uniaxial case as NR(σij) - ND(σij) NR(σ) - ND(σ) = Δ p Δp σ2 M σ2 eq maxRν s . (4.25) Using the damage equivalent stress σ = σeqR1/2 ν gives the possibility to derive the number of cycles to rupture of a multiaxial state of stress defined by σeq max , Rν and the accumulated plastic strain range Δp from only one experimental point NR(Δ p,σM) of the Manson--Coffin curve (knowing the exponent s) if the approximation ND/NR = const is made: NR(σij) NR(σM) = Δ p Δp σ M σM -2s . (4.26) 4.2.3 Sensitivity Analysis The general method is described in Sect. 2.4.6. It is applied here to the number of cycles-to-crack-initiation (NR) found in Sect. 4.2.2 in order to obtain the relative influence of the loading and of the material parameters on NR: NR=ND+ Dc 2Δp 2ES σ2 eq maxRν s , ND= pD 2Δp σu-σy σeq max - σy m , (4.27) withRν =2 3 (1 + ν)+3(1- 2ν)T 2 X. The relative error δNR NR is determined by the logarithmic derivative of the above equation in the same manner as for ductile failure of Sect. 3.2.3: ln(NR -ND)=lnDc -ln2-lnΔp +s(ln2+lnE+lnS-2lnσeq max -lnRν). (4.28) Here we take the absolute value δx = |dx| as the sign of the error is not known: δ(NR - ND) NR-ND =δNR NR NR NR-ND-δND ND ND NR-ND, δND ND = δ pD pD + δΔp Δp+ ln σu - σy σeq max - σy m δm m +mδ(σu -σy) σu-σy +mδ(σeq max - σy) σeqmax-σy , δRν Rν =δν ν |6T2 X-2 3|ν Rν +δTX TX 6(1-2ν)T2 X Rν . (4.29)

200 4 Low Cycle Fatigue The coefficients SNR Ak of the sensitivity matrix of Sect. 2.4.6 are defined by δNR NR = k SNR Ak δAk Ak, (4.30) SNR TX =NR-ND NR 6s(1 - 2ν)T 2 X Rν , SNR σeqmax =NR-ND NR 2s+ND NRm σeqmax σeqmax-σy, SNR Δp=NR-ND NR +ND NR =1, SNR E =NR-ND NR s, SNR ν =NR-ND NR |6T2 X-2 3 |νs Rν , SNR σy =ND NRm σy σu-σy+ σy σeq max - σy , SNR pD=ND NR, SNR m =ND NRm ln σu - σy σeq max - σy , SNR σu =ND NR mσu σu-σy, SNR S =NR-ND NR s, SNR s =NR-ND NRs ln 2ES σ2 eq maxRν , SNR Dc =NR-ND NR. (4.31) The value of those coefficients are the height of the boxes in Fig. 4.5 for the following set of parameters representing an average of many materials: TX =1,Rν =2.07, σeq max = 400 MPa, σeq max/σy =1.5, E = 200000 MPa, ν =0.3, σu/σy =2,S =2MPa,s =5,m =2,andNR/ND =2. The loading is represented by the triaxiality ratio, the stress, and the ac- cumulated plastic strain. The influence of an error on the stress is the largest (and is larger than for ductile failures) but the influence of the accumulated plastic strain is small. The parameters which do not need a large accuracy are m, pD and Dc . Altogether, do not expect an accuracy better than a factor 2 on the number of cycles to rupture.

4.2 Fast Calculation of Structural Failures 201 Fig. 4.5. Relative importance of each parameter in low cycle fatigue 4.2.4 Cyclic Elasto-Plastic Stress Concentration As for the Neuber method described in Sect. 3.2.4, it is possible to determine the plastic strain range under the small scale yielding assumption from both • A reference elastic calculation and • The cyclic stress-strain curve of the material in tension-(compression). In fact, as far as free edges are concerned and as long as plasticity remains very localized (this is often the case in fatigue), the strain energy density (SED) method gives better results in cyclic loading than the Neuber method. An illustrative example is shown in Sect. 4.4.2. This is why the cyclic Neu- ber method for unidimensional cases only is described here. Such a case is encountered on free edges of thin structures for which the state of stress is local tension-compression, with a stress triaxiality TX =1/3a ndastr e s s triaxiality function Rν =1. 4.2.4.1 Cyclic Neuber Method TheNeubermethodinfatigueiswrittenintermsofstress,strain,andplastic strain ranges over a cycle and is based on the local equality ΔσΔ =(ΔσΔ )elas at the stress concentration point, (4.32)

202 4 Low Cycle Fatigue which is also written as ΔσΔ = K2 T E (Δσn)2 , (4.33) with KT as the stress concentration coefficient in elasticity and σn as the nominal stress (see Fig. 3.4). A law of cyclic plasticity has to be considered in order to estimate the ranges Δσ,Δ ,Δ p,andΔp = |Δ p| (the accumulated plastic strain incre- ment over half a cycle). The cyclic power law (4.9), Δ p = Δσ Kc Mc , (4.34) may be used but further explicit results will be obtained with the linear law Δ =Δσ E +Δσ-2σy Cy , (4.35) Δp=|Δ p|= Δσ -2σy Cy , (4.36) which comes from the consideration of a linear kinematic hardening only where X = Cy p. The equality Δσ E +Δσ-2σy Cy Δσ=K2 T E (Δσn)2 (4.37) gives the platic stress range Δσ when KTΔσn > 2σy for cyclic plasticity to occur. Equation (4.36) gives the accumulated plastic strain increment per cycle as δp δN =2Δp =2Δσ - 2σy Cy . (4.38) If the loading is symmetric, σmax = -σmin =Δσ/2 gives the maximum and minimum stresses reached locally at the most loaded point. If the loading is non-symmetric, the maximum stress σmax has to be de- termined first by use of the monotonic Neuber method (see Sect. 3.2.4). Equation (4.37) gives Δσ and the stress corresponding to the mimimun load is σmin = σmax - Δσ. (4.39) We will consider next the SED method. In order to deal with non- symmetric loading we first need its expression for the monotonic case.

4.2 Fast Calculation of Structural Failures 203 4.2.4.2 Monotonic SED Method The strain energy density (SED) method assumes that at the stress concen- tration point, the strain energy density in confined plasticity is identical to the strain energy density at the same point, but calculated in elasticity. For 1D monotonic loadings, 0 σd = elas 0 σelasd elas = K2 T 2E σ2 n. (4.40) The local stress in plasticity, σ>σ y , is estimated by solving this equation coupled with the constitutive law = σ/E + R-1(σ - σy)=σ/E + g(σ), where R(p) is the hardening rule. For 3D monotonic loadings,themethodsolv es ij 0 σijd ij = elas ij 0 σelas ij d elas ij =1 2 (σij ij)elas , (4.41) locally written at the stress concentration point with the Hencky--Mises law p = g(σeq) as a complementary equation. It may be rewritten as σ2 eqRν 2E + σeq σy σeqg (σeq)dσeq = 1 2 (σij ij)elas . (4.42) The term (σij ij)elas comes from the elastic reference computation, it is equal to σelas eq 2Relas ν /E with σelas eq and Relas ν as the von Mises stress and the triaxiality function calculated in elasticity, respectively. The method gives σeq and p in plasticity. It needs the value of the triaxial- ity function Rν . For general three-dimensional cases we use the proportional loading assumption Rν = Relas ν .Weu s eRν = 1 for points located on free edges in plane stress. For points located on free edges in plane strain (see Sect. 2.1.4 for details concerning the calculation of the stress triaxiality in two-dimensional cases) we use Rν =1.27. Let us explicitly describe the three-dimensional method in two useful cases: (a) Monotonic SED method with linear isotropic hardening R = Cyp.The von Mises stress in plasticity σeq is a solution of σ2 eqRν 2E + σ2 eq-σ2 y 2Cy =1 2 (σij ij)elas , (4.43) which leads to the closed-form expression

204 4 Low Cycle Fatigue σeq = E (σij ij)elas + E Cy σ2 y Rν+E Cy (4.44) and defines the auxiliary ratio kSED = σeq σelas eq . (4.45) The accumulated plastic strain is p=σeq-σy Cy. (4.46) (b) Monotonic SED method with nonlinear isotropic hardening R = Ry ∞(1- exp (-byp)). One has to solve the following equation numerically: σ2 eqRν E +(Ry ∞ + σy)g(σeq) - 1 by σeq-σy =1 2 (σij ij)elas , (4.47) where p = g(σeq)=- 1b ln R∞ + σy - σeq R∞ . The graphs of Fig. 4.6 show how the SED method differs from the Neuber method. Fig. 4.6. Cyclic Neuber and SED methods 4.2.4.3 Cyclic SED Method For locally-cyclic 1D state of stress, to obtain a closed-form solution, the SED method considers

4.2 Fast Calculation of Structural Failures 205 Δ 0 ΔσdΔ = Δ elas 0 ΔσelasdΔ elas = K 2 T 2E (Δσn)2 (4.48) instead of (4.37) altogether with the cyclic constitutive law (4.34) or the linear law (4.35). For three-dimensional loadings, the SED method gives the equivalent stress range (Δσ)eq as the solution of Δ ij 0 Δσij dΔ ij = Δ ij 0 Δσij dΔ ij elas , (4.49) which has to be considered coupled with a law of cyclic plasticity Δ ij = Δ ij(Δσij )andwhereΔσij and Δ ij stand for the stress and strain ranges. In case of linear kinematic hardening, X = 2 3 Cy p, and with the hypoth- esis of a proportional loading, the cyclic plasticity law is Δ ij = 1+ν E Δσij-ν E Δσkkδij +Δ p ij, Δ p ij= 3 2Cy ΔσD ij (Δσ)eq (Δσ)eq - 2σy , (4.50) with the accumulated plastic strain increment over half a cycle equal to Δp = (Δσ)eq - 2σy Cy . (4.51) The closed-form expression for the equivalent stress range is then (Δσ)eq = E (Δσij Δ ij)elas + E Cy 4σ2 y Rν+E Cy . (4.52) To finish, the method defines the auxiliary ratio kcyclic SED = (Δσ)eq (Δσ)elas eq . (4.53) Compared to the monotonic case, the three-dimensional cyclic method for linear kinematic hardening is formally obtained by replacing σeq with (Δσ)eq, σelas eq with (Δσ)elas eq ,(σij ij)elas with (Δσij Δ ij)elas,andσy with 2σy. Note that the same replacements within the Neuber monotonic expression for linear isotropic hardening gives the closed-form solution for the Neuber cyclic method with linear kinematic hardening. 4.2.4.4 Cyclic SED Method Applied to Fatigue Failures Applying the cyclic method takes 3 steps:

206 4 Low Cycle Fatigue 1. Perform the elastic reference computation To simplify, consider the case of proportional loading for which all applied loads or displacements have fixed directions and are proportional to the scalar function of time α(t), periodical between αmin < 0andαmax > 0. Due to elasticity's linearity, a single computation performed for the con- stant reference value α = αref is needed. It gives the map of von Mises stress σref eq (M), the stress triaxiality T ref X(M),andRν =Rref ν (M). Then, in any point of the structure, σelas eq (M, t)= |α(t)| αref σref eq(M), Rν(M, t)=Rref ν (M), σelas eq min(M)=- αmin αref σref eq(M), σelas eq max(M)= αmax αref σref eq(M). (4.54) The equivalent stress range at any point of the elastic computation is then (Δσelas)eq = σelas eq max + σelas eq min (4.55) and (Δσij Δ ij)elas = (Δσelas)2 eqRref ν E =(αmax + |αmin|)2 σref eq 2Rref ν E . (4.56) 2. Apply the cyclic SED method Determine the most loaded point as the point where the damage equiv- alent stress (σ = σelas eq R1/2 ν ) is maximum. Use, for instance, Eq. (4.52) to determine at this point the equivalent stress range (Δσ)eq in localized plasticity. The accumulated plastic strain increment per cycle is (4.51): δp δN = 1cycle ˙pdt =2Δp. (4.57) If the loading is non-symmetric, i.e., if αmin = -αmax , use the monotonic SED method (4.44) or (4.47) to determine the maximum von Mises stress σeq max . The von Mises stress for α = αmin is then σeq min =(Δσ)eq - σeq max . (4.58) If the loading is symmetric, simply take σeq max = σeq min = (Δσ)eq 2. 3. Calculate the damage and the number of cycles to rupture Once p = pD is reached, the damage D increases twice per cycle, each time corresponding to yield in tension (plastic strain increment Δp+, damage

4.2 Fast Calculation of Structural Failures 207 increment ΔD+) and compression (plastic strain increment Δp- , damage increment ΔD-). For the fatigue loading between αmin and αmax to consider a linear kine- matic hardening leads to a stabilized stress-strain cycle, Δp+=Δp- =Δp=1 2δp δN, (4.59) and a damage increment per cycle δD δN = 1cycle ˙ Ddt =ΔD+ +ΔD- . (4.60) With sufficient accuracy for fatigue applications, neglect the coupling of the energy density release rate Y with damage and consider that it does not vary much between the applied load inducing the reach of the yield stress and the maximum load αmax inducing the maximum von Mises stress σeq max , i.e., ΔD+ = Ymax S sΔp+ and Ymax ≈ σ2 eq maxRν 2E . (4.61) Close to the minimum load αmin inducing the minimum von Mises stress σeq min , ΔD- = Ymin S sΔp- and Ymin ≈ σ2 eq minRν 2E . (4.62) The damage increment over one cycle of loading is then δD δN = (σ2s eqmin+σ2s eq max)Rs ν (2ES)s Δp if Δσeq>2σy, p>pD (4.63) and δD δN = 0 otherwise. Then the damage after N cycles is D(N)=(σ2s eqmin+σ2s eq max)Rs νΔp (2ES)s (N - ND) , (4.64) where ND = pD 2Δp is the number of cycles to reach p = pD. Finally, NR = ND + (2ES)sDc (σ2s eqmin+σ2s eq max)Rs νΔp (4.65) is the number of cycles-to-mesocrack-initiation. For a complex history of loading, a numerical integration of the damage evolution law is necessary to obtain the mesocrack initiation condition of D=Dc.

208 4 Low Cycle Fatigue 4.2.5 Safety Margin and Crack Growth In fatigue, the sensible parameter on which to evaluate the security is the number of cycles. A safe design, for which the estimated number of cycles of loading for the whole life of a component is Nservice , may be defined as Nservice < NR Saf , (4.66) where NR is the number of cycles to rupture determined by a calculation tak- ing into account the estimated history of loading and Saf is the safety factor. Saf = 20, 10, or 5, depending on the "state of the art" of the application. Once the mesocrack is initiated, the low cycle crack growth is generally pretty fast due to the high level of loading. So, there is often no need of a crack growth calculation. It is sufficient to check the condition of crack arrest or to check the whole ductile rupture by instability using the "R-curve" method described in Sect. 3.2.5. 4.3 Basic Engineering Examples The same basic geometries and directions of loading as in Sect. 3.3 are ex- amined here from the point of view of low cycle fatigue. The change is in the cyclic calculation of the stress concentration and the life duration expressed in terms of the number of cycles. Isotropic damage without the microdefects closure effect allows for closed-form solutions. 4.3.1 Plate or Members with Holes or Notches Consider, as in Sect. 3.3.1, any problem of a structure with a geometrical weakness to which corresponds a uniaxial stress concentration coefficient KT, but with a cyclic loading on the nominal stress σn here: σelas = KTσn -→ σmax elas = KTσmax n , Δσelas = KTΔσn . (4.67) Values of coefficients KT for many cases are given in handbooks (see bibliog- raphy). Plasticity occurs at least in the neighborhood of the extremal values of the stress and the cyclic SED uniaxial correction applies as the critical point is assumed to be at a free surface, σmax = kSEDσelas Δσ = kcyclic SED Δσelas -→ σmax = kSEDKTσmax n , σmin = KT kSEDσmax n - kcyclic SED Δσn ,(4.68)

4.3 Basic Engineering Examples 209 with kSED and kcyclic SED given by the monotonic and cyclic SED methods of Sect. 4.2.4 (Eqs. (4.45) and (4.53)). • If the loading is periodic at zero mean stress, equations of Sect. 4.2.1 apply: the number of cycles leading to a mesocrack initiation for a stress range Δσn =2σM is NR= pD 2Δ p σu - σy σM-σy m+ Dc 2Δ p 2ES σ2 M s , (4.69) with σM and Δ p given by the cyclic SED (or the Neuber) method. If 8 material parameters are too much, there is a possibility to derive a much simpler formula if one low cycle fatigue experimental result is known: -- Assume that a maximum stress σM0 and a plastic strain range Δ p0 give a known number of cycles to rupture, NR0 , -- As the number of cycles ND to reach the damage threshold is often small in comparison to NR, it is neglected. Then NR≈Dc 2Δ p 2ES σ2 M s . (4.70) -- As the material parameters verify, NR0≈ Dc 2Δ p0 2ES σ2 M0 s . (4.71) Then, the number of cycles to failure reads: NR ≈ NR0 Δ p0 Δ p σM0 σM 2s . (4.72) • If the loading is not periodic but if σM(N)andΔ p(N) are known as func- tions of the number of cycles by the SED correction, the first integration of Sect. 4.2.1 applies: δD δN = σ2 M 2ES s 2Δ p , (4.73) but the second integration is replaced by Dc = NR 0 σ2 M(N) 2ES s 2Δ p(N)dN, (4.74) where the number of cycles to reach the damage threshold is neglected. This gives the number of cycles to mesocrack initiation as the implicit solution of a nonlinear equation, usually solved by use of mathematical software.

210 4 Low Cycle Fatigue 4.3.2 Pressurized Shallow Cylinders It is the same example as in Chap. 3 except that the pressure varies periodi- cally between 0 and PM (Fig. 4.7) Fig. 4.7. Cyclic pressurized cylindrical cylinder Let us recall from the stress analysis of the pressurized cylinder of Sect. 3.3.2 that σeq=√3 2 PRcyl tcyl ,T X=σH σeq=1 √3, and Rν =5-4ν 3 , (4.75) with P as the internal pressure, Rcyl as the cylinder radius and tcyl as its thickness. The difference with the monotonic loading is in the plastic constitutive equation which must take into account the effect of cyclic loading by the kinematic hardening. There are two possibilities (Fig. 4.8): Fig. 4.8. Elastic (left) and plastic (right) shakedown in cyclic loading

4.3 Basic Engineering Examples 211 1. The material has a small kinematic hardening for the stress considered; there is adaptation or elastic shakedown after the very first cycle which makes all the subsequent cycles elastic. The accumulated plastic strain rate remains zero and there is no damage and no failure by low cycle fa- tigue. There can be failure by high-cycle fatigue, in that case use the two-scale damage model (applications in Chap. 6). This condition of adaptation arises if σeqmax≤2σy or Pmax≤ 4 √3 σy tcyl Rcyl . (4.76) 2. The material has a kinematic hardening high enough for the stress consid- ered, σeq max > 2σy, so that hysteresis loops exist, leading to a stabilized cycle of plastic shakedown. Then ˙p = 0 and the phenomenon of low cycle fatigue occurs. In this case, the damage law, ˙ D= σ2 eqRν 2ES(1 - D)2 s ˙p if p>pD, (4.77) has to be integrated once over a cycle to give δD δN and once over the whole process. Considering linear kinematic hardening and neglecting the variation of the damage over one cycle, δD δN =2 σeq max 2σy σ2 eqRν 2ES(1 - D)2 s dσeq Cy(1 - D) (4.78) or δD δN= 2 Cy(2s +1) Rν 2ES(1 - D)2 s σ2s+1 eq max - (2σy)2s+1 1-D . (4.79) For the second integration, Dc 0 (1-D)2s+1dD= 2 Cy(2s +1) Rν 2ES s σ2s+1 eq max - (2σy)2s+1 NR ND dN (4.80) or NR=ND+2s+1 2s +2 1-(1-Dc)2s+2 2 Cy Rν 2ES s σ2s+1 eq max - (2σy)2s+1 ,N D=pD 2Δp , (4.81)

212 4 Low Cycle Fatigue with pD= pD σu-σy σeq Max 2 - σy m , Δp= σeqmax -2σy Cy , σeqmax =√3 2 PmaxRcyl tcyl , and Rν =5-4ν 3. (4.82) For design purposes, it is interesting to see that the ratio Rcyl/tcyl acts on the number of cycles to rupture at the power (2s +1). 4.3.3 Cyclic Bending of Beams Cyclic bending is the fatigue process by which kids or older people break a metallic wire with an increase of the temperature which may burn the fingers! This is the same problem of a beam loaded in circular bending of Sect. 3.3.3, but here the applied curvature 1/ρ is periodic with a mean value equal to 0 (Fig. 4.9). Please refer to Sect. 5.3.4 for the consideration of the coupling with temperature. The critical point where the mesocrack will initiate is of course on the upper or lower part of the beam where the plastic strain varies between pmax and pmin = - pmax, a value related to the radius of curvature ρ by the simple Bernoulli theory of beams in which the elastic strain is neglected: lρ = l pmax h2 or pmax=h 2ρ. (4.83) Then the problem reduces to a simple case of tension-compression plastic- strain imposed between -h/2ρ and h/2ρ, where the redistribution of stress due to plasticity and damage is neglected. Fig. 4.9. Cyclic bending of a beam

4.4 Numerical Failure Analysis 213 Back to Sect. 4.2.1 and neglecting also the number of cycles to reach the damage threshold, we have NR=Dc 2Δ p 2ES σ2 M s , (4.84) with Δp= pmax- pmin = hρ. The term σM is the stress corresponding to pmax which may be deter- mined from the cyclic stress-strain curve of the material. Taking Δ p = 2σM Kc Mc , (4.85) this shows that the number of cycles to a mesocrack initiation is proportional to the radius of curvature at the power (1 + 2s Mc ),whichisontheorderof2 for steel (as s ≈ Mc/2), as follows: NR=Dc 2 8ES K2 c s ρh 1+ 2s Mc . (4.86) 4.4 Numerical Failure Analysis Practical applications concern structures made of different mechanical com- ponents and different materials submitted to complex loadings, fatigue load- ings here. The full computations of whole structures are difficult to perform as a fully-coupled damage analysis is computer-time consuming and as, com- pared to monotonic applications, the time increments are multiplied by a fac- tor of 10 to 10000 cycles of fatigue. The two ways to handle Continuum Damage Mechanics in low cycle fa- tigue are: • The fully coupled analysis which needs big computers and modern computation methods such as sub-structuring and parallelism. It is of course the best quality one can expect for structures computation. It is also the easiest way for an FE code user to make the calculation and analyze the results. The use of a large time increment method (P. Ladev` eze 1989) eventually coupled with parallelism computing allows the user to save time by calculating the stabilized cycle straightforwardly. The damage maps may be drawn at any time increment. The most loaded point is easily determined as the location of the maximum damage. The time or number of cycles to rupture corresponds to the reach of the critical damage Dc or the phenomenon of strain localization (see Sect. 1.6).

214 4 Low Cycle Fatigue • The post-processing analysis which needs a reference computation performed either in elasticity or elasto-plasticity, and the application of a post-processor solving the damage constitutive equations cycle by cycle, with a time step integration for each cycle. This assumes of course no damage coupling with the strain behavior and in most cases yields a lower bound on the number of cycles to rupture that is a safe result regarding the security. Furthermore, for periodic loadings there is a possibility to apply the jump-in-cycles procedure of Sect. 2.1.5 to save computer time. 4.4.1 Effects of Loading History (R. Desmorat and J. Besson 2003) Due to the nonlinearities occurring in the damage growth, the accumulation of the damages created by different amplitudes of loading is not simple. Their order of occurrence has an effect that is sometimes beneficial, sometimes not. Let us illustrate this using some examples. The material is the SOLDUR 355 steel of Sect. 3.4.2 but with kinematic hardening here. Anisotropic damage and microdefects closure effect are considered together with (see Sect. 1.5.3): • E = 230000 MPa, ν =0.3 for elasticity • σy = 375 MPa as yield stress •Xy ∞ =120MPa,γy=25,Cy=γyXy ∞ = 3000 MPa for hardening • pD =2.5 · 10-2, σu = 474 MPa, m =2.5 for the damage threshold • ha =0,S =0.43 MPa, s =4,η =2.8, Dc =0.5 for damage The calculations are performed with the ZeBuLon computer code using the full elasto-plastic damage coupling with the implicit scheme of Sect. 2.2.5. The damage threshold is determined by (1.117) of Sect. 1.4.1 for multilevel fatigue applications. It is pD= pD σu-σy σM1 - σy m (4.87) when damage initiates during the first level of stress range σM1.Itis pD = 1/m pD σu-σy σM2-σy+p1/m 1 σM2 - σM1 σM2 - σy m (4.88) when damage initiates during the second level of stress range σM2 after n1 cycles, at the first level up to an accumulated plastic strain p(n1)=p1. The mesh is quite simple: a single volume element! Each cycle is dis- cretized with a minimum of 40 time steps automatically calculated for opti- mized convergence. Considering several levels of 1D loadings, it has been shown in Sect. 4.2.1 that the deviation from the linear accumulation rule of Palmgreen--Miner

4.4 Numerical Failure Analysis 215 is due to the damage threshold. In fact, a numerical analysis avoiding any approximation gives the same effect, but in a more complete manner. A set of two-level loadings is considered here, made of n1 cycles of a first symmetric cyclic loading at constant strain range Δ 1, followed by n2 cycles of a second symmetric loading at constant Δ 2 up to mesocrack initiation in the range of 10 to 104 cycles. First, it is interesting to see the variation in the number of cycles leading to the damage threshold ND as a function of the number of cycles to rupture NR. Figure 4.10 shows that the ratio ND/NR increases largely with NR,a s shown by many experiments (A. Pineau 1980). Fig. 4.10. Evolution of the number of cycles-to-damage-threshold in low cycle fatigue Second, after the damage threshold, the evolution of the damage is not too far to be linear as a function of the number of cycles (Fig. 4.11). This justifies some early fatigue theories where the damage was set as D = N/NR, but here it should be D = N - ND /(NR - ND). Last, the accumulation diagram corresponding to the two-level fatigue loading of Fig. 4.3 is computed for two different strain ranges. Figure 4.12 shows the deviation with respect to the Palmgreen--Miner linear rule repre- sented here by the straight line [(1,0),(0,1)]. It is somewhat more precise than the diagram of Fig. 4.4 drawn for the same values of ND/NR. Additional simu-

216 4 Low Cycle Fatigue Fig. 4.11. Evolution of the damage in low cycle fatigue for different strain ampli- tudes lations and experiments show that the deviation is more and more important as the difference between the two loading amplitudes increases. 4.4.2 Multiaxial and Multilevel Fatigue Loadings As an example, consider the biaxial testing steel specimen of Fig. 4.13 which exhibits stress concentrations, localized plasticity, and damage at notches. The sample is 120 mm long and 4.5 mm thick, which allows for the plane stress assumption. A multilevel fatigue loading is applied and the failure conditions are determined after a single elastic reference computation by use of the cyclic SED method of Sect. 4.2.4, followed by the time integration of the unified damage law. The edges are in pure tension with a stress triaxiality ratio of 1/3 which corresponds to Rν =1. The experiment is performed on the triaxial testing machine of Fig. 4.14. Two in-phase proportional loads F1(t)=F2(t)=F (t)a r eappliedo nthe lateral sides of the specimen. The total loading consists of thirteen blocks i of cyclic F (i)(t) varying between a zero minimum load and a constant maximum load F (i) max (Fig. 4.15). The first block is made of 38000 cycles at F (1) max =35 kN, then the load is increased by 5 kN every 100 cycles up to F (13) max =95kN. Failure, characterized by a mesoscopic crack of 0.5 mm in the edge, occurs at this last level after N (13) Rexp = 3050 cycles. This corresponds to a total number of cycles to rupture of 42150.

4.4 Numerical Failure Analysis 217 The material is a 2-1/4 CrMo steel at room temperature. For strains smaller than 4%, the monotonic plastic behavior is approximated by a linear hardening R = Cyp; for cyclic loading with strains smaller than 4%, it is approximated by a linear kinematic hardening X = 2 3 Cy p.Thefulls etof material parameters defined in Sects. 1.4 and 1.5 is: • E = 200000 MPa, ν =0.3 for elasticity • σy = 180 MPa as yield stress • Cy = 6000 MPa for hardening • σu=Ry ∞ + σy = 450 MPa as ultimate stress • pD =0.12, m =2,σ∞ f = 140 MPa, S =2.8MPa ,s =2,Dc =0.2for damage with a damage threshold in fatigue given by pD = pD σu - σ∞ f Δσ 2 -σ∞ f m . (4.89) The procedure of the numerical prediction is as follows: 1. Perform the elastic reference computation for a load F1 = F2 = Fref . Define for each level αmin = Fmin/Fref =0a n dαmax = Fmax/Fref (with αref = 1). The von Mises stress at the edge concentration point is σref eq = 129.2MPaforFref = 10 kN. At this point, Rν =1and Fig. 4.12. Nonlinear damage accumulation in two-level fatigue loadings

218 4 Low Cycle Fatigue Fig. 4.13. Biaxial testing specimen (J.P. Sermage and J.M. Virely 1998) E (σ )elas = E (ΔσΔ )elas = αmaxσref eq 2 . (4.90) Check that for each level (Δσ)elas > 2σy so that plasticity (at least) must occur locally. 2. Apply the Strain Energy Density method for each level to take into account the plasticity. Calculate the maximum stress from the monotonic SED method: σmax = E (σ )elas + E Cy σ2 y 1+E Cy . (4.91)

4.4 Numerical Failure Analysis 219 Fig. 4.14. Triaxial testing machine ASTREE of LMT-Cachan Fig. 4.15. Multilevel fatigue loading Calculate the stress range Δσ, the plastic strain range Δ p,a ndthe plastic strain increment over one cycle of the considered level δp δN: Δσ= E (ΔσΔ )elas +4 E Cy σ2 y 1+E Cy , (4.92) δp δN =2Δ p =2Δσ - 2σy Cy . (4.93)

220 4 Low Cycle Fatigue At the beginning of the last level, the accumulated plastic strain is p=38000δp δN (1)+100δp δN (2) + ...+ 100 δp δN (12) =47.06 . (4.94) 3. Calculate the damage and the number of cycles to rupture. (a) Determine the number of cycles at damage initiation (ND) The damage threshold for the first level F (1) max =35kNisp(1) D =6.7. Then ND = p(1) D 2Δ (1) p = 6650 cycles . (4.95) Check that ND < 38000 cycles so that the damage initiates at this level. (b) Calculate the damage increment for each level According to (4.63), δD δN = (σ2s eqmin+σ2s eq max)Rs ν 2(2ES)s δp δN = σ2s max +(Δσ - σmax)2s 2(2ES)s δp δN. (4.96) (c) Determine the number of cycles to rupture (N (13) R) The damage increments over each block are summed up to D = Dc . At the beginning of the last level, D = (38000-ND) δD δN (1)+100 δD δN (2)+...+100 δD δN (12) =0.042 (4.97) and a number of cycles at crack initiation N (13) R is estimated as N (13) R =Dc -0.042 δD δN (13) = 3790 cycles , (4.98) compared to N (13) Rexp = 3050 and which corresponds to a total number of cycles NR = 39100 + 3790 = 42890 instead of the 42150 cycles obtained experimentally. The accumulated plastic strain at failure is then pR =47.06 + 3790 δp δN (13) = 112.6 . (4.99) From the first level to the last, the accumulated plastic strain per cycle ( δp δN) varies from 0.110-2 to 1.73 10-2 whereas the damage per cycle (δD δN )v aries from 8.94 10-7 to 4.17 10-5.

4.4 Numerical Failure Analysis 221 4.4.3 Damage and Fatigue of Elastomers (S. Cantournet and R. Desmorat, 2002) Elastomers, at least for fatigue purposes, may be modeled by hyp erelas- ticity with internal friction coupled with damage. No plasticity! A dis- sipative phenomenon occurs, however, due to internal sliding of the macro- molecular chains on themselves and the black carbon filler particles. Internal viscosity is also an additional dissipative mechanism not taken into account in this section. The unified damage law governed by the accumulated plastic strain rate used up to now is useless. Fortunately, its generalization to any dissipative phenomenon described in Sect. 1.4.5 applies. It just needs to be formulated within the finite strains framework (see Sect. 3.4.1), replacing with the Green--Lagrange deformation E, σ with the second Piola--Kirchhoff stress tensor S, and with internal variables: • The internal inelastic strain Eπ (instead of π). It is associated with the opposite of a stress denoted by Sπ . • The internal sliding variable α associated with the residual microstress tensor X. • The isotropic damage variable D, associated with the opposite of the energy density release rate Y . 4.4.3.1 Hyperelasticity with Internal Friction Coupled with Damage The state potential is (for the isothermal case), ρ0ψ =(1- D)[w1(E)+w2(E - Eπ)] + 1 2Cxα : α, (4.100) with ρ0 as the density of the undeformed material and where • w1 is a hyperelastic energy density such as the Mooney, Hart--Smith or Lambert--Diani--Rey densities. For incompressible materials, J =det F = 1and w1 = moon1(I1 - 3) + moon2(I2 - 3) Mooney, w1 = h1 exp h3(I1 - 3)2 dI1 +3h2 ln I2 3 Hart--Smith, w1 = h1 exp(h3(I1 - 3)a1)dI1 +3h2 dI2 Ia2 2 Lambert--Diani--Rey. (4.101) Here,I1=trCandI2=1 2 (tr C)2 - tr C2 are the first two invariants of the dilatation tensor C = F TF ;andmooni and hi are the hyperelas- ticity material parameters. For quasi-incompressible materials, the third

222 4 Low Cycle Fatigue invariant I3 = J 2 does not remain strictly equal to unity. A compress- ibility term that is a function of I3 is often introduced. For example, the Mooney density for compressible or quasi-incompressible elastomers is written as w1 = moon1(I1 -I3 -2)+moon2(I2 -2I3 -1)+1 2 Kv(I3 - 1)2 , (4.102) where Kv is the compressibility modulus. • w2 is the second order term of the Mooney--Rivlin development with in- elastic strain Eπ , w2 =4C20 [tr(E - Eπ)]2 = C20 (I1 - 2trEπ - 3)2 . (4.103) For incompressible materials, the internal pressure P is calculated from the boundary conditions using a pressure-displacement FE formulation. The state laws then become S=ρ0∂ψ ∂E J =1 =(1- D)∂(w1 + w2) ∂E -PC-1, Sπ=-ρ0∂ψ ∂Eπ =(1- D)∂w2 ∂E, X=ρ0∂ψ ∂α =Cxα, Y = -ρ0∂ψ ∂D=w1+w2. (4.104) This defines the effective stresses ˜ S=S 1-Dand˜ Sπ =Sπ 1-D. For compressible or quasi-incompressible materials, the first law of (4.104) is simply S=ρ0∂ψ ∂E =(1- D)∂(w1 + w2) ∂E. (4.105) The reversibility criterion (such as f<0 ⇒ hyperelasticity) is: f= Sπ 1-D-X -σs = ˜ Sπ - X : ˜ Sπ - X - σs , (4.106) with σs the reversibility limit in the Sπ stress plane. The dissipation potential is F=f+ γ 2CxX:X+ S (s + 1)(1 - D) YS s+1 , (4.107) giving rise to the evolutions laws through the normality rule, ˙ Eπ =˙ μ∂F ∂Sπ , ˙ α= - ˙μ∂F ∂X, and ˙ D=˙ μ∂F ∂Y , (4.108)

4.4 Numerical Failure Analysis 223 with ˙μ as the internal sliding multiplier determined from the consistency condition f =0, ˙f =0.Theyleadto ˙ Eπ = ˙μ 1-D ˜ Sπ -X ˜ Sπ -X , ˙ X= Cx ˙ Eπ -γX˙ π (1 -D), (4.109) and the damage evolution law for elastomeric materials valid for monotonic loading as well as fatigue loading: ˙ D = YS s ˙ π if π>πD D=Dc -→ mesocrack initiation, (4.110) where π = t 0(1-D)˙ μdt = t 0 ˙ Eπ dt is, as expected, the cumulative measure of the internal sliding. Compared to hyperelasticity, 8 additional material parameters are intro- duced: • The reversibility threshold σs • C20, Cx ,andγ for internal friction: the parameters C20 and Cx model the hysteresis loops when the parameter γ models the stress softening • πD, S, s,andDc for damage evolution and mesocrack initiation 4.4.3.2 Hysteresis and Cyclic Softening of Filled Rubber With neither damage nor viscosity, the model represents the hysteresis and the stress softening of filled elastomers. Figure 4.16 shows the cyclic tensile curves of styrene butadiene rubber (SBR) filled with silica particles. Note that in terms of hyperelasticity, considering Hart--Smith density al- lows for a good modelling of the up-turn at very large strains. For fatigue applications, take the model which best represents the hysteresis loops in the range of deformation under consideration. 4.4.3.3 Fatigue Curve of Filled Natural Rubber The model of hyperelasticity with internal friction coupled with damage al- lows us to compute the number of cycles to rupture in unidimensional fatigue. The numerical procedure is detailed in the next section for structures but ap- plies, of course, to cyclic tension. Consider here a filled natural rubber (NR) tested both in cyclic tension and fatigue. The material parameters are

224 4 Low Cycle Fatigue • moon1 =1.848 MPa, moon2 =0.264 MPa, Kv = 1188 MPa • σs =1MPa,C20 =1MPa,Cx =10MPa,γ =5 • πD =0,S =5.6MPa,s =5,Dc =0.2 Fig. 4.16. Cyclic tensile curve of styrene butadiene rubber (SBR) with Hart-- Smith density. The dotted line represents experimental results from A. Lapra (2001) (h1 =1.6MPa,h2 =0.28 MPa, h3 =5.29 10-4 , σs =1.16 MPa, C20 =0.14 MPa, Cx =0.93 MPa, γ =0.57, D =0) The fatigue curve of the maximum applied elongation λmax (larger prin- cipal component of the transformation gradient F ) versus the number of cycles to rupture NR is calculated and compared to experiments with suc- cess in Fig. 4.17. The measured elongation to rupture in tension, λR =7.2, is also reported on the diagram which shows the ability of the single gen- eralized damage law ˙ D =(Y/S)s ˙ π to model monotonic as well as fatigue damages. 4.4.3.4 Fatigue of a Metal/Elastomer Joint As an example, consider the case of the double lap joint of Fig. 4.18 submit- ted to fatigue loading. Half of the joint is meshed in three dimensions with 27-node quadratic elements. The bottom ends are fixed and the same dis- placement U(t)=U(t) e3 is applied cyclically on the top end between U =0 and U = Umax = 45 mm at a loading rate of 100 mm/min. Considering the damage pattern, the most damaged zones are the corners points of the rub- ber parts where a crack initiates (after a number of cycles N exp R = 30), with a damage propagation mainly along the interfaces. The metallic parts are made of steel (E = 200000 MPa, ν =0.3) which remain elastic during the test. The elastomer is made of filled natural rubber.

4.4 Numerical Failure Analysis 225 Fig. 4.17. Experimental and calculated fatigue curves for filled natural rubber (NR) (mean elongation λmean =2.53) Fig. 4.18. Metal/elastomer joint (dimensions in mm)

226 4 Low Cycle Fatigue The uncoupled procedure to estimate both the fatigue damage and the number of cycles to rupture is the one described in Sect. 2.1. It is detailed here for the damage law considered: Step 1. Perform the nonlinear structure FEA with no damage up to a stabilized cycle. This constitutes the reference computation. The result of the analysis is the history of the stresses Sij(t)orS(t), the strains Eij(t)orE(t), and the internal variables Sπ(t), Eπ(t), X(t), and α(t). It is also the global hysteretic response of the structure force F vs displacement U . Step 2. Determine the most loaded point where Y = w1 + w2 is max- imum in order to calculate the damage increment (step 3), the dam- age history (step 4), and the number of cycles to rupture (step 5) at this point. If damage maps are needed, perform the steps 3 to 5 at the Gauss points of the damaged zone considered. Step 3. Calculate the damage increment over one cycle. The calcu- lation is made over the stabilized cycle as a post-processing of the reference computation. This is usual in fatigue as it makes the anal- ysis much faster with rather high accuracy, δD δN = 1cycle Y (t) S s ˙ π(t)dt = 1cycle w1(E(t)) + w2(E(t) - Eπ(t)) S s ˙ Eπ(t) dt. (4.111) Step 4. Calculate the damage history at the considered point(s). The derivative δD δN is constant for a given maximum applied displacement Umax . Then, D(N)= δD δN ·(N -ND), (4.112) with ND as the number of cycles at damage initiation. Here, ND =0 as πD =0. Damage maps may then be drawn. The computed damage pattern is in accordance with the experiment: it exhibits a damage larger in the rubber corner points and is localized along the interfaces (Fig. 4.19). Step 5. Calculate the number of cycles to crack initiation corre- sponding to D = Dc: NR=ND+Dc δD δN at the most loaded point. (4.113) These calculations have been made for the metal/elastomer joint. The number of cycles at crack initiation corresponds to the reach of D = Dc at the corner point A. The result is NR = 39 cycles, compared to N exp R =30which corresponds to an accuracy of about 30%.

4.4 Numerical Failure Analysis 227 Fig. 4.19. Damage pattern at crack initiation in the metal/elastomer joint (mesh of half of the joint) 4.4.4 Predeformed and Predamaged Initial Conditions As in Sect. 3.4.7 for ductile failures, it is interesting to know how the number of cycles to rupture can be modified in low cycle fatigue by changes in the initial conditions of the main variables. Forming processes, accidents, or over loadings may induce, for a "forming" or an "accident" stress σ0 eq, initial fields of: • The accumulated plastic strain p0 • The corresponding value of the strain hardening variables R0 and X0 • The stored energy w0 s ≈A(σ0 eq-σ∞ f )p1/m 0, • The damage D0 or D0 • The internal residual stresses They have to be introduced as initial conditions in the structure calculation, at each Gauss point if a finite element analysis is used, to determine the stresses σeq(t)andσH(t), as well as the plastic strain p(t)orΔp. They also have to be introduced in the damage law. • The initial plastic strain (p0) or the stored energy density (w0 s)m odi- fies the number of cycles corresponding to the damage initiation (ND)

228 4 Low Cycle Fatigue through the change in damage threshold written in terms of accumulated plastic strain. For a fatigue loading with a periodic, signed von Mises stress between -σeq min and σeq max applied after the forming process or the accident, the stored energy threshold reads ws =A(σu -σ∞ f ) 1/m pD = A(σ0 eq-σ∞ f )p1/m 0 +A σeq min+σeq max 2 -σ∞ f (p1/m D -p1/m 0) (4.114) and corresponds to the accumulated plastic strain threshold p = pnew D, pnew D = 1/m pD σu-σ∞ f 1 2(σeq min + σeq max)- σ∞ f + p1/m 0 1 2(σeq min + σeq max)- σ0 eq 1 2(σeq min + σeq max)- σ∞ f m , (4.115) becoming pnew D =p0ifp0≥p0 D= pD σu-σ∞ f σ0 eq-σ∞ f 1/m . • The initial damage corresponding to p0 ≥ pD acts in the integration of the damage rate from D0 to Dc . For example, in the case of periodic, proportional loading of Sect. 4.2.2, the formula (4.24) is replaced by NR = pnew D -p0 2Δp +Dc 2Δp 2ES σ2 eq maxRν s if p0 <p0 D NR=Dc-D0 2Δp 2ES σ2 eq maxRν s if p0≥p0 D . (4.116) 4.4.5 Hierarchic Approach up to Non-Proportional Effects , As for ductile failure predictions in Sect. 3.4.8, the different models of low cy- cle fatigue may be classified in an increasing order of accuracy corresponding (unfortunately) to an increasing order of difficulty. • The Manson--Coffin law is certainly the first model to consider for an early design with a periodical loading or if only the plastic strain range is known. The number of cycles-to-crack initiation (NR) at the critical point where the state of stress is one dimensional is simply NR = CMC Δ p γMC or NR ≈ 2 pR Δ p 2 . (4.117)

4.4 Numerical Failure Analysis 229 • If the loading is periodic by blocks, the linear Palmgreen--Miner rule may give an order of magnitude of the result but without the possibility to know the sign of the error: ni NRi =1,N R= ni. (4.118) • When the local loading is 3D, the Manson--Coffin law does not apply but if it is proportional and periodic the integrated unified damage law may be used. For a symmetric periodic loading, NR=ND+ Dc 2Δp ES σ2 eq maxRν s , with ND = pD 2Δp σu-σ∞ f σeqmax-σ∞ f m . (4.119) The equations require knowledge of the value of 5 material damage pa- rameters plus E, ν, σ∞ f ,andσu . They can be reduced to one by using the equivalence between 1D and 3D through the damage equivalent stress σ if one point of the Manson--Coffin curve is known: NR(σij) NR(σM) ≈ Δ p Δp σ M σM 2s . (4.120) • The last possibility is the integration in time of the unified damage law if the loading is not periodic but is a complex function of time, either 1D or 3D, either for isotropic or anisotropic damage, and either deterministic or random by the Monte Carlo method: ˙ D = YS s|˙ p| if ws>wD. (4.121) In case of periodic loadings, the stored energy damage initiation criterion is equivalent to ˙ D =0 if p>pD = pD σu -σ∞ f (Δσ)eq 2 -σ∞ f m . (4.122) Remark -- Note that the extension of the Neuber and the Strain Energy Density methods is a big help in determining Δ p or Δp from an elastic calculation. In matters related to plasticity, classical isotropic and kinematic hardening laws have been considered so far. The Armstrong--Frederick nonlinear law ˙ X=2 3C˙ p - γX ˙p represents the Baushinger effect of the apparent yield

230 4 Low Cycle Fatigue stress decrease in cyclic loadings and also the cyclic stress softening of non- symmetric strain-controlled loadings. But it is not suitable for more com- plex hardening mechanisms such as non-proportionality effects or ratcheting, which is the continuous increase of the plastic strain at constant stress range (even when no damage occurs). Other kinematic hardening laws must then be considered. They are usually written for undamaged materials and need to be coupled with damage by the effective stress concept. • A better modelling of hardening (for a wider range of plastic strains or for uniaxial ratcheting) is obtained by use of several kinematic hardening va riable s Xi related to nonlinear laws (Z. Mroz 1967), coupled here with either isotropic or anisotropic damage (no summation on subscripts i): X= i Xi, ˙ Xi=23Ci˙ ep-γiXi˙ r, ˙ p =(H˙ epH)D with ˙ ep=nX˙ r=32 ˜ σD-X (˜ σ-X)eq ˙ r, (4.123) where ˙ p = nX ˙p is the plastic strain rate in plasticity (D = 0)a nd ˙ ep=nX˙ r is the effective plastic strain rate in plasticity coupled with damage. • Another way is to keep only one kinematic variable but to introduce in its evolution law a term taking into account the rotation of the stress vec- tor to model the ratcheting and non-proportional effects. Many nonlinear laws have been proposed but are most often not coupled with damage (H. Burlet and G. Cailletaud 1987, A. Benallal and D. Marquis 1988, E. Tanaka 1994, N. Ohno and J.D. Wang 1994, T. Kurtyka 1996, S. Cal- loch 1996, M. Fran¸ cois 2000). For instance, the Burlet--Cailletaud model states that ˙ X=23C˙ p-γ(X:nX)nX˙p (4.124) and the Ohno--Wang model uses ˙ X=23C˙ p-γ(X:X)α X: ˙ p X . (4.125) In order to introduce the damage coupling, one way is to define a non-associated potential FX such as the nonlinear kinematic hardening law derived from F = f + FX . Replacing the stress σ by the effective stress ˜ σ in F before taking the derivatives gives the nonlinear kinematic hardening law fully coupled with damage. For instance, the potential FX=3γ 4C(X:X)α1 X:nX α2 and nX=3 2 E: eD-2 3Cα (E: eD-2 3Cα)eq (4.126)

4.4 Numerical Failure Analysis 231 gives ˙ X=23C˙ ep - γα2(X : X)α1 X : nX α2-1nX ˙ r - γα1(X : X)α1-1 X : ˙ ep α2 X , (4.127) with the first back stress term proportional to nX as in the Burlet-- Cailletaud law and the second one proportional to X as in the Ohno-- Wang law. • Finally, the treatment for plastic anisotropy is similar to the one for the ductile failure case (see Sect. 3.4.8). Use as yield function: f= (˜ σ-X):h:(˜ σ-X)-R-σy where histheHilltensor (4.128) and take F=f+34X:C-1:Γ:X (4.129) as the dissipation potential with the state law X = 2 3C:αandwith C and Γ as material-dependent fourth order tensors. The nonlinear anisotropic kinematic hardening law with no damage (C-1 : Γ assumed to be symmetric) becomes ˙ X=23C:˙ p-Γ:X˙p. (4.130) The coupling of the kinematic hardening evolution law with damage is gained using the thermodynamics framework as ˙ p =˙ r∂F ∂σand˙ α=-˙ r∂F ∂X (4.131) lead to ˙ X=23C:˙ ep-Γ:X˙ r, (4.132) where ˙ ep =˙ r h :(˜ σ-X) (˜ σ-X):h:(˜ σ-X)and˙ p=(H˙ ep H)D.

5 Creep, Creep-Fatigue, and Dynamic Failures Generally, an elevation of temperature in most materials induces a decrease of their strength and a sensitivity to the strain rate. Then, creep and creep- fatigue failures are associated with temperature and time.Theya r ea s - sociated with temperature because these phenomena are thermally activated from mid to elevated temperatures that are above about one third of the absolute melting temperature for metals. The time association arises because the temperature induces viscous effects depending explicitely upon time. From a physical point of view, creep damage in metals is essentially the nucleation and growth of intergranular microcracks up to crystals triple points where the coalescence of microcracks induce a mesocrack. Under fa- tigue loading, a net of intragranular microcracks develops and interacts with the creep microcracks net. From the mechanical point of view, this interaction is nonlinear and so is the cumulation of damages resulting of dif- ferent stress amplitudes. In polymers, damage occurs as a result of rupture of molecular bonds in zones of defects or impurities that induce a strain rate effect with temperature, particularly the transition state or rubber state. Modelling creep effects was done during the 20th century, beginning with E.N. Andrade (1910) and F.H. Norton (1929). The introduction of a dam- age variable was in fact first made for creep by L.M. Kachanov (1958), Y.N. Rabotnov (1968), and used then by J. Lemaitre (1971), J. Hult (1972), F.A. Leckie, and D. Hayhurst (1974). Its extension to creep-fatigue damage was followed by J.L. Chaboche and J. Lemaitre (1974), M. Chranowski (1975) to become an engineering tool to design mechanical components against creep or creep-fatigue failures (J. Skrzypek and A. Ganczarski 2002). This chapter has the same organization as others with a visco-plastic stress concentration analysis, an expression of the yield stress for adia- batic deformations strain rate and temperature-dependent, and examples of creep-fatigue, dynamic analysis for crash problems and penetration of projectiles.

234 5 Creep, Creep-Fatigue, and Dynamic Failures 5.1 Engineering Considerations All engineering components submitted to loadings at elevated temperature may be subjected to creep damage effects in quasi-static loadings and to creep-fatigue damage effects in cyclic loadings. This is the case for all metallic materials and polymers. These effects can be classified with respect to the lifetime: • Short range effects in rockets components where the lifetime is of a few minutes or in the coating of the steel ladles in the metallurgy of steel elab- oration where the lifetime is only on the order of 200 to 500 service hours. • Middle range effects in gas turbines of airplanes or car engines where the lifetime is on the order of 5000 to 10000 hours. • Large range effects in the chemistry industry and thermal or nuclear power plants where the lifetime is of the order on 10 to 50 years. • Extremely large range duration as those considered in the conservation of radioactive wastes -- up to 100, 1000, or even 10000 years! The analysis grows more difficult as the time range increases at least for three reasons: as the time increases there are additional physical effects like diffusion, corrosion, and aging which are not usually taken into account in the mechanical constitutive equations; there is a time scale of some months or years above which there is almost no possibility to perform tests and ensure good identification of the material parameters; last but not least, the probability of the occurrence of unpredicted events increases with time. Furthermore, be careful at the two extrema of the plastic strain rates where viscous effects must be taken into account even at room temperature: •˙ p > 1--104 s-1 is the range of rates occurring in shocks, crash, or loadings by accident. It is usually called dynamic plasticity because it happens at room temperature but it is formally labelled as visco-plasticity as the strain rate modifies the material response, especially if the reference identification has been performed at usual strain rates of about 10-4 s-1. For example, the usual engineering yield stress may increase 10--50% at high strain rates of about 104 s-1. •˙ p < 10-10 s-1 at the other extreme is the range which may exist in steels at room temperature loaded at small stresses, below the engineering yield stress. The resulting slow creep or relaxation may change the stress concentrations, induce leakage in pressurized vessels, or decrease the tension in the cables of pre-stressed oncrete by relaxation of the steel cables associated with the creep of the concrete. 5.2 Fast Calculation of Structural Failures Despite the fact that temperature and time add two more variables, it is possible to perform approximate calculations of the damage to help in early

5.2 Fast Calculation of Structural Failures 235 design, considering of course isotropic damage without any effect of microde- fects closure in compression. The difficulty is knowing with a good accuracy from a structural analysis the state of local stresses or, better, the state of local plastic strains which are the inputs of any damage evaluation. 5.2.1 Uniaxial Behavior and Validation of the Damage Law 5.2.1.1 Creep Damage Pure creep is the time evolution of the plastic strain under constant stress. Generally, the damage begins to grow at the minimum strain rate after the primary creep and increases the strain rate up to rupture (Fig. 5.1). Fig. 5.1. Damage during a pure creep test on superalloy IN 100 at 1000◦C (J. Lemaitre and J.L. Chaboche 1985) The first law proposed in 1958 to describe the creep damage is the unidi- mensional Kachanov law without any threshold: ˙ D= σ AD(1 - D) rD , (5.1) where AD and rD are material parameters depending upon the temperature. The time-to-rupture tR at constant stress and constant temperature is the solution of this differential equation for D = Dc , with the initial condition t=0→D=0, tR =1-(1-Dc)rD+1 rD+1 σ AD -rD . (5.2)

236 5 Creep, Creep-Fatigue, and Dynamic Failures This helps us draw from experiments the isochronous curves which give the time-to-rupture function of the constant stress applied (Fig. 5.2). Fig. 5.2. Isochronous curves of superalloy IN 100 at different temperatures (J. Lemaitre and J.L. Chaboche 1985) This kind of tests may be helpful in the validation of the unified damage law for creep damage if the plastic strain to rupture pR and the plastic strain at the inflexion point corresponding to the threshold pD are recorded. The integration of the differential law for σ = const is particularly easy: ˙ D= σ2 2ES(1 - D)2 s |˙ p| if p > pD (5.3) or Dc 0 (1-D)2sdD= σ2 2ES s pR pD d p , (5.4) leading to pR - pD = σ2 2ES -s 1 2s +1 1 - (1 - Dc)2s+1 -1 . (5.5) The slope of the best straight line fitting the points log( pR - pD)vslogσ for different creep tests "must" give -2s, close to the value identified by the procedures of Sects. 1.4.4 and 2.4.

5.2 Fast Calculation of Structural Failures 237 5.2.1.2 Creep-Fatigue Damage If the loading is a sequence of constant stresses with hold times and un- loadings or if it is a cyclic loading, the phenomenon of fatigue occurs as a superimposed effect. It is called creep-fatigue interaction because the earliest models were a combination of two terms: one for creep, and one for fatigue without or with couplings to obtain a model of nonlinear interaction. The simple Taira rule of linear interaction (1952) applies to isothermal uniaxial cyclic loading with 0 ≤ σ ≤ σmax and with a hold time of Δt.IfNR is the number of cycles to rupture corresponding to a time tR ≈ Δt · NR;if NRF is the number of cycles to rupture in pure fatigue (Δt ≈ 0) for the same stress range; and if tRC is the time-to-rupture in pure creep for the same maximum stress σ = σmax for all t, the Taira rule reads: tR tRC+NR NRF =1. (5.6) Easy to apply, it may give an order of magnitude of the time or of the number of cycles to rupture if nothing else is available. An interesting point, the unified damage law developed in Chap. 1, ˙ D= σ2 2ES(1 - D)2 s |˙ p| if p> pD , (5.7) can represent both creep damage and fatigue damage as the damage rate is governed by the plastic strain with no difference for creep and fatigue as, from the point of view of strains, a fatigue loading is nothing more than cyclic visco-plasticity. Numerically, it is possible to show that the interaction between creep damage and fatigue damage is nonlinear if a damage threshold and kinematic hardening are taken into consideration (see Sect. 5.4.2). A small creep reduces considerably the fatigue life, a physical property which is not contained in the Taira rule. 5.2.2 Case of Proportional Loading The case of proportional loading allows us to solve a 3D problem by ma- nipulation of scalars only as all the tensors are colinear (see Sect. 2.1.2). As already stated, many engineering problems involve one load or multiple loads all varying proportionately to one parameter to ensure the local property of proportional loading. In monotonous creep, if the history of stress is known as a function of time σ(t) at the critical point, one only has to calculate the von Mises equivalent stress σeq(t) and the constant triaxiality ratio (σH/σeq). In the unified damage law, the accumulated plastic strain rate is replaced by the

238 5 Creep, Creep-Fatigue, and Dynamic Failures pure viscous Norton law in which the yield stress and the hardening are neglected here (but not the coupling with the damage), ˙p = σeq K0 N(1 - D) N0 . (5.8) One has to solve a differential equation fully similar to Kachanov law (5.1), ˙ D= σ2 eqRν 2ES(1 - D)2 s σeq K0 N(1 - D) N0 if p>pD (5.9) or D 0 (1 - D)2s+N0dD = t tD σ2 eq(t)Rν 2ES s σeq(t) K0 N N0 dt, (5.10) where the time tD to reach the damage threshold pD is given by pD= tD 0 σeq K0 N N0 dt. (5.11) Then, D =1- 1-(2s+N0+1) t tD σ2s+N0 eq(t) Rs ν (2ES)s (K 0 N)N0 dt 1 2s+N0 +1 (5.12) and the time-to-rupture tR is given by tR tD σ2s+N0 eq(t) Rs ν (2ES)s (K 0 N)N0 dt = 1 - (1 - Dc)2s+N0+1 2s+N0+1 . (5.13) For example, for a constant state of stress pD = pD and tRC =tDC+ 1-(1-Dc)2s+N0+1 2s + N0 +1 (2ES)s K0 N N0 σ2s+N0 eq Rs ν , tDC = pD K0 N σeq N0 . (5.14) The difference with an uniaxial case characterized by the same equivalent stress σ = σeq lies only in the triaxiality function Rν and gives an easy way to solve any 3D problem (in proportional loading!), tRC(σij) - tDC(σij) tRC(σ) - tDC(σ) = R-s ν, (5.15) with tDC(σij)=tDC(σ)= pD σ K0 N -N0 .

5.2 Fast Calculation of Structural Failures 239 The case of creep-fatigue (non-monotonous creep) is also treated by the above equations ((5.12) and (5.13)) if the same assumptions apply. The integral is only a bit more difficult to calculate. For example for the periodic repeated loading of Fig. 5.3, the damage increment over one cycle δD δN = 1cycle ˙ Ddt (assume D is constant over one cycle in the calculation of the integral) is given by the integral involving the stress rate during loadings and unloadings where | ˙ σeq| =˙ σfeq considered constant, Fig. 5.3. Creep-fatigue periodic loading dD= σ2 eq(t)Rν 2ES(1 - D)2 s σeq(t) K0 N(1 - D) N0 dt with dt = dσeq ˙ σfeq , (5.16) δD δN= Rν 2ES(1 - D)2 s 1 K0 N(1 - D) N0 × 2 σeq max 0 σ2s+N0 eq dσeq ˙ σfeq + Δt 0 σ2s+N0 eq maxdt . (5.17) A second integration over the number of cycles gives the condition to rupture, Dc 0 (1 - D)2s+N0δD = Rν 2ES s 1 K0 N N0 × 2 2s+N0+1 σ2s+N0 +1 eq max ˙ σfeq + σ2s+N0 eq maxΔt (NR - ND) , (5.18) where ND is the number of cycles to reach the damage threshold (see Sect. 1.4.1): ND≈pD Δt K0 N σeq max N0 with pD = pD 2σu σeq max m , (5.19) NR = ND+1-(1-Dc)2s+N0+1 2s + N0 +1 (2ES)s K0 N N0 σ2s+N0 eq maxRs ν × 2 2s+N0+1 σeq max ˙ σfeq +Δt -1 . (5.20)

240 5 Creep, Creep-Fatigue, and Dynamic Failures In the last brackets, the first term corresponds to fatigue damage and the sec- ond to creep damage. The last equation involves temperature-dependent ma- terial parameters which may become time-dependent in the integral through the eventual history of temperature. Here again, the number of cycles to rupture of a 3D problem is easily deduced from the known number of cycles to rupture of an uniaxial case characterized by the stress σ(t) which varies between 0 and σM = σeq max , NR(σij ) - ND(σij) NR(σM) - ND(σM) = R-s ν. (5.21) Equations (5.14) and (5.20) allow us to determine the 3D creep-fatigue interaction diagram NR/NRF function of tR/tRC for a given stress triaxi- ality where: • NRF is the number of cycles to rupture in pure fatigue (hold time Δt =0), NRF = NDF + 1 -(1 - Dc)2s+N0+1 (2ES)s K0 N N0 ˙ σfeq 2σ2s+N0+1 eq max Rs ν (5.22) • tRC is the time to rupture in pure creep, tRC =tDC+ 1-(1-Dc)2s+N0+1 2s + N0 +1 (2ES)s K0 N N0 σ2s+N0 eq maxRs ν (5.23) • NR is the number of cycles to rupture in creep-fatigue • tR = NRΔt is the time spent in creep One has (NRF - NDF) 2 2s+N0+1 σeq max ˙ σfeq = tRC - tDC (5.24) and (NR-ND) 2 2s+N0+1 σeq max ˙ σfeq +Δt = tRC - tDC , (5.25) which lead to (NR-ND) tRC-tDC NRF -NDF +(NR -ND)ΔttRC -tDC tRC-tDC =tRC-tDC (5.26) and, therefore, the 3D nonlinear creep-fatigue interaction through the values of the thresholds ND, NDF, tD, tDC: NR-ND NRF-NDF+ tR-tD tRC - tDC =1, (5.27)

5.2 Fast Calculation of Structural Failures 241 where the stress triaxiality and the maximum von Mises stress σeq max are the same for fatigue, creep and creep-fatigue. Note that a damage evolution with no threshold (pD = 0) implies tDC = tD =0a ndNDF = ND =0. In that case, eq. (5.27) recovers the Taira rule (5.6) of linear creep-fatigue interaction. If the reference creep time to rupture tRC(σM) and fatigue number of cycles to rupture NRF(σM) are known from an uniaxial loading (Rν =1)at the same σeq max = σM as the 3D loading, one can write the 3D creep-fatigue interaction as NR(σij ) - ND(σij) NRF(σM) - NDF(σM) + tR(σij) - tD(σij) tRC(σM) - tDC(σM) = R-s ν . (5.28) 5.2.3 Sensitivity Analysis As in Chap. 3 (Sect. 3.2.3) for the plastic strain to rupture and in Chap. 4 (Sect. 4.2.3) for the number of cycles to rupture, it is possible to perform a sensitivity analysis for the time to rupture in creep in accordance with the general method of Sect. 2.4.6. Start with the closed-form solution in proportional loading (5.14), where tR =tD+1-(1-Dc)2s+N0+1 2s+N0+1 2ES σ2 eqRν s K0 N σeq N0 , (5.29) with tD = pD K0 N σeq N0 (5.30) and Rν = 23(1 + ν)+3(1- 2ν)T2 X. (5.31) Taking the logarithm gives ln(tR - tD)=ln 1 - (1 - Dc)2s+N0+1 - ln(2s + N0 +1) +sln 2ES σ2 eqRν + N0 ln K0 N σeq , (5.32) with ln 1 - (1 - Dc)2s+N0 +1 =ln(1- exp [(2s + N0 +1)ln(1- Dc)]) (5.33) and the derivative dln 1 - (1 - Dc)2s+N0 +1 = (2s + N0 + 1)(1 - Dc)2s+N0 1 -(1 - Dc)2s+N0+1 dDc - (1 - Dc)2s+N0 +1 ln(1 - Dc) 1 -(1 - Dc)2s+N0+1 dN0 - 2(1 - Dc)2s+N0 +1 ln(1 - Dc) 1 - (1 - Dc)2s+N0+1 ds. (5.34)

242 5 Creep, Creep-Fatigue, and Dynamic Failures Taking the derivative with the notation δx = |dx| to ensure upper bounds on the errors gives δ(tR - tD) tR-tD =δtR tR tR tR-tD-δtD tD tD tR-tD, δtD tD = δ pD pD +N0δK0 N K0 N +N0δσeq σeq +N0 ln K 0 N σeq δN0 N0, δRν Rν =|6T2 X-2 3|ν Rν δν ν +6(1-2ν)T2 X Rν δTX TX. (5.35) The sensitivity on the rupture time is finally δtR tR = k StR Ak δAk Ak ,whereeach StR Ak is the sensitivity coefficient of the parameters Ak with respect to the time to rupture tR, StR TX=tR-tD tR 6s(1 - 2ν)T 2 X Rν , StR σeq =N0+tR-tD tR 2s, StR E =tR-tD tR s, StR ν =tR-tD tR |6T2 X-2 3 |νs Rν , StR K0 N =N0, StR N0 =N0 ln σeq K0 N+tR-tD tR 1 2s+N0 +1+(1-Dc)2s+N0+1ln(1-Dc) 1 -(1 - Dc)2s+N0+1 , StR pD=tD tR, StR S =tR-tD tR s, StR s =tR-tD tRs ln σ2 eqRν 2ES + 2 2s+N0 +1+ 2(1-Dc)2s+N0+1ln(1-Dc) 1 - (1 - Dc)2s+N0+1 , StR Dc =tR-tD tR (2s + N0 + 1)(1 - Dc)2s+N0Dc 1 -(1 - Dc)2s+N0+1 . To give relative values of these coefficients, an example of average values of the parameters representative of many materials is visualized by the height of the boxes in the scheme of Fig. 5.4. This is for σeq = 100 MPa, TX =1, Rν =2.07, and tD/tR =1/2 as quantities defining the loading and E = 140000 MPa, ν =0.3, K 0 N = 700 MPa·s1/N0 , N0 =8, pD =0.2, S =0.15 MPa, s =2,andDc =0.2 as values of the material parameters at a mid-level temperature.

5.2 Fast Calculation of Structural Failures 243 R t R tS R tE N N R tN K 0 0 R t0 N eq eq R t eq X X R tX T R R S SS S E E S KK S N N S S T T S t t ν σ + δ + δ + δ + δ + σ + δ = δ ν c c R t c D pD pD R tpD R tS D D S S SS S δ + ε + δ + ε 1.2 10 15 8 110.8 0.1 0.5 0.6 Fig. 5.4. Relative importance of each parameter in creep failures Here again, the parameters which have the largest influence on the ac- curacy of the time to failure are those defining the loading and particularly the stress acting on both the plastic strain and the damage rates. Note the extreme importance of the Norton exponent N0. The damage exponent s, the damage threshold pD and the critical damage Dc are found to be of less importance. For creep-fatigue, the calculation is very similar as only one logarithmic function is added, giving rise to two more terms related to the loading: the loading rate ˙ σeq and the hold time Δt, and to three sensitivity terms Sσeq max , Ss ,a ndSN0 for δσeq max σeqmax,δs s,a nd δN0 N0 . The number of cycles to rupture is given by (5.20) and the sensitivity to the hold time Δt or the fatigue stress rate ˙ σfeq are

244 5 Creep, Creep-Fatigue, and Dynamic Failures SNR Δt =NR-ND NR Δt 2 2s+N0+1 σeq max ˙ σfeq +Δt + ND NR SNR ˙ σf eq =NR-ND NR 2 2s+N0+1 σeq max ˙ σfeq 2 2s+N0+1 σeq max ˙ σfeq +Δt . (5.36) 5.2.4 Elasto-Visco-Plastic Stress Concentration Representing time-dependent viscosity effects such as creep and relaxation by post-processing an elastic computation is a difficult task as the reference calculation is time-independent. In the case of localized visco-plasticity (small scale yielding),such a reference computation coupled with the Neuber method allows us to deter- mine the history of the von Mises stress and the accumulated plastic strain. In case of fully (visco-)plastified mechanical components (large scale yielding), a time-dependent reference computation is needed. In order to de- rive a fast method, the idea is to perform an elasto-visco-plastic computation only on a Representative Volume Element with the nominal strain n(t)o r stress σn(t) as uniaxial loading, and to use the corresponding solution coupled with the knowledge of the notch elastic stress concentration coefficient KT. 5.2.4.1 Small Scale Yielding -- the Neuber Method In the case of visco-plasticity confined in a small stress concentration area, the main part of the structure remains elastic and is submitted to a relaxation state on the yielding part. Apply the Neuber method coupled with Norton law to yield σ2 eqRν E +σeqp =(σij ij)elas and ˙p = σeq -R-Xeq - σy KN N . (5.37) For a given triaxiality ratio, this gives a relationship between the von Mises stress and the plastic strain σeq = E2p2 +4ERν (σij ij)elas - Ep 2Rν , (5.38) and leads to the law p(t)andthenσeq(t) at the stress concentration point as the solution of the following first order differential equation: ˙p= 1 2Rν E2p2 +4ERν (σij ij)elas - Ep - R(p) - Xeq(p) - σy KN N . (5.39)

5.2 Fast Calculation of Structural Failures 245 This leads to a decreasing von Mises stress over a long period of time and corresponds to a relaxation deformation process. 5.2.4.2 Large Scale Yielding (M. Chaudonneret 1978, 1985) For the case of a structure undergoing a full visco-plastic state of deformation, the complete nonlinear computation is difficult to avoid! Nevertheless this can be done for the engineering cases of notches by following an extended Neuber procedure based on an uniaxial visco-plastic reference calculation made only on a volume element, on which the nominal stress σn(t)o rstr ain n(t)is applied. The loading may be creep, fatigue, or creep-fatigue. The information concerning the geometry of the notch is introduced in the rate form of the Neuber heuristic σ = σelas elas of Chap. 3 through the use of the elastic stress concentration coefficient KT (see Fig. 3.4): σ˙ +˙ σ =K2 T(σn ˙ n +˙ σn n) , (5.40) where the couple (σ, ) is determined from the stress-strain field at the most loaded point of the notch and where σn and n is the nominal stress and strain, respectively. Coupled with the strain partition, = e+ p=σ E+ p and n=σn E + p n, (5.41) one gets: ˙ σ=1 2σ+E p K2 T [(2σn + E p n)˙ σn+Eσn˙ p n]-Eσ˙ p . (5.42) This expression associated with a viscosity law such as the Norton law, ˙ p = |σ-X|-R-σy KN N sgn(σ - X)a n d˙ p=|˙ p| , (5.43) coupled with the consideration of both nonlinear isotropic hardening R = R(p) and kinematic hardening ˙ X=C˙ p - γX|˙ p| allows us to determine the stress and strain histories, σ(t)and (t). This just needs the use of a step-by- step differential scheme such as the Euler or better Runge--Kutta schemes. If the reference computation is made in elasticity, the method gives back the expression (5.37) for small scale yielding in which Rν =1,σeq = σ,and p= p. 5.2.4.3 Mesocrack Initiation Calculate the damage by performing the time integration of the unified dam- age law, ˙ D= σ2 2ES s | ˙ p| if p>pD, (5.44)

246 5 Creep, Creep-Fatigue, and Dynamic Failures D(t)= t tD σ2(t) 2ES s |˙ p(t)|dt, (5.45) with tD as the time at damage initiation given by pD = tD 0 |σ(t) - X(t)|-R(t) - σy KN N dt. (5.46) A mesocrack initiates when D = Dc for a time t = tR. Remark -- In the previous equations, σ(t) replaces the effective stress ˜ σ of the fully coupled analysis. This means that the Neuber method is in fact ˜ σ =K2 Tσn n (5.47) and gives an estimation of the effective stress directly. 5.2.4.4 Large Scale Yielding -- Approximate Method When the material is largely visco-plastic, i.e., when elasticity is negligible, a simpler, but 3D, form than the previous Neuber method may be derived. The Neuber fundamental hypothesis becomes ˜ σ p=K2 Tσn n for the uniaxial case, (5.48) or ˜ σeqp = K2 Tσeq npn for the 3D case, (5.49) where ˜ σand˜ σeq are the effective stress and effective von Mises stress, respec- tively, at the most loaded point. The Neuber heuristic (5.49) considered altogether with the pure viscous Norton law, ˙p = ˜ σeq K0 N N0 and ˙pn = σeq K0 N N0 , (5.50) leads to K0 N ˙p1/N0p = K2 TK0 N ˙p1/N0 npn (5.51) and p=K2N0 N0 +1 T pn and ˙p=K2N0 N0 +1 T ˙pn, (5.52) where K 2N0 N0 +1 T acts as a creep strain concentration coefficient. The effective stress is then ˜ σeq=K0 N˙p1/N0 =K 2 N0 +1 TK0 N ˙p1/N0 n =K2 N0 +1 T σeqn . (5.53)

5.2 Fast Calculation of Structural Failures 247 The damage initiated at the stress concentration point after a service time tD is a solution of pD = tD 0 ˙p(t)dt = K 2N0 N0 +1 T tD 0 ˙pn(t)dt, (5.54) i.e., when pn(tD)=K - 2N0 N0 +1 T pD. Failure occurs when D(t = tR) reaches locally Dc with D = t tD ˜ σ2 eqRν 2ES s ˜ σeq K0 N N0 dt = K 4s+2N0 N0 +1 T (2ES)s (K 0 N)N0 t tD σ2s+N0 eq n (t)Rs ν(t)dt (5.55) where K 4s+2N0 N0 +1 T acts as a damage rate concentration coefficient. An example is given in Sect. 5.3.2. 5.2.5 Safety Margin and Crack Growth In creep, the security is governed by the duration without any accident so that the essential parameter is the time t. A safe design of a component must prove that the service time is below the time tR of a crack initiation somewhere in the structure. Here, we introduce again a safety factor Saf which defines the safety margin tservice < tR Saf . (5.56) If creep fatigue is involved, the engineering parameter can be either the num- ber of cycles N or the accumulated time t and the safety margins are defined as Nservice < NR Saf or tservice < tR Saf . (5.57) When dealing with service durations larger than several years, much care must be taken as the identification of the parameters is most often based on short range tests. In situ control of components in service and updated cal- culations are advised each time new information arrives. Anyway, the safety factor must be large enough so that Saf = 5, 10, 20, or more depending on the expected duration of the component. A more advanced concept consists of evaluating the rupture probability while taking into account the scatter of the material parameters and the uncertainties upon the loading. There is no simple way to determine the crack growth rate but the nu- merical simulation by a structure calculation with elements removal in elasto- visco-plasticity coupled with damage is possible. The viscosity, playing a reg- ularization role, ensures the convergence of the numerical algorithms (see Sect. 1.6.2).

248 5 Creep, Creep-Fatigue, and Dynamic Failures 5.3 Basic Engineering Examples Here we describe some simple results that can help us quickly estimate creep or creep-fatigue effects on failure of mechanical components. The accuracy is poor as the temperature increases the nonlinearities regarding to stress- strain and time relations. If an accuracy of a few percent may be expected in predictions in elasticity, it increases to 10--20% in plasticity and up to 50-- 100% in visco-plasticity. Only fatigue is worse: a factor of 10 (1000% !) may happen in high cycle fatigue! 5.3.1 Strain Rate and Temperature-Dependent Yield Stress What is called "dynamic plasticity" is in fact visco-plasticity as the high strain rates play a role even at room temperature. Furthermore, the short times involved induce almost adiabatic plasticity for which the effect of plas- tic dissipation increases the temperature. Here we derive an approximate formula to obtain the yield stress as well as function of the strain rate and the temperature, from its value at room temperature or an other reference temperature. The effect of the temperature T is introduced by considering the visco- plastic strain as a thermally-activated phenomenon governed by the Arrhe- nius law which makes the unidimensional plastic strain rate dependent on the temperature, as in ˙ p ≈ gσ, p(σ, p)exp - H T , (5.58) where the parameter H is related to the energy of activation of the process. We then introduce the pure viscous Norton law at a reference temperature T0, ˙ p = σ K0 N N0g p( p)exp H T0-H T . (5.59) First, consider the engineering yield stress σy02(˙ p0,T0) corresponding to a plastic strain p0 =0.210-2, a reference plastic strain rate ˙ p0 ,a ndthe reference temperature T0: σy02(˙ p0 ,T0)=K 0 N ˙ p0 g p( p0) 1/N0 . (5.60) Second, consider the engineering yield stress σy02(˙ p,T) corresponding to a larger plastic strain rate ˙ p and a larger temperature T , σy02(˙ p,T)=K 0 N ˙ p g p( p0) exp - H T0-H T 1/N0 . (5.61)

5.3 Basic Engineering Examples 249 Finally, for the 3D case, ˙ p becomes ˙p and the engineering yield stress (both strain-rate- and temperature-dependent) is approximately given by σy02(˙ p,T)≈ σy02(˙ p0,T0) ˙p ˙ p0 1/N0 exp - H N0 1 T0-1 T , (5.62) an expression which needs the knowledge of: • The Norton parameters K 0 N and N0 at the reference temperature T0 not too far from the temperature considered because, unfortunately, they are not exactly constant with the temperature, • The yield stress σy02 at a reference strain rate ˙ p0 and temperature T0, and • The parameter H "adjusted" on the yield stress at least at one other temperature. To finish, expression (5.62) can also be used at room temperature, particularly in dynamics problems such as shocks, crash, or perforation, considering ˙ p0 ≈ ˙ 0 so that σy02(˙ p)=σy02(˙ 0) ˙p ˙ 0 1/N0 . (5.63) At room temperature, the exponent N0 is large (N0 ≈ 20 to 100) and the only possibility to identify its value for each material is to perform relaxation tests at large values of initial strain rate. For steels, the plastic strain rate may vary over several decades in a few hours (Fig. 5.5). Fig. 5.5. Relaxation tests to identify pure viscous Norton parameters for 316 stain- less steel at room temperature (J. Lemaitre and J.L. Chaboche 1985)

250 5 Creep, Creep-Fatigue, and Dynamic Failures 5.3.2 Plates or Members with Holes or Notches This is the same problem as in Sects. 3.3.1 and 4.3.1 where a hole or a notch increases the nominal stress σn on its edge due to the elastic concentration coefficient KT. Consider the case of a fully visco-plastic component where the damage may initiate and reach the critical localized damage at the stress concentration point. Use the approximate Neuber method of Sect. 5.2.4 which states for a local uniaxial state of stress σ and ≈ p that ˜ σ =K2 Tσn pn , (5.64) and consider the pure viscous Norton law: ˙ p = ˜ σ K0 N N0 and ˙ pn = σn K0 N N0 , (5.65) with ˜ σ = σ/(1 - D) as the effective stress at the stress concentration point. Determine then the history of the strain p(t) and the effective stress ˜ σ(t). The local damage is given by (5.55) and a mesocrack initiates at the time tR when D reaches the critical value Dc . 5.3.2.1 Creep Mesocrack Initiation Consider first the case of creep: a constant far field σ∞ leads to a constant nominal stress σn (see Fig. 3.4). The full procedure takes 3 steps: 1. Perform the reference calculation The solution pn(t) for creep at σn = const is pn(t)= σn K0 N N0 t. (5.66) 2. Apply the approximate Neuber method The Neuber heuristic and the Norton law lead to p(t)=K 2N0 N0 +1 T pn(t) (5.67) and the effective stress is ˜ σ=K2 N0 +1 TK0 N˙ 1/N0 pn =K2 N0 +1 T σn = const. (5.68) 3. Calculate the damage evolution The damage initiates at t = tD when the plastic strain reaches the damage threshold pD locally, tD=K- 2N0 N0 +1 T pD K0 N σn N0 . (5.69)

5.3 Basic Engineering Examples 251 For a stress concentration coefficient of KT = 3, this means that the damage initiates at the stress concentration point for a time tD that is 3 to 9 times shorter that the time tDn of damage occurrence in the entire cross section as tDn = pD K0 N σn N0 . The damage history is D(t)=K 4s+2N0 N0 +1 T σ2s+N0 n (2ES)s (K 0 N)N0(t - tD). (5.70) Finally, failure occurs when D = Dc for a creep time tR represented by tR=K- 2N0 N0 +1 T pD K0 N σn N0 + K- 4s+2N0 N0 +1 T (2ES)s K 0 N N0 Dc σ2s+N0 n . (5.71) The second term (tertiary creep) of the time to rupture varies as the inverse of the stress to the power (2s + N0) which can be on the order of 5 to 20 that of a very large stress sensitivity. Then be careful when defining a safety factor. 5.3.2.2 Creep-Fatigue The far field σ∞(t) varies periodically between 0 and σ∞ max , with a hold time Δt at σ∞ max . The nominal stress varies between 0 and σnm a x in the same manner. This is creep-fatigue for which the resolution is similar to the one detailed in Sect. 5.2.2. The approximate Neuber method allows us to again calculate the history of the accumulated plastic strain p(t) and the damage D(t) at the stress concentration point. The three-step procedure is the same as for the creep case: 1. Perform the reference calculation One has to calculate the plastic strain increment per cycle, δpn δN = 1cycle| ˙ pn|dt. (5.72) During the monotonous part of the loading, consider an applied load linear in time with σn =˙ σfn t,where ˙ pn = σn K0 N N0 = ˙ σfn K0 N N0 tN0 =⇒ Δ pn = 1 (N0 +1)(K 0 N)N0 σN0+1 nm a x ˙ σfn . (5.73)

252 5 Creep, Creep-Fatigue, and Dynamic Failures During the creep part, Δ pn = σnm a x K0 N N0 Δt. (5.74) Then, δpn δN = σnm a x K0 N N0 2 N0 +1 σnm a x ˙ σfn +Δt . (5.75) 2. Apply the approximate Neuber method The Neuber heuristic ˜ σeqp = K2 T σn n and the previous Norton law give the local plastic strain as p(t)=K 2N0 N0 +1 T pn(t) , (5.76) the local plastic increment per cycle as δp δN=K2N0 N0 +1 T δpn δN, (5.77) and the effective stress at the stress concentration point as ˜ σ(t)=K 2 N0 +1 TK0 N ˙p1/N0 n (t)=K 2 N0 +1 T σn(t) . (5.78) 3. Calculate the damage evolution Damage initiates after a number of cycles N = ND when p = δp δNN reaches the damage threshold pD. The corresponding number of cycles is then ND= pD δp δN =K- 2N0 N0 +1 T pD δpn δN , (5.79) with pD given by (5.19) of Sect. 5.2.2, pD = pD 2σu σeq max m =K- 2m N0 +1 T pD 2σu σnm a x m . (5.80) The damage history is given by the time integration of the damage law, ˙ D= ˜ σ2 2ES s ˜ σ K0 N N0 if p>pD , (5.81) first over one cycle, δD δN = 1cycle ˙ Ddt, then over the whole loading. Dur- ing the monotonous loading part with ˙ σn =˙ σfn = const, as in Sect. 5.2.2,

5.3 Basic Engineering Examples 253 ˙ D= ˜ σ2s+N0 (2ES)s (K 0 N)N0 = K 4s+2N0 N0 +1 T ˙ σf 2s+N0 n (2ES)s (K 0 N )N0 t2s+N0 (5.82) gives a damage growth of ΔD= K 4s+2N0 N0 +1 T (2s + N0 + 1)(2ES)s(K0 N )N0 σ2s+N0 +1 nm a x ˙ σf 2s+N0+1 n . (5.83) During the creep part of each cycle, ˙ D= K4s+2N0 N0 +1 T (2ES)s (K 0 N )N0 σ2s+N0 nm a x =⇒ ΔD= K4s+2N0 N0 +1 T (2ES)s (K 0 N )N0 σ2s+N0 nm a xΔt. (5.84) Then, δD δN = K 4s+2N0 N0 +1 T (2ES)s (K 0 N )N0 σ2s+N0 nm a x 2 2s+N0+1 σnm a x ˙ σn +Δt (5.85) and the number of creep-fatigue cycles to rupture corresponds finally to D(NR)= δD δN · (NR - ND)=Dc so that NR =ND+K-4s+2N0 N0 +1 T (2ES)s K 0 N N0 Dc σ2s+N0 nm a x × 2 2s+N0+1 σnm a x ˙ σn +Δt -1 with ND = K- 2(N0+m) N0 +1 T pD (2σu)m K 0 N N0 σN0+m nm a x 2 N0 +1 σnm a x ˙ σfn +Δt -1 . (5.86) Even for such a complex case, the number of cycles to rupture by mesocrack initiation is fully determined from the knowledge of the nominal strain σn(t) and the elastic stress concentration coefficient KT. Again, the sensitivity to the stress is high and a small hold time has already a strong negative effect on the component lifetime. 5.3.3 Pressurized Shallow Cylinder From the analysis of the Sect. 3.3.2 (Fig. 3.6), the stresses are expressed as a function of the applied pressure P , the radius Rcyl, and the thickness tcyl of the cylinder as

254 5 Creep, Creep-Fatigue, and Dynamic Failures σeq(t)=√3 2 P (t)Rcyl tcyl ,T X=σH σeq=1 √3, and Rν =5-4ν 3 . (5.87) The problem is to determine the time of a mesocrack initiation, tR, when the pressure is kept constant (creep) or when it varies periodically with periods of hold time Δt at P = Pmax (creep-fatigue). We neglect here the time-to- damage initiation. For creep, the integration of the damage law with a pure viscous Norton law is straightforward: ˙ D= σ2 eqRν 2ES(1 - D)2 s σeq K0 N(1 - D) N0 (5.88) or Dc 0 (1 - D)2s+N0dD = σ2 eqRν 2ES s σeq K0 N N0 tR , (5.89) and finally: tR = 1-(1-Dc)2s+N0+1 2s+N0+1 (2ES)sK 0 NN0 5-4ν 3 s √3 2 PmaxRcyl tcyl 2s+N0 . (5.90) What is important is that tR varies as the pressure P to the power 2s + N0, which can be on the order of 10 to 15 for metals. This means that an increase of the pressure of 5% may reduce the time to an explosion by a factor of about 2 or more! For creep-fatigue induced by a pressure maintained constant at P = Pmax for N periods of time Δt, the integration of the damage law is the one of Sect. 5.2.2 (Eqs. (5.16) to (5.20)), with of course the partic- ular values (5.87) for the state of stress and stress triaxiality and a con- stant pressure rate ˙ Por- ˙ P during the loading or unloading parts of the cycle. The number of cycles to rupture is NR = (1 - (1 - Dc)2s+N0 +1)(2ES)sK 0 NN0 (2s+N0+1) 5-4ν 3 s √3 2 PmaxRcyl tcyl 2s+N0 × 2 2s + N0 +1Pmax ˙ P +Δt -1 . (5.91) In practical applications, the creep term is almost always much larger than the fatigue term, i.e.,

5.3 Basic Engineering Examples 255 Δt 2 2s + N0 +1Pmax ˙ P. (5.92) Again, this means that the fatigue damage may sometimes be neglected, but never the creep damage. 5.3.4 Adiabatic Dynamics Post-Buckling in Bending This is the same problem as the plastic post-buckling of beams treated in Sect. 3.3.3 except that it corresponds to a crash or a shock problem where dynamic plasticity, that is visco-plasticity, occurs. Then two phenomena must be considered: • The strain rate effect which requires us to consider a visco-plastic consti- tutive equation. • The large increase in temperature due to a plastic dissipation in a short time which necessitates the consideration of the thermomechanical cou- pling. The problem is made as simple as possible in order to obtain the energy absorbed in the material in a closed-form useful for qualitative discussion about the influence of each parameter. • The geometrical description is in Fig. 3.7 of Chap. 3 where the Bernoulli hypothesis allows us to write = M2y h. (5.93) • The energy absorbed by the full plastic hinge of the beam l = πh/2is W =2bl h/2 0 tM 0˙ w dtdy, (5.94) where tM is the time to achieve the process and ˙ w is the plastic power density ˙ w=σ˙ p. (5.95) • The visco-plastic constitutive equation is the pure viscous Norton law ritten with the damage effective stress ˜ σ = σ/(1 - D), where the coupling with the temperature is a power function approximation of the Arrhenius term exp H T : ˙ p = ˜ σ K0 N N0 T T0 HN , (5.96) where T0 is the reference temperature at which the material parameters K0 N and N0 are identified. HN is the temperature exponent on the order of 5 to 10 for steels in the range of 100 to 500◦C.

256 5 Creep, Creep-Fatigue, and Dynamic Failures • The damage constitutive equation is the simplified expression (assuming the strain hardening saturated) obtained in Sect. 3.2.1 with the damage threshold pD taken to be equal to zero. The coupling of the damage with the temperature is neglected as at least part of it is already taken into account through the plastic strain p,sothat D=Dc p pR . (5.97) • The temperature derives from the adiabatic condition written as the heat equation, ρCh ˙ T=˙ w, (5.98) where ρ is the density, ρ = 7800 kg/m3 for steels, Ch is the specific heat, and Ch ≈ 500 J/kg ◦C for steels. Then ˙ T= ˙ w ρCh or T=T0+ w ρCh . (5.99) • Some other hypotheses can make the person in charge of the calculation happy: -- Elastic strain neglected so that p = -- Process at constant strain rate, ˙ =const=˙ → =˙ t The calculation is now easy: ˙ w=K0 N 1-Dc p pR T T0 - HN N0 ˙ N0 +1 N0 p , (5.100) w 0 1+ w ρChT0 HN N0 dw = t 0K0 N 1-Dc ˙ pR t ˙ N0+1 N0 dt, (5.101) ρChT0N0 HN +N0 1+ w ρChT0 HN +N0 N0 - 1 = K0 N t-Dc ˙ pR t2 2 ˙ N0+1 N0, (5.102) or w = ρChT0 1+ (HN + N0)K 0 N ρChT0N0 1 - Dc ˙ 2 pR t ˙ N0+1 N0 t N0 HN +N0 -1 . (5.103) Taking the total time tM as the kinematic measure of the process, ˙ =˙ (y)= 2 M tM yh. (5.104) The energy absorbed, W =2bl h/2 0 w(y, tM)dy,is

5.4 Numerical Failure Analysis 257 W =2blhρChT0 1 2 0 1+(HN + N0)K0 N (2 M) N0 +1 N0 ρChT0N0t1/N0 M × 1-Dc M pR u u N0+1 N0 N0 HN+N0du-1 2 , (5.105) with M = πh-πh/2 πh/2 =1andl = πh/2 for a full bending. Without any coupling nor damage, ˙ w0=K0 N˙ N0 +1 N0 p (5.106) and W0 = blh N0K0 N 2N0 +1 N0 +1 N0 M t-1/N0 M. (5.107) In both cases, the energy absorbed increases as the process is faster but the increase is weak as N0 is always large and tM is always short, thus keeping the variations of the term t-1/N0 M small. Some applications show that the coupling with the damage is more impor- tant than the coupling with the temperature. In (5.105), the damage coupling is governed by the term Dc M/ pR while the temperature coupling is mainly governed by the dimensionless ratio K 0 N /ρChT0t1/N0 M . Altogether they lead to a ratio W/W0 on the order of 0.7 to 0.9 for metals. 5.4 Numerical Failure Analysis At high temperatures, many materials become visco-plastic and the main local loadings encountered in mechanical components are creep, creep-fatigue, and relaxation. Viscosity enhances the stress redistribution, with a strong effect on damage and failure. A structure computation made in elasto-visco-plasticity coupled with damage gives the damage map history and the crack initiation conditions. If the damage constitutive equations are not available in an FE code, imple- ment them by use of the numerical schemes of Chap. 2. For non-isothermal loadings, it is important to have a complete set of material parameters for the temperature range of the application in mind. Identify the parameters at a few constant temperatures (see for instance Sects. 1.4.4, 1.5.1.1 and 2.4). Use the least square method to fit the temperature dependency with non- linear functions of T . Don't be afraid to use nonlinear functions as smooth functions are better than linear interpolation. For example, for a material parameter A, a general possibility is A=a1+a2T+a3exp(a4T). (5.108)

258 5 Creep, Creep-Fatigue, and Dynamic Failures The use of the anisotropic damage law is again advised as it needs only one additional material parameter which in practice may be taken as η =3. The consideration of the quasi-unilateral conditions of microdefects closure is not necessary if the loading remains positive as is often the case in creep and creep-fatigue. A fully-coupled analysis is very costly and for cyclic loading, one may use an elasto-visco-plasticity computation followed by a damage post-processing (uncoupled analysis). An example is given in Sect. 5.4.3. Oneoftheveryfirstthingtodoistotestthenumericalimplementationof the constitutive laws on a simple reference calculation (and also the quality of the mesh, the time increments, and the convergence of the computation). The academic problem of the hollow sphere under external pressure is especially designed for this purpose (see Sect. 5.4.1). It uses simple assumptions for both viscosity and damage. 5.4.1 Hollow Sphere under External Pressure (A. Benallal, R. Billardon and L. Moret--Bailly 1991) This example has been designed to check the numerical procedures introduced in an FE code. It is built on the possibility to exhibit a closed-form solution in elasto-visco-plasticity fully coupled with damage when the material behavior is modelled by the following constitutive equations of perfect visco-plasticity (no hardening) with a linear Norton law: = e+ p, e=1+ν E(1-D)σ- ν E(1-D)trσ1, ˙ p=32 σD σeq ˙p, with ˙p = σeq 1-D-σy Ky N Ny with Ny =1. (5.109) The damage evolution law is written as ˙ D=Ys S0 ˙p (5.110) so that S0 = Ss recovers the unified damage law ˙ D =(Y/S)s ˙p. With s =0 and σy = 0, it corresponds to the simple law ˙ D= σeq S0K0 N(1-D) (5.111)

5.4 Numerical Failure Analysis 259 which does not take into account the triaxiality effect. But when considered altogether with ν =0.5, it allows for a closed-form solution of the hollow sphere problem. Consider an external pressure loading P (t) applied on the sphere of Fig. 5.6. The solution at time t, at a radius point r,isoftheform D =1- g(t)+ f(t) S0K0 Nr3 σeq =(1- D) σy (1 - exp (-μt)) + ˙f(t) r3 , (5.112) where μ = E/K0 N and g(t)=1- σy S0K0 N t-1 μ+1 μ exp (-μt) . (5.113) • Up to mesocrack initiation (which occurs at the inner radius when D(a)=1), f(t)= 1 α -βg(t)+ β2g2(t)+2α Π(t) - S0K 0 N(g2(t) - 1)ln ba , (5.114) where Π(t)= t 0 P(τ)dτ , α = 1 b6-1 a6 3S0K0 N , andβ=2 3 1 a3-1 b3 . (5.115) Z p C B A r mm 30. 42. r P(t) b a Fig. 5.6. Hollow sphere under external pressure and FE meshing

260 5 Creep, Creep-Fatigue, and Dynamic Failures • Beyond mesocrack initiation, the time evolutions of the radius c(t)ofthe spherical damaged zone and of the function f(t) satisfying the coupled differential equations are P (t)=2σyg(t)ln b c(t) + 2σy 3S0K0 N f(t) - 23 ˙f(t)g(t) 1 b3- 1 c3(t) + ˙f(t)f(t) 3S0K 0 N 1 b6- 1 c6(t) ˙ c(t)=σy c4/3(t) 3f(t) + c(t) ˙f(t) 3f(t) . (5.116) Fig. 5.7. a Loading history. b Damage vs time at Gauss points A, B and C. c von Mises stress vs time at Gauss points A, B and C. d Damage initiation front c(t) (FE solution: open circles; closed-form solution: solid line). e Damage vs radius for different times. f von Mises stress vs radius for different times

5.4 Numerical Failure Analysis 261 This problem is used to check an FE implementation in ABAQUS (the UMAT VISCOENDO of LMT-Cachan). The mesh made of forty 8-node quadrilateral elements is depicted in Fig. 5.6 where the boundary conditions are indicated. Due to axial symmetry, one quarter of the sphere is modelled. The pressure history is given in Fig. 5.7a. 5.4.1.1 Validation of the FE implementation Figures 5.7b and 5.7c illustrate the evolutions with time of the damage D(t) and von Mises stress σeq(t) at the three Gauss points A, B,a ndC marked in Fig. 5.6. The agreement between the analytical solution (con- tinuous line) and the FE analysis (open circles) validates the numerical implementation. The curves of Fig. 5.7d for times t4 to t7 give an idea of the propagation of the damage initiation front radius c(t). The slight deviation between the two solutions observed is due to the fact that in the closed form solution, Dc is taken to be equal to 1 instead of 0.9 for FE computations, and hence leads to a larger time for initiation. Figure 5.7e shows the damage redistribution along the radius obtained with ABAQUS or different times t1 to t7 (see Fig. 5.7a). Since the numerical critical value for damage is taken as Dc =0.9, t4 appears as the time to the initiation of a mesocrack at an inner radius of a = 30 mm. 5.4.1.2 Interpretation of the Results Figure 5.7f shows the role of the coupling of the damage model with elasto- visco-plastic equations. Since the fully-coupled approach has been used in this example, both the effect of the damage gradient within the structure and the effect of the damage front advance (modelled by the removal of completely broken elements) on the stress field can be observed: first, at the beginning of the loading (between times t2 and t4), the redistribution of the equivalent stress σeq is only due to the damage evolution (which is quicker at the inner radius); second, beyond the time to mesocrack ini- tiation t4 , although the pressure load is constant, very large increases in the von Mises stress correspond to the propagation of the front which be- comes the effective inner radius. In other words there is a growth of the inner cavity. Besides, it can be noticed in Figs. 5.7c and 5.7f that the point B plays the role of the "skeletal" point of the "Reference Stress Method" (D.L. Mariott and F.A. Leckie 1970), where the equivalent stress remains constant during the pure creep loading (for t greater than t2) despite the redistribution of the stresses within the structure.

262 5 Creep, Creep-Fatigue, and Dynamic Failures 5.4.2 Effect of Loading History: Creep-Fatigue Let us study again creep-fatigue interaction but with now the full set of elasto- visco-plasticity coupled with damage constitutive equations of Table 1.3. The loading is described in Fig. 5.3. The material is a stainless alloy IN 100 at 827◦C and the material parameters are • For elasticity: E = 170000 MPa • For viscosity (Norton law): KN = 450 MPa·s1/N and N =7.5 • For isotropic hardening modelling cyclic softening: R∞ = -15 MPa, b = 100 with an initial yield stress σy =30MPa • For kinematic hardening: C = 138000 MPa, γ = 1200 (then X∞ = C/γ = 115 MPa) • For damage: S =0.2MPa,s =1, pD =0.005, and Dc =0.3 The damage threshold pD is a constant equal to pD. A numerical resolution of the constitutive laws is necessary to plot the creep-fatigue interaction diagram of NR/NRF vs tR/tRC for a given maximum stress σM , a fatigue stress rate ˙ σf , and different hold times Δt (with NR as the number of creep-fatigue cycles and tR = NR · Δt a sthetim espe ntin creep). The computation is performed here on a single element in ABAQUS by using VISCOENDO UMAT. Fig. 5.8. Computed creep-fatigue interaction diagram for the stainless alloy IN 100 at 827◦C (J.P. Sermage 1998) Using the above, we obtain a strong nonlinear creep-fatigue interaction (Fig. 5.8): the larger the maximum stress the stronger the nonlinearity, as

5.4 Numerical Failure Analysis 263 observed experimentally for this material. The material response obtained is very sensitive to creep as a small hold time reduces the lifetime substantially: for a maximum stress of σM = 200 MPa (corresponding to NRF = 1720 cycles, tRC =18· 104s), 10% of creep decreases by half the lifetime. Another important result is that this nonlinearity is mainly governed by the kinematic hardening. Setting R = const = R∞ does not change the results much. 5.4.3 Creep-Fatigue and Thermomechanical Loadings (J.P. Sermage, J. Lemaitre and R. Desmorat 2000) Both coupled and uncoupled analyses are compared here to experimental results concerning the Maltese cross shape specimen of Fig. 4.13, loaded by two forces in its plane, F1 and F2 . The specimen is heated with a controlled eddy current heating system which ensures a "uniform" temperature field at ±5◦C. The real temperature is measured by thermocouples and introduced as a given temperature field in the structure calculation. Fig. 5.9. Tests performed

264 5 Creep, Creep-Fatigue, and Dynamic Failures Six tests are performed with forces histories F1(t), F2(t), and temperature histories given in Fig. 5.9. The first test performed at room temperature is the multilevel fatigue test of Chap. 4. The tests 2 to 6 are: • Two in-phase creep-fatigue interaction tests with F1 = F2 between 0a ndFmax = 28 kN at constant temperature T=580◦C (test 2) and T=620◦C (test 3). The loads F1max = F2max =28kNhaveaholdtime of Δt = 40 s. The period of the loading is Δt +2δt =50s. • One multilevel out-of-phase non-proportional loading test at T=580◦C (test 4). The maximum applied loads are F1max = F2max = 28 kN for the first 1000 cycles, F1max = F2max = 35 kN for the next 1000 cycles, and then F1max = F2max = 38 kN up to failure. • One thermal fatigue test at constant loads F1 = F2 = Fmax =32kN (after an initial load from 0 to Fmax in 50 s) and variable temperature (test 5). The temperature varies between the maximum 580◦Ca ndthe minimum 300◦C within a period of 600 s. • One sequential non-proportional loading test (test 6). The specimen is submitted to a non-proportional loading in sequences of 4 cycles of periodic F1(t) between 0 and Fmax =35kNatF2 = 0 followed by 4 cycles of periodic F2(t) between 0 and Fmax =35kNatF1 =0;the duration of a loading-unloading is 20 s which corresponds to 160 s per full cycle. These histories of loading are the inputs: • For a fully coupled FE analysis using ABAQUS and VISCOENDO UMAT. • For an uncoupled analysis using ABAQUS and VISCOENDO but with no damage. The results are then the inputs of a post-processor damage calculation in order to perform the "a posteriori" time integration of the unified damage law. The drawing of the specimen is given in Sect. 4.4.2. The material is a 2-1/4 CrMo steel. A first identification of the elasto-visco-plasticity and damage ma- terial parameters has been made at different temperatures (20◦C, 100◦C,..., 580◦C). The temperature dependency of the parameters is then modelled through a fitting with nonlinear functions of the temperature given in Ta- ble 5.1. In the range 580◦C--620◦C, the viscosity parameters are assumed to remain constant (equal to those identified at 580◦C). A thermomechanical validation is presented in Figs. 2.7 and 2.8. Cases 2 to 6 are calculated first by the uncoupled method of a visco- plasticity ABAQUS computation of a few cycles followed by a damage calcu- lation (see Sect. 2.1.3). On HP 700 working stations, each FE computation takes a few hours when about one minute is needed for the damage calculation at the most loaded point. Each case is also computed using the fully-coupled method VISCOENDO-ABAQUS but as all the cycles must be calculated with

5.4 Numerical Failure Analysis 265 small time increments to ensure the convergence of the algorithm: each case takes about 1 week (!!) of computation on an HP 700. The final results of the number of cycles-to-crack-initiation, both from experiments and from calculations, are summarized in Table 5.2 and in Fig. 5.10. The accuracy of the fully-coupled analysis is good for such com- plex loadings. The uncoupled analysis is of course less accurate (but so much cheaper!). It loses its feature of being conservative when the loadings become non-proportional. Ta b l e 5 . 1 . Material parameters for a 2-1/4 CrMo in the range 20◦C--580◦C Poisson's ratio νν = const ν =0.3 Young's modulus E E(T)=e1 [1 - exp(e2T)] + e3 e1 = 31800 MPa e2 =1.88 10-3 ◦C-1 e3 = 199800 MPa Yield stress σy σy(T)=k1 [1 - exp(k2T)] + k3 k1 =70MPa k2 =1.58 10-3 ◦C-1 k3 = 191.5MPa Thermal expansion α α(T)=α1 + α2T α1 =1.110-5 ◦C-1 α2 =3.66 10-9 ◦C-2 Isotropic hardening R R∞ = r1[1+exp(r2T)]+r3 r1 =0.78 MPa r2 =610-3 ◦C-1 r3 =4.5MPa b=2 Kinematic hardening X γ(T)=γ1 [1 + exp(γ2T)] + γ3 X∞(T)=x1 - x2T x1=150MPa x2 =0.216 ◦C-1 γ1 =0.392 γ2 =9.69 10-3 ◦C-1 γ3 = 140.5 Viscosity parameters K(T)=k1 + k2T + k3 exp T -k4 k5 ) N(T )=n1 exp [-(n2T )n3 ]+n4 k1=190 k2 =0.25 ◦C-1 k3 =2.7 k4 = 372.7 k5 =35.32 n1 =10.315 n2 =0.022 ◦C-1 n3 =4.89 n4 =2.41 Damage D pD(T )=p1T + p2 S(T)=s1 [1 - exp(s2T)] + s3 s=2 Dc =0.2 p1 = -0.000285 p2 =0.2657 s1 =0.108 s2 =0.0052 s3 =2.81

266 5 Creep, Creep-Fatigue, and Dynamic Failures To finish, note that the results are very sensitive to temperature. The same computation with a slight difference in the applied temperature gives a very different number of cycles to failure: for test 2, a temperature of 590◦C instead of 580◦C leads to a number of cycles-to-crack-initiation of 300 instead of 420. Ta b l e 5 . 2 . Calculated and experimental numbers of cycles at mesocrack initia- tion NR Comparisons Test performed Experiments Fully-coupled Uncoupled analysis analysis Test 2 & 3 Creep-fatigue NR(580◦C) = 331 NR = 420 NR = 266 NR(620◦C) = 100 NR = 115 Test 4 Out of phase non-proportional loading NR=2356 NR=2135 NR=1130 Te s t 5 Thermal fatigue NR =56 NR =48 NR =27 Te s t 6 Sequential non-proportional loading NR=196 NR=230 NR=273 Fig. 5.10. Comparison between predicted numbers of cycles to mesocrack initiation and experimental results

5.4 Numerical Failure Analysis 267 5.4.4 Dynamic Analysis of Crash Problems (F. Lauro, B. Bennani, S. Tison, P. Croix 2003) Crash problems or dynamic failures on metallic or polymer structures gen- erally involve a large range of plastic strain rates whose effects have to be taken into account through visco-plasticity and, furthermore, through visco- plasticity coupled with damage. As an example, consider a notch extruded tube of rectangular cross section impacted in bending as represented in Fig. 5.11. Fig. 5.11. Dimensions and finite element model of impacted tube (half by sym- metry) The constitutive equations are those of Table 1.3: elasto-(visco-)plasticity coupled with damage but associated to the Hill criterion due to the plastic anisotropy induced by the process of extrusion. The material is an aluminum alloy 6014 T7 with the following values of the material parameter identified from tension-compression experiments described in Sects. 1.4.4 and 1.5.1:

268 5 Creep, Creep-Fatigue, and Dynamic Failures • Elasticity: E = 70000 MPa, ν =0.33 • Plasticity: -- Hill criterion f = 32 σ 1-D:h: σ 1 - D 1/2 =σvwithhastheHill fourth order tensor (see Sect. 3.4.8) with 6 independent material pa- rameters, -- In the longitudinal direction for ˙ ≈ 10-3 s-1: yield stress σy = 240.6 MPa, ultimate stress σu = 275 MPa, rupture strain R ≈ 0.5 -- The effect of the strain rate is assumed saturated in this crash applica- tion so that the viscous law is simply modelled by a σv(p)lawentered point by point in the FE input file: σv (MPa) 240.6 264.5 273 278.8 340.3 410 p 0 0.034 0.05 0.065 0.5 1 • Damage: pD =0.05, s =2,S =1.22 MPa, Dc =0.36 Fig. 5.12. Experimental and numerical simulation of the crack path The calculation is performed with PAMCRASH 2000 code with 15614 shell elements and 7 integration points in the thickness. The propagation of the crack is simulated by element removal when the damage D reaches Dc at all its integration points. The full calculation up to rupture in 5 ms in the experiment takes 22 hr on an HP workstation. The corresponding experiment is performed with an impactor reaching thetubeat3m/s .Thec o mpa ris o nbetw e e nthen u m e ric alsim ulatio na nd the experiment is shown in Fig. 5.12 for the failure path and in Fig. 5.13 for the load displacement curve. The agreement is satisfactory for the path and the maximum load. For the energy absorbed, the numerical simulation results are ≈ 20 % lower than the experiment.

5.4 Numerical Failure Analysis 269 Fig. 5.13. Load-displacement curve 5.4.5 Ballistic Impact and Penetration of Projectiles (T. Børvik, O.S. Hopperstad, T. Berstad and M. Langseth 2001) The penetration of projectiles at high speed is a difficult problem as it involves adiabatic shear localization, thermal plastic instabilities, and high gradients of stresses, as shown in Fig. 5.14. Fig. 5.14. Description of the mechanism of penetration

270 5 Creep, Creep-Fatigue, and Dynamic Failures Nevertheless, it is possible to use elasto-visco-plasticity coupled with dam- age constitutive equations described in Sect. 1.5 and a finite element numeri- cal procedure as long as the effects of temperature are represented by proper functions. For the latter one may use either the expression of the yield stress function of the strain rate and the temperature derived in Sect. 5.3.1, σy(˙ p,T)≈ σy(˙ p0,T0) ˙p ˙ p0 1/N exp - H N 1 T0-1 T , (5.117) or the Johnson--Cook model (1983) modified by M. Ortiz (1997), σeq = σy0 + KJC p1/MJC 1+ ˙p ˙ p0 CJC 1 - T - T0 Tm - T0 mJC , (5.118) where σy0, KJC, MJC, CJC,˙ p0,andmJC are material parameters, T0 is the room temperature, and Tm is the melting temperature of the material. In fact, the Johnson--Cook model is a particular case of the general frame- work of Sect. 1.5, where the yield function without kinematic hardening and damage reads σeq =σy+R+σv (5.119) if the following functions for the yield stress σy, the isotropic hardening R, and the viscous stress σv are adopted together with: T =T-T0 Tm-T0, σy(T)=σy0 (1 - T mJC) , R(p, T)=KJC p1/MJC (1 - T mJC) , σv(˙ p, p, T )= 1+ ˙p ˙ p0 CJC - 1 σy0 + KJC p1/MJC (1 - T mJC) . (5.120) Introducing the isotropic damage variable D with ˙ r=˙ p(1 - D), σeq =(1- D) σy0 + KJC r1/MJC 1+ ˙ r ˙ p0 CJC (1 - T mJC) , (5.121) which is the constitutive relation used for numerical simulation in the fol- lowing example, the damage evolution law derived from (3.15) and (3.16) considering ductile damage and proportional loading, ˙ D= Dc pR- pD˙p if p> pD, (5.122) we can rewrite pR as a modified version of the Johnson--Cook model:

5.4 Numerical Failure Analysis 271 pR =[a1 + a2 exp(a3TX)] 1+ ˙ r ˙ p0 a4[1+a5T ]. (5.123) They are implemented for large strains in LS-DYNA Finite Element using a fully vectorized backward-Euler integration algorithm for 3D, shell, and 2D analysis. The crack growth is simulated by an element killing procedure which removes the element when the damage reaches its critical value Dc . This makes the result dependent on mesh size. All the material parameters may be identified from tension tests at dif- ferent temperatures following the procedure described in Sect. 2.4. Their val- ues characterizing elasto-visco-plasticity and damage for Weldox 460E steel are: E(T0) = 200000 MPa, ν =0.33, σy0 = 490 MPa, KJC = 807 MPa, MJC =1.37, ˙ p0 =5· 10-4s-1, CJC =0.0114, T0 = 293◦K, Tm = 1800◦K, mJC =4, pD =0,s =1, andDc =0.3. The case we are taking into consideration is a blunt nose projectile with a diameter of 20 mm, a length of 80 mm and a mass of 0.197 kg, launched by a compressed gas gun, at velocities V just below and above the ballistic limit of non-penetration, against circular targets of thickness 12 mm, diameter 500 mm, and clamped in a rigid frame. Initial velocities 150 <V <400 m/s and residual velocities are measured and a digital high-speed camera is used for visualization and measurement of the penetration process, as shown in Fig. 5.15. Fig. 5.15. Numerical and experimental kinetic perforation of a 12-mm thick Wel- dox 460E steel plate at initial velocity of 303.5 m/s

272 5 Creep, Creep-Fatigue, and Dynamic Failures Numerical simulations are carried out to determine the ballistic limit curves and are compared with the experiments. The computations use 10280 4-node axisymmetric elements with one integration point. The mesh size in the impacted region giving the best result compared to experiments is 0.25 × 0.2m m 2 , giving 60 elements over the largest thickness of the plate. The projectile is modelled as an elasto-plastic material. The contact between the projectile and the target is made without friction by a penalty formulation. For the example of Fig. 5.15 the initial velocity of the projectile is 303.5 m/s, the residual velocity after perforation is 193 m/s, compared to 200 m/s measured in experiments. A comparison between the numerical simulations and experiments is also given in Fig. 5.16 for the ballistic limit curve where a limit of 193 m/s is found against 185 m/s in experiments. Note that 220 m/s is found with a coarse meshing of 30 elements in the thickness instead of 60 for the fine mesh. Fig. 5.16. Ballistic limit curve for a 12-mm thick target of Weldox 460E steel 5.4.6 Predeformed and Predamaged Initial Conditions After the forming processes, accidents, or over loadings, the internal variables may have non-zero initial values for a following structure analysis: accumu- lated plastic strain p0, corresponding values of strain hardening R0 and X0, stored energy w0 s , damage D0, and internal residual stresses σ0. Introduced as initial values in the structure calculation and in the damage analysis, they modify the resulting time or number of cycles to mesocrack initiation.

5.4 Numerical Failure Analysis 273 • In pure 3D creep the integration of the unified damage law of Sect. 5.2.2 is modified as follows: ˙ D= σ2 eqRν 2ES(1 - D)2 s σeq KN0(1 - D) N0 . (5.124) If σeq = const, an initial working time t =0suchasD0 = D(t =0)makes p0 = p(t = 0) larger than the damage threshold pD, yielding D D0 (1 - D)2s+N0dD = t 0 σ2 eqRν 2ES s σeq KN0 N0 dt (5.125) D =1- (1 - D0)2s+N0+1 - (2s + N0 +1) σ2s+N0 eq Rs ν (2ES)s (K 0 N)N0 t 1 2s+N0+1 . (5.126) The time-to-mesocrack-initiation t0 RCisreachedforD=Dcin t0 RC = (1 - D0)2s+N0+1 - (1 - Dc)2s+N0+1 2s+N0+1 (2ES)s K 0 N N0 σ2s+N0 eq Rs ν , (5.127) which makes a decrease in the time to rupture in comparison to the time tRC of mesocrack initiation without any predamaged initial condition: tRC = tDC+ 1-(1-Dc)2s+N0+1 2s + N0 +1 (2ES)s K0 N N0 σ2s+N0 eq Rs ν (5.128) as t0 RC tRC = 1 - tDC tRC (1 - D0)2s+N0 +1 - (1 - Dc)2s+N0+1 1 -(1 - Dc)2s+N0+1 < 1 . (5.129) • In 3D creep-fatigue, with the same assumptions and notations as in Sect. 5.2.2, the difference is again in the time integration of the dam- age from D0 to Dc, N0 R = (1 - D0)2s+N0+1 -(1 - Dc)2s+N0+1 (2s+N0+1) 2 2s+N0+1 σeq max ˙ σfeq +Δt (2ES)s K 0 N N0 σ2s+N0 eq Rs ν , (5.130) which gives, in the same manner as for creep, a reduced number of cycles to rupture: N0 R NR = 1-ND NR (1 - D0)2s+N0+1 - (1 - Dc)2s+N0+1 1 -(1 - Dc)2s+N0+1 < 1 . (5.131)

274 5 Creep, Creep-Fatigue, and Dynamic Failures 5.4.7 Hierarchic Approach up to Viscous Elastomers , The accuracy of a prediction of the evolution of any system decreases as the number of causes increases! Then, predictions for creep, creep-fatigue, or dynamic failures involving temperature and time dependencies do not expect the same accuracy as for ductile or low cycle fatigue failures. The simplest models are nevertheless relevant in the comparison of different solutions in early design. • The early Kachanov model may be used for uniaxial constant states of stress in order to draw a net or to interpolate some experimental isochronous curves, ˙ D= σ AD(1 - D) rD . (5.132) • Likewise, the linear Taira rule of creep-fatigue interaction is quite easy to use for uniaxial periodic loadings with hold time, tR tRC+NR NRF =1. (5.133) • For more complicated loadings such as 3D, time-varying loadings and/or temperature-varying loadings, we advise using a numerical integration of the unified damage law, ˙ D = YS s|˙ p| if ws >wD (5.134) with the material parameters eventually functions of the temperature. • In the case of proportional loading, closed-form solutions may be obtained and, if the state of stress is constant, simple relations relate the time or the number of cycles to rupture in 3D and 1D, provided the equality in stresses σ = σeq and the equality of the hold times Δt for creep-fatigue hold: tRC(σij) - tDC(σij )=[tRC(σ) - tDC(σ)] R-s ν NR(σij) - ND(σij)=[NR(σ) - ND(σ)] R-s ν . (5.135) • For small scale yielding visco-plasticity, the complex numerical analysis may be avoided by applying the extended Neuber method using the Nor- ton law. For large scale yielding, an approximate method which needs the full computation may also be used, but on a RVE only (see Sect. 5.2.4). • In dynamic problems, if only the yield stress, function of the strain rate, and the temperature are needed, use: σy(˙ p, T )=σy(˙ p0,T0) ˙p ˙ p0 1/N0 exp - H N0 1 T0-1 T (5.136) or the Johnson--Cook model.

5.4 Numerical Failure Analysis 275 • For complex problems, there is no way to escape from a numerical analysis but often the fully coupled analysis may be avoided by the post-processing of an elasto-visco-plastic calculation performed with D =0. The previous hierarchic approach applies to metals or polymers which can be modelled by classical elasto-visco-plasticity as long as no damage occurs. For specific materials and loadings such as polymers loaded at high strain rates, the hardening, the viscosity laws, or even the whole model can be different from the laws described in this book. Most often, the models found in the literature for specific material behaviors do not consider damage. Sometimes they are built for low strain rates such as time-independent plasticity-like models. Model updating consists then in extending these models either to damage or to viscosity effects. Recall that a simple way to make an existing model coupled with damage consists of using the effective stress concept: replace, for instance, the stress σ in the elasticity law and in the yield criterion of the undamaged material by the effective stress ˜ σ for the damaged material. Examples for the hardening laws are given in Sects. 3.4.8 and 4.4.5. For plasticity-like models with a yield criterion defined in the stress space as f = 0, a simple way to introduce the viscosity is to replace the consistency condition f =0a nd˙f=0bya viscositylaw σv = σv(˙ p)s u cha sf= σv . This is how elasto-visco-plasticity can be build from the elasto-plasticity framework. As a last example, consider the model of hyperelasticity with internal sliding for elastomers of Sect. 4.4.3. With the notations of Sect. 4.4.3, the reversibility domain of undamaged elastomers is f= ˜ Sπ -X -σs<0 (5.137) and the internal sliding is gained from the condition f =0a nd ˙f =0. A possible modelling for viscous elastomers submitted to creep or creep- fatigue is to consider a viscosity law σv = σv(˙ π) and to determine the internal sliding multiplier from f = σv . For the Norton law this means σv=KN˙ π1/N -→ ˙ π = ˜ Sπ - X -σs KN N . (5.138) Except for the consistency condition replaced by eq. (5.138), the whole set of constitutive equations remains unchanged, provided the stresses S and Sπ are replaced by the effective stresses ˜ Sand˜ Sπ . The constitutive equations for quasi-incompressible materials are ˜ S=S 1-D=∂(w1+w2) ∂E, ˜ Sπ =Sπ 1-D=∂w2 ∂E,

276 5 Creep, Creep-Fatigue, and Dynamic Failures ˙ Eπ =˙ π ˜ Sπ -X ˜ Sπ -X , ˙ X= Cx ˙ Eπ -γX˙ π (1 -D), Y=w1+w2, ˙ D = YS s ˙ π if π>πD, (5.139) with f<0 -→ hyperelasticity, π = t 0 ˙ Eπ dt as the cumulative measure of the internal sliding, and D = Dc as the mesocrack initiation condition.

6 High Cycle Fatigue High cycle fatigue is probably the most difficult phenomenon to handle within solid mechanics and is, by consequence, the main cause of failures of mechan- ical components in service. The difficulty comes from the early stage of dam- age which initiates defects at a very small micro- or nanoscale under cyclic stresses below the engineering yield stress. Even during the evolution of the damage, there is no easy precursor to detect the danger of a failure! The purpose here is not to be pessimistic but to caution readers when dealing with the design of a component which can be subjected to cyclic stresses during 105,106,107 cycles or more. Nothing to see! But something to do! From the physical point of view, the repeated variations of elastic stresses in metals induce micro-internal stresses above the local yield stress, with dissipation of energy via microplastic strains which arrest certain slips due to the increase of dislocations nodes. There is formation of permanent micro slip bands and decohesions, often at the surface of the material, to produce the mechanism of intrusion-extrusion. After this first stage located inside the grains, where the microcracks follow the planes of maximum shear stress, there is a second stage in which the microcracks cross the crystal boundaries to grow more or less perpendicular to the direction of the maximum principal stress up to coalescence to produce a mesocrack. For polymers or concrete, the physical mechanisms are different but are also characterized by debondings and microdecohesions which induce the same effects on the mesoscale. The phenomenon of fatigue was recognized around 1830 by M. Albert in Germany about mine chains but it was A. W¨ ohler who really gave the starting point on research on fatigue by its "W¨ ohler curve" (1860). These researches were mainly stimulated at first by the safe design of bridges and railways: Fairbarn (1864) in England, Bauschinger (1886) in Germany, and Lechatelier (1909) in France until the first book on fatigue by Cough in 1926. After that came the need of more research in the aeronautics industry, then nuclear power plants and off shore structures, concrete structures, and then the automobile industry.

278 6 High Cycle Fatigue The specific items of this chapter are the fatigue limit criteria,the use of the two-scale damage model and stochastic approaches either for random loadings or for random distributions of initial microdefects in order to improve the knowledge of the remaining life of structures in service. 6.1 Engineering Considerations High-cycle fatigue is considered when the cyclic loadings induce stresses close to but below the engineering yield stress so that the number of cycles to initiate a mesocrack is "high," that is larger than 105. The plastic strain is usually not measurable on a mesoscale but dissipation exists on a microscale to induce the phenomenon of damage. The main cause of high cycle fatigue is vibrations of large amplitude at a zero mean stress or at small amplitude with a large mean stress. Then a major way to avoid high cycle fatigue failures is to try to avoid vibrations or at least to reduce their levels. Thes e c o ndc a u s eofhighcyclefatigu eisthestress concentrations. As the "meso" behavior of the materials is elastic, there is no possibility of plastic shakedown to reduce the stress level and the stress concentration coefficient is the one calculated by an elastic analysis (KT = 3 for a hole in a large plate). Then the risk of high cycle fatigue failures is often decreased by a careful design of notches that is as smooth as possible and a careful machin- ing that is as polished as possible to minimize roughness in the corresponding zones. The corrosion is an external factor which increases the rate of fatigue damage by the phenomenon of passivation-depassivation at the tips of the microcracks. More generally, be careful each time a component is subjected to fatigue in an aggressive atmosphere; there is no suitable models to precisely quantify its effect. The fatigue limit, that is the stress below which no damage fatigue occurs, is another snare because the "true" or asymptotic fatigue limit (σ∞ f ) for a given material historically decreases as the possibility to increase the number of cycles in experiments goes on: 108,1010,1012 cycles with ultrasonic loadings! This is the reason to fix an engineering fatigue limit (σf) corresponding to the stress which yields a number of cycles to rupture of 106 or 107.Notethat107 cycles correspond to a test of almost 4 days at 30 Hertz. A minimum of 10 tests for a good mean value takes a month and ahalf! Last, but not the least, is the scatter which is always large in high cy- cle fatigue. A factor of 10 on the number of cycles to rupture of "simi- lar" tests is not abnormal! A probability analysis is advised each time it is possible.

6.2 Fast Calculation of Structural Failures 279 6.2 Fast Calculation of Structural Failures As the state of mesostrain is elastic, the calculation of the stress is easy in most cases and sometimes it may be found in handbooks of stress concentra- tion coefficients from a nominal stress simply calculated on the basis of load equilibrium equations. Nevertheless, many specific effects of the phenomenon of fatigue must be taken into account in the damage evaluation which often needs to consider the effect of microdefects closure in compression. 6.2.1 Characteristic Effects in High-Cycle Fatigue Stress intensity effects are quite complex because they include amplitude, mean value, and history. The effect of the stress amplitude Δσ is represented by the W¨ ohler curve which gives, from experiments in tension-compression (or other load mode) at constant amplitude, Δσ or σmax as a function of the number of cycles to rupture NR (Fig. 6.1). Fig. 6.1. Fatigue curve of a XC 10 steel drawn from a very large number of tests (Doc. CETIM 1992) In the range of small stresses, the curve has a quasi-asymptotic shape which means that a small variation of stress corresponds to a large variation in the number of cycles to rupture and explains the large scatter. In fact, this curve depends on the mean stress ˉ σ =(σmax + σmin)/2. The range of stress corresponding to a fixed value of the number of cycles to rupture decreases as the mean stress increases. This effect is represented by

280 6 High Cycle Fatigue the Goodman diagram shown in Fig. 6.2. This diagram also shows the big difference of the fatigue strength of materials in tension and compression. While important in tension-compression, such effect of mean stress practically does not exist in torsion or shear. Fig. 6.2. Goodman diagram of 35 NCD 16 steel for NR ≈ 106 cycles (Doc. CETIM 1992) When the loading is not periodic, there is an effect of the load history. The accumulation of damage due to different sequences of loading depends on the order of appearance of the sequences, as shown in Fig. 6.3 for a two- level loading: this is a sequence of n1 cycles of range Δσ1 corresponding on the W¨ ohler curve to a number of cycles to rupture NR1 and a sequence of n2 cycles of range Δσ2 corresponding to NR2 in such a way that n1 + n2 = NR is the number of cycles to rupture of the two-level test. This dependence of the order of the stress amplitudes applied is called the nonlinear accumulation of fatigue damages. Nevertheless for many sequences of different amplitudes or for random loading, this effect is much less pronounced and the linear Palmgreen--Miner rule may apply at least as a rough approximation so that ni NRi =1. (6.1) This is the straight line [(1, 0), (0, 1)]inFig.6.3.

6.2 Fast Calculation of Structural Failures 281 Fig. 6.3. Accumulation diagram of Maraging steel for two levels of stress range Δσ = 1655 MPa and 965 MPa (J.L. Chaboche 1985) The fatigue behavior under multiaxial states of stress is even more compli- cated. Unfortunately not many experimental results exist. Non-proportion- al loadings seem to increase the fatigue strength in a way that is somewhat similar to cross hardening in plasticity. The temperature also plays a role but its softening effect is easier to model. The state of the material itself also has an effect on the fatigue. The defects are sources of microcrack initiations and the surfaces are usually weaker than the plain material: within a uniform state of stress the first fatigue crack always initiates on the surface. This is due to easy plastic slips that glide close to the surface in the process of intrusion-extrusion. Initial conditions such as a pre-hardening or a pre-damage, due to metal forming for example, usually modify the fatigue life (see Sect. 6.4.5). A scale effect is generally observed in such a way that the number of cycles to rupture of a thin specimen is higher than for a thicker specimen loaded by the same stress. This is due to the lower probability of having a large defect in the thin specimen than in the thicker one. It seems also that the gradient of the stresses plays a role. For example, the number of cycles needed to initiate a mesocrack in pure bending is higher than in pure tension for the same level of maximum stress (see Sect. 6.4.6). 6.2.2 Fatigue Limit Criteria In quick design, a safe criterion is to manage to have a state of stress below the fatigue limit where no damage may occur. This is easy to say! But it is not so easy to practice for at least two reasons.

282 6 High Cycle Fatigue The notion of fatigue limit is not rigorous as nobody has waited an infinite number of cycles! As already mentioned earlier, only a conventional fatigue limit in tension (σf) can be defined objectively, at least from a statistics point of view, as the maximum stress which corresponds to 106 or 107 cycles. But experiments on metals show that a rupture may occur for number of cycles as high than 1010 or 1012 cycles (C. Bathias 2000). Then, another limit is defined as the asymptotic fatigue limit σ∞ f corresponding to an "estimated" asymptote of the W¨ ohler curve. For multiaxial states of stress there is no definitively admitted scalar function of the stress components, a fatigue norm, to compare with the fatigue limit in tension. There is nothing like the von-Mises criterion in plasticity. An equivalent would be the damage equivalent stress σ eq based on the total elastic energy density (see Sects. 1.2.2 and 7.2.1) but it does not take into account the effect of mean stress. Nevertheless, a fast estimation of fatigue safety is σ max <σf , (6.2) with σ = σeqR1/2 ν, σeq = 32σD ij σD ij ,σ H=13σkk, Rν = 23(1 + ν)+3(1- 2ν) σH σeq 2 . (6.3) 6.2.2.1 Sines Criterion Based on phenomenological considerations, it is a function of the range of octahedral shear AII defined in proportional loading (σ = σΣ Σ with Σeq =1)by AII=1 2 32 (σD ijmax-σD ij min)(σD ijmax-σD ij min)= ΔσΣ 2 (6.4) and of the mean value of the hydrostatic stress ˉ σH=1 2 (σHm a x+ σHmin) (Crossland criterion uses the maximum value σHm a x of σH). Then the safety criterion is written as AII 1-3bSˉ σH<σf, (6.5) where bS is a material-dependent parameter on the order of 10-3 to 10-2. 6.2.2.2 Dang Van Criterion Based on micromechanics, it is related in metals to the first plastic slip band which initiates in the weakest oriented crystal on which the elastic shakedown

6.2 Fast Calculation of Structural Failures 283 is assumed to happen. If σf is the fatigue limit in tension-compression and τf the fatigue limit in shear or torsion, the criterion is written as a function of the maximum value of the shear stress over a cycle in time and in direction and of the hydrostatic stress σH.UsingσI as the principal stresses, we have max maxI,J (σI(t) - σJ (t)) 2 τf - τf-σf 2 σf 3 σH(t) <1. (6.6) It is represented in the graph of shear τ and hydrostatic stresses σH by the inner domain limited by two straight lines (Fig. 6.4). Fig. 6.4. Dang Van diagram criterion In order to check if a loading, proportional or not, is below the conven- tional fatigue limit, verify that its path is fully in the inner domain. 6.2.3 Two-Scale Damage Model in Proportional Loading For some precise but still quick evaluation of the safety for proportional and periodic loadings, it is possible to check by the two-scale damage model of Sect. 1.5.5 (see also Sect. 2.3) if the number of cycles to rupture will or will not reach a given limit of 105,106,107 or more. Recall that this model has the advantage to take into account the real history of the loading and can be used for multilevel fatigue loading as in Sects. 4.2.1 and 4.4.2 for low cycle fatigue or random fatigue.

284 6 High Cycle Fatigue On the mesoscopic scale, a high cycle fatigue proportional loading is char- acterised by σ = σΣ(t)Σ, p = 0 , and σΣ(t) between σmin and σmax , (6.7) with the normalization Σeq = 3 2ΣD ij ΣD ij =1(σΣ is the signed von Mises stress). For the model, high cycle fatigue corresponds to a stress range lower than twice the yield stress (Δσ = σmax - σmin < 2σy) but, due to kinematic hardening, to a stress range larger than twice the asymptotic fatigue limit (Δσ>2σ∞ f). On the microscopic scale, considering the two-scale damage model leads to a proportional loading only in terms of (micro) deviatoric stresses and strains with then: σμD=σμ Σ(t)ΣD , μp = 32 μ pΣ(t)ΣD, and Xμ =Xμ Σ(t) ΣD . (6.8) Due to the Eshelby--Kr¨ oner localization law ˜ σμ= σμ 1-D=σ-2G(1-β) μp, (6.9) the hydrostatic stress at microscale becomes σμ H =(1- D)˜ σμ H =(1- D)σH (6.10) and is a function of the hydrostatic stress on the mesoscale (σH = σkk/3= σΣΣkk/3) and the microdamage (Dμ = D). The stress triaxiality at mi- croscale is then Tμ X=σμ H σμ eq =(1-D)σH σμ eq =σH ˜ σμ eq. (6.11) It is a function of the von Mises stress on the microscale. Then, in order to perform the time integration of the unified damage law at microscale, ˙ D= Yμ S s ˙pμ , (6.12) with Y μ as the strain energy release rate (here without the microdefects closure effect) such that Yμ= σμ2 eq Rμ ν 2E(1 - D)2 and Rμ ν = 23(1 + ν)+3(1- 2ν)Tμ X2, (6.13) one needs to determine the effective stress ˜ σμ Σ(t) and the plastic strain pΣ(t) on the microscale (see Fig. 6.5). First, the localization law (6.9) considered within the yield criterion f μ = (˜ σμ-Xμ)eq-σ∞ f =|σΣ-Xμ Σ|-σ∞ f with linear kinematic hardening

6.2 Fast Calculation of Structural Failures 285 Fig. 6.5. Stress-strain cycles at mesoscale and at microscale ˙ XΣ =Cy(1-D)˙ pΣ leads to ˙ ˜ σμ Σ =Cy(1-D)˙ pΣ and a plastic strain rate ˙ μ pΣ that is linearly dependent on the meso stress rate (with generally Cy G): ˙ μ pΣ= ˙ σΣ G and G=3G(1-β)+Cy(1-D)≈3G(1-β). (6.14) The plastic strain increment over one cycle is then: δpμ δN =2(Δσ-2σ∞ f) G if Δσ>2σ∞ f, δpμ δN =0 if Δσ<2σ∞ f, (6.15) and vanishes (as already mentioned) for any stress range smaller than 2σ∞ f. In that case the model predicts no failure, this is the endurance domain. Second, the maximum and minimum signed von Mises stresses do not vary much as ˜ σμ Σmax ≈ σ∞ f +Cy(1-D) G (σmax-σ∞ f)≈σ∞ f ˜ σμ Σmin ≈-σ∞ f +Cy(1-D) G (σmin+σ∞ f )≈-σ∞ f. (6.16) Considering then ˜ σμ eq≈σ∞ f , the damage increment over one cycle is δD δN =ΔD+ +ΔD- , (6.17)

286 6 High Cycle Fatigue with ΔD+ = tb(σμ b) te(σμ e)˙ Ddt≈ σ∞2s f (2ES)sG σΣ(tb) σΣ(te) Rν ξ =Σkk σ σ∞ f s dσ, ΔD- = tc(σμ c) td(σμ d)˙ Ddt≈ σ∞2s f (2ES)sG σΣ(tc) σΣ(td) Rν ξ =Σkk σ σ∞ f s dσ, (6.18) and Rν (ξ)=23(1 + ν)+13(1 - 2ν)ξ2 . (6.19) Define next the minimum and maximum normalized stresses as ξmin =Σkk σmin σ∞ f and ξmax =Σkk σmax σ∞ f (6.20) and introduce the dimensionless function φ , φ (ξmin ,ξmax)= ξmax ξmin+2 Rs ν (ξ)dξ + ξmax -2 ξmin Rs ν (ξ)dξ, (6.21) which can be approximated by the following form that is conservative for the number of cycles to rupture, better for small s, φ (ξmin ,ξmax) ≈ ξmax - ξmin - 2 [Rs ν (ξmin)+Rs ν (ξmax)] . (6.22) This allows us to write the damage increment per cycle as δD δN = σ∞ 2 f (1+ν) 3ES s 2(Δσ - 2σ∞ f) G if Σkk =0(e.g. shear) δD δN=σ∞2s+1 f φ (ξmin ,ξmax) Σkk(2ES)sG if Σkk =0. (6.23) Damage will initiate after a number of cycles ND when the damage thresh- old pD is reached on the microscale. According to (6.14), the plastic strain increment for half a cycle is (for linear kinematic hardening and assuming D = const over a cycle), Δ μ pΣ=1 2 δpμ δN=Δσ-2σ∞ f G =Δσμ Σ-2σ∞ f Cy(1-D), (6.24) withD=0aslongas: pμ≤pD= pD σu -σ∞ f Δσμ Σ 2 -σ∞ f m . (6.25)

6.2 Fast Calculation of Structural Failures 287 See Sect. 1.4.1 for the expression of the damage threshold in fatigue. There is then no microdamage as long as N<ND. Considering a periodic loading, we have ND= pD 2|Δ μ pΣ| and pD = pD G Cy m σu - σ∞ f Δσ 2 -σ∞ f m (6.26) or ND=1 4 pD Gm+1 Cm y (σu-σ∞ f)m Δσ 2 -σ∞ f m+1 . (6.27) The formulae for the number of cycles at crack initiation are finally (often with G≈3G(1 - β)): NR=ND+ 3ES σ∞2 f (1+ν) s GDc 2(Δσ - 2σ∞ f) if Σkk=0 NR=ND+ Σkk(2ES)sGDc σ∞ 2s+1 f φ σmin σ∞ f Σkk, σmax σ∞ f Σkk if Σkk =0. (6.28) They show that there is a mean stress effect in tension-compression (of course better described if the microdefects closure parameter h is intro- duced, see next part), no mean stress effect in shear as experimentally ob- served as for Σkk = 0, and the number of cycles to rupture depends only on the stress range. The formulae for the approximation (6.22) are detailed in Sects. 6.2.4 and 6.3.1. They show more explicitly that an increase of the stress triaxiality lowers the fatigue asymptote and reduces then (compared to tension-compression) the conventional fatigue limit of multiaxial loadings with Σkk > 1. The accumulation of damages due to two successive loadings with different stress ranges Δσ1 and Δσ2 is obtained, as in Sect. 4.2.1. A bilinear damage accumulation is obtained for a non-zero damage threshold and the Miner rule is recovered if pD =0:ifni is the number of cycles spent at the stress range Δσi , NR = n1 + n2 the total number of cycles to rupture corresponding to a two-level fatigue case, then n1 NR1+n2 NR2 1-ND1 NR1 1-ND2 NR2 =1 if n1≤ND1 n1 NR1 ND2 ND1 NR1 NR2+n2 NR2 =1 if n1>ND1. (6.29)

288 6 High Cycle Fatigue Finally, for a symmetric fatigue loading with zero mean stress, i.e., with σeq min = σeq max = σmax , one can compare the number of cycles to rupture in 3D to the number of cycles in tension-compression (case Σkk =0), NR(σij) - ND(σij ) NR(σmax) - ND(σmax) =Σkk φ - σmax σ∞ f , σmax σ∞ f φ -Σkk σmax σ∞ f , Σkk σmax σ∞ f . (6.30) For 3D deviatoric states of stress, use the fatigue reference in shear with σeq min = σeq max = √3τmax (case Σkk =0)to obtain NR(σD ij) - ND(σD ij) NR(√3τmax) - ND(√3τmax) =1. (6.31) 6.2.3.1 Case with Microdefects Closure Effect If the mean stress effect is of first importance, it is of course better to use the two-scale damage model with microcracks closure effect: introducing the pa- rameter h<1 leads to a damage growth larger in tension than in compression as Yμ=1+ν 2E σμ ij + σμ ij + (1-D)2 +h σμ ij - σμ ij - (1-hD)2 - ν 2E σμ kk 2 (1-D)2+h -σμ kk 2 (1 - hD)2 . (6.32) For simplicity, consider here the case of a tension-compression loading on a mesoscale ((6.8) with σΣ(t)=σ(t)andΣ =diag[1, 0, 0]) with ˜ σμ eq≈σ∞ f and ˜ σμ H = σH = σ. Neglecting the damage within the expression for the strain energy release rate gives Yμ≈σ∞2 f2E Rνh , (6.33) with ((2.35)--(2.37) of Sect. 2.1.2) Rνh = 1+ν 9 × 2+ σ σ∞ f 2 +2 -1+ σ σ∞ f 2+h -2- σ σ∞ f 2+2h 1 - σ σ∞ f 2 - ν σ σ∞ f 2 -νh - σ σ∞ f 2 . (6.34) It also leads to the same expression as for the damage increment and the number of cycles to rupture as previously but with Rν replaced by Rνh , i.e., with φ replaced by

6.2 Fast Calculation of Structural Failures 289 φh (ξmin ,ξmax)= ξmax ξmin+2 Rs νh (ξ)dξ + ξmax -2 ξmin Rs νh (ξ)dξ, (6.35) where Rs νh (ξ)=Rs νh σ σ∞ f = ξ or φh (ξmin ,ξmax) ≈ ξmax - ξmin - 2 [Rs νh (ξmin)+Rs νh (ξmax)] . (6.36) For tension compression (Σkk =1,ND unchanged), NR = ND + (2ES)sGDc σ∞ 2s+1 f φh σmin σ∞ f ,σmax σ∞ f . (6.37) 6.2.4 Sensitivity Analysis For ductile damage, low cycle fatigue, and creep failures (see Sects. 3.2.3, 4.2.3, and 5.2.3) the relative influence of the loading and the material pa- rameters is calculated as an application of the general method of Sect. 2.4.6. Here this is the influence on the number of cycles to rupture in periodic proportional loading obtained in Sect. 6.2.3: Eq. (6.28) with the approximate formula (6.22) for φ (ξmin ,ξmax)gives ND=1 4 pD Cm y 3E(1-β) 2(1+ν) m+1 (σu - σ∞ f)m Δσ 2 -σ∞ f m+1 NR=ND+ (2ES)s3E(1 - β)Dc 2(1 + ν)σ∞ 2s f σmax-σmin-2σ∞ f Σkk [Rs νmin+Rs ν max] , (6.38) where the proportional loading is written as σ=σΣ with Σeq=1andTX=13Σkk (6.39) and where Δσ=σmax-σmin, G≈3G(1 - β) , Rν min = Rν (ξmin) , Rν max = Rν (ξmax) , (6.40) with ξmin =Σkk σmin σ∞ f , ξmax =Σkk σmax σ∞ f. Taking the logarithmic derivative gives dND ND and d(NR - ND) NR-ND .

290 6 High Cycle Fatigue Ta k i n g δAk = |d Ak| for each material parameter Ak , the sensitivity on the number of cycles to rupture is δNR NR = k SNR Ak δAk Ak ,wherethecoefficients SNR Ak are the sensitivity coefficients of the parameters Ak on the number of cycles to rupture NR: SNR TX =SNR Σkk=NR-ND NR 2σ∞ f Σkk Δσ-2σ∞ f Σkk +2s 3(1-2ν)ξ2 minRs-1 ν min+ξ2 maxRs-1 ν max Rs νmin+Rs νmax , SNR σmin = -ND NR (m +1)σmin Δσ-2σ∞ f +NR-ND NR -σmin Δσ-2σ∞ f Σkk +2s 3(1-2ν)ξ2 minRs-1 ν min Rs νmin+Rs νmax , SNR σmax = ND NR (m +1)σmax Δσ-2σ∞ f +NR-ND NR σmax Δσ-2σ∞ f Σkk +2s 3(1-2ν)ξ2 maxRs-1 ν max Rs νmin+Rs νmax , SNR E =ND NR(m+1)+NR -ND NR (s +1), SNR ν= 1+ ND NRm ν 1+ν+NR-ND NR 2sν 3 (1-ξ2 min)Rs-1 ν min +(1- ξ2 max)Rs-1 ν max Rs νmin+Rs ν max , SNR β = 1+ND NRm β 1-β, SNR Cy =ND NR m, StR pD=ND NR, SNR σ∞ f =ND NR (m +1)σ∞ f Δσ 2 -σ∞ f - mσ∞ f σu-σ∞ f +2NR - ND NR × (1 - 2ν)s 3ξ2 minRs-1 ν min+ξ2 maxRs-1 ν max Rs νmin+Rs ν max -s+ σ∞ f ΣkkΔσ - 2σ∞ f , SNR σu =ND NR mσu σu-σ∞ f, SNR m =ND NRmln G Cy σu-σ∞ f Δσ 2 -σ∞ f , SNR S =NR-ND NR s,

6.2 Fast Calculation of Structural Failures 291 SNR s =NR-ND NRs ln σ∞ 2 f 2ES+Rs νminlnRν min+Rs ν maxlnRν max Rs νmin+Rs ν max , SNR Dc =NR-ND NR. As in the other chapters, the values of those coefficients are represented by the height of the boxes in Fig. 6.6 for the following set of parameters chosen as an average of many materials and identical for the mesoscopic param- eters to those used for ductile and low cycle fatigue failures: σmax = 250 MPa, σmin = -250 MPa, TX =3 Σ kk =1 ,Rνmax =Rνmin =2 .75, E = 200000 MPa, ν =0.3, σ∞ f = 200 MPa, σu/σ∞ f =2,Cy = E/100, β=2 15(4 - 5ν)/(1 - ν), G≈3G(1 - β) = 121000 MPa, ND/NR =1/2, m=2,S=2MPa,ands=5. For ductile, low cycle fatigue, and creep failures, the quality of the result, i.e., the number of cycles to rupture in this case, is mainly influenced by the accuracy of the stress, here twice 5.8 mitliplied by its relative error. Using the two-scale damage model gives more emphasis to the exponents m and s and increases the uncertainties by a larger number of parameters involved. Only pD and Dc are of less importance as in the previous chapters. Fig. 6.6. Relative importance of each parameter in high cycle fatigue If the sensitivity in terms of stress range Δσ = σmax - σmin and mean stress σ =(σmax + σmin)/2 are preferred to the sensitivity in terms of σmin and σmax ,calculate,then SNR σ= σ σmin SNR σmin+ σ σmax SNR σmax SNR Δσ =1 2 Δσ σmax SNR σmax - Δσ σmin SNR σmin . (6.41)

292 6 High Cycle Fatigue For the previous set of material parameters, SNR σ =0asσ =0andSNR Δσ= 11.6 here. 6.2.5 Safety Margin and Crack Growth The proper parameter for the evaluation of the risk of fatigue failure is the number of cycles, as already mentioned in Sect. 4.2.5 for low cycle fatigue. • If the number of cycles of loading service Nservice is known, a safe design is defined from the calculated number of cycles to rupture NR for the in service history of loading, and a safety factor Saf given by rules or by the state of the art of the domain of application Saf = 100, 10, 5, ...: Nservice < NR Saf . (6.42) • Due to a large scatter in high cycle fatigue, a better definition of the safety margin uses the probability concept. It may include the uncertainties of the loading and the material properties but it needs information on their stochastic character. Instead of the previous equation, consider as safety design criterion: Prob (NR >Nservice) < 1 SafPr , (6.43) where 1 SafPr must be very small (SafPr =102, 103,...105 or more). This means a stochastic analysis is difficult to perform as the accuracy is al- ways poor for the low values of the probability density (nevertheless see Sect. 6.4.4). Finally, if a mesocrack initiates, it is important to check if it is dangerous regarding a possible fast propagation by instability or fatigue growth. • The criterion for a fracture by instability is when the structure strain energy release rate G reaches the toughness of the material Gc . G is calculated from the fracture mechanics concepts as a function of the far field loading σ∞ > 0 and the length of the mesocrack initiated δ0 stated in Sect. 1.6.3. δ0= Gc σ2 u 2EDc + σu pR . (6.44) Classically, G ≈ κ σ2 ∞πδ0 E where κ is a shape factor, so one has to check G<Gc or κσ2 ∞π E Gc σ2 u 2E Dc + σu pR <Gc . (6.45)

6.2 Fast Calculation of Structural Failures 293 The toughness Gc disappears and σ∞ <σu 1 πκ Dc 2 +E pR σu . (6.46) Due to the numerical value of the material parameters, this criterion is satisfied most of the time, at least for metals. • But the crack may continue to grow under the same fatigue loading. The simplest model to evaluate the fatigue crack growth rate is the general- ized Paris law written for a crack of area A in a 3D medium: δA δN = GηP/2 max - GηP/2 min CηP/2 P , (6.47) where Gmax ≈ κσ2 ∞ max πA1/2 E ,Gmin≈κσ2 ∞ min πA1/2 E ,andwhereηPand CP are material-dependent parameters determined by experiments and are different from the parameters of the Paris law written for the crack length in 2D problems. If the loading is periodic, σmax = const, σmin = const, and in order to obtain the evolution of the crack surface A as a function of the number of cycles N one has to solve (ηP =4) δA δN = κηP/2 σηP ∞max-σηP ∞ min CηP/2 P π E ηP/2 AηP/4 , (6.48) with the initial condition N =0→ A = A0 ≈ δ2 0, A A0A-ηP 4δA=κηP/2σηP ∞max-σηP ∞ min CηP/2 P π E ηP/2 N, (6.49) A = δ 4-ηP 2 0 + 4-ηP 4 κηP/2 σηP ∞max-σηP ∞ min CηP/2 P π E ηP/2 N 4 4-ηP . (6.50) One may also calculate the number of cycles N to reach the complete failure by instability: Gmax =Gc or κσ2 ∞ maxπA 1/2 E =Gc. (6.51) That is A = EGc κπσ2 ∞ max 2 , (6.52) N = EGc κπσ2 ∞ max 4-ηP 2 1 δ 4-ηP 2 0 + 4-ηP 4 κηP/2 σηP ∞max-σηP ∞ min CηP/2 P π E ηP/2 . (6.53)

294 6 High Cycle Fatigue 6.3 Basic Engineering Examples High-cycle fatigue occurs for mesostresses below or close to the yield stress so that they can be calculated in elasticity. At least something simple! For many simple geometries, the stress concentration coefficient at the critical points KT may be found in handbooks (see bibliography). In the following, KT is supposed to be known. 6.3.1 Plates or Members with Holes or Notches The weakness comes from a sharp variation of the geometry where the maxi- mum stress is at the surface border, uniaxial, and related to the normal stress σn by σ=KTσn (6.54) or for cyclic loading Δσ=KTΔσn. (6.55) • For periodic loading at zero mean stress, one may use the solution given by the two-scale damage model in proportional loading with Σkk =1 (eq. (6.28) with the approximate formula (6.22)), NR=ND+ (2ES)sGDc 2σ∞ 2s f (KTΔσ - 2σ∞ f )Rs ν max ND=1 4 pD Gm+1 Cm y (σu-σ∞ f)m KT Δσ 2 -σ∞ f m+1 , (6.56) where G≈3G(1 - β)and Rν max = Rν (ξmax)= 23(1 + ν)+ 13(1 - 2ν) KTσmax σ∞ f 2 . (6.57) This is nothing more than directly using the experimental W¨ ohler curve at zero mean stress for the stress range KTΔσ. • But if the mean stress σ is not zero it helps to derive the number of cycles to rupture NR(σ)fromtheW¨ ohler curve known at σ =0: NR(Δσ, σ)=ND(Δσ)+ (2ES)sGDc σ∞ 2s f (KTΔσ - 2σ∞ f )(Rs ν min+Rs ν max), (6.58) with (2ES)sGDc σ∞ 2s f (KTΔσ - 2σ∞ f ) =2[NR(Δσ, σ =0)- ND(Δσ)] Rs ν max.

6.3 Basic Engineering Examples 295 Note that the number of cycles to damage initiation ND does not depend on the mean stress. Then, NR(Δσ, σ) - ND(Δσ) NR(Δσ, σ =0)- ND(Δσ) = 2Rs ν max Rs νmin+Rs ν max . (6.59) The ratio of the triaxiality functions represents the effect of mean stress already described by the Goodman diagram. For a better description of the mean stress effect, replace Rν by Rν h. Figure 6.7 gives Rν and Rν h versus KTσ/σ∞ f (recall that Eq. (6.34) and therefore the curve for Rν h apply only to the tension-compression case). To help a bit more, take ND = NR/2 as a rough approximation. • If the cyclic loading is piecewise periodic with a number of cycles ni(Δσi , σi)fo rthei-th sequence of loading of stress range Δσi and of mean stress σi, ni = NR, use a cumulation equation similar to eq. (6.29). Fig. 6.7. Effect of mean stress through the triaxiality function Rν or Rν h for ν =0.3andh =0.2 6.3.2 Pressurized Shallow Cylinders This is the same problem as in Sect. 4.3.2, and Fig. 4.7, except the damage equation (here damage acts on a microscale). The state of stress, function

296 6 High Cycle Fatigue of the radius of the cylinder Rcyl, its thickness tcyl, and the internal relative pressure P (t) varying between Pmin and Pmax is σ = 00 0 0 PRcyl tcyl 0 00 PRcyl 2tcyl (6.60) orσ=√3 2 PRcyl tcyl Σ with Σ = 00 0 02 √30 001 √3 in order to have Σeq =1. ThenΣkk= 3 √3 =√3. Now it is the same problem as in the previous section (Sect. 6.3.1) as well. For periodic loading, σmin = √3 2 Pmin Rcyl tcyl,σmax=√3 2 Pmax Rcyl tcyl ,Δσ = √3 2 (Pmax - Pmin) Rcyl tcyl , NR=ND+ (2ES)sGDc σ∞ 2s f Δσ-2σ∞ f Σkk Rs ν Σkk σmin σ∞ f +Rs ν Σkk σmax σ∞ f , ND=1 4 pD Gm+1 Cm y (σu-σ∞ f)m Δσ 2 -σ∞ f m+1 . (6.61) The rupture condition can also be expressed as a function of the number of cycles to rupture read on the W¨ ohler curve at zero mean stress using Fig. 6.7: NR(Δσ, σ) - ND(Δσ) NR(Δσ, σ =0)- ND(Δσ) = 2Rs ν √3Δσ 2σ∞ f Rs ν √3 σmin σ∞ f +Rs ν √3 σmax σ∞ f . (6.62) For two-level fatigue loading, apply eq. (6.29). For cyclic loading, stepwise periodic, perform as in Sect. 4.4.2. If damage initiates during the first level, then D =(n1 -ND)δD δN (1)+n2δD δN (2)+...+nkδD δN (k)=Dc → NR= k i=1 ni, (6.63) with the damage increment per cycle on a microscale given by (6.23).

6.3 Basic Engineering Examples 297 6.3.3 Bending of Beams This is the same problem as in Sect. 4.3.3 (Fig. 4.9) except that the beam remains elastic, within domain of application of the two-scale damage model. The simple Bernoulli hypothesis applied to pure circular bending of a part of beam of height h, of inertia moment I gives the maximum elastic stress as a function of the momentum applied M (I = bh3/12 for a rectangular cross section of width b), σmax = Mmaxh I. (6.64) Then for a periodic movement of the beam described by M = Mmax sin ωt, the problem of fatigue reduces to a simple tension compression case between σmax and σmin = -σmax at the two surfaces of the beam where the stress is maximum. Equations (6.56) directly apply with KT =1. For a two-level piece wise periodic movement, the equations in (6.29) also apply. For multilevel high cycle fatigue loading, use eq. (6.63). 6.3.4 Random Loadings Sometimes the problem to solve is of a random nature known only by stochas- tic properties. This is the case of the wheel suspensions of a car driven on a rough road. This is the case of planes flying in turbulent clouds. This is also the case of any mechanical component for which the in service loading is not precisely known. The only way to find statistics on the number of cycles to rupture by the two-scale damage model in which the loading is a random variable is to use the numerical method of Monte Carlo, as explained in Sect. 6.4.4. Nevertheless some indications may be obtained in a closed-form if a very simple damage model is used. Consider here the very crude model restricted to loadings at zero mean value, δD δN = σ M-σ∞ f σu-σ∞ f c and D=Dc →N=NR, (6.65) where δD δN is the damage increment per cycle of maximum damage equivalent stress σ M =(σeqR1/2 ν )max and of range Δσ =2σ M, σ∞ f is the asymptotic fatigue limit, σu is the ultimate stress, and c is also a material parameter. The number of cycles to rupture NR for a periodic loading σ M=constis Dc 0 δD = σ M-σ∞ f σu-σ∞ f c NR 0δN (6.66) NR = σ M-σ∞ f σu-σ∞ f -cDc and δD=δN NR Dc . (6.67)

298 6 High Cycle Fatigue Consider now a random proportional loading σ = σΣ(t) Σ (with Σeq =1) where the signed damage equivalent stress σ = σΣ(t)R1/2 ν is a Gaussian process given by its probability density P (σ ) which fits many applications with large numbers of random loading parameters, P(σ )= 1 ˉ ˉ σ √2π exp- σ 2 2ˉ ˉ σ 2, (6.68) where ˉ ˉ σ is the standard deviation associated with σ and σ 2 = σ2 ΣRν .The stress triaxiality function is constant equal to Rν = 2 3 (1+ν)+3(1-2ν) Σkk 3 2. For a narrow band process, the probability density of the maximum values of the stress σ is given by P(σ M)=- 1 P(0) ∂P(σ ) ∂σ (σ =σ M), (6.69) which is a Rayleigh's law: P(σ M)= σ M ˉ ˉ σ 2exp-σ 2 M 2ˉ ˉ σ 2. (6.70) It will give rise to rupture only if the standard deviation ˉ ˉ σ is large to ensure enough stresses σ M above the asymptotic fatigue limit. Within a set of N cycles the number of cycles dN for which σ M σ M σ M +dσ MisdN=NP(σ M)dσ Mor dN=Nσ M ˉ ˉ σ 2exp-σ 2 M 2ˉ ˉ σ 2dσ M, (6.71) but the mean damage D at the cycle N is D = ∞ 0 DcdN NR = ∞ 0 σ M-σ∞ f σu-σ∞ f cdN (6.72) or D=N (σu-σ∞ f )c ∞ σ∞ f (σ M-σ∞ f)c·σ M ˉ ˉ σ 2exp-σ 2 M 2ˉ ˉ σ 2dσ M , (6.73) orwithx= ˉ ˉ σ σ M andJ= ˉ ˉ σ σ∞ f 0 ˉ ˉ σ σ∞ f 1 x-1 c1 x3 exp- 1 2x2 dx: D= Nσ∞c f (σu-σ∞ f )cJ. (6.74) The integral J = J c, ˉ ˉ σ σ∞ f can be numerically integrated by mathematical software as a function of the W¨ ohler exponent c and the ratio ˉ ˉ σ /σ∞ f ofthe standard deviation ˉ ˉ σ of the loading process to the fatigue limit σ∞ f. Finally, the number of cycles N R which corresponds to the rupture for the mean value of the damage D = Dc is

6.3 Basic Engineering Examples 299 NR= σu-σ∞ f σ∞ f cDc J. (6.75) It is interesting to calculate the value of the maximum stress σ Mequiv for a constant amplitude process which would give the same number of cycles to rupture, σ Mequiv - σ∞ f σu-σ∞ f -cDc = σu -σ∞ f σ∞ f cDc J, (6.76) σ Mequiv = σ∞ f 1+ J ˉ ˉ σ σ∞ f 1/c . (6.77) Fig. 6.8. Factor of equivalence between a random and a periodic fatigue process The graph of Fig. 6.8 gives the value of J 1/c as a function of the ratio ˉ ˉ σ /σ∞ f for different c. The curves are obtained for a zero mean stress with a maximum stress range directly related to the value of the standard deviation ˉ ˉ σ .Whe nitisto olo w(ˉ ˉ σ /σ∞ f <≈ 0.1 to 0.3), there is no rupture. It is interesting to note that the scatter correction factor J 1/c varies only from 0 to less than 1 in a large range of both the ratio ˉ ˉ σ /σ∞ f andtheW¨ ohler curve nonlinearity parameter c.

300 6 High Cycle Fatigue Then, knowing the standard deviation ˉ ˉ σ of a Gaussian process for the signed damage equivalent stress σ = σΣR1/2 ν , it is easy to calculate the max- imum stress σ Mequiv of an equivalent periodic process (the exponent c always fitsaW¨ ohler curve in the large number of cycles to rupture). Report this equivalent stress directly on the W¨ ohler curve in order to obtain the number of cycles to rupture corresponding to the random process. Nice, isn't it? Of course more accurate results may be obtained with a better fatigue model but the price to pay is numerical calculations with the Monte Carlo method. 6.4 Numerical Failure Analysis As pointed out many times, high cycle fatigue occurs in the elastic range. The nice thing is that the computations needed for design purposes are per- formed in elasticity. For most materials, elasticity linearity allows for the superposition of solutions: if the loading is proportional (see Sect. 2.1.2), i.e., if all applied loads and displacements are proportional to the same scalar function of time α(t), perform only one computation for the reference load- ing αref. Store the stress and strain fields obtained (σref(M)a nd ref(M)) and have in mind that there is no need for additional computation to get the stress and strain fields at any time t as σ(M, t)= α(t) αref σref(M)a n d (M, t)= α(t) αref ref(M) . (6.78) If a few applied loads or displacements vary independently, compute the reference elastic solutions for each load or displacement. The stress and strain fields history are obtained by superposition, yielding σ(M, t)= i αi(t) αref i σref i(M)a n d (M, t)= i αi(t) αref i ref i(M) . (6.79) These elastic fields are then the inputs of a fatigue structure analysis, either to check the safety by use of fatigue limit criteria or to estimate the number of cycles to failure by a damage analysis. The bad thing is that the straightforward use of the W¨ ohler curve to read the number of cycles to rupture (or at least to mesocrack initiation) is not always an easy task for real structures. The use of a damage post-processor (such as DAMAGE 2000 described in Sect. 2.3.3) is often necessary. The calculations are made at the most loaded point only or at the structure's Gauss points to draw damage maps. 6.4.1 Effects of Loading History (J.P. Sermage 1999) Most of the characteristic effects of high cycle fatigue described in Sect. 6.2.1 may be predicted by the unified damage law within the two-scale dam-

6.4 Numerical Failure Analysis 301 age model of Sect. 6.2.3. Some numerical results obtained with the post- processor DAMAGE 2000 are shown in the following for the values of the ma- terial parameters characteristic of a steel at room temperature: E = 200000 MPa, ν =0.3, σ∞ f =200MPa,Cy=2000MPa,σu =600MPa, pD=0.05, m =1,S =0.3MPa,s =2,h =0.2, Dc =1. 6.4.1.1 Influence of the Mean Stress The consideration of the microdefects closure parameter h in the model allows us to obtain the influence of the mean stress in compression. This difference of behavior between tension and compression leads to larger numbers of cycles to rupture in the same range as that for the decreasing mean stress ˉ σ (Fig. 6.9). Fig. 6.9. Effect of mean stresses on the W¨ ohler curve The same results are also plotted for tension-compression and shear load- ings at a fixed number of cycles to rupture NR =105 (Fig. 6.10). As already pointed out, a remarkable result is that the shear mean stress ˉ τ does not have any effect in shear in the range considered, as observed experimentally. Fig. 6.10. Computed effect of mean stress in tension-compression and shear

302 6 High Cycle Fatigue 6.4.1.2 Nonlinear Damage Accumulation Another important feature of fatigue is the nonlinearity of the accumulation of damages due to loadings of different stress amplitudes. Consider here a two- level loading at zero mean stress as represented in Fig. 6.11: n1 cycles at σmax = σ1followedbyn2 cycles atσmax = σ2 suchasNR =n1+n2.NR1 and NR2 are the numbers of cycles to rupture corresponding to constant amplitude loadings Δσ1 and Δσ2 . The results are compared with the linear Palmgreen--Miner rule n1/NR1 +n2/NR2 =1inthen2/NR2 vs n1/NR1 plot in Fig. 6.11. The nonlinear damage accumulation is here obtained as a bilinear accumulation rule. n1 σ n2 t 0 0.2 0.4 0.6 0.8 1 σM1 0 0.2 0.4 0.6 0.8 1 σM1 > σM2 σM1 < σM2 Palmgreen-Miner rule n1 NR1 n2 NR2 σM2 Fig. 6.11. Damage accumulation diagram 6.4.1.3 Biaxial High-Cycle Fatigue Consider next a plate under a biaxial fatigue loading. Plane stress conditions and proportional loading are assumed and the in-plane stresses σ1 and σ2 va ry proportionally between (-σ1max and +σ1max)a nd(-σ2max and +σ2max). Figure 6.12 shows the stress contours corresponding to numbers of cycles to rupture NR =104, 105, 106 cycles for in-phase cyclic loadings. The contour corresponding to the damage equivalent stress criterion σ = σeqR1/2 ν =σf= 210 MPa is also drawn and fits well with the two-scale damage model for NR =106.

6.4 Numerical Failure Analysis 303 Fig. 6.12. Biaxial high cycle fatigue 6.4.1.4 Effect of Non-Proportional Loading The effect of a non-proportional loading is considered here for a num- ber of cycles to rupture, NR =105 cycles. First we consider an alternate loading of stress range Δσ1 =2σ1max until about NR/2cycle sinafir st direction (named 1) and then a second alternate loading of stress range Δσ2 =2 σ2max in the orthogonal direction (named 2) corresponding to NR.Figure 6.13 shows that to obtain the same number of cycles (NR =105)in non-proportional loading (square points) as in proportional loading (contour reproduced from Fig. 6.12), a higher state of stress is needed. This is an effect similar to that in plasticity where non-proportional loading induces an over strain-hardening or cross hardening. 6.4.2 Non-Proportional Loading of a Thinned Structure (M. Sauzay and A. Carmet 2000) As an example, consider a tube of total length L = 250 mm, external radius Re =28.7 mm, internal radius Ri =27.5 mm, and thickness t =1.2 mm. The middle part of the tube has been thinned with a grindstone on one side, leading to a gradually thinner zone of stress concentration, where the fatigue cracks will initiate (see Fig. 6.14). The thickness of the thinner part varies from 1.2 to 0.6 mm.

304 6 High Cycle Fatigue Fig. 6.13. Effect of non-proportional loading 6.4.2.1 Elastic FE Analysis The structure has been numerically analyzed and tested in tension, torsion, and tension-torsion fatigue loadings. Elastic computations in tension and in torsion give the meso stress fields σref1 and σref2 to be used as inputs for DAMAGE 2000 post-processing analysis, with the tension-torsion treated as a linear combination of σref1 and σref2. The meshing comprises 5120 3 and 4 node Kirchhoff--Love shell elements (full and reduce integrations here give the same results). For the structure loaded in torsion, the local state of stress in the thinned zone is shear with an overstress coefficient σzθ/σzθ n =1.76 (where the nominal stress σzθ n is the shear stress in the original tube of constant thickness t). For the structure loaded in tension, the state of stress is uniaxial in the center of the thinned zone with an over stress coefficient σzz/σzz n =1.66 (again, "nominal" is related to the tube of constant thickness). The axial stress is even larger at the beginning of the transition zone with σzz/σzz n =2.03 but also with a hoop stress.

6.4 Numerical Failure Analysis 305 Fig. 6.14. Picture (M. Grange) of the broken thinned shell 6.4.2.2 Proportional Fatigue Loadings The numbers of cycles to mesocrack initiation, NR, are calculated by use of DAMAGE 2000 post-processor. The material is a ductile steel with material parameters: E = 200000 MPa, ν =0.3, σy = 380 MPa, σu = 474 MPa, Cy = 50000 MPa, σ∞ f = 180 MPa, pD =0.025, m =3,S =2.6MPa,s =2, h =0.2, Dc =0.3. The experiments have been performed at a 5 Hz frequency. The numerical simulations compare well with the experimental results in Fig. 6.16 where the two straight lines represent a relative error NR/N exp R of4and1/4.Behappy with a factor of 4 in fatigue! 6.4.2.3 Non-Proportional Fatigue Loadings Four tension-torsion high cycle fatigue tests have also been performed at LEDEPP-ARCELOR at a frequency of 3 Hz. The non-proportional loading paths for the axial force F andthetorsiontorqueC are shown in Fig. 6.15. The maximum applied force is Fmax = 14000 N and the maximum (or min- imum) applied torque Cmax = 420 Nm (or Cmin = -Cmax). The results are given in Table 6.1.

306 6 High Cycle Fatigue Ta b l e 6 . 1 . Tension-torsion of the thinned shell Test Fmin Fmax Type Location of N exp R N comp R crack initiation a -1 in phase transition zone 1.13 · 105 4 · 105 b 0.1 in phase thinner part 4.86 · 105 4.4 · 105 c0 . 19 0 ◦ out of phase thinner part 3.72 · 105 6.9 · 105 d -19 0 ◦ out of phase thinner part 2.3 · 105 11.6 · 105 Fig. 6.15. Cyclic loading paths of tension-torsion The model gives a correct estimation of the number of cycles to meso crack initiation with a factor of at most 5 between computed and experimental numbers of cycles, N comp R and Nexp R , even for out-of-phase fatigue loadings. The corresponding 4 points are also reported in Fig. 6.16. This shows the ability of the model to predict high cycle fatigue failures in complex loadings.

6.4 Numerical Failure Analysis 307 Fig. 6.16. Comparison between computations and experiments 6.4.3 Random Distribution of Initial Defects The scatter in high cycle fatigue tests or in fatigue failures is always very large. A factor of 10 (1000%!) on the numbers of cycles to rupture around 106 for "identical" tests may happen. Since W. Weibull's studies (1939), independent of the experimental conditions, we know that the main reason is the initiation of the fatigue phenomenon on microdefects of different sizes. The number of cycles to rupture is as high as the probability of existence of a "big" defect is small. This is why small components have a larger lifetime than bigger ones. In the two-scale damage model, the only two material parameters intro- duced on a microscale are the kinematic hardening coefficient (Cy)whichis taken identical to its value on a mesoscale and the yield stress which is the asymptotic fatigue limit (σ∞ f ) on a mesoscale. The fatigue limit σ∞ f repre- sents the local weakness due to hidden defects in the material, therefore it is the natural candidate for the random parameter responsible for the high cycle fatigue scatter. Instead of guessing or measuring (but how?) the characteristics of micro- internal defects to identify a random distribution of initial damage, it is much easier to use or perform a series of fatigue tests loaded identically in tension- compression to obtain numbers of cycles to rupture (NRi) around 106 cycles. The distribution of NR for the stress considered as the engineering fatigue

308 6 High Cycle Fatigue limit σf is thus recorded. To go further we have to find the distribution of σ∞ f which would give the NRi recorded. This is a deterministic calculation if σ∞ f is expressed as a function of NR. Taking the result of the simplified two-scale damage model of Sect. 6.2.3, it is not possible to invert the formula (6.28) (even with the simplifying assumption of (6.22)) to derive σ∞ f in a closed-form as ND=1 4 pD Gm+1 Cm y (σu-σ∞ f)m (σmax - σ∞ f )m+1 NR=ND+ (2ES)sGDc 2σ∞ 2s f σmax-σ∞ f Σkk [Rs νmin+Rs ν max] , (6.80) where the numbers of cycles are calculated for the engineering fatigue limit sothatσmax =σf andRνmin =Rνmax =Rν Σkkσmax σ∞ f . A numerical analysis similar to the Monte Carlo method is needed while assuming a fixed NRi characterizing the scatter of the engineering fatigue limit σf and corresponding to a number of specimens imax (imax =20in Fig. 6.17 for the example of the ductile steel of of Sect. 6.4.2 ). Fig. 6.17. Histogram of the number of cycles to rupture corresponding to σmax = σf = 230 MPa at 106 cycles First, the material parameters are determined by the procedure of Sects. 1.4.4 and 2.4 applied on the experimental W¨ ohler curve drawn from

6.4 Numerical Failure Analysis 309 the mean value of the number of cycles for each stress range. Then σ∞ fis calculated for the 20 measured NRi from (6.80) using mathematical software. The NRi distribution is represented by the histogram of Fig. 6.18. The abscis- sas are discrete values σ∞ fpofσ∞ f and each ordinate is the number of values σ∞ f in between each σ∞ fp andσ∞ f p+1 .Asthen u mbe rofte stsism o stofte n low (≤ 20) statistically, a difficulty arises in the choice of the number of σ∞ fp that determine the shape of the probability curve. A number of intervals pmax ≈ 2+√imax is considered, a good compromise between exceedingly low (flat distribution) and exceedingly large numbers of values (also a flat distribution). Fig. 6.18. Histogram of the asymptotic fatigue limit σ∞ f Once fitted, this distribution is considered a characteristic of the material and may be introduced as input together with the values of the material parameters in any fatigue calculation by the Monte Carlo method. 6.4.4 Stochastic Resolution by Monte Carlo Method The Monte Carlo method is a numerical method to determine the stochastical response of any nonlinear model to random inputs by solving a large number of deterministic realizations of the inputs and by performing a statistical analysis on the results. Let's consider the histogram of the fatigue limit σ∞ fin Fig. 6.18. It is an approximation of the statistical distribution of σ∞ f and the first task is to regularize this discrete histogram by a known probability law or by curve fitting. For example, the histogram of Fig. 6.19 is a regularization

310 6 High Cycle Fatigue with 25 intervals of the histogram of Fig. 6.18 and the graph Pσf(σ∞ f )in Fig. 6.19 is the corresponding probability density fitted by a truncated β-- function: Pσf(σ∞ f)=1 220β σ∞ f 220,30,2.5 if σ∞ f ≥ 160 MPa (6.81) Fig. 6.19. Regularized histograms of σ∞ f and corresponding probability density

6.4 Numerical Failure Analysis 311 and Pσf = 0 elsewhere, with β(x,a,b)= Γ(a+b) Γ(a) · Γ(b) xa-1(1 - x)b-1 and Γ(z)= ∞ 0 tz-1 exp (-t)dt. (6.82) Then, the general procedure for a structural analysis is as follows: 1. An elastic structural analysis gives the state of the 3D stress history at the critical point(s) (Gauss point(s) for a finite element analysis). 2. The damage parameters are supposed to be known, including the statis- tics of the asymptotic fatigue limit σ∞ f such as its histogram or its prob- ability density (Fig. 6.19). 3. Consider a number pmax of discrete possible values σ∞ fpofσ∞ f .Inthe following example, it is 25 but a larger number (up to 100) is better. 4. Calculate the pmax values of the number of cycles to rupture NR p corre- sponding to the stress history with a post-processor such as DAMAGE 2000 for the two-scale damage model. They represent the failure statis- tics. 5. Draw the histogram of the results with the same ordinate np for NR p and σ∞ fp. 6. Calculate for the considered structure the mean number of cycles to rup- ture, NR = npNRp np , (6.83) its standard deviation, NR = ni(NRi - NR)2 np , (6.84) its histogram, or its probability law. This procedure has been applied to many values of unidimensional cyclic stresses corresponding to the W¨ ohler curve of ductile steel whose damage parameters are those used in Sect. 6.4.3. The numbers of cycles to rupture are calculated by means of the simplified two-scale damage model of Sect. 6.2.3 (also Eq. (6.80) of Sect. 6.4.3). Figure 6.20 shows the results: • For the mean value NR of the number of cycles to rupture as a function of the maximum stress σmax . The line fits the experimental W¨ ohler curve drawn almost exactly, with only one test for each stress. • For the histogram of N R corresponding to the three stresses. • For the standard deviation N R where it is interesting to see how it in- creases with the number of cycles to rupture as it is always found by experiments. This shows that it is not so complicated to take into account the scatter in high cycle fatigue failures predictions!

312 6 High Cycle Fatigue Fig. 6.20. Mean value and standard deviation of the number of cycles to rupture 6.4.5 Predeformed and Predamaged Initial Conditions Other types of damage high cycle fatigue failures are influenced by the ini- tial state of the materials (A. Galtier 1998). It is mainly an initial plastic strain p0, an initial damage D0, and an initial residual stress σres induced by the thermomechanical history of casting, metal forming, welding, and also damages by accident. Let's assume that the initial or residual quantities p0, D0,andσres ij exist but that they have been obtained for states of stresses larger than the in- service states of stresses that lead to high cycle fatigue (otherwise it would be low cycle fatigue!). The reference structure analysis is still elastic and those values are introduced in the two-scale damage model as initial values of the differential scheme. The conditions D(t =0)=D0, p(t =0)=p0, p(t =

6.4 Numerical Failure Analysis 313 0)= p 0 ,andX(t =0)=X0 satisfy the equilibrium equation div σres =0 (or σres ij,j = 0) for a static problem. For a plastic state, local tension leads to p 0=p0 100 0-1 20 00- 1 2 and X0 = Cyp0 10 0 0-1 20 00- 1 2 . (6.85) Figures 6.21 and 6.22 describe the effect of an initial plastic strain p0 that is smaller than the damage threshold pD and an initial damage D0 associated with the corresponding plastic strain, respectively, on steel at room temperature. The W¨ ohler curves are calculated by the damage post-processor DAMAGE 2000 with the following values of the material parameters: E = 200000 MPa, ν =0.3, σ∞ f =200MPa,Cy=2000MPa,σu =600MPa, pD =0.05, m =1,S =0.3MPa,s =2,h =0.2, and Dc = 1. This influence maybeofafactor10onNR. Fig. 6.21. Influence of an initial plastic strain on the W¨ ohler curve (J.-P. Sermage 1998) Fig. 6.22. Influence of an initial damage D0 = Dc/5=0.2o ntheW¨ ohler curve (J.-P. Sermage 1998)

314 6 High Cycle Fatigue If their values are known, residual stresses σres ij can be added to the loading stresses. 6.4.6 Hierarchic Approaches up to Surface and Gradient Effects , For other types of failure, we advise beginning any prediction of high cycle fatigue rupture using the simplest model, especially if only a few material parameters are known. • In early design it is often sufficient to check if the state of stress is below the fatigue limit conditions. In 1D, the only effect to take into account is the effect of mean stress and the simplest model is the Goodman diagram shown in Fig. 6.2. An elementary geometric calculation gives the following as non-failure conditions: σmax <σf +ˉ σ 1- σf σu or σmin > -σf +ˉ σ 1+ σf σu . (6.86) • For 3D state of stress, use one of the fatigue limit criteria of Sect. 6.2.2: the damage equivalent stress σ or, better, the Sines or Dang Van criterion for non-proportional loading. • Again, in early design, the Palmgreen--Miner rule is not so bad in mod- elling sequences of different levels of stress range. Together with the W¨ ohler curve, it allows for the determination of the number of cycles to rupture corresponding to a given history of unidimensional stress. • For 3D proportional loadings use the two-scale damage model of Sect. 6.2.3 integrated either numerically or in a closed form for periodic loading. • For random loading there is, at least for a first approach, a nice simple for- mula in Sect. 6.3.4, eq. (6.77). Otherwise the Monte Carlo method applies together with the two-scale damage model used as a post-processor. • For complex loadings such as 3D, non-cyclic and/or non-proportional loadings, the W¨ ohler curve can be used only to identify the two-scale damage model. The number of cycles NR or the time tR to mesocrack initiation is calculated by post-processing the elastic computation and by performing the time integration of the two-scale damage model constitu- tive equations (see Sect. 2.3). The most loaded point is where the damage D is maximum. The number of cycles to rupture NR corresponds to the reach of the critical damage Dc at this point, as described in Sect. 6.4.2. • It is also possible to consider a random distribution of initial defects as explained in Sect. 6.4.3, which allows for the possibility to express the results in terms of probability modelling of the large scatter observed in high cycle fatigue. Then, as in Sect. 6.4.4, the Monte Carlo method may be applied to any kind of loading.

6.4 Numerical Failure Analysis 315 • For more accurate predictions, one has to consider the fatigue weakness on any surface as plastic slips occur more easily on the surface grains that are well oriented with respect to the loading direction. Intrusion- extrusion mechanism takes place; it leads to microplastic strains that are larger on free surfaces than inside and then to lower numbers of cycles to rupture. This surface effect may be taken into account in the two-scale damage model through the localization law. The microscale stress used in the initial two-scale damage model (without meso plastic strain), σμ Eshelby = σ -3G(1-β) μp, (6.87) is calculated by means of the Eshelby--Kr¨ oner localization law for a spher- ical inclusion fully embedded in an RVE. It has to be changed at the free surface. Fig. 6.23. Inclusions for the two-scale damage model On the basis of the work of A. Cox (1989) and A. Deperrois & K. Dang Van (1990) a surface localization law can be built and used to describe the scale transition of the two-scale damage model (M. Sauzay 2000). Following these authors, consider a hemispherical inclusion in an RVE located along a free edge (Fig. 6.23) and for the sake of simplicity take D =0,˜ σμ = σμ,a nd p =0.If x3 is the normal to the free surface (denoted Γ), x the coordinates of a point in the RVE, the microscale stresses taking into account the existence of the free edge (σ x3 =0onΓ) are not uniform anymore, i.e., σμ(x)=σμ Eshelby - 3 r=1 Γ σμ r3Eshelby(x )C(r)(x , x)dΓ , (6.88) with C(1)(x , x)andC(2)(x , x) as the Cerruti tensors and C(3)(x , x)= B(x , x) as the Boussinesq tensor. Using the expression (6.87) for σμ Eshelby allows us to obtain the formal localization law on a free surface as σμ(x)=σ + M(x): μp , (6.89)

316 6 High Cycle Fatigue with M as a fourth order localization tensor that is non-symmetric (the direction 3 plays a particular role) and dependent on the position of the considered point inside the inclusion. Using indexical notation, we have Mijkl = Eijpq - Γ C(r) ij (x , x)Er3pq dΓ (SEshelby - I)pqkl , (6.90) with SEshelby as the Eshelby tensor. A dimensionless tensor m is also defined, such as Mijkl = -2G(1 - β)mijkl (6.91) and M. Sauzay (2000) gives, for ν =0.3, the average value of the inclusion of coefficients mijkl : m1111 = m2222 =1.24 , m1122 = m2211 = -m3311 = -m3322 =0.24 , m1212 = m1221 = m2112 = m2121 =0.5 , m1313 = m1331 = m3113 = m3131 =0.26 , m2323 = m2332 = m3223 = m3232 =0.26 . (6.92) The other coefficients are equal to zero. For 0.2 ≤ ν ≤ 0.4, the value for mijkl does not depend much on the Poisson ratio. The localization law to be used at surfaces is finally σμ ij surf = σij - 2G(1 - β)mijkl μp kl, (6.93) also written as σμ 11 surf = σ11 - 2G(1 - β)(m1111 p 11 + m1122 p 22) , σμ 22 surf = σ22 - 2G(1 - β)(m1122 p 22 + m1111 p 22) , σμ 12 surf = σ12 - 4G(1 - β)m1212 p 12, σμ 13 surf = -4G(1 - β)m1313 p 13, σμ 23 surf = -4G(1 - β)m2323 p 23, σμ 33 surf = -2G(1 - β)m3311 ( p 11+ p 22) . (6.94) For FE computation of structures loaded in high cycle fatigue, one has then different localization laws for surface elements and inside elements. For a homogeneous mesoscopic stress field it leads to an increase of the microscale plastic strain on free surfaces and, by consequence, a significant decrease of the number of cycles to mesocrack initiation (of about 30%) in surface than in plain material. From a mechanical point of view this explains why the mesocrack initiation on free surfaces is always observed in uniform stress field specimens. • Another characteristic effect of high cycle fatigue is the sensitivity to the gradient of the stress field. This gradient effect is illustrated here in

6.4 Numerical Failure Analysis 317 cyclic bending where the most loaded points are on the upper and lower edges of a beam: the number of cycles to mesocrack initiation is always larger in cyclic bending than in the equivalent homogeneous tension com- pression case (I. Findley 1956). This is nothing peculiar as the chance to find a large defect in the upper or lower parts of the beam cross section is lower than the chance to find the same defect in the whole cross section. Such a gradient effect is observed in bending, but not in torsion (I.V. Pa- padopoulos and V.P. Panoskaltsis 1996), and can be taken into account within the two-scale damage model by considering the nonlocal localiza- tion law, ˜ σμ = σ - c0|| σH||1 + c1 2σ - 2G(1 -β) μp , (6.95) instead of the Eshelby--Kr¨ oner law, where σH = σkk/3 is the mesoscale hydrostatic stress, and || σH|| is the norm of its gradient (vanishing in shear). Two new material parameters are introduced: -- c0, homogeneous to a length, is a phenomenological parameter iden- tified from experimental results (such as high cycle fatigue bending tests). -- the parameter c1, homogeneous to a square length, is naturally intro- duced from a homogenization procedure applied to non-uniform stress fields. It comes from the second order term of Taylor development of the stress tensor on the mesoscale. c1 is found to be equal to δ2 0/40 (E. Aifantis 1995) where δ0 is the size of the RVE (see Sect. 1.6.3). The effect of c1 on the crack initiation conditions is not clear (it does not act for linear fields) and c1 = 0 is probably a good choice to start with. Consider as reference the tension-compression loading between -σmax and +σmax . The meso stress field is homogeneous with vanishing gradient terms in the localization law (6.95). The number of cycles to rupture is then given by the initial two-scale damage model (numerical computation or analytical solutions of Sect. 6.2.3). For simplicity, consider the approx- imate expression (6.38) for zero mean stress with no damage threshold pD =0: NR= (2ES)sGDc 4σ∞ 2s f σmax-σ∞ f Σkk Rs ν max , (6.96) where Σkk =1andRν max = 2 3(1+ν)+1 3(1 - 2ν)σ2 max σ∞2 f . Consider then a circular bending test in the elastic range for which the stress field is locally uniaxial, with the same maximum and minimum applied stresses as for the tensile test: σ=M Iy and σmax=-σmin=M Id2, (6.97)

318 6 High Cycle Fatigue with d either the diameter or the height of the beam, such as y = d/2 and y = -d/2, correspond to the upper and lower sides of the beam, and with I as its bending inertia momentum. As the stress field is linear in y, the stress gradient is σ = 0 2σmax d0 where || σ|| = 2σmax d . (6.98) Apply the localization law with the gradient effect (6.95) at the most loaded point y = ±d/2 (the second order terms vanish): ˜ σμ = σ -2G(1-β) μp and σ = σ -c0|| σH||1, (6.99) which is identical to the Eshelby--Kr¨ oner localization law but where the gradient effect is taken into account through the new loading term σ . Writing σ = σ Σ Σ (proportional loading) gives σ Σ=σmax, Σ= 1 - 2c0 d00 0 -2c0 d0 00 - 2c0 d , Σeq =1, (6.100) and allows us to use (6.96) directly, but with Σkk =1- 6c0 d instead of Σkk = 1 to obtain the number of cycles to rupture in bending N R. Developing the expression for Rν max we end up with N R NR= σmax σ∞ f -1 σmax σ∞ f -1 1-6c0 d 23(1 + ν)+13(1 - 2ν)σ2 max σ∞2 f 23(1 + ν)+13(1 - 2ν) 1 - 6c0 d σ2 max σ∞2 f s . (6.101) Then for the same maximum applied stress σmax in tension-compression, we have N R >NR (6.102) in bending, i.e., a number of cycles to rupture increased in bending com- pared to the homogeneous tension-compression case. If the fatigue limits are defined for a given number of cycles for which no failure is observed, this corresponds to a fatigue limit in bending that is larger than the fa- tigue limit in tension-compression, as observed experimentally. The ratio N R /NR is drawn in Fig. (6.24) as a function of the ratio σmax/σ∞ f , with s as the damage exponent and c0/d as the material and

6.4 Numerical Failure Analysis 319 geometry parameters. Knowing c0 and d, σmax , σ∞ f ,ands, the Fig. 6.24 allows us to determine the factor with which to multiply the number of cycles to rupture classically calculated to obtain a better accuracy in bending. Inversely, from experiments made on specimens of height or di- ameter d, the knowledge of the ratios N R /NR, σmax/σ∞ f , and the damage exponent s allows us to determine the material parameter c0 . Fig. 6.24. Gradient effect in bending function of σmax/σ∞ f For more general cases of stress gradients, use the localization law (6.95) within the two-scale damage model.

7 Failure of Brittle and Quasi-Brittle Materials A material is considered brittle when it brakes without any irreversible strains and without any dissipation prior to cracking (e.g., glass and some ceramics). It is considered quasi-brittle when a dissipation prior to cracking exists with no or negligible permanent strains (e.g., concrete and some ceramics). The main mechanism is atomic decohesions to induce a fast propagation of a crack by instability. Nevertheless, the quasi-brittle materials may have some reversible slidings of nano- or microcracks considered as initial defects to induce a loss of energy by friction. Both mechanisms are dangerous because there is no precursor to wake up the attention of observers. The first scientific study of brittle failure was carried out by A.A. Griffith around 1920, introducing the concept of energy of decohesion used in frac- ture mechanics by cracking through the strain energy release rate variable G. But the study contained nothing about damage prior to crack initiation! In 1939 W. Weibull introduced the idea of statistical distribution of initial defects, giving rise to a model of probability of failure written in terms of stress and of the volume considered. Since then, many models of quasi-brittle materials are based on initial microdefects (F. McClintock 1973, S.B. Bat- dorf 1974, A.G. Evans 1978, A. Pineau 1983) or are damage models that are deterministic (Z.P. Baˇ zant 1984, J. Mazars 1985, G.Z. Voyiadjis 2002) or stochastic (F. Hild 1990). The specific topics of this chapter are the overall rupture criteria for brit- tle materials, debonding, probabilistic approaches for brittle and quasi- brittle materials, delamination of composites, and dynamic failures of concrete and ceramic structures. Long term, time-dependent behavior related to viscous effects of creep and relaxation is addressed in Chap. 5. 7.1 Engineering Considerations The materials subjected to brittle or quasi-brittle failures are ceramics, con- cretes, cements, glasses, rocks, brittle matrix composites, quenched steels . . .

322 7 Failure of Brittle and Quasi-Brittle Materials Their strain to rupture is small ( R < 2 · 10-2) and their toughness is at most on the order of a few MPa√m. The design of structures made of brittle materials is difficult because there is no place for plastic shakedown in case of overloading, but reinforcements help. For rough estimations meso stress criteria may be applied, but for pre- cise estimations the statistical distribution of internal defects must be taken into consideration. Unfortunately, they cannot be precisely evaluated by non- destructive methods. A possible alternative is to deduce a probabilistic infor- mation from the scatter of test results by an inverse method (see Sect. 6.4.3) for high cycle fatigue (F. Hild 1994). To illustrate this point, let us determine the probability density of the relative size of defects in a brittle material on which many rupture tests have been performed. The following simplified assumptions are made: • 10 to 20 rupture tests are available in simple tension on the same geometry. • For each specimen, the area density of the initial defects in the plane normal to the stress where the failure will occur is D0. Then the rupture stress σR is simply given (see Sect. 1.4.1) by the effective stress concept. For brittle failures, σR is related to an initial damage, σR =σu(1-D0)o rD0 =1- σR σu , (7.1) where σu is the rupture stress of the material without any defect. On a practical level, it is the maximum value of σR measured, assuming that in the set of specimens, at least one has no defects (or only some very small ones). The damage D0 is now a random variable (as is σR) for which the probability density resulting from the tests is P (σR). The probability for σR to have values bounded by σa and σb is P (σa <σR <σb)= σb σa P (σR)dσR . (7.2) It is also the probability for the decreasing function D0(σR)=1- σu/σR to have values bounded by D0(σb)=D0b and D0(σa)=D0a . Considering the inverse function σR = σu(1 - D0), we then have P (D0b <D0(σR) <D0a)= σu(1-D0a) σu(1-D0b) P (σR)dσR , (7.3) or by the change of variable σR = σu(1 - D0), P (D0b <D0(σR) <D0a)=- D0b D0a P (σu(1 - D0)) · (-σudD0) , (7.4) which shows that the probability density of initial damage D0 is

7.1 Engineering Considerations 323 P (D0)=σuP (σu(1 - D0)) . (7.5) For example, if σR obeys a Gaussian distribution, P (σR)= 1 ˉ ˉ σR√2π exp -(σR - ˉ σR)2 2ˉ ˉ σ2 R, (7.6) where ˉ σR is the mean value of the rupture stress and ˉ ˉ σR its standard devia- tion, the probability density of D0 is given by P (D0)= σu ˉ ˉ σR√2π exp - (σu(1 - D0) - ˉ σR)2 2ˉ ˉ σ2 R (7.7) or P (D0)= 1 ˉ ˉ σR σu √2π exp- D0 -1+ˉ σR σu 2 2ˉ ˉ σ2 R σu , (7.8) also a Gaussian distribution for D0.Themeanv alueofD0 is: D0 =1- ˉ σR σu (7.9) and its standard deviation is D0= ˉ ˉ σR σu . (7.10) Fig. 7.1. Histogram of initial damage D0 deduced from the histogram of rupture stress There is an easy way to obtain a statistical input for stochastic analysis of failure. Instead of using a continuous probability law (such as a Gaussian law), a discrete numerical treatment is possible, as shown in Fig. 7.1, where the histogram of initial damage is simply deduced from a set of stresses to

324 7 Failure of Brittle and Quasi-Brittle Materials rupture by D0i =1- σRi/σu .Ifimax is the number of tests (usually low, here imax = 20), using pmax ≈ 2+√imax (here pmax =6)a sthen u mbe r of intervals for the histograms is a good compromise between exceedingly low (flat distribution) and exceedingly large numbers of values (also a flat distribution). 7.2 Fast Calculations of Structural Failures Structural calculations for brittle failures, fortunately, do not involve any plastic strain. They may be performed in elasticity or simply taken in hand- books of stress concentration coefficients. The bad news, as already men- tioned, is the random character of brittle failures due to initial defects con- sidered (or not considered) as initial damage. Nevertheless, some meso stress criteria give orders of magnitude of the conditions of brittle failures and the Weibull model is a first useful approach of the statistical characteristic of brittle rupture. 7.2.1 Damage Equivalent Stress Criterion The simplest criterion to be used for the rupture of brittle or quasi-brittle materials is the damage equivalent stress σ deduced from the thermodynam- ics framework in Sect. 1.2.2. It is based on the total elastic energy whose amount at rupture is supposed to be a characteristic value for each material regardless of the state of stress: σ = σeqR1/2 ν with Rν = 23(1 + ν)+3(1- 2ν) σH σeq 2 , (7.11) where Rν is the triaxiality function, σH is the hydrostatic stress, σH = σkk/3, σeq is the von Mises stress, σeq = 3 2(σij - σHδij)(σij - σHδij). If σu is the ultimate stress in pure tension, the rupture criterion is written as σ = σu in three dimensions (7.12) and simply σ = σu in the uniaxial case as Rν =1.Hereweassumethesame behavior in tension and compression. Figure 7.2 shows the large difference due to the triaxiality between the damage equivalent stress σ and the von Mises (plastic) equivalent stress σeq, often used by mistake as a rupture criterion. An improvement consists of taking into consideration the quasi-unilateral condition of microdefects closure. Back to Sect. 1.2.4 and eq. (1.46), the complementary elastic energy is

7.2 Fast Calculations of Structural Failures 325 w e (σij)=ρψ e =1+ν 2E σ + ij σ + ij 1-D + σ - ij σ - ij 1-hD -ν 2E σkk 2 1-D + -σkk 2 1-hD , (7.13) where . are the Macaulay brackets. Fig. 7.2. Damage equivalent stress criterion function of the triaxiality ratio For a tensile stress σ , w e(σ )= 1 2E(1-D) (1+ν)σ 2 - νσ 2 = σ 2 2E(1 - D) . (7.14) This tensile stress is equivalent to the 3D case if w e (σ )=w e(σij). (7.15) In intrinsic notations, this is equivalent to σ = (1 + ν) σ +: σ +- ν tr σ 2 + 1 - D 1 - hD [(1 + ν) σ -: σ - - ν -tr σ 2] . (7.16) Remember that h is on the order of 0.2 and the rupture criterion is still σ =σu, (7.17)

326 7 Failure of Brittle and Quasi-Brittle Materials where D is here the relative surfacic fraction of microdefects at rupture Dc . The stress at rupture in tension is still σ = σ+ R = σu, but the stress at rupture in pure compression is now |σ- R| = σu 1-hDc 1-Dc 1/2, a small difference indeed. For materials like concrete, a much larger difference is obtained in the following definition of a damage equivalent strain and also in Sect. 7.4.1. Sometimes a simpler criterion is used for the fracture of concrete where it is observed that the microcracks are often oriented in the direction normal to the positive (tension) principal strains. As a consequence, the damage equivalent strain is defined by (J. Mazars, 1984): = + : + = 1 2+ 2 2+ 3 2 , (7.18) where 1, 2,a nd 3 are the principal strains and where i = i if i > 0, i = 0 elsewhere. Fig. 7.3. Damage criteria in a plane stress case: σeq , σ (ν =0.3,h =0.2,Dc = 0.3), In tension, = +. In compression, = √2ν| -| (ν is the Poisson ratio). The criterion normalized to the rupture stress in pure tension σ+ u orinpure compression σ- u is obtained as =σ+ u E =√2ν|σ- u| E, (7.19) which gives σ+ u =0.28 |σ- u | for ν =0.2. Figure 7.3 shows the difference between the last two criteria compared to the von Mises criterion in plane stress and proportional loading.

7.2 Fast Calculations of Structural Failures 327 7.2.2 Interface Debonding Criterion Consider a composite or two rigid elements A and B bound together by a film of glue I. It is represented by a 2D surface medium of "zero" thickness normal to the direction x3, as shown in Fig. 7.4. Fig. 7.4. Interface at mesoscale The continuity of the strain and stress vectors through the interface en- sure a state of plane strains 13 = 23 = 0 and a state of antiplane stresses σ11 = σ22 = σ12 = 0. The occurrence of two damage mechanisms, a normal debonding in mode I due to the normal stress σ33 and a shear debonding in mode II due to the shear stresses σ13 and σ23, allows us to consider the thermodynamic potentials of Sects. 1.2 and 1.4 written as functions of the following interface equivalent stress, σIeq = σ33|σ33| + σIR τI R 2 (σ2 13+σ2 23) 1/2 , (7.20) where . are the Macaulay brackets and |.| is the absolute value. It takes into account the unilateral character of interfaces which do not ex- hibit any damage in compression. The ratio of the ultimate tension stress σIR to the ultimate shear stress τ I R represents the large difference in strength which may exist between tension and shear of interfaces. In supermarkets, you may buy glues with large σIR or large τ I R depending on their use! The criterion of debonding of interfaces written σIeq = σIR -→ interface crack initiation is σ33|σ33| σI2 R +σ2 13+σ2 23 τI2 R =1. (7.21) It gives: • Rupture in pure tension for σIeq = σ33 = σIR • No rupture in pure compression as σIeq =0 • Rupture in pure shear for σIeq = σIR τI R |σ13| = σIR (or σIR τI R |σ23|), i.e., |σ13| = τ I R

328 7 Failure of Brittle and Quasi-Brittle Materials For mixed modes loading: • A tension decreases the strength in shear • A compression increases the strength in shear This criterion requires the knowledge of two material parameters: the stresses to rupture in pure tension σIR and in pure shear τ I R . It is represented in Fig. 7.5. Fig. 7.5. Interface criterion in the tension and shear stress plane 7.2.3 The Weibull Model This model takes into consideration the volume effect for which the prob- ability to find a large defect is greater in a large volume than in a small one. • The probability density of the defects considered as initial damages D0 is supposed to be a power function where mw is the Weibull modulus, P (D0)=mw(1 - D0)mw -1 . (7.22) • The rupture criterion is related to the damage equivalent stress σ = σeqR1/2 ν (it was the maximum principal stress in original Weibull model), σ =σw(1-D0)o rD0 =1- σ σw , (7.23)

7.2 Fast Calculations of Structural Failures 329 where σw is the ultimate stress to rupture of a hypothetic sample without any defect. It is also called Weibull stress. • Then, the probability of rupture PF0 of any RVE loaded by a stress σ is the probability for which σ >σw(1-D0)orD0 > 1- σ /σw . Considering the damage D0 bound by 1, PF0 = 1 1- σ σw P(D0)dD0 = σ σw mw . (7.24) • The Weibull theory considers the weakest link hypothesis which states that the rupture of the whole structure of volume V is achieved as soon as the rupture of an elementary volume V0 is initiated. • Considering the probability of rupture PF0 of the RVE on which σw is defined as the probability of rupture of the volume V is expressed as (W. Weibull 1939) PF =1- exp - V V0 PF0 (7.25) or PF =1- exp - V V0 σ σw mw . (7.26) • For structures subjected to non-uniform stress fields another effect that arises is related to the probability that the largest defect exists precisely where the stress concentration lies. To take into account this effect, it is convenient to introduce the concept of an effective volume Veff related to the elastic energy as it governs the phenomenon of rupture (F. Hild 1994). If we = σ 2(M)/2E is the elastic energy density field and wem a x= σ 2 max/2E, the elastic energy density at the stress concentration point of the structure is Veff = V σ 2(M)dV σ 2 max ≤V. (7.27) • Finally, the Weibull formula to use is PF =1- exp - Veff V0 σ σw mw . (7.28) 7.2.3.1 Use of the Weibull Model To apply the model, one needs the value of the elasticity parameters as well as of the Weibull parameters: • An elastic analysis of a structure of volume V gives the stress field σ (M) and the maximum stress at the stress concentration point. It gives also the energy density field we(M)andthenVeff.

330 7 Failure of Brittle and Quasi-Brittle Materials • Use Weibull formula (7.28) where V0 is the volume of the uniform stress part of the specimens tested to identify Weibull parameters σw and mw. • The identification of Weibull parameters needs imax =10to20e xpe ri- ments on specimens of cross section S0,lengthL,volumeVeff = V0 = S0L, and corresponds to a failure probability PF = PFL. To complete the iden- tification, proceed as follows: 1. Draw the cumulative histogram of the rupture stresses σR .Usepmax ≈ 2+√imax intervals and put in the ordinates the number of specimens p=p(σR<σ Rp) broken under the maximum stress σRp of the pth interval. 2. Use PFL ≈ p/(imax + 1) (or any other) as the probability estima- tor to change the histogram into an experimental probability density PFL(σR). 3. Identify σw = σwL and mw by curve fitting of the previous experimen- tal PFL(σR)law, PFL =1- exp - σR σw mw . (7.29) Do it by performing a linear regression in the ln[- ln(1 -PFL)] vs ln σR diagram. The slope of the curve is then the Weibull modulus mw and the ordinate at ln σR =0is- ln σmw w which yields σw . 7.2.3.2 From Brittle to Quasi-Brittle Failure (F. Hild 1994) A structure made of "brittle" material components often exhibits a quasi- brittle behavior (B. Coleman 1958, D. Krajcinovic 1981). To illustrate this point, consider here as a "structure" a fiber bundle made of carbon or ceram- ics fibers and modelled as a set of n fibers in parallel, loaded with the same applied displacement u. The fibers of length L, cross section S0,a ndv ol- ume V behave elastically with a Young's modulus E. The failure probability of a fiber PFL is given by the Weibull law, PFL =1- exp - σR σwL mw , where σwL = σw V V0 1/mw . (7.30) The loading is displacement-controlled. For large n, the number of broken fibers is given by nb ≈ PFLn, (7.31) which corresponds to a number, n - nb ≈ (1 - PFL)n, of unbroken fibers. The applied load is F = i σiS0 , (7.32)

7.2 Fast Calculations of Structural Failures 331 with σi = 0 for the broken fibers and σi = E for the remaining ones, i.e., F =(1- PFL)nS0E (7.33) or FS = E(1 - PFL) , (7.34) with S = nS0 as the total cross section area. Setting D = PFL defines the damage variable of Continuum Damage Mechanics as the failure probability of fibers. The mean applied stress ˉ σ=F/Sisthen ˉ σ=E(1-D) (7.35) and the bundle has quasi-brittle behavior. Fig. 7.6. Quasi-brittle stress-strain response of a ceramic fiber bundle (E = 400000 MPa, σwL = 500 MPa) The damage evolution is obtained by this analysis. For monotonic loading, D = D( )=1- exp - E σwL mw (7.36) or if the strain energy release rate Y = 1 2 E 2 is introduced, D = D(Y )=1- exp - 2EY σ2 wL mw 2 . (7.37)

332 7 Failure of Brittle and Quasi-Brittle Materials The thermodynamics framework of such a damage model (called Marigo model) is given in Sect. 7.4.1. The stress-strain curve obtained for a large number of ceramics fibers is given in Fig. 7.6 and the corresponding damage evolution in Fig. 7.7. If Weibull parameters are unknown, the stress-strain curve can be used to iden- tify them using simple (nonlinear) curve fitting. Note also that the unloadings are elastic with no permanent strain: the Young's modulus of the damaged bundle is the effective modulus ˜ E=E(1-D). Fig. 7.7. Damage evolution of a ceramic fiber bundle (E = 400000 MPa, σwL = 500 MPa) 7.2.4 Two-Scale Damage Model for Quasi-Brittle Failures It is possible to calculate quasi-brittle failure conditions by use of the two- scale damage model of Sect. 1.5.5. Consider here the case of a proportional monotonic loading with σ = σΣ(t)Σ,Σeq = 1, no plasticity on the mesoscale ( p = 0), and no damage threshold ( pD =0). Ascalar μ pΣ is defined to quantify the microplasticity, as follows: μp = 32 μ pΣΣD and ˙ σμ Σ=Cy˙ μ pΣ≈Cy˙ σΣ G. (7.38) Here, Cy/G 1andG≈3G(1 - β). Once the yield stress on the microscale (equal to the asymptotic fatigue limit σ∞ f ) is reached, we can assume ˙ σμ≈0

7.2 Fast Calculations of Structural Failures 333 and the von Mises stress on the microscale remains quasi equal to σ∞ f:σμ≈ σ∞ f .The time integration of the damage law (coupled with (7.38)) allows us to calculate the damage D at a given mesostress σ and then the quasi-brittle failure conditions when D reaches the critical damage Dc , such that D≈ σ∞2s f G(2ES)s σΣ σ∞ fRs ν Σkk σΣ σ∞ f dσΣ, (7.39) with Rν (ξ)= 2 3(1+ν)+1 3(1 - 2ν)ξ2 as in Sect. 6.2.3. The function Rν (ξ) varies significantly over the integration interval and an approximate formula for the stress to failure is derived for small values of s: σΣR≈σ∞ f + 3G(1 - β)(2ES)sDc σ∞ 2s fRs ν (Σkk) . (7.40) For compression-like loading (σ<0), considering the parameter h within the damage law allows us to calculate the stress at failure in compression (σ- R) that is much larger than in tension (σ+ R) and to show that σ+ R-σ∞ f |σ- R|-σ∞ f ≈hs. (7.41) Coupled with the previous knowledge of the asymptotic fatigue limit σ∞ f and the damage exponent s (from fatigue experiments), this result can be used to identify the microdefects closure parameter h. For concrete, for example, σ∞ f is neglected, s =1,andσ- R /σ+ R =10givesh ≈ 0.1. 7.2.5 Sensitivity Analysis The sensitivity analysis of brittle failure is a special case as the rupture is not defined by a number like the plastic strain, time, or number of cycles in Sects. 3.2.3, 4.2.3, 5.2.3, and 6.2.4 of previous chapters but by the stress itself, through the damage equivalent stress σ . For example, σ =σu -→ rupture. (7.42) In order to perform the calculation in the spirit of the general method de- scribed in Sect. 2.4.6, let us consider the ratio σ /σu and derive how much it differs from 1. Furthermore, consider also the influence of initial defects in writing σu(1 - D0) as the previous ultimate stress. Rupture corresponds then to Rupt =1,with Rupt = σ σu(1-D0), (7.43) where σ = σeqR1/2 ν ,Rν=2 3(1 + ν)+3(1- 2ν)T 2 X,andTX = σH σeq .

334 7 Failure of Brittle and Quasi-Brittle Materials Taking the logarithm and the derivative with absolute values of the rela- tive errors gives δRupt Rupt = δσeq σeq +(3T2 X-1 3)ν Rν δν ν +3(1-2ν)T2 X Rν δTX TX +δσu σu+D0 1-D0 δD0 D0, (7.44) which defines SRupt Ak as the coefficients of the sensitivity matrix of Sect. 2.4.6. Therefore, δRupt Rupt = k SRupt Ak δAk Ak, (7.45) with SRupt σeq =1, SRupt TX =3(1-2ν)T2 X Rν , SRupt σu =1, SRupt ν =|3T2 X-1 3|ν Rν , SRupt D0=D0 1-D0 . (7.46) As in the other chapters, the diagram in Fig. 7.8 shows the relative values of the influence of all the parameters by the height of the boxes for a set of parameters representing mean values for brittle materials: TX =1= ⇒Rν = 2.07, ν =0.2, and D0 =0.05. Fig. 7.8. Relative importance of each parameter in brittle failures In comparison to other failures, the sensitivity is much lower. But the random value of the initial defects is not here taken into consideration: in practice, this is this parameter that governs the uncertainties. 7.2.6 Safety Margin and Crack Propagation Most of the time, brittle failures occur by a fast propagation of a crack once the mesocrack is initiated. To avoid such an event, the state of stress anywhere in the structure must have a value below the rupture stress with a safety factor Saf. We advise checking to ensure that σ max<σu Saf . (7.47)

7.2 Fast Calculations of Structural Failures 335 Due to the statistical effect of initial defects, a probabilistic safety margin is preferred each time it is possible: Prob(σ max≥σu)< 1 SafPr , (7.48) where σu is a random variable and σ max may also be a random variable due to the uncertainties of the loadings. The statistically admissible risk defined by 1/SafPr depends on many fac- tors: knowledge of the material, knowledge of the loading, the quality of the mechanical analysis, the consequences of an eventual accident, and also sub- jective human factors. Therefore, SafPr =102, 103,...,105 or more. The safest design cannot have SafPr = ∞.I ti s ,h o w e v e r ,ad e s i g n which minimizes the consequences of a failure. In this spirit, the "fail- safe" design consists of two or three parallel systems for one major resisting function. Once a mesocrack is initiated, it is difficult to avoid the complete failure. Its size calculated in Sect. 1.6.3 does not contain the plastic term (1.252) as the material is considered fully elastic, i.e., δ0≈ Gc σ2 u 2E Dc . (7.49) A fast crack propagation will be avoided if the strain energy release rate G for this mesocrack is smaller than the toughness Gc : G<Gc with G≈ κσ2 ∞πδ0 E, (7.50) where κ is a shape factor and σ∞ is the far field stress, κσ2 ∞πδ0 E <Gc. (7.51) The result does not depend on the toughness anymore but it depends on the critical damage, as in σ∞ σu < Dc 2πκ , (7.52) with 0.2 <Dc < 0.5and1≤ κ<10 so that 0.06 < σ∞ σu <0.28. (7.53) These are indeed small values due to the large crack length δ0 initiated by damage in brittle materials. They are often exceeded in practice, which

336 7 Failure of Brittle and Quasi-Brittle Materials is safe as long as no crack exists but not otherwise. Anyway, this explains why it is so difficult to design crack arrests in structures made of brittle materials! 7.3 Basic Engineering Examples The same cases of stress concentrations in cylinders or beams as in the pre- vious chapters are treated here, assuming the structures are made of brittle materials. It is somewhat simpler as plasticity is ignored but any defect may play an important role. The design of notches or geometry variations and their machining or forming must be done with much care. Furthermore, any scratch or surface damage in service must be controlled and examined from the point of view of residual strength. 7.3.1 Plates or Members with Holes and Notches The uniaxial local stress at the critical point of stress concentration is sup- posed to be determined via a structural calculation or from the elastic stress concentration coefficient KT and the nominal stress σn (see Fig. 3.4 and handbooks), σ=KTσn. (7.54) The stress condition for a mesocrack initiation is simply σR=KTσnR=σu. (7.55) In case of a 3D state of stress, the damage equivalent stress with or without the microdefects closure effect associated with an initial damage may be used: σ =σu. (7.56) For design purposes, it is interesting to express the admissible stress σ max or the ratio σ max/σu corresponding to a given probability of failure derived from the Weibull model of Sect. 7.2.3: σ max σu = - V0 Veff ln(1 - PF) 1 mw . (7.57) Figure 7.9 shows how it varies with the probability PF,theratioV0/Veff,and mw as parameters. This graph helps us choose the safety factor Saf of Sect. 7.2.6. For example, in order to ensure a failure probability below 10-5 with mw =7andV0/Veff = 10-1, the safety factor Saf = σu/σ max must be larger than 7.2. It shows also that the variation of Saf is on the order of 2 when the Weibull modulus mw varies from 7 to 15 or when the volume fraction V0/Veff varies from 10-1 to 10-3.

7.3 Basic Engineering Examples 337 Fig. 7.9. Admissible damage equivalent stress for a given failure probability 7.3.2 Pressurized Shallow Cylinders The structural analysis of Sect. 3.3.2 and Fig. 3.6 is again recalled for a long circular cylinder of radius Rcyl and thickness tcyl that is submitted to an increasing relative pressure P , yielding σeq=√3 2 PRcyl tcyl , σH = PRcyl 2tcyl , TX=σH σeq=1 √3, Rν =5-4ν 3. (7.58) The condition of rupture is still σ = σu except if some defect D0 must be taken into consideration. In that case, σ = σeq Rν = σu(1 -D0), (7.59)

338 7 Failure of Brittle and Quasi-Brittle Materials and the pressure to bursting PR is PR= 2 √5-4ν tcyl Rcyl σu(1 - D0) . (7.60) Using ν =0.3, this gives a pressure that is ≈ 12% lower (even with D0 = 0) than the von Mises stress criterion σeq = σu sometimes used! 7.3.3 Fracture of Beams in Bending Sorry, this question is as simple as the first undergraduate course about strength of materials! Assume a portion of a rectangular beam of width b and height h loaded in pure bending by a bending moment M (Fig. 3.7). According to the Bernoulli hypothesis, the maximum stress at the upper and lower part of the height is σmax=M Ih2, (7.61) where I = bh3/12 is the inertia moment. Writing the condition of crack initiation with an eventual defect D0, σmax = σu(1 - D0) (7.62) gives the value of the bending moment at crack initiation MR, MR=2I h σu(1 -D0), (7.63) or for the rectangular cross section, MR=bh2 6 σu(1 -D0). (7.64) For considering fixed value of the moment and D0 =0, σmax = 6MR bh2 . (7.65) Once the crack initiated reaches a length of δ0 , a (very) rough estimation of the maximum stress is σ max = 6MR b(h-δ0)2 . (7.66) If σ max >σu (except if D0 is large and localized only on the edge), the crack length increases, leading to a total fracture by instability. Conclusion: If you try to initiate a small crack in a brittle component stress controlled by bending, you will obtain two components! But it may work if you try it by strain or controlled displacement.

7.4 Numerical Failure Analysis 339 7.4 Numerical Failure Analysis The high level of damage encountered in components or parts of struc- tures made of quasi-brittle materials is usually made acceptable by the pres- ence of reinforcements: laminate composites are multi-layered, concrete is reinforced by bars or cables, and ceramic matrix composites (CMC) are fiber-reinforced. Modern design solutions need to live with this damage and the corre- sponding computations are necessary for evaluations. By chance, reinforce- ments often prevent the strain localization phenomenon and one can expect nonlinear, but stable, damage computations. As quasi-brittle materials behave quasi elastically, specific damage models may be formulated. 7.4.1 Quasi-Brittle Damage Models , Quasi-brittle materials are usually modelled by elasticity coupled with dam- age (no plasticity!) and with a damage law of the form D = D(Y )o r D = D( ), as justified in Sect. 7.2.3 from a Weibull analysis of a fiber bundle. Such damage models mainly apply to ceramics and composites. The quasi-brittle material of main interest in civil engineering is concrete which exhibits very different behaviors in tension and in compression. An engineering design assumption is allowing its tensile strength to be equal to zero! This is of course not fully satisfactory and such an assumption is difficult to introduce in numerical computations, with the classical question: what is tension and what is compression for 3D states of stress? Fortunately, the use of the mathematical tools of Sect. 1.2.4 allows us to build suitable damage models for quasi-brittle materials and with a reduced number of material parameters. 7.4.1.1 Marigo Model of Elasticity Coupled with Damage (1981) The Marigo model is written in the thermodynamics framework with the total strain associated with the stress σ and the damage D associated with the opposite of the strain energy release rate Y as state variables. The Helmholtz free energy has the simple expression ρψ=1 2(1-D) :E: , (7.67) with E as the elasticity tensor. The damage criterion (such as f<0 ⇒ elasticity) is written as f=Y-κ(D), (7.68)

340 7 Failure of Brittle and Quasi-Brittle Materials where κ(D) is a function of the damage and κ(0) = YD is the damage thresh- old in terms of elastic energy density. The term SM = dκ dD is the consolida- tion modulus and linear consolidation corresponds to κ(D)=SD + YD,with SM=S=const. The law of elasticity coupled with damage derives from the Helmholtz potential as σ=E(1-D): or = 1+ν E(1-D)σ- ν E(1-D)tr σ1. (7.69) The strain energy release rate is Y=1 2 :E: = σ 2 2E(1-D)2 , (7.70) where σ = σeqR1/2 ν is the damage equivalent stress. The damage evolution law derives from the dissipative potential, taken here as FD = f (associated model), through the normality law ˙ D=˙ μ ∂FD ∂Y =˙ μ, (7.71) with ˙μ as the damage multiplier calculated by means of the consistency con- dition f =0and ˙f = 0. The damage evolution law is then ˙ D= ˙Y SM. (7.72) For monotonic loading, D = 0 as long as Y ≤ YD . The integration of the previous law gives, of course, D= κ-1(Y)i f Y>YD , (7.73) where κ-1(Y ) is the damage function. For complex loadings such as non- monotonic and/or 3D loadings, considering the damage surface FD = f =0 gives a damage simply related to the maximum value of the strain energy release rate Ymax over the loading, Ymax =s u p τ∈[0,t]Y(τ), (7.74) and D = κ-1(Ymax)=D(Ymax)s u c h a sY<YD =⇒ D =0. (7.75) A simple but general damage evolution law is: D = κ-1(Ymax)= Ymax - YD S s , (7.76) with YD, S,ands as the damage parameters.

7.4 Numerical Failure Analysis 341 A damage law adapted to concrete either in tension or compression is (C. Laborderie 1991) D=κ-1 Lab(Ymax)=1- 1 1+ Ymax - YD S s. (7.77) A damage law adapted to composite materials is (P. Ladev` eze and E. Le Dan- tec 1992) D=κ-1 Lad(Ymax)= √Ymax - √YD S (7.78) and the Weibull damage law of Sect. 7.2.3 may be written as D=κ-1 w (Ymax)=1- exp - Ymax Sw sw , (7.79) with S, s,orSw , sw as material parameters. Note that these models yield symmetric behavior in tension and in com- pression. 7.4.1.2 Marigo Model with Microdefects Closure Effect This section gives a simple extension of the Ladev` eze--Lemaitre isotropic dam- age framework of Sect. 1.2.4 to quasi-brittle materials. The model uses a single damage variable D corresponding to a damage state that is either tension-like or compression-like (or a mix). Take as state potential the following: ρψ = 1+ν 2E σ + : σ + 1-D + σ - : σ - 1-hD - ν 2E tr σ 2 1-D + -trσ 2 1-hD , (7.80) from which =1+ν E σ + 1-D+ σ - 1-hD - ν E tr σ 1-D- -trσ 1 - hD 1 (7.81) and Y=1+ν 2E σ + : σ + (1-D)2 +h σ - : σ - (1-hD)2 - ν 2E tr σ 2 (1-D)2+h -trσ 2 (1 - hD)2 , (7.82) with the elasticity law and the strain energy release rate density as functions of the microdefects closure parameter h. Keeping the damage criterion unchanged f = Y - κ(D) still leads to D = κ-1(Ymax)=D(Ymax) . (7.83)

342 7 Failure of Brittle and Quasi-Brittle Materials Due to the introduction of h<1, the elasticity law is different in tension and in compression: σ =σ+=E(1-D) intension σ = σ- = E(1 - hD) in compression. (7.84) The damage growth is also different for tension and compression. For the same loading intensity | |, Y=Y+= σ+2 (1-D)2 =1 2E 2 -→ D = κ-1 1 2 E 2 max (tension) Y=Y-=h σ-2 (1-hD)2 = h2E 2 -→ D= κ-1 h2E 2 max (compression) (7.85) with the damage induced by compression being smaller than the damage induced by tension. An example of the model response is given in Fig. 7.10. Fig. 7.10. Stress-stain curve for Marigo model with microdefects closure effect (E = 30000 MPa, linear law D = Ymax/S, S =5· 10-4 , h =0.057) The model applies to any state of stress. It is quite simple with material parameters E and ν for elasticity, YD as the damage threshold (which may be taken to be equal to zero for concrete), and S, s,a ndh as the damage parameters. We recommend using the simple damage evolution law (7.76)

7.4 Numerical Failure Analysis 343 D = κ-1(Ymax)= Ymax - YD S s . (7.86) 7.4.1.3 Anisotropic Damage Model for Concrete For concrete, it is sufficient to consider damage anisotropy with a quasi- unilateral effect acting on the hydrostatic stress only in the general thermo- dynamics framework of Sects. 1.2 and 1.5. First, the Gibbs specific free enthalpy is represented by ρψ = 1+ν 2E tr HσDHσD + 1 - 2ν 6E tr σ 2 1-trD + -tr σ 2 , (7.87) with H =(1 - D)-1/2 so that the elasticity law becomes =ρ∂ψ ∂σ =1+ν E˜ σ-ν Etr ˜ σ1 (7.88) and defines the symmetric effective stress as ˜ σ =(HσDH)D + 13 tr σ 1-trD- -trσ 1. (7.89) The energy release rate tensor Y = ρ ∂ψ ∂D is the thermodynamics variable associated with D (see Sect. 1.2.3). Second, use the Mazars strain damage criterion (f<0 -→ elasticity) yielding f = - κ(tr D)a n d = + : +, (7.90) where κ(tr D) is chosen to ensure that at low cost (two damage parameters only), the damage rate in compression is lower than that in tension: κ(tr D)=a · tan tr D aA +arctan κ0 a , (7.91) where κ0 is the damage threshold. The terms A and a are the dimensionless damage parameters. The anisotropic damage evolution law can be derived from the non- associated damage potential F = F (Y ; )=Y : 2+ , ˙ D=˙ μ∂F ∂Y =˙ μ 2+ . (7.92) The damage multiplier ˙μ is determined from the consistency condition f =0 and ˙f = 0. The damage law finally reads as

344 7 Failure of Brittle and Quasi-Brittle Materials ˙ D = κ-1 ( ) 2+ 2 ˙ (7.93) or ˙ D = A 1+ a 2 -1 2+ 2 ˙ if >κ max DI = Dc -→ mesocrack initiation. (7.94) It ensures a damage rate that is proportional to the square of the positive part of the total strain tensor and in accordance with the damage anisotropy observed in concrete in tension and compression (see Sect. 1.4.5). Fig. 7.11. Stress-stain curve for the anisotropic damage model (E = 42000 MPa, ν =0.2, κ0 =510-5 , A =5103 , a =2.93 10-4 , Dc =0.92) A nonlocal anisotropic damage model is simply obtained by replacing in the damage criterion with the nonlocal Mazars equivalent strain, nl=1 Vr V W (x - s) (s)dV, (7.95) where W (x - s) is a nonlocal weight function (such as (2.113) or (2.114) of Sect. 2.2.7) and where Vr = V W (x - s)dV . Consider then f = nl -κ(tr D), keeping F = Y : 2+ unchanged so that the nonlocal anisotropic damage evolution law reads: ˙ D = A 1+ nl a 2 -1 2+ 2 ˙ nl if nl >κ max DI = Dc -→ mesocrack initiation. (7.96)

7.4 Numerical Failure Analysis 345 The local model has a total of 6 material parameters: E, ν for elasticity, κ0 as damage threshold, and A, a,andDc as damage parameters. An example of the concrete stress-strain curve is given in Fig. 7.11. Finally, when permanent strains have a major effect, as in cyclic loading or in dynamics, use the Laborderie model (see Sect. 7.4.3) or others, taking into account the microdefects closure effect, damage anisotropy, and inelastic strains (A. Dragon and D. Halm 1998, F. Ragueneau 1999). 7.4.1.4 Damage Model for Composite Laminates Elementary Layers (P. Ladev` eze 1986) This model takes into account different damage mechanisms with different ef- fects in tension and compression. Consider here laminates made of orthotropic layers or plies (long fiber reinforcement). In such composite materials, damage occurs at different levels: • In the elementary plies with several degradation mechanisms, different scalar damage variables such as DF for fiber breakage, DT for transverse cracking, and DS for shear damage are considered. • Damage at the interfaces leads to the phenomenon of delamination. The simple 2D quasi-brittle mesomodel for elementary plies described here is an extension of the Marigo model to orthotropy. The Gibbs energy is represented by ρψ = σ11 2 2E1(1 - DF) + φ( -σ11 ) 2E1 -1 2 ν21 E2+ν12 E1 σ11σ22 + σ22 2 2E2(1 - DT) + -σ22 2 2E2+ σ2 12 2G12(1 - DS) , (7.97) with the usual symmetry ν21/E2 = ν12/E1, e1 in the fiber direction and φ as the microdefects closure function. The initial model considers φ = -σ11 2 (instantaneous modulus recovery in compression). A thermodynamically con- sistent choice taking into account the nonlinear elastic response in compres- sion is (B. Desmorat 2002) φ= -1 bD ln 1 - bD -σ11 2 , (7.98) with bD as a material parameter. This leads to an effective Young's modulus ˜ E- 1 in compression that is different from the effective modulus in tension ˜ E+ 1: ˜ E- 1 = E1 for the instantaneous recovery; E- 1 = E1(1 - bD -σ11 2 )forthe nonlinear response. The elasticity law coupled with damage yields the following from the thermodynamics potential

346 7 Failure of Brittle and Quasi-Brittle Materials 11 = σ11 E1(1 - DF) - -σ11 E- 1 - ν21 E2σ22, 22 = σ22 E2(1 - DT) - -σ22 E2 -ν12 E1σ11, 12 = σ12 2G12(1 - DS) . (7.99) The energy release rate densities associated with the damage variables are YF = σ11 2 2E1(1 - DF)2 , YT = σ22 2 E2(1 - DT)2 , YS= σ2 12 2G12(1 - DS)2 . (7.100) Damage evolution laws such as (7.78) can be used for each damage variable (up to a critical damage Dc equal to 1). An adequate choice for organic matrix composites is to consider brittle fiber breakage, DF = 0 or 1 depending on the fiber rupture stress σRF, and mixed evolution of damage for tranverse cracking and shear damage (P. Ladev` eze and E. Le Dantec 1992): ˆ Y =sup [0,t] {YS + bTYT} , DT = ˆ Y -√YTD ST , DS = ˆ Y -√YSD SS , (7.101) with bT, ST , YTD , SS,andYTS as the damage parameters. In tension, the stress-strain curves are similar to those obtained for the Marigo model. Note that the model can be completed to take into account the plastic-like behavior in the ±45◦ directions. See Sect. 7.4.4 for an application mixing both layers degradation and interfacial delamination. 7.4.2 Failure of Pre-stressed Concrete 3D Structures (F. Gatuingt and F. Ragueneau 2001, 2004) Consider first concrete structures reinforced with passive bars and/or active (pre-stressed) cables. Mesh the concrete parts with 2D or 3D finite elements of size varying from 0.01 m (cement) or 0.1 m (concrete) to usually 0.3 m or more for large structures or uniformly loaded zones. Use a law of elasticity coupled with damage for the concrete elements. Model the bars and the cables

7.4 Numerical Failure Analysis 347 with 1D elements with interpolation functions of the same type as those for the 2D or 3D connecting elements and use elasto-plasticity or elasto-plasticity coupled with isotropic damage for the steel reinforcements (see Sect. 1.5.2). It is usually not necessary to model damage in bars and cables as the designed solutions tend to prevent it: • For monotonic loading applications, the value of the uniaxial strain in the steel parts must remain lower than the damage threshold pD or the rupture strain pR. • For cyclic or dynamic loadings, compute at least the accumulated plastic strain p or the stored energy ws for comparison with the damage thresh- old in terms of plastic strains pD or in terms of stored energy wD (see Sect. 1.4.1). Still, for the steels, use monotonic hardening only for monotonic applications; use kinematic hardening (or both kinematic and isotropic hardening) for cyclic and dynamics applications. Finally, the numerical problem of the application of the pre-stresses in the active cables is not so simple. A possible procedure for damage computations withpre-stressedcablesisasfollows: 1. Estimate the cables tensile stress σ0 and enter it at the Gauss points of the cables elements. 2. Use a finite element interpolation to transform it into elementary nodal loads {Fe} (with the notations of Sect. 2.2.1) at the FE nodes of the cables elements, {Fe} = Ve [B]T {σ} dV. (7.102) They represent the loading applied by the concrete body on the cables. 3. Change the sign of previous nodal loads to obtain the loading applied, by the cables on concrete. This defines the loading equivalent to the cables action. 4. The computation of the structure submitted to previous equivalent load- ing gives both initial deformation and damage states due to the applica- tion of the pre-stress. Do not model the cables at this stage. 5. Consider finally the cables as passive elements in further structure com- putations. To correctly model the cables plastification, do not forget to decrease, in the FE input file, the cables yield stress to σy0 = σy - σ0 (σy is the yield stress of the material). Start the computation from the previous initial deformation state. The stress, strain, and damage fields numerically obtained take into account the cables pre-stress. As an example, consider the short term behavior of the concrete structure in Fig. 7.12 is representative of a ring of a power plant containment vessel reinforced by half circular steel bars and pre-stressed by metallic cables. The

348 7 Failure of Brittle and Quasi-Brittle Materials diameter of the ring is 46.8 m, its thickness is 0.9 m, and only a height of 0.4 m is meshed (see Fig. 7.13). A vertical compressive stress of 8.5 MPa is applied to model the weight of the upper part of the structure (not meshed). There are two symmetric anchoring parts and the steel reinforcement is made of 88 rectangular stirrups (not considered in the computations), 4 circular reinforcement bars and 2 pre-stressed half-circular cables. The finite element analysis of the ring is made in 3D with the bars and the cables modelled with 2-node bar elements and the concrete part with of 8-node bricks. The C.E.A. CASTEM 2000 computer code is used. Fig. 7.12. Concrete ring and its steel reinforcement Both the passive steel bars and the active metallic cables are assumed to be perfectly plastic. The concrete is modelled with the anisotropic damage model of the previous section and the corresponding material parameters are • E=190000MPa,ν =0.3,andσy=500MPaforthesteelbarsof diameter 25 mm • E = 190000 MPa, ν =0.3, and σy = 1814 MPa for the active cables with cross sections of 5143 mm2

7.4 Numerical Failure Analysis 349 • E = 42000 MPa, ν =0.2, κ0 =510-5, A =5103,anda =2.93 10-4 for concrete (with a rupture stress in compression σ- u =38MPaandapeak stress in tension σ+ u =4MPa) The pre-stress is introduced using the above procedure to a tensile stress σ0 = 385 MPa along the cables so that when the cables are considered passive, their yield stress is decreased from σy = 1814 MPa to σy0 = σy - σ0 = 1429 MPa in the CASTEM input data file. Note that enforcing the pre-stress leads to an initial cracking localized at the lower side of the anchoring parts (see Fig. 7.13 in which the displacements have an amplification factor of 724). Fig. 7.13. Undeformed and pre-stressed structures An internal pressure P (t) is then applied. The damage fields are computed up to Pmax =9105 Pa for which the average damage intensity corresponds to a structure that has already collapsed. Due to the steel reinforcement, a non-uniformly deformed mesh is obtained (see Fig. 7.14 in which the dis- placements have an amplification factor of 633). Fig. 7.14. Undeformed structure and deformed structure at Pmax =9105 Pa The evolution of the principal damages at point A and at the cross section center point B (Fig. 7.13) are plotted in Fig. 7.15 as functions of the cables pre-stressing tension and then as functions of the pressure intensity P .

350 7 Failure of Brittle and Quasi-Brittle Materials Fig. 7.15. Principal damages at points A and B during pre-stress application and during pressure loading This simple test shows the possibility of using 3D anisotropic damage computations of reinforced concrete structures up to a very high damage level and up to plastification of the reinforcement steels. It illustrates the fact that initial cracking patterns often exist in such structures. The steel re- inforcements prevent any localization modes and there is no need to introduce strain localization limiters. Coupled with the consideration of a safety criterion D<Dgiven ,the s e computations can be used to design civil engineering structures at their most loaded parts. 7.4.3 Seismic Response of Reinforced Concrete Structures (F. Ragueneau and J. Mazars 2001) Dynamics and seismic FE analyses need efficient and robust modelling for both space and time discretizations. Explicit schemes are often used (such as the Newmark scheme) and some include numerical damping for computation reasons. Seismic loading looks like a random fatigue loading, but quick, so that it is given as the seism acceleration history (also called seism accelero- gram).

7.4 Numerical Failure Analysis 351 Geometric simplifications are welcome and are sometimes possible for civil engineering buildings made of walls and flats naturally meshed by beams and plates. For reinforced concrete parts, a homogeinized behavior must be con- sidered. A possibility consists of the choice of a multilayered beam (or plate) element which averages concrete and steel nonlinear constitutive equations (see Fig. 7.16). Using beam or plate kinematics or multilayered beam mod- elling conserves the steel reinforcement ratios as well as their location through their effect on the beam inertia. Fig. 7.16. Example of a frame frame discretized by multilayered beam elements For seismic civil engineering applications, consider a damage model with permanent strains for concrete and use elasto-plasticity for steels (up to dam- age initiation, see Sect. 7.4.2) or elasto-plasticity coupled with isotropic dam- age if computations up to a total collapse are performed. Note that the main advantage of such multifiber type finite elements is the uniaxial implemen- tation of each layer's constitutive law, leading to efficient computations in dynamics. As illustrated next, an accurate modelling of concrete behavior is necessary, the major role of the dynamics force variation enhances the effect of the microdefects closure modelling on the seismic response of the structure. Ta b l e 7 . 1 . Steel reinforcements of the walls Sa, Sb (mm2)S c( m m 2) Level 5 15.9 78.4 Level 4 28.3 78.4 Level 3 94.4 110.2 Level 2 188.9 138 Level 1 289.4 138 As an example, consider the 1/3rd mock-up of Fig. 7.17 on the "C.E.A." shaking table ("CAMUS" experiment) computed for the "Nice S1" accelero- gram that is representative of earthquake far field and for the "San Francisco 1957" accelerogram representative of earthquake near field. It is composed of 2 parallel walls linked by 6 square slabs and is anchored on the shaking table

352 7 Failure of Brittle and Quasi-Brittle Materials by a highly reinforced footing. Table 7.1 lists the steel reinforcement cross sections for each wall. Fig. 7.17. CAMUS mock-up (P. Bish and A. Coin 1998) The mock-up is loaded by a horizontal displacement parallel to the walls. Steel bar bracing systems disposed perpendicularly to the loading direction prevent torsional modes. The complete experimental sequence is an accelero- gram made of Nice 0.24 g, followed by San Francisco 1.13 g, Nice 0.40 g, and Nice 0.71 g (Fig. 7.18) modified in time with a ratio 1/√3totakeinto account the similarity rules. 7.4.3.1 FE Modelling and Eigenmode Adjustment The choice of a multilayered beam modelling is made with all the constituents restricted to beam kinematics, but with nonlinear material behavior.

7.4 Numerical Failure Analysis 353 Fig. 7.18. Earthquake accelerograms • The Laborderie model is used for concrete where only the uniaxial con- stitutive equations are needed. They introduce 11 material parameters: E and ν for elasticity; αt , αc ,a ndσclos for the microdefects closure effect; YtD and YcD as damage thresholds in tension and compression; and St , st , Sc ,andsc for damage. Elasticity with permanent strains due to damage is represented by = σ E(1-D+)- -σ E(1-D-)+ αtD+ E(1 - D+) g (σ)+ αcD- E(1 - D-) (7.103) and the damage evolution laws are D+ =1- 1 1+ Y + max - YtD St st D- =1- 1 1+ Y - max - YcD Sc sc, (7.104) where Y+ = σ 2 2E(1 - D+)2 + αtg(σ) E(1 - D+)2 Y- = -σ 2 2E(1 - D-)2 + αcσ E(1-D-)2 , (7.105) and where the microcrack closure function g(σ) is defined as follows

354 7 Failure of Brittle and Quasi-Brittle Materials g(σ)=σ + -σ 2 2σclos if σ>-σclos , g(σ)=- σclos 2 if σ ≤-σclos . (7.106) The set of material parameters, here for a concrete with a maximum compressive strength of 35 MPa and tensile strength of 3 MPa, are: E = 22·109Pa,YtD =127Pa,YcD =6·104 Pa,St =1.11·10-4Pa, st =1.2, Sc =1.89·105Pa, sc =1.4, αt =106Pa, αc = -40·106Pa, and σclos =1.3 · 106 Pa. The stress-strain response of the model in tension- compression is given in Fig. 7.19. Fig. 7.19. Stress-strain curve for the Laborderie model • The steels are assumed to be elasto-plastic (no damage). They have a Young's modulus E = 200 109 Pa, a yield stress σy = 414 106 Pa, and an ultimate stress σu = 480 106 Pa. The LMT-Cachan computer code EFICOS (J.F. Dub´ e, C. Laborderie, J. Ma- zars 1994) is used with the Newmark scheme for the time discretization. Figure 7.17 shows the mock-up modelling as well as the finite element mesh. The maximum element size is limited to 30 cm in the less loaded zones with a total of 22 elements, each made of 20 layers. The additional mass and the weight load of each floor are concentrated at each storey (black circles). The stiffness of the springs below the shaking table is identified so as to fit the first two eigenmodes measured on the non-damaged (virgin) structure.

7.4 Numerical Failure Analysis 355 7.4.3.2 Seismic Structure Response Figure 7.20 gives both the experimental and numerical responses of the struc- ture. The computed horizontal mock-up top displacement compares well with the measured one. Shocks are induced as microcracks close when the vertical mode is acti- vated. Experimental observations show a vertical acceleration of the shaking table. The vertical force variations are computed (Fig. 7.21) and a compar- ison with the experiment (summarized in Table 7.2) demonstrates that the Laborderie model for concrete, representing permanent strains due to dam- age and the strong difference of behavior in tension and in compression, is relevant to seismic analyses. Fig. 7.20. Horizontal top displacement Fig. 7.21. Vertical force variations

356 7 Failure of Brittle and Quasi-Brittle Materials A small change in the microcrack closure function through the value of σclos , responsible for the gradual stiffness recovery in compression, has a big influence on the results on a structural level (it activates the second vibration mode here). In conclusion, it is of first importance in dynamics to properly model the microdefects closure effect for loaded concrete structures. Ta b l e 7 . 2 . Maximum dynamics forces (kN) Model Experiments Nice 0.24 g 119 138 San Francisco 1.13 g 160 198 Nice 0.40 g 132 146 Nice 0.71 g 190 248 7.4.4 Damage and Delamination in Composite Structures (O. Allix and P. Ladev` eze 1992--98) Damage of composite laminates is complex, with different damage mecha- nisms in each ply of the stacking structure but also with delamination and crack propagation at the interfaces (Fig. 7.22). Based on the damage models of Sect. 7.4.1 for the orthotropic layers, a mesomodel can be built, allowing for the computation of damage and delamination in laminate structures. Fig. 7.22. Damage mechanism in laminates (left). Laminate modelling (right) For engineering applications, perform first the whole structural compu- tation in elasticity using laminated plates theory (with no damage and with perfect interfaces). Then reanalyze the most loaded zones by meshing every layer and interface using damage models. For 3D reanalyses, the Gibbs energy for a single layer (7.97) must be completed with normal stresses terms:

7.4 Numerical Failure Analysis 357 ρψ = σ11 2 2E1(1 - DF) + φ( -σ11 ) 2E1 + σ22 2 2E2(1 - DT) + -σ22 2 2E2 - ν12 E1 σ11σ22 + σ33 2 2E3(1 - DT) + -σ33 2 2E2 - ν13 E3 σ11σ33 - ν23 E2 σ22 σ33 +σ2 12 2G12(1 - DS) + σ2 23 2G23(1 - DS) + σ2 13 2G13(1 - DS) , (7.107) with φ as a nonlinear function such as (7.98) and where the subscripts 1, 2, and 3 designate the fibers direction, the transverse direction inside the layer, and the normal direction, respectively, and . stands for the positive part. The elasticity coupled with damage laws is derived from the Gibbs potential. A delay effect is introduced here for regularization purpose within the damage evolution laws: for the damage variables DS and DT, one considers ˙ DSorT= ˙ D∞ 1 - exp -a κ-1 Lad( ˆ Y)-DS or T , (7.108) which recovers the laws DS or T = κ-1 Lad( ˆ Y)= √ˆ Y -√YD SS or T of Sect. 7.4.1 for low strain rates and which bounds the damage rates to ˙ D∞ at high strain rates (with ˙ D∞ and a as material parameters). Note that the inelastic strains in the layers (due to the microcracks sliding with friction) are taken into account through the consideration of a plasticity-like yield function, such as f<0 corresponding to elasticity and f = 0 to internal sliding: f = ˜ σ2 12 +˜ σ2 23 +˜ σ2 13 + χ2(˜ σ2 22 +˜ σ2 33)-R-τy≤0, (7.109) with R as the hardening function, τy as the yield stress and χ as a material parameter. The effective stresses are then ˜ σ11=σ11, ˜ σ22 = σ22 1 -DT - -σ22 , ˜ σ33 = σ33 1 -DT - -σ33 , ˜ σij = σij 1-DS (i =j). (7.110) Next, mesh the imperfect interfaces by using interface elements (iso- parametric elements here) with the interface damage model developed by O. Allix and P. Ladev` eze (1992). It considers an interface energy per unit area function of the components σi3 of the normal stress vector (constant across the interface) and 3 damage variables d1, d2,andd3 (anisotropic interface): Ψ = σ33 2 2k3(1 - d3) + -σ33 2 2k3+σ2 13 2k1(1-d1)+ σ2 23 2k2(1 - d2) , (7.111)

358 7 Failure of Brittle and Quasi-Brittle Materials where n= e3 is the interface normal (see also Fig. 7.4 of Sect. 7.2.2). The interface stiffness terms ki are material parameters which depend on the thickness estimated for the physical interface (1 μm here). The variables associated with the stresses σi3 are the displacement dis- continuities [[ui]] at the interface and the interface elasticity law coupled with damage derived from the thermodynamics potential Ψ : [[u1]] = ∂Ψ ∂σ13 = σ13 k1(1-d1), [[u2]] = ∂Ψ ∂σ23 = σ23 k2(1-d2), [[u3]] = ∂Ψ ∂σ33 = σ33 k3(1 - d3) - -σ33 k3, (7.112) as do the strain energy release rates, Y1=∂Ψ ∂d1 = σ13 2k1(1 - d1)2 , Y2=∂Ψ ∂d2 = σ23 2k2(1 - d2)2 , Y3=∂Ψ ∂d3 = σ33 2k3(1 - d3)2 . (7.113) The interface damage evolution law is written here in a delayed form bounding the damage rate (with SI, sI, ˙δ∞ and aI the interface damage parameters), as represented by ˙δ = ˙δ∞ 1 - exp -aI ˆ YI SI sI - δ ˆ YI =[Y γ0 3 +(γ1Y1)γ0 +(γ2Y2)γ0]1/γ0 , (7.114) whered1=d2=d3=δhere. Perform then the damage post-processing of the zone of interest such as around perforations, holes, or rivets. Use as boundary conditions the dis- placement field along the multilayered plate medium plane computed in the elastic reference calculation. Be careful to apply this field on a single medium line along the border of the reanalyzed zone: imposing displacements all over the thickness nodes would lead to edges effects and non-physical damaged zones localized along this border. As an example, consider the M55J/M18 high modulus carbon-fiber/epoxy- resin laminate with stacking sequence [03/ ± 452/90]S and which is loaded in tension (Fig. 7.23). The testing specimen is 50 mm in width, 150 mm in gauge length, and has a 10 mm diameter hole. The ply thickness is 0.125 mm. The tensile test is performed at a fixed displacement rate of 0.5 mm·min-1 .Fig- ure 7.24 shows the evolution of the X-ray revealed damage map near the hole for an increasing applied load. Rupture is obtained for a load of 430 MPa.

7.4 Numerical Failure Analysis 359 Fig. 7.23. Carbon-fiber/epoxy-resin M55J/M18 holed specimen At 55% of the rupture load, both transverse cracking (in 90◦ -plies near the hole) and matrix cracking (in the 0◦ -plies near the hole in the fiber direction, phenomenon also called "splitting") occur. Delamination initiates later, at about 80% of the rupture load. The delaminated area develops and remains located between the two splitting lines. At 97% of the rupture load, its length is about the equivalent of two hole diameters. Fig. 7.24. X-ray photographs of the M55J/M18 holed specimen (D. Lev` eque 1998) The damage reanalysis of the circular zone around the hole is performed by post-processing an initial elastic multilayered plate analysis. The DSDM LMT-Cachan computer code is used with the following material parameters: • Single ply in the orthotropy framework ( e1: fibers direction): E1 = 311000 MPa, E2 = 6350 MPa, E3 = 20000 MPa, ν12 = ν13 =0.35, ν23 =0.48, G12 = G13 = G23 = 4870 MPa, σRF = 1760 MPa, bT =0,

360 7 Failure of Brittle and Quasi-Brittle Materials YSD = YTD =0,SS =2.55 MPa1/2, ST =1.96 MPa1/2, ˙ D∞ = 500 s-1, a =1,χ =1.3, τy =17MPa,R(p) = 1445 · p1/2 MPa. • 0◦-0◦ interface: k1 = k2 = k3 =4· 105 N/mm-3, γ0 =1.6, γ1 = γ2 =0.4, aI =1, ˙δ∞ = 1000 s-1, SI =0.66 N/mm-1, sI =0.2. •± θ interfaces: k1 = k2 =3· 104 N/mm-3, k3 =4· 104 N/mm-3, γ0 =1.2, γ1 = γ2 =0.4, aI =1, ˙δ∞ = 1000 s-1, SI =0.54 N/mm-1, sI =0.5. The damage maps computed in the layers and interfaces are given in Figs. 7.25 and 7.26. The delaminated areas (in black) correspond to the zones where the damage d3 = 1. Note that when the 0◦ -fibers break near the hole, the local load is transferred by shear in the matrix in the adjacent fibers. The shear damage DS is then the indicator for splitting. Fig. 7.25. Computed damage maps at the interfaces (at rupture load) Fig. 7.26. Computed damage maps in the layers (at rupture load)

7.4 Numerical Failure Analysis 361 In conclusion, damage mechanics is an adequate tool to predict the dam- age pattern in composite materials and structures but it needs an impor- tant material database. It models interface cracking and delamination phe- nomenon and can therefore be used to optimize the layers sequence. Finally, note that in such quasi-static fracture the material constants ˙ D∞, a, ˙δ∞,and aI do not play an important role but they become of most importance in dynamic cases such as chock problems. 7.4.5 Failure of CMC Structures (F. Hild, P.-L. Larsson, F.A. Leckie 1994) Due to long fiber reinforcement, ceramic matrix composites (CMC) are or- thotropic and quasi-brittle. The strength of structures made of CMC can be checked either by using the Weibull analysis of Sect. 7.2.3 or Continuum Damage Mechanics. The aim of this section is to illustrate the second possibil- ity with the orthotropic damage model for composite layers (see Sect. 7.4.1) extended to transverse isotropy. The 3D elasticity coupled with damage model is obtained by completing the thermodynamics potential (7.97) with terms ensuring that the direc- tions 2 and 3 play the same role. Perform then the damage computations in a fully coupled FE analysis, bearing in mind that once strain localization takes place, a mesocrack should be initiated and the FE solutions become mesh-dependent. As an example, consider a spinning disk and a spinning ring made of CMC fiber reinforced in the hoop direction (Fig. 7.27). Both the disk and the ring have an outer radius a =0.3 m. The inner radius of the ring is b = a/2=0.15 m. The two structures are thin enough for the plane stress assumption to apply and the cylindrical coordinates system (r, φ) is chosen. The loading is due to a rotation at the angular velocity ω and ρ denotes the material density. The constitutive model is elasticity coupled with damage and is locally orthotropic (tangential to the fibers direction). The damage variable is defined as the percentage of broken fibers and is given by the corresponding failure probability (Eq. (7.37) with σφφ = Eφ(1 - Dφ) φφ). Thus Dφ =1- exp - L L0 2EφYφ φ2σ2 w mw 2 and Yφ= σ2 φφ 2Eφ(1 - Dφ)2 (7.115) if φφ>0a nd˙ φφ > 0 and where the Weibull parameters mw and σw are identified from tensile tests made on fibers of length L0 and φ is the fiber volume fraction in the hoop direction. Due to distributed pull-out in these spinning structures, the evolution of fiber breakage is not dictated by the length of the fibers but by the strength over which, once a fiber is broken, the tensile stress field recovers its original

362 7 Failure of Brittle and Quasi-Brittle Materials level. This length is a function of the fiber radius Rf and the interfacial shear stress τI which is assumed to be constant along the interface cracks. For weak interfaces (τI < 10 to 15 MPa here), a shear lag analysis using the global load sharing assumption gives (R.B. Henstenburg and S.L. Phoenix 1989, W.A. Curtin 1989) L= Rfσφφ φτI(1 - Dφ) (7.116) and leads to a damage law representing the gradual fiber multifragmentation which is less conservative than the initial Weibull law: Dφ =1- exp - 2EφYφ φ2σ2 c mw+1 2 and σc = σmw w L0τI Rf 1 mw +1 . (7.117) Fully coupled computations are performed with the ABAQUS code under a plane stress assumption. Satisfactory results are obtained with only 20 elements. The material parameters are: • Eφ = 140 109 Pa, Er =20109 Pa, Grφ =13109 Pa, and νrφ =0.214 for elasticity • mw =4,φσw = 1450 106 Pa, L0 =12.610-3 m, and φσc = 1300 106 Pa for damage Fig. 7.27. Analyzed structures

7.4 Numerical Failure Analysis 363 Figure 7.28 compares the stress field in the hoop direction of the ring obtained for elasticity coupled with damage to the stress field obtained in pure elas- ticity. There is a stress redistribution and the global stiffness of the damaged structure softens as the applied load increases. 100 200 300 400 500 600 700 800 900 0.15 0.2 0.25 0.3 Stress (MPa) Radius, r (m) Elasticity coupled with damage Elasticity Fig. 7.28. Hoop stress in the ring σφφ as a function of the radius (ρω2 = ρω2 loc = 2.26 · 1010 kg·m-2 ·s-2) 0 0.05 0.1 0.15 0.2 0 0.05 0.1 0.15 0.2 0.25 0.3 Damage Radius, r (m) Dc Dφ(r) Localization Fig. 7.29. Damage in the disk as a function of the radius (ρω2 = ρω2 loc =1.87 · 1010 kg·m-2 ·s-2)

364 7 Failure of Brittle and Quasi-Brittle Materials The damage field computed in the disk is given in Fig. 7.29 where the critical damage Dc =0.18 corresponds to strain localization occurrence. Note that the model predicts strain localization and therefore, mesocrack initiation inside the structure. There is also a difference in the computed load levels at localization ρω2 loc between the two structures studied: ρω2 loc =1.87 · 1010 kg·m-2·s-2 for the disk and ρω2 loc =2.26 · 1010 kg·m-2·s-2 for the ring. These values are found to be 20 to 25% larger than the values obtained with the initial Weibull law (7.115) which corresponds to a more conservative design, i.e., heaviest mechanical components. To conclude, FE damage analyses of quasi-brittle CMC structures can be performed up to strain-damage localization (the failure criterion considered here). They give the location of the fiber reinforcement weakness in the ring and can be used to design non-uniformly reinforced disks and rings and to optimize the fiber density distribution. 7.4.6 Single and Multifragmentation of Brittle Materials (C. Denoual and F. Hild 1997) Pure brittle materials may break either by single cracking or multifragmenta- tion depending on the stress rate. This is the case for glass, concrete, ceramics, and rocks when impacted by a projectile. At low stress rate, failure occurs as a result of a single crack propagation with a high degree of scatter. A classical analysis using the σ criterion (see Sect. 7.2.1) or Weibull analysis (see Sect. 7.2.3) gives the failure conditions. In dynamics, fragmentation occurs with a more deterministic behavior and the microcrack pattern can be computed using Continuum Damage Mechanics. In order to make proper predictions, it is important to know a priori the transition between the two mechanisms. The Weibull model corresponds to the initiation and immediate growth of a crack in a brittle material. In dynamics, the degradation mechanism is com- plex because only a part of the unstable defects or flaws lead to microcrack growth. This is due to a stress relaxation (or obscured) zone which develops around each initiated microcrack during the propagation of the stress wave. To illustrate this phenomenon, the microcrack initiation is represented on the space-time graph of Fig. 7.30 where the first initiation occurs at time t1 at the space location M1 for the stress σ (t1). This produces an obscured zone of volume Vobs as a function of t - t1 in which no flaws become unstable. Assuming self similar relaxation (or interaction) zones of size governed by a constant fraction kcL of the longitudinal stress wave velocity cL,wehave Vobs = Vobs(t - t1)=κ [kcL · (t - t1)]3 , (7.118) where κ is a shape parameter. The quantity kcL · (t - t1) is a representative length of the relaxation zone around a microcrack. At time t2 corresponding to σ (t2) >σ (t1), a second microcrack starts to propagate and produces its

7.4 Numerical Failure Analysis 365 own obscured zone (Fig. 7.30). The third and fourth defects do not nucleate here as they are obscured by the first two microcracks. Fig. 7.30. Defects obscuration in a space-time graph To model this dynamic process consider, as in a Weibull analysis, a flaw distribution λtot described by a Poisson process of intensity, λtot(σ )=λ0 σ σ0 mw , (7.119) with mw as the Weibull modulus and σ0 as the scale parameter relative to a reference flaw density λ0 .Thequ a ntityλtot represents the mean number of flaws that may break in a unit volume for a local stress less than or equal to σ . At the beginning of the loading, no interactions occur and the crack den- sity (denoted by λcrack) is equal to the total density of the flaws able to break, λtot . Due to the dynamic relaxation process, λcrack becomes smaller than λtot following the law dλcrack dt = dλtot dt ·[1-Pobs], (7.120) with λcrack(t = 0) = 0 and where Pobs is the probability of defects obscuration or relaxation which defines the damage variable, D ≡ Pobs =1- exp - t 0 dλtot dτ Vobs(t - τ)dτ . (7.121) Knowing the local stress history σ (t) gives the flaw distribution history λtot(t) (7.119), then the probability of defects obscuration (7.121), and finally by time integration of (7.120) the crack density.

366 7 Failure of Brittle and Quasi-Brittle Materials 7.4.6.1 Quasi-Static Weibull Model Recovered The Weibull model corresponds to the case of failure due to a single defect (weakest link hypothesis). Setting Vobs = const = Veff as the effective volume (7.27), the probability of failure is equal to Pobs , i.e., PF =1- exp - t 0 dλtot dτ Veffdτ =1- exp (-λtotVeff) , (7.122) which recovers Weibull failure probability (7.28), or PF =1- exp - Veff V0 σ σw mw (7.123) for the Poisson process (7.119). 7.4.6.2 Fragmentation to Multifragmentation Transition A closed-form solution of previous set of equations (7.119)--(7.122) can be derived in the case of the impact loading σ =˙ σt with constant stress rate ˙ σ: λtot =λ0 ˙ σ σ0 mw tmw = λc ˆtmw , λcrack = λc mw mw +3 (mw +3)! 6mw! mw mw+3 γ mw mw +3, 6mw! (mw +3)!ˆ tmw+3 , D = Pobs =1- exp - 6mw! (mw +3)!ˆtmw . (7.124) The function of the dimensionless time ˆt = t/tc introduces the character- istic time tc ,str e s sr ate ˙ σc , and microcrack density λc .Thete r mγ is the incomplete gamma function, γ(a, x)= x 0 ta-1 exp (-t)dt, such that tc = σmw 0 κ(kcL)3λ0 ˙ σmw 1 mw +3 andλc=1 Vc = λ1 mw 0˙ σ κ1 3 kcLσ0 3mw mw +3 . (7.125) The characteristic volume Vc contains, on average, one flaw that may break at the characteristic time tc (λcVc =1). The applied stress denoted here, Σ, is related to the local or effective stress via σ =Σ/(1 - D) so that the stress-rate-dependent tensile strength σu is given by dΣ/dσ =0or σu = σc (mw +2)! 6e·mw! 1 mw +3 where σc = σmw 0˙ σ3 κ(kcL)3λ0 1 mw+3 . (7.126)

7.4 Numerical Failure Analysis 367 This is the dashed line (stress-rate-dependent) in the dimensionless tensile strength versus dimensionless stress rate diagram (Fig. 7.31) in which the solid circles (average) and bars (standard deviation) are given by Monte- Carlo simulations (500 realizations for each point). Figure 7.31 also shows the stress-rate-independent results for a classical Weibull analysis from which the mean failure stress is (Γ is the Euler Γ-function) σ= σ0 (λ0Veff) 1 mw Γ 1+ 1 mw (7.127) and the corresponding standard deviation is σ= σ0 (λ0Veff) 1 mw Γ 1+ 1 mw - Γ2 1+ 1 mw . (7.128) Fig. 7.31. Normalized tensile strength σu/σc vs normalized stress rate ˙ σ/˙ σt for mw =10andVeff =1/λ0 (C. Denoual and F. Hild 1997) The stress-rate-independent regime ˙ σ<˙ σt corresponds to single fragmen- tation. It is obtained from the classical Weibull analysis when the weakest link hypothesis is made. The regime ˙ σ>˙ σt corresponds to multifragmen- tation. It is dependent on the stress rate and is obtained from the dynamic obscuration mechanism. The transition between both regimes occurs at the stress rate ˙ σ=˙ σt, defined as the intersection between "quasi-static" and "dynamic" strengths,

368 7 Failure of Brittle and Quasi-Brittle Materials σu(˙ σ=˙ σt)=σ, (7.129) giving ˙ σt = σ0kcL(λ0κ)1 3 (λ0Veff)mw+3 3mw 6e · mw! (mw +2)!Γmw+3 1+ 1 mw 1 3 . (7.130) Remark --When ˙ σ>˙ σt , Continuum Damage Mechanics can be used to model the multifragmented microcrack pattern. According to the definition of damage as the probability of obscuration, ln(1 - D)=- t 0 dλtot dτ Vobs(t- τ)dτ = - t 0 dλtot dτ κ[kcL ·(t- τ)]3dτ and a damage evolution law for high stress rates (> ˙ σt) is obtained by eliminating the explicit dependency upon time: -d3 dt3 ln(1 - D)=6κ(kcL)3λtot (σ ) , with D(t =0)=0, ˙ D(t =0)=0,a nd¨ D(t =0)=0due to λtot(t =0)=0.Using Y = σ 2/2E, it can be written as a function of the strain energy release rate, d2 dt2 1 1-DdD dt = 6κ(kcL)3 V0 2EY σ2 w mw 2 . To conclude, the damage law at low stress rate has to be of the form D = D(Y ) when a differential equation in time is needed at high stress rate. 7.4.7 Hierarchic Approach up to Homogenized Behavior , Failure of brittle or quasi-brittle components is mainly governed by initial defects that are random in their size and space distribution. Therefore, the accuracy of prediction is often poor for at least two reasons: high scatter of basic tests results to identify the parameters and ignorance of the state of initial defects. Nevertheless, speaking of probabilities gives a sense to these uncertainties. For brittle materials or interfaces: • In absence of any information other than an ultimate stress, use the dam- age equivalent stress criterion (and not the von Mises stress!), σ = σeqR1/2 ν = σu with Rν = 23(1+ν)+3(1-2ν) σH σeq 1/2 . (7.131) Introducing the microdefects closure is an improvement if some compres- sion occurs.

7.4 Numerical Failure Analysis 369 • The Mazars damage equivalent strain is better for concrete: = + : + = σ+ u E = ν√2σ- u E. (7.132) • For interfaces a debonding criterion which needs two material parameters may be applied: σ33|σ33| + σIR τI R 2 (σ2 13+σ2 23) 1/2 =1. (7.133) • The Weibull model should be used to characterize the probability of rup- ture but the material parameters need 10 to 20 specimens for their iden- tification: PF =1- exp - Veff V0 σ σw mw . (7.134) Using the two-scale damage model is a way to predict the rupture of quasi- brittle materials that occurs when a dissipation prior to cracking exists (if some fatigue results complete the identification database!) but several other damage models have their specific applications: • The Marigo model with or without microdefects closure effects is a general model valid for most materials while the anisotropic damage model of Sect. 7.4.1 is suitable for concrete • The Laborderie model with permanent strains and microdefects closure effects in dynamics (seismic effects on civil engineering structures) • Mesomodels for composites where three damage variables are considered • Probabilistic models for ceramics and fragmentation in dynamics Finally, elasticity and damage models for reinforced concrete are of main im- portance in civil engineering. Due to the size of the structures, it is interesting in FE computations to avoid meshing the steel bars and the concrete body separately. Homogenization procedures give the equivalent elastic properties of heterogeneous materials. They apply to undamaged reinforced concrete and uniaxial bar reinforcement, yielding orthotropic elasticity characteristics. For example, if the steel spacing is the same in the two tranverse directions, tranverse isotropy is obtained with longitudinal and transverse Young's mod- uli EL and ET, Poisson ratios νLT and νT and shear moduli GLT and GTT : EL = EL(φ, Ec ,Es ,...) , ET = ET(φ, Ec ,Es ,...) , νLT = νLT(φ, Ec,Es,νc,νs), νT = νT(φ,Ec,Es,νc,νs), GLT = GLT(φ, Ec,Es,νc,νs), GTT= ET 2(1+νT), (7.135) whose specific expressions depend on the homogenization procedure. They are functions of steel volume fraction (φ), the elastic properties of concrete (Ec , νc) and steel (Es , νs).

370 7 Failure of Brittle and Quasi-Brittle Materials The question of coupling with damage arises then and one needs to take into account the microcrack closure effect in concrete. One of the simplest possible models uses the anisotropic and damage framework of Sect. 7.4.1, but extended to tranverse anisotropy, ρψ = σ11 2 2˜ E+ L + -σ11 2 2˜ E- L + σ22 2 + σ33 2 2˜ E+ T + -σ22 2 + -σ33 2 2˜ E- T - νLT EL (σ11σ22 + σ11σ33) - νTT ET σ22σ33 + σ2 12+σ2 13 2GLT + σ2 23 2GTT , (7.136) where the coupling with damage is reduced to the minimum by making the damage variable DL act on the longitudinal modulus, the damage variable DT on the tranverse modulus, and by neglecting the coupling of the ratios νij/Ej and the shear moduli with damage: ˜ E+ L = EL(φ, Ec(1 - DL),Es ,...) , ˜ E- L = EL(φ, Ec(1 - hDL),Es ,...) , ˜ E+ T = ET(φ, Ec(1 - DT),Es ,...) , ˜ E- T = ET(φ, Ec(1 - hDT),Es ,...) , (7.137) where h is the microdefects closure parameter. The damage evolution laws are written as D = D(Y )la w s(s u cha s Eqs. (7.76) to (7.79)) DL = DL(YLm a x)a n dDT = DT(YTm a x) , (7.138) with YLm a x and YTm a x as the maximum values reached during the loading of the longitudinal and transverse strain energy release rates YL =ρ∂ψ ∂DL and YT=ρ∂ψ ∂DT . (7.139) Using the simple mixture laws EL =φEs +(1-φ)Ec and ET = φ Es+1-φ Ec -1 (7.140) gives: YL =(1-φ)Ec 2 σ11 2 ˜ E+2 L + h -σ11 2 ˜ E-2 L YT≈1-φ 2Ec σ22 2 + σ33 2 (1 - DT)2 + h -σ22 2 + -σ33 2 (1 - hDT)2 (7.141)

7.4 Numerical Failure Analysis 371 which take into account (through h) the much lower damage growth for con- crete in compression than in tension. ... Congratulations to all readers who read up to this last page! ...

Bibliography 1. Introduction to Continuum Damage Mechanics, L.M. Kachanov (Marti- nus Nijhoff Dortrecht, The Netherlands 1986) 2. Continuum Damage Mechanics Theory and Applications, D. Krajcinovic, J. Lemaitre, CISM Lectures (Springer, Berlin Heidelberg New York 1987) 3. A Course on Damage mechanics, J. Lemaitre (Springer, Berlin Heidel- berg New York 1992--1996) 4. Damage Mechanics, D. Krajcinovic, North Holland Series in Appl. Math and Mech (Elsevier, 1996) 5. Modeling of Material Damage and Failure of Structures, J. Skrzypek, A. Ganczarski (Springer, Berlin Heidelberg New York 1999) 6. Advances in Damage Mechanics: Metals and Metal Matrix Composites, G.Z. Voyiadjis, P.I. Kattan (Elsevier, 1999) 7. Continuous Damage and Fracture, ed. by A. Benallal (Elsevier, 2000) 8. Handbook of Materials Behavior Models, ed. by J. Lemaitre (Academic Press, New York 2001) 9. Damage Mechanics with Finite Elements, P.I. Kattan, G.Z. Voyiadjis (Springer, Berlin Heidelberg New York 2002) 10. Formulas for Stress and Strain, R.J. Roark (Mc Graw Hill, New York 1965) 11. Stress Concentration Factors, R.E. Peterson (Wiley, New York 1974) 12. Handbook of Formulas for Stress and Strain, W. Griffel (Frederick Ungar, 1976)

Index ABAQUS, 175, 187, 261, 264, 362 accumulated plastic strain, 10 accumulation of damage, 196 adaptation, 211 adiabatic, 255 Aifantis, 113, 317 Albert, 277 Allix, 2, 356 aluminum, 175, 190 aluminum alloy, 267 Amar, 135 analysis fully coupled, 213 post-processing, 214 stochastic, 323 Andrade, 233 anisotropy, 21 composites, 344 damage, 4 induced, 44, 51, 111 plastic, 189 Armstrong--Frederick, 46, 229 Arrhenius, 255 ASTREE, 26, 219 Børvik, 269 Baˇ zant, 112--114, 321 Babuska, 112 ballistic limit, 272 Batdorf, 321 Bathias, 282 Bauschinger, 277 Belytschko, 112, 114 Benallal, 65, 69, 77, 97, 230, 258 Bennani, 267 Berstad, 269 Berthaud, 18, 44 Besson, 97, 103, 105, 172, 214 BFGS method, 125 bifurcation, 66 Billardon, 22, 65, 77, 88, 97, 117, 174, 184, 187, 258 Bish, 352 Boussinesq, 315 Broyden, 125 buckling, 158 post-∼, 255 Burlet, 230 Cailletaud, 230 Calloch, 64, 190, 230 Cano, 70 Cantournet, 221 carbon-fiber/epoxy-resin, 358 Carmet, 303 CASTEM, 348 ceramic, 364 ceramic matrix composites, 361 Cerruti, 315 Chaboche, 4, 10, 233, 281 Chaudonneret, 245 Chow, 4 Chranowski, 233 Chrysochoos, 28 Chu, 177 Claise, 23 Clausius--Duhem inequality, 9

376 Index Coffin, 191 Coin, 352 Coleman, 330 composites, 2, 13, 339, 346, 361 concrete, 13, 343, 346, 364 condition consistency, 10, 43, 46, 340 Kuhn--Tucker, 10 quasi-unilateral, 12, 33 constitutive equations, 8, 45, 46 convergence, 99, 103, 111 Cordebois, 6, 172 CORRELI, 23 Cough, 277 Cox, 315 crack arrest, 152, 208, 336 initiation, 27, 33, 65 orientation, 73 crash, 267 creep, 237 -damage, 33, 233, 240, 255 -fatigue, 237, 239, 251, 262 Crisfield, 94 criterion damage ∼, 339 Dang Van, 282 Hill, 268 of debonding, 327 rupture, 324 Sines, 282 von Mises, 10, 45 yield, 45, 83 Croix, 267 cross identification, 132, 166, 178 Curtin, 362 curve isochronous, 236 Manson--Coffin, 192, 193 R-∼, 153 W¨ ohler, 38, 64, 193 cyclic plasticity, 202 damage accumulation, 196, 217, 287, 302 anisotropic, 5, 15, 18, 34, 40, 57, 59, 75, 80, 171, 343 criterion, 65, 171, 339, 344 critical, 31, 65 definition, 3 equivalent strain, 326 equivalent stress, 11, 79, 157, 166, 188, 324, 328 hydrostatic, 6 interface, 358 isotropic, 5, 10, 52, 53, 55, 75, 80 multiplier, 340 non-local ∼ model, 114, 344 parameters, 47, 78, 138, 340, 343 quasi-brittle, 33, 183, 339 tensorial, 4 threshold, 27, 43, 76, 130, 161, 300 two-scale ∼ model, 283, 332 DAMAGE 2000, 119, 305, 311 Dang Van, 315 de Borst, 114 deep drawing, 170 delamination, 345, 356 Denoual, 364, 367 Deperrois, 315 Desmorat B., 345 Desmorat R., 14, 34, 97, 105, 172, 214, 221, 263 digital image correlation, 23 dissipation, 43, 60, 70, 222 distribution, 26, 278, 309, 365 Gaussian, 113, 323 Doghri, 65, 77, 88, 97, 117, 174 Dolbow, 112 Doudard, 64 Dragon, 345 Dub´ e, 354 Dufailly, 17, 22, 48, 50, 135, 143 dynamic plasticity, 142, 234, 248, 255 earthquake, 351 effective volume, 329, 366 EFICOS, 354 elastic predictior, 117 elastic predictor, 95 elasticity change, 17, 54, 178 elasto-(visco-)plasticity, 27, 45, 53, 55, 57, 59, 78, 267 elastomers, 221, 274 elementary layer, 345 Elshelby, 120 energy density, 218 effective elastic ∼, 12, 34, 85

Index 377 release rate, 10, 12, 32, 80 strain ∼,41 energy, stored, 8, 9, 27, 38, 41, 197 Engel, 2 Eshelby, 62, 116, 316 Eshelby--Kr¨ oner law, 62, 116, 284, 315 Evans, 321 exponential law, 98 extrusion, 172 Fairbarn, 277 fatigue asymptotic ∼ limit, 29, 37, 61, 64, 278, 282 creep-∼, 237, 251, 262 engineering ∼ limit, 36, 278, 282 mean stress effect, 62, 81, 287, 295 multilevel, 216 non-proportional, 305 fiber bundle, 330 Findley, 317 finite strains, 167, 221 Fl´ orez-L´ opez, 181 Fletcher, 125 Forest, 114 FORGE 2, 174 forming limits, 170 fragmentation, 366 frames, 181, 271, 351 Fran¸ cois, 190, 230 friction, 221, 223 fully coupled analysis, 213 function shape ∼,91 triaxiality ∼,11 Galtier, 64, 312 Ganczarski, 233 Gatuingt, 346 Gauss--Newton method, 124 Gaussian distribution, 113, 323 geomaterials, 176 Geymonat, 65 Gibbs energy, 345, 356 potential, 8, 357 specific free enthalpy, 343 glass, 364 Golfarb, 125 Goodman diagram, 280 gradient effect, 316 Grange, 173, 305 Green--Lagrange, 167, 221 Griffith, 321 Gupta, 190 Gurson, 176 Halford, 191 Halm, 345 hardening isotropic, 8, 45 kinematic, 8, 45, 82 Hart--Smith, 221 Hayhurst, 77, 233 heat capacity, 8, 70 Helmholtz potential, 8, 340 Hencky--Mises, 150, 161, 203 Henstenburg, 362 Hessian, 123, 125 Hild, 23, 321, 322, 329, 361, 364, 367 Hill, 66, 189, 268 homogenization, 61, 317, 369 Hopperstad, 269 Hult,1,233 hydrostatic sensitivity parameter, 6 hyperelasticity, 221, 275 identification, 47, 64, 120, 127, 135 cross ∼, 178, 181 image correlation, 23, 138, 185 impact, 269, 366 impact loading, 366 implicit scheme, 96, 117 IN 100 stainless alloy, 236, 262 Inconel alloy, 48 initial defect, 307, 322 interface damage, 358 internal friction, 41 sliding, 41, 43, 223, 275 intrusion-extrusion, 281 Jacobian, 124 matrix, 100, 107 terms, 101 Jaumann, 168 Johnson--Cook, 270 jump procedure, 88

378 Index Kachanov, 1, 3, 233, 235 Kirchhoff--Love, 304 Klingele, 2 Kr¨ oner, 62, 116, 120 Krajcinovic, 4, 330 Kuhn--Tucker condition, 10 Kurtyka, 190, 230 Laborderie, 341, 353, 354 Ladev` eze, 3, 11, 14, 168, 213, 341, 345 Lambert--Diani, 221 laminates, 345, 356 Langseth, 269 Lapra, 224 large scale yielding, 166, 245 Larsson, 361 Lauro, 267 law conduction, 70 elasticity, 10, 14, 70 evolution, 70 exponential, 51, 98 Hencky--Mises, 150, 161 Norton, 51, 98, 244, 245, 248, 254, 255, 258 Paris, 293 state, 9, 70 unified damage, 32, 37, 41 Lechatelier, 277 Leckie, 4, 77, 233, 261, 361 Le Dantec, 341, 346 Lemaitre, 1, 8, 11, 14, 33, 77, 120, 263 Lev` eque, 359 Levenberg--Marquardt method, 125 limit analysis, 166, 181 limit curve, 172 ballistic ∼, 272 localization ∼, 171 strain ∼, 164 stress ∼, 165 Lin, 114 Lin--Taylor, 120 localization Eshelby--Kr¨ oner law, 62, 116, 284, 315 limiters, 112, 350 strain ∼, 175 strain ∼, 65, 114, 170 tensor, 316 Lorentz, 114 LS-DYNA, 271 Luong, 64 Mac Clintoch, 141 Manson, 191 Manson--Coffin curve, 192, 193 maraging steel, 281 Marigo, 339 Mariott, 261 Marquis, 137, 190, 230 matrix ceramic ∼ composites, 361 Jacobian, 100, 107 sensitivity, 135, 146, 200, 242, 290, 334 Maugin, 168 Mazars, 44, 73, 321, 326, 350, 354 McClintock, 321 Melenk, 112 mesocrack initiation, 27, 31, 34, 65 method θ-, 98, 106 BFGS, 125 Gauss--Newton, 124 Levenberg--Marquardt, 125 Monte Carlo, 309 Neuber, 147, 150, 152, 155, 201, 244 Newton, 94, 124 SQP, 123, 125 strain energy density ∼, 201, 203 Meyers, 190 microdefects closure, 12, 171, 288, 324 effect, 55, 59, 341 parameter, 13 microhardness, 22, 186 microstress, 41, 62, 221 Miner rule, 197 Mises signed von ∼ stress, 82 von ∼ criterion, 10, 45 von ∼ equivalent stress, 11 Mo¨ es, 112 Molinari, 69 Monte Carlo method, 308 Mooney, 221 Moreau, 91 Moret--Bailly, 258 Morrow, 191

Index 379 Moussy, 172 Mroz, 112, 230 Mulhaus, 114 multifragmentation, 362, 364 Murakami, 4 Needleman, 141, 176 negative part, 13, 15 Neuber method, 147, 150, 152, 155, 201, 244 Newton--Raphson method, 94, 124 Nguyen Q.S., 91 Nocedal, 123 non-local damage model, 114, 344 nonlinear accumulation, 280 normality rule, 9, 177, 222 Norton law, 43, 98, 233, 244, 245, 248, 254, 255, 258 Oˇ zbolt, 113 Oh, 112 Ohno, 230 Onat, 4 Ortiz, 270 Palmgreen--Miner rule, 195, 215, 229, 280, 302 PAMCRASH 2000, 268 Panoskaltsis, 317 Papadopoulos, 317 parameter necking, 35 viscosity, 50, 128, 265 Paris law, 293 perturbation, 69, 103 Phoenix, 362 Pietruszczak, 112 Pijaudier-Cabot, 113 Pilvin, 122 Pineau, 191, 215, 321 Piola--Kirchhoff, 167, 221 plastic corrector, 92, 96 hinges, 160, 181, 255 Poisson process, 365 polymers, 13, 75, 167, 275 porosity, 176 positive part, 13, 15 post-buckling, 158, 255 post-processing analysis, 78, 85, 115, 214 post-processor DAMAGE 2000, 119, 301, 305, 311 potential Gibbs ∼, 8, 343, 357 Helmholtz ∼, 8, 70, 339 of dissipation, 9, 26, 42, 45, 222 state ∼, 8, 15, 41, 221 powders, 176 pre-stress, 234, 346 predamaged, 184, 227, 272, 312 predeformed, 184, 227, 272, 312 principle of strain equivalence, 8, 10, 11, 42 second, 9 probabilistic safety margin, 335 proportional loading, 82, 160 quasi-brittle materials, 321, 339 R-curve, 153 Rabotno v,5,233 Ragueneau, 345, 346, 350 Ramtani, 44 random loading, 297, 314 Representative Volume Element, 75 Rey, 221 Rice, 66, 141 Riks, 94 rocks, 364 Rousselier, 112, 176 Rousset, 190 Roux, 23 rubber, 86, 223 Rudnicki, 66 Saanouni, 172 safety factor, 152, 208, 247, 292, 334 Sauzay, 21, 34, 303, 315 scale effect, 281 scatter, 247, 292, 299, 307 SED method, 203, 204, 216 seismic loading, 350 sensitivity, 135, 146, 200, 242, 290, 334 Sermage, 130, 134, 218, 262, 263, 300, 313 Shah, 2 shakedown, 210

380 Index Shanno, 125 shape function, 91 shear band, 67, 112 Shi, 112 SIDOLO, 120, 132 Sidoroff, 6 Simo, 91, 103 Sines fatigue criterion, 282 Skrzypek, 233 sliding, 41, 43, 223, 275 small scale yielding, 86, 148, 201 Socie, 191 SQP method, 123, 125 stabilized cycle, 49, 88, 131, 211, 226 steel, 21, 39, 64, 75, 171, 256 2-1/4 CrMo, 129, 132, 217, 265 316 stainless, 249 35 NCD 16, 280 dual phase, 64 ferritic, 36, 158 low carbon, 187 SOLDUR 355, 21, 214 Weldox 460E, 271 stirrups, 348 stochastic analysis, 292, 297, 309, 323 strain accumulated plastic ∼ ,10 energy density, 11, 41, 218 energy release rate, 292 equivalence principle, 8 finite, 167 strains finite, 221 stress back, 45, 62, 231 concentration, 147, 201, 208, 244 coefficient, 148, 154 effective, 5, 8, 12, 13, 31, 34, 42, 104, 116, 119, 189, 322 hydrostatic, 11 interface equivalent ∼, 327 mean, 301 nominal, 148 Piola--Kirchhoff, 221 signed von Mises ∼,82 ultimate, 36 viscous, 45 Weibull, 329 yield, 248 Taira rule, 237, 274 Tanaka, 230 tangent operator, 66, 72 consistent ∼, 92, 111 Taylor, 91, 103 thermodynamics, 7 Tison, 267 toughness, 74, 154, 292, 335 Tracey, 141 triaxiality, 11, 34, 145, 150 effective ∼ function, 81 function, 11, 86 Truesdell, 168 Tvergaard, 141, 176, 177 UDIMET 700 alloy, 193 ultrasonic waves, 17 unified damage law, 32, 37, 41 variables of state, 7 Vincent, 190 Virely, 218 virtual work principle, 91 VISCOENDO, 261, 262, 264 Voigt, 91 Voyiadjis, 321 W¨ ohler curve, 38, 64, 193, 279, 301, 313 Wang, 230 weakest link hypothesis, 329, 366 Weibull, 307, 321 model, 328, 366 modulus, 328, 361 stress, 329 Wempner, 94 Wright, 123 yield criterion, 45, 83 yield stress, 22, 248 ZeBuLon, 171, 214 Zyczkowski, 190